# Introduction to Semiconductor Physics and Devices 3031084578, 9783031084577

##### This classroom-tested textbook provides a self-contained one-semester course in semiconductor physics and devices that i

121 82 4MB

English Pages 337 [325] Year 2022

Preface
Contents
Part I Fundamental Physics
1 Principles of Quantum Mechanics
1.1 Why Quantum Mechanics?
1.2 Wave–Particle Duality
1.3 Wavelength of a Free Particle in Terms of Its Energy
1.4 Energy Quantization
1.6 The Wave Function
1.7 The Wave Function of a Free Particle
1.8 Schrödinger's Equation
1.8.1 Time-Dependent Schrödinger's Equation
1.8.2 Time-Independent Schrödinger's Equation
1.9 Probabilistic Interpretation and the Collapse of the Wave Function
1.10 Measurable and Unmeasurable in Quantum Mechanics
1.11 Electron States in a Hydrogen Atom
1.12 Spin
1.13 Degeneracy
1.14 Indistinguishability of Quantum Particles
1.15 Spin-Statistics Theorem
1.16 Pauli's Exclusion Principle
1.17 Problems
1.17.1 Solved Problems
1.17.2 Practice Problems
1.17.3 Solutions
2 Crystal Structure of Solids
2.1 Periodic Table of Elements
2.2 Chemical Bonding
2.3 Crystal Lattices
2.3.1 Atomic Order in Solids
2.3.2 Bravais Lattices
2.3.3 Unit Cell, Primitive Cell, and Crystal Basis
2.3.4 Volume Density and Atomic Packing Fraction
2.4 Basic Cubic Structures
2.5 Formation of Diamond Structure
2.6 Miller Indices
2.6.1 Determination of Miller Indices
2.6.2 Miller Indices for Cubic Structures
2.7 Imperfections and Impurities in Solids
2.8 Problems
2.8.1 Solved Problems
2.8.2 Practice Problems
2.8.3 Solutions
3 Equilibrium Statistical Mechanics
3.1 Microstates and Macrostates
3.2 Thermal Equilibrium
3.3 Postulate of Equal A Priori Probabilities
3.4 Grand Canonical Distribution
3.5 Fermi-Dirac Distribution
3.6 Boltzmann Approximation
3.7 Fermi Energy at Low Temperatures
3.8 Problems
3.8.1 Solved Problems
3.8.2 Practice Problems
3.8.3 Solutions
4 Band Theory of Solids
4.1 Bloch's Theorem
4.2 Energy Bands
4.2.1 Physical Origin of the Energy Bands
4.2.2 The First Brillouin Zone
Brillouin Zones
One-Dimensional Crystal
Band Gap
The Energy-Momentum Diagrams in Three Dimensions
Quasimomentum
4.2.3 Phase Velocity vs. Group Velocity
Phase Velocity
Group Velocity
4.2.4 Bloch Oscillations
4.3 Conduction Types of Solids
4.3.1 Band Filling and Electrical Conductivity
4.3.2 Metals and Semimetals
4.3.3 Dielectrics and Semiconductors
4.4 Conduction and Valence Bands
4.5 Holes
4.6 Effective Mass Tensor
4.7 Problems
4.7.1 Solved Problems
4.7.2 Practice Problems
4.7.3 Solutions
Part II Semiconductors in and out of Equilibrium
5 Semiconductors in Equilibrium
5.1 Density of States
5.2 Equilibrium Carrier Concentration
5.3 Energy Probability Distribution
5.4 Density of States Effective Mass vs. Conductivity Effective Mass
5.4.1 Density of States Effective Mass
5.4.2 Conductivity Effective Mass
Electrons
Holes
5.4.3 Thermal Velocity
5.5 Intrinsic Semiconductors
5.6 Doping and Extrinsic Semiconductors
5.7 Impurity Energy Levels
5.8 Statistics of Donors and Acceptors
5.9 Mass Action Law
5.10 Charge Neutrality Equation
5.11 Ionization Regimes
5.11.1 Complete Ionization
5.11.2 Intrinsic Regime
5.11.3 Carrier Concentration in a Semiconductor with One Type of Doping at Not Too High Temperatures
5.11.4 Electron Freeze-Out Regime
5.12 Numerical Determination of Fermi Energy and Carrier Concentrations
5.13 Problems
5.13.1 Solved Problems
5.13.2 Practice Problems
5.13.3 Solutions
6 Carrier Concentration and Electric Potential
6.1 Electron and Hole Concentrations in a Non-uniform Electric Potential
6.2 Poisson's Equation
6.3 Approximate Solution of Poisson's Equation
6.3.1 Problem Formulation
6.3.2 Debye Screening
6.3.3 Depletion Approximation
6.3.4 Validity Range of the Depletion Approximation
6.4 Band Diagrams and Band Bending
6.5 Electric Potential in a Semiconductor from Poisson's Equation
6.5.1 Exact Solution of Poisson's Equation
6.5.2 Numerical Results
6.6 Problems
6.6.1 Solved Problems
6.6.2 Practice Problems
6.6.3 Solutions
7 Generation–Recombination Processes
7.1 Recombination Mechanisms
7.2 Charge Carrier Dynamics
7.2.1 Generation and Recombination Rates
7.2.2 Recombination Time Approximation
7.4 Auger Recombination
7.5.1 Electron and Hole Capture and Emission by the Traps
7.5.2 The Principle of Detailed Balance
7.5.3 The Net SRH Recombination Rate
7.5.4 SRH Recombination Time
7.6 Surface Recombination
7.7 Quasi-Fermi Energies
7.8 Problems
7.8.1 Solved Problems
7.8.2 Practice Problems
7.8.3 Solutions
8 Carrier Transport
8.1 Flux and Electric Current Density
8.2 Diffusion Current
8.3 Drift Current
8.4 Conductivity and Resistivity
8.5 Current–Voltage Measurements
8.5.1 Photoconductivity
8.5.2 Hall Effect
8.6 Temperature and Doping Level Dependence of Mobility
8.7 Einstein's Relation
8.8 Continuity Equation
8.9 Problems
8.9.1 Solved Problems
8.9.2 Practice Problems
8.9.3 Solutions
Part III Semiconductor Devices
9 Metal–Semiconductor Contact
9.1 Reasons to Study
9.2 Energy Band Diagram
9.3 SCR Capacitance
9.4 Ohmic Contact
9.5 Rectification in a Metal–Semiconductor Contact
9.5.1 Metal/n-Type Semiconductor Junction
Qualitative Considerations
9.5.2 Reverse Saturation Current Density of a Schottky Diode
9.5.3 Metal/p-Type Semiconductor Junction
9.6 Non-ideality Effects
9.7 Problems
9.7.1 Solved Problems
9.7.2 Practice Problems
9.7.3 Solutions
10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)
10.1 MOSFET Schematics and Operation Principle
10.2 Qualitative Description of MOSFET I-V Curve
10.3 Quantitative Description of a MOSFET I-V Curve
10.4 Determination of the Threshold Voltage
10.4.1 Energy Band Diagram of a MOS Structure at Zero Gate Voltage
10.4.2 Energy Band Diagram of a MOS Structure for Non-zero Gate Voltage
10.4.3 Oxide Voltage
10.4.4 Flat-Band Voltage
10.4.5 Threshold Voltage
10.5 Capacitance–Voltage Measurements
10.6 Problems
10.6.1 Solved Problems
10.6.2 Practice Problems
10.6.3 Solutions
11 PN Junction Diode
11.1 The Structure of a pn Junction
11.2 The Energy Band Diagram of a pn Junction at Zero Bias
11.3 PN Junction Under an External Bias
11.4 SCR Capacitance
11.5 Current–Voltage Relation of a pn Junction Diode
11.5.1 Charge Carrier Concentrations Near the Boundaries of the SCR
11.5.2 Current–Voltage Relation of an Ideal pn Junction Diode
11.5.3 Current Densities in a pn Diode
11.5.4 SCR Recombination Current
11.6 Problems
11.6.1 Solved Problems
11.6.2 Practice Problems
11.6.3 Solutions
12 Optoelectronic Devices
12.1 Solar Cells (SCs)
12.1.1 SC Operation
12.1.3 Light Absorption
12.1.4 SC Current–Voltage Relation
12.2 Light-Emitting Diodes (LEDs)
12.2.1 LED Operation
12.2.2 LED Spectrum
12.2.3 LED Efficiency
12.2.4 Increasing the LED Efficiency
12.3 Semiconductor Lasers
12.3.1 Stimulated Emission and Einstein's Coefficients
12.3.2 Generation of Light
12.3.3 Semiconductor Laser Operation
The Structure of a Semiconductor Laser
Threshold Current
Laser Spectrum
12.4 Problems
12.4.1 Solved Problems
12.4.2 Practice Problems
12.4.3 Solutions
Appendices
A.1 A Crash Course in Complex Numbers
A.2 Proof of Bloch's Theorem
A.3 Properties of Si, Ge, and GaAs
A.4 Evaluation of Exponential Integrals
Index
##### Citation preview

Mykhaylo Evstigneev

Introduction to Semiconductor Physics and Devices

Introduction to Semiconductor Physics and Devices

Mykhaylo Evstigneev

Introduction to Semiconductor Physics and Devices

Mykhaylo Evstigneev Department of Physics and Physical Oceanography Memorial University of Newfoundland St. John’s, NL, Canada

ISBN 978-3-031-08457-7 ISBN 978-3-031-08458-4 https://doi.org/10.1007/978-3-031-08458-4

(eBook)

Preface

When I was assigned to teach physics of device materials at Memorial University of Newfoundland 7 years ago, I got excited. Who would not be happy to tell the students about such diverse areas as quantum mechanics, statistical physics, theory of solids, electrodynamics, and crystallography, not to mention some cool electronic applications, in a one-semester course? This opportunity was especially thrilling, because the majority of my audience consisted of second-year engineering students with little or no prior knowledge about most of these subjects. It is always great to be the first to tell young people about something tremendously important. Finding a suitable text is the first challenge an instructor faces before teaching a course. This choice is usually made based on two factors: the knowledge the instructor intends to impart to the students and their background preparation level. There are many excellent books on semiconductor physics. But some of them implicitly assume the readers’ familiarity with the topics mentioned above, while others dig into those topics too deeply and are more suitable for the advanced undergraduate or graduate physics students. Neither description applied to my audience. Hence, I wrote a few pages on quantum mechanics and a few on statistical physics, which I shared with the students as a handout. As I was teaching this course in the following years, I added more material to those notes, which finally developed into this book. The book contains three roughly equal parts, each of which can be covered in about one month’s time. The first part, Fundamental Physics, gives the background information students will need to understand the rest of the text: quantum mechanics, crystal structure of solids, statistical mechanics, and band theory of solids. In the second part, this information is applied to explain the basic properties of semiconductors, namely the concentration of charge carriers in equilibrium, the interrelation between the carrier concentration and a non-uniform electric potential, the generation-recombination processes, and, finally, the response of the charge carriers to an electric field. The third part applies what the students have learned

v

vi

Preface

earlier in the book to explain some semiconductor devices: the Schottky diodes, the MOSFETs, the pn junction diodes, and some optoelectronic applications thereof. Since my intention was to give only slightly more material than can be delivered within a one-semester course, many topics were left out. For example, the sizerelated effects in the semiconductor devices and the bipolar transistor are not discussed. An interested reader is referred to a number of excellent texts to fill those gaps, such as: K. Brennan, The Physics of Semiconductors (Cambridge University Press, 1999) J.P. Collinge and C.A. Collinge, Physics of Semiconductor Devices (Kluwer Academic Publishers, 2002) J.A. del Alamo, Integrated Microelectronic Devices: Physics and Modeling (Pearson, 2018) C. Hamaguchi, Basic Semiconductor Physics (Springer, 2010) C. Hu, Modern Semiconductor Devices for Integrated Circuits (Pearson, 2009) M. Grundmann, The Physics of Semiconductors (Springer, 2010) J.P. McKelvey, Solid State and Semiconductor Physics (R.F. Krieger Publishing Company, 1966) R.S. Muller and Th.I. Kamins, “Device Electronics for Integrated Circuits” (Wiley, 2002) D. Neamen, Semiconductor Physics and Devices (McGraw-Hill, 2003) C. Papadopoulos, Solid-State Electronic Devices (Springer, 2014) R.F. Pieret, Semiconductor Device Fundamentals (Addison-Wesley Publishing Company, 1996) D.K. Schroder, Semiconductor Material and Device Characterization (Wiley, 2006) K. Seeger, Semiconductor Physics (Springer, 2004) R.A. Smith, Semiconductors (Cambridge Univ. Press, 1978) S.M. Sze and M.K. Lee, Semiconductor Devices (Wiley, 2012) S.M. Sze and K.K. Ng, Physics of Semiconductor Devices (Wiley, 2007) P.Y. Yu and M. Cardona, Fundamentlals of Semiconductors (Springer, 2010) Reading a book like this is best done with pencil and paper. Ideally, a student should understand the material well enough to be able to explain it to another student. At the end of each chapter, the student will find problems that should, hopefully, strengthen their understanding of the chapter material. Each of the problem sections consists of three parts: solved problems, practice problems, and solutions. Students are encouraged to first try and tackle the problems by themselves and look into the solutions only if they are stuck. Although I made every effort to make this book free of errors, I cannot guarantee that it is. I will greatly appreciate it if the readers inform me about any typo and mistake they find, or offer any other suggestions and criticism by email at [email protected]. I would like to thank my students and colleagues for their input. I am indebted to Dr. Michael Morrow for sharing his own materials with me when I got to teach this course for the first time. It has been a great pleasure to discuss pertinent

Preface

vii

subjects with Drs. Anatoliy Sachenko and Igor Sokolovskyi from the Institute of Semiconductor Physics in Kyiv, Ukraine. Last but not least, I thank Gleb Evstigneev for his suggestions that helped me improve the style of this text. I dedicate this book to Ukraine, my brave home country. St. John’s, NL, Canada

Mykhaylo Evstigneev

Contents

Part I Fundamental Physics 1

2

Principles of Quantum Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.1 Why Quantum Mechanics? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Wave–Particle Duality . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.3 Wavelength of a Free Particle in Terms of Its Energy . . . . . . . . . . . . . 1.4 Energy Quantization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5 Radiation Spectrum of Hydrogen . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6 The Wave Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.7 The Wave Function of a Free Particle . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.8 Schrödinger’s Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.8.1 Time-Dependent Schrödinger’s Equation . . . . . . . . . . . . . . . . . 1.8.2 Time-Independent Schrödinger’s Equation . . . . . . . . . . . . . . . 1.9 Probabilistic Interpretation and the Collapse of the Wave Function . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.10 Measurable and Unmeasurable in Quantum Mechanics . . . . . . . . . . . 1.11 Electron States in a Hydrogen Atom . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.12 Spin . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.13 Degeneracy . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.14 Indistinguishability of Quantum Particles . . . . . . . . . . . . . . . . . . . . . . . . . . 1.15 Spin-Statistics Theorem . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.16 Pauli’s Exclusion Principle . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.17 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.17.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.17.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.17.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

3 3 5 7 8 9 11 14 15 15 17

Crystal Structure of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.1 Periodic Table of Elements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2 Chemical Bonding . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 Crystal Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.1 Atomic Order in Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

41 41 42 43 43

17 21 23 24 24 25 26 27 28 28 29 31

ix

x

Contents

2.3.2 Bravais Lattices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.3 Unit Cell, Primitive Cell, and Crystal Basis . . . . . . . . . . . . . . 2.3.4 Volume Density and Atomic Packing Fraction . . . . . . . . . . . Basic Cubic Structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Formation of Diamond Structure . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Miller Indices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.1 Determination of Miller Indices . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.6.2 Miller Indices for Cubic Structures . . . . . . . . . . . . . . . . . . . . . . . Imperfections and Impurities in Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.8.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.8.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.8.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

44 45 47 48 50 51 51 52 53 54 54 55 56

3

Equilibrium Statistical Mechanics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.1 Microstates and Macrostates . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.2 Thermal Equilibrium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.3 Postulate of Equal A Priori Probabilities . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.4 Grand Canonical Distribution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.5 Fermi-Dirac Distribution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.6 Boltzmann Approximation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.7 Fermi Energy at Low Temperatures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 3.8.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

61 61 62 63 64 67 69 69 73 73 74 74

4

Band Theory of Solids. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.1 Bloch’s Theorem . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Energy Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.1 Physical Origin of the Energy Bands . . . . . . . . . . . . . . . . . . . . . 4.2.2 The First Brillouin Zone . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.2.3 Phase Velocity vs. Group Velocity . . . . . . . . . . . . . . . . . . . . . . . . 4.2.4 Bloch Oscillations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Conduction Types of Solids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.1 Band Filling and Electrical Conductivity . . . . . . . . . . . . . . . . . 4.3.2 Metals and Semimetals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3.3 Dielectrics and Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Conduction and Valence Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.5 Holes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.6 Effective Mass Tensor . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.7 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.7.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.7.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.7.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

81 81 83 83 84 90 94 96 96 97 97 98 99 101 104 104 105 106

2.4 2.5 2.6

2.7 2.8

Contents

xi

Part II Semiconductors in and out of Equilibrium 5

6

Semiconductors in Equilibrium . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.1 Density of States . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.2 Equilibrium Carrier Concentration . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.3 Energy Probability Distribution . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 Density of States Effective Mass vs. Conductivity Effective Mass . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.1 Density of States Effective Mass . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.2 Conductivity Effective Mass . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.3 Thermal Velocity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Intrinsic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.6 Doping and Extrinsic Semiconductors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.7 Impurity Energy Levels . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.8 Statistics of Donors and Acceptors . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.9 Mass Action Law . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.10 Charge Neutrality Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.11 Ionization Regimes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.11.1 Complete Ionization . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.11.2 Intrinsic Regime . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.11.3 Carrier Concentration in a Semiconductor with One Type of Doping at Not Too High Temperatures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.11.4 Electron Freeze-Out Regime . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.12 Numerical Determination of Fermi Energy and Carrier Concentrations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.13 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.13.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.13.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.13.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

115 115 119 121

Carrier Concentration and Electric Potential . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.1 Electron and Hole Concentrations in a Non-uniform Electric Potential . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.2 Poisson’s Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3 Approximate Solution of Poisson’s Equation . . . . . . . . . . . . . . . . . . . . . . 6.3.1 Problem Formulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.2 Debye Screening . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.3 Depletion Approximation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.3.4 Validity Range of the Depletion Approximation . . . . . . . . . 6.4 Band Diagrams and Band Bending . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5 Electric Potential in a Semiconductor from Poisson’s Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5.1 Exact Solution of Poisson’s Equation . . . . . . . . . . . . . . . . . . . . . 6.5.2 Numerical Results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.6 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

151

122 122 123 125 126 127 128 130 132 133 134 134 136

137 138 140 142 142 143 144

151 152 154 154 155 156 158 160 161 161 164 167

xii

Contents

6.6.1 6.6.2 6.6.3 7

8

Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 167 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 167 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 168

Generation–Recombination Processes . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.1 Recombination Mechanisms . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2 Charge Carrier Dynamics . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2.1 Generation and Recombination Rates . . . . . . . . . . . . . . . . . . . . . 7.2.2 Recombination Time Approximation . . . . . . . . . . . . . . . . . . . . . 7.3 Radiative Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.4 Auger Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5 Shockley-Read-Hall (SRH) Recombination . . . . . . . . . . . . . . . . . . . . . . . . 7.5.1 Electron and Hole Capture and Emission by the Traps . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5.2 The Principle of Detailed Balance . . . . . . . . . . . . . . . . . . . . . . . . 7.5.3 The Net SRH Recombination Rate . . . . . . . . . . . . . . . . . . . . . . . . 7.5.4 SRH Recombination Time . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.6 Surface Recombination . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.7 Quasi-Fermi Energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.8 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.8.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.8.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.8.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

171 171 173 173 176 177 178 180

Carrier Transport . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.1 Flux and Electric Current Density . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.2 Diffusion Current . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3 Drift Current . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.4 Conductivity and Resistivity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.5 Current–Voltage Measurements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.5.1 Photoconductivity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.5.2 Hall Effect . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.6 Temperature and Doping Level Dependence of Mobility . . . . . . . . . 8.7 Einstein’s Relation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.8 Continuity Equation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.9 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.9.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.9.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.9.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

197 197 199 199 201 202 202 202 204 205 206 208 208 208 209

180 182 183 184 186 187 189 189 190 191

Part III Semiconductor Devices 9

Metal–Semiconductor Contact . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.1 Reasons to Study . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.2 Energy Band Diagram . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.3 SCR Capacitance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

215 215 215 218

Contents

9.4 9.5

Ohmic Contact . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Rectification in a Metal–Semiconductor Contact . . . . . . . . . . . . . . . . . . 9.5.1 Metal/n-Type Semiconductor Junction . . . . . . . . . . . . . . . . . . . 9.5.2 Reverse Saturation Current Density of a Schottky Diode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.5.3 Metal/p-Type Semiconductor Junction . . . . . . . . . . . . . . . . . . . Non-ideality Effects . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 9.7.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

219 221 221

Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET) . . . . 10.1 MOSFET Schematics and Operation Principle . . . . . . . . . . . . . . . . . . . . 10.2 Qualitative Description of MOSFET I − V Curve . . . . . . . . . . . . . . . . 10.3 Quantitative Description of a MOSFET I − V Curve . . . . . . . . . . . . . 10.4 Determination of the Threshold Voltage . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4.1 Energy Band Diagram of a MOS Structure at Zero Gate Voltage . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4.2 Energy Band Diagram of a MOS Structure for Non-zero Gate Voltage . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4.3 Oxide Voltage . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4.4 Flat-Band Voltage . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.4.5 Threshold Voltage . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.5 Capacitance–Voltage Measurements . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.6 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.6.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.6.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 10.6.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

233 233 235 237 239

PN Junction Diode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.1 The Structure of a pn Junction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.2 The Energy Band Diagram of a pn Junction at Zero Bias . . . . . . . . . 11.3 PN Junction Under an External Bias . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.4 SCR Capacitance . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5 Current–Voltage Relation of a pn Junction Diode . . . . . . . . . . . . . . . . . 11.5.1 Charge Carrier Concentrations Near the Boundaries of the SCR . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5.2 Current–Voltage Relation of an Ideal pn Junction Diode . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5.3 Current Densities in a pn Diode . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.5.4 SCR Recombination Current . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.6 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.6.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.6.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11.6.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

257 257 258 260 262 263

9.6 9.7

10

11

xiii

223 225 226 228 228 229 230

239 240 242 243 244 245 248 248 249 249

263 264 267 268 269 269 270 271

xiv

12

Contents

Optoelectronic Devices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1 Solar Cells (SCs) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1.1 SC Operation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1.2 Spectral Irradiance (Spectral Intensity) . . . . . . . . . . . . . . . . . . . 12.1.3 Light Absorption . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.1.4 SC Current–Voltage Relation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2 Light-Emitting Diodes (LEDs) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.1 LED Operation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.2 LED Spectrum . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.3 LED Efficiency . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.2.4 Increasing the LED Efficiency . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3 Semiconductor Lasers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3.1 Stimulated Emission and Einstein’s Coefficients . . . . . . . . . 12.3.2 Generation of Light . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.3.3 Semiconductor Laser Operation . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.4 Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.4.1 Solved Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.4.2 Practice Problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 12.4.3 Solutions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

275 275 275 276 278 280 283 283 283 284 288 289 289 293 294 300 300 301 301

Appendices . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.1 A Crash Course in Complex Numbers . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.2 Proof of Bloch’s Theorem . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.3 Properties of Si, Ge, and GaAs . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.4 Evaluation of Exponential Integrals . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . A.5 Planck’s Radiation Law . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .

305 305 308 311 314 315

Index . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 319

Part I

Fundamental Physics

Chapter 1

Principles of Quantum Mechanics

1.1 Why Quantum Mechanics? As far back as ca. 2700 years ago, some natural philosophers speculated that the building block of matter is a small particle they called an atom; its Greek name ατ oμoν means “indivisible.” Given its correctness, it comes as a surprise that atomism was a disputed idea for two and a half millennia. Science is not all about brilliant ideas and deep insights into the nature’s ways. It is also about healthy skepticism and reluctance to accept a particular theory before every competing theory is ruled out. People who were critical of atomism were not necessarily bad scientists; quite the opposite is true about many of them. The simple reason why it took so long for atoms to enter the mainstream of science is that seeing is believing. Atoms are too tiny to be seen even in the best optical microscope. One had to rely on the indirect evidence rather than direct observation of atoms. For example, one can look at the barely visible small objects, such as pollen, coal dust, and similar particles suspended in water. Their irregular Brownian motion can be interpreted as caused by the unequal number of hits they receive from different sides at each instant of time. The hits are coming from atoms. Another example: chemists noticed that the masses of substances participating in chemical reactions are related to each other as integer numbers. This can be taken as an evidence of the minimal building blocks of matter that form chemical compounds by reacting with each other. But with a bit of imagination, one can think of other (wrong) explanations of these facts based on the information that was available in the pre-nineteenth century science. The big breakthrough was made by Joseph Thomson in 1897, who discovered that atoms are not as indivisible as previously believed. Thomson was interested in the flow of electric current between two metal plates placed against each other inside a vacuum tube. He showed that the current is carried by the negatively charged

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_1

3

4

1 Principles of Quantum Mechanics

particles (the electrons), whose charge-to-mass ratio could be measured by studying the deflection of an electron beam in electric and magnetic fields. The next step was made in the 1910s by Geiger, Marsden, and Rutherford, who studied the transmission of alpha-particles through a thin metal foil. Their angular distribution signaled that alpha-particles underwent collisions with the positively charged nuclei thousands of times heavier than the electrons orbiting around it. At a slightly earlier time, another line of research was actively being developed: the electromagnetism. It became established that an accelerated charge emits electromagnetic waves. Now, circular motion is a special type of an accelerated motion. An electron orbiting around the nucleus should emit electromagnetic waves, thereby losing energy and approaching the nucleus very quickly. Eventually, the electron should fall into the nucleus. An atom consisting of a heavy nucleus with light electrons orbiting around it cannot be stable. One might have thought that this model was lacking some important piece of information that would explain the stability of atoms. But what was actually needed was an all-out revision of everything that physicists knew at that time. New physics had to be created, which we know as quantum mechanics. The first step toward its creation was made by Max Planck in 1900, who derived the thermal radiation spectrum of a body that absorbs all of the incident radiation.1 The crucial step in his derivation was an assumption that the energy of an electromagnetic wave is directly proportional to its frequency. Making assumptions, especially as strong as this one, is dangerous. Planck had to take this desperate step simply because nothing else worked. So, how does quantum mechanics explain the stability of atoms? At the most fundamental level, acceleration of an electron means that its state of motion changes; when this happens, an electron emits an electromagnetic wave. In quantum mechanics, the concept of the state of motion is replaced by that of a quantum state. Similar to the classical picture, it is only when an electron changes its quantum state that it emits an electromagnetic wave. Unlike the classical state of motion, quantum states of an electron in an atom are not characterized by continuous variables such as electron’s velocity and position. Rather, quantum states are described by a not too large set of discrete parameters, called quantum numbers. To each quantum state corresponds its own energy. When an electron goes from a higher-energy quantum state to a lower-energy one, it emits an electromagnetic wave. Out of all electron states in an atom, there is a special one with the lowest energy. It is called the ground state. An electron in the ground state cannot lose energy anymore; the only way out of the ground state is up to a higher-energy state. For this reason, an electron cannot fall into the nucleus. This physical picture allows to make an important statement that atoms radiate light only of well-defined discrete energies that correspond to the energy differences between different quantum states. This is indeed what is going on in real life, as was established by the spectrometrists well before the advent of quantum mechanics.

1 This

derivation is presented in Appendix A.5.

1.2 Wave–Particle Duality

5

Quantum mechanics has a huge predictive power. Not only does it explain quantitatively the stability of atoms and their radiation spectra, but also it tells us why and how atoms interact with each other to form small molecules or large crystalline structures. It explains the properties of electrons in solids, in particular, in semiconductors that form the basis of electronic devices. At present, it revolutionizes the whole computer industry by introducing quantum computers that operate based on its rules. It is impossible to understand anything in modern physics without a solid knowledge of quantum theory. The purpose of this chapter is to give the reader just enough background information in quantum mechanics to be able to understand the rest of the book.

1.2 Wave–Particle Duality There is an obvious difference between waves and particles. A particle is a localized point-like object with well-defined mass, m, position, r, and velocity, v, and also energy, E, and momentum, p.  A free particle moves with a constant velocity from the initial position r0 . At a given time t > 0, its position is r = vt + r0 . Its kinetic energy is E = mv 2 /2, and its momentum is p = m v. A wave, on the other hand, is a time-dependent perturbation that propagates in space. This perturbation may be, e.g.,2 pressure and density variations in a sound wave, liquid level oscillations in a surface wave, or electric and magnetic fields in an electromagnetic wave. A plane wave is completely delocalized in space. It is described by the wave function, which is proportional, e.g., to sin(k · r − ωt), where k is the wave vector and ω is the angular frequency of the wave, related to its frequency, f , as ω = 2πf . If one fixes the position r, then the wave will repeat itself with the periodicity T = 1/f = 2π/ω, which is the period of the wave. If one takes a snapshot of the wave at a fixed time t, one will find that the wave repeats itself in space with the space period λ, the wavelength. The magnitude of the wave vector is  The direction of k is the direction of related to the wavelength, λ, by λ = 2π/|k|. wave propagation. The velocity of the wave is the velocity with which a particular peak of the wave function moves. It is obtained from the condition of constant phase:  k λ k k · r − ωt = const, giving r = vt + r0 with v = k kω2 = ω kk = ωλ 2π k = T k . k Before the twentieth century, it was believed that the distinction between particles and waves was clear-cut. Atoms and electrons were thought to be particles, whereas light was considered to be a wave. The situation changed when it was discovered that sometimes particles behave like waves, and waves behave like particles. This is called the wave–particle duality.

2 Some Latin abbreviations commonly used in the scientific literature are: e.g. = exempli gratia (for example), cf. = confer (compare), i.e. = id est (that is), etc. = et cetera (and so on), i.a. = inter alia (among others), viz. = videlicet (namely), vs. = versus (against), etc.

6

1 Principles of Quantum Mechanics

The first indication that waves displayed particle properties was discovered by Max Planck (1900), who tried to explain thermal radiation of bodies that do not reflect incident light but absorb it completely. Even though their absorption coefficient is 1 and reflection coefficient is 0, these so-called black bodies do radiate light when heated; the higher their temperature, the more light they produce. In order to understand the experimentally observed spectrum, Planck had to postulate that light propagates in elementary quanta, which were later called photons. Each photon carries the energy proportional to the frequency, E = hf = h¯ ω with the proportionality constants being h = 6.6260704 . . . · 10−34 J · s = 4.13566766 . . . · 10−15 eV · s; h¯ = 1.0545718 . . . · 10−34 J · s = 6.58211951 . . . · 10−16 eV · s. The constant h is called Planck’s constant, and h¯ = h/(2π ) is known as the reduced Planck constant. The values of h and h¯ can be established by fitting the experimental black-body radiation spectrum with Planck’s theoretical formula. An independent test of the theory, which also allows one to measure Planck’s constant, is the photoelectric effect, that is, light-induced emission of electrons by metal surfaces. As was found experimentally, the energy of the electrons produced is proportional to the frequency of the incident light with the proportionality constant h. This finding was interpreted by Albert Einstein (1905) as an indication of the fact that light quanta give their energy hf to the electrons in the metal, thus enabling them to leave the metal. About two decades later, Arthur Compton (1923) studied the scattering of Xrays by electrons. He found that the wavelength of the scattered X-rays was shifted with respect to the incident X-ray wavelength. In order to explain these findings, Compton postulated that light quanta carry not only energy, but also momentum, which is inversely proportional to the wavelength p=

h , λ

with the proportionality coefficient once again being Planck’s constant. A year later, Louis de Broglie (1924) proposed that this momentum–wavelength relation is more general and applies not only to photons, but to all particles as well. The particle waves are characterized by the wavelength λ=

h . p

The fundamental difference between waves and particles is that waves are capable of exhibiting the phenomenon of interference, where two coherent waves

1.3 Wavelength of a Free Particle in Terms of Its Energy

7

either magnify each other constructively or suppress each other destructively. In 1925, Clinton Davisson and Lester Germer observed the interference of electrons reflected by different crystalline planes of a nickel sample. The results of their experiment indicated that the wavelength of a particle is indeed given by de Broglie’s formula. Later, wave properties of atoms and other particles were also demonstrated experimentally. What photons, electrons, and atoms have in common is that these waves can propagate in vacuum; they do not require a medium to carry them. One may wonder about other waves that do require such a medium: do they behave like particles? It turns out that they do. For example, sound propagates in discrete chunks, or quanta, called phonons. The quantum nature of sound exhibits itself in the specific temperature dependence of the heat capacity of solids. There are all sorts of elementary excitations in solids that sometimes behave as particles and sometimes as waves, such as waves quanta of charge density (plasmons) or magnetization (magnons). The wave–particle duality is hard to understand intuitively, but it is supported by a plenty of experimental evidence.

1.3 Wavelength of a Free Particle in Terms of Its Energy It is often more convenient to express the de Broglie wavelength of a free particle in terms of its energy rather than its momentum. Such an expression is obtainable from the particle’s energy–momentum relation, E(p), which can be inverted to obtain the magnitude of momentum as a function of energy. Hence, λ=

h . p(E)

The kinetic energy of a massive particle is √ p2 h ⇒ p = 2mE ⇒ λ = √ E(p) = = 2m 2mE

 h2 . 2mE

In particular, the combination of Planck’s constant and electron mass, me , under the square root has the numerical value h2 2 = 150.412 . . . eV · Å , 2me so the wavelength (in Angstroms) of a free electron is related to its energy (measured in electron-volts) as

8

1 Principles of Quantum Mechanics

 λ=

150.4 eV Å. E

The wavelength of any other particle of mass m can be quickly found as  λ=

150.4 me . E m

As for the massless photons, the energy–momentum relation is E = hf = cp, where c is the speed of light in vacuum. A photon’s de Broglie wavelength is then just its wavelength: λ=

h hc hc c = = = . f p hf E

The product of Planck’s constant and the speed of light has the numerical value hc = 1.23985 . . . eV · µm, so, numerically, the relation between photon wavelength and energy is λ=

1.24 eV · µm . hf

1.4 Energy Quantization An important conclusion that can be drawn from the wave nature of particles is that a particle in a confined geometry cannot have an arbitrary energy. Rather, its energy must be quantized. This statement is demonstrated by two examples. Example 1 A particle between two walls. Consider a particle of mass m, which bounces between two parallel walls separated by the distance d. Every time the particle hits a wall, it gets reflected. If the particle is viewed as a wave, this must be a standing wave. Hence, the distance between the walls must equal an integer multiple of half-wavelength: d = nλ/2, where n is an integer, see Fig. 1.1. We can combine this with de Broglie’s formula to establish the allowed values of momentum p = nh/(2d) with n = 1, 2, 3, . . .. It then follows that the energy of the particle confined between two walls assumes quantized values of E=

h2 p2 = n2 . 2m 8md 2

9

Fig. 1.1 The wave patterns of a particle between two walls at the three lowest energies

Fig. 1.2 The wave patterns of a particle traveling on a circle at the three lowest energies

Example 2 A particle on a circle. Suppose now that a particle can move on a circular path of radius r. Then, the wave associated with the particle must have a wavelength such that the circular path length is its integer multiple; otherwise, the wave will interfere with itself destructively. This implies the quantization condition 2π r = nλ = nh/p, n = 1, 2, 3, . . ., see Fig. 1.2. We obtain the possible momentum values p = nh/(2π r) and the allowed energies E=

h2 p2 = n2 2 2 . 2m 8π r m

1.5 Radiation Spectrum of Hydrogen A hydrogen atom consists of a heavy proton and a single electron that orbits around it. Electron mass and charge are me = 9.109 . . . · 10−31 kg, qe = −e = −1.602 . . . · 10−19 C. The magnitude of the electron charge, |qe | = e, is called the elementary charge. Because a proton is 1836 times heavier than an electron, it can be considered as stationary. The total energy of the electron is the sum of its kinetic energy and the potential energy of its electrostatic interaction with the nucleus: E=

e2 p2 − ke , 2me r

10

1 Principles of Quantum Mechanics

where ke = 8.987 . . . · 109 Nm2 /C2 is Coulomb’s constant, related to the vacuum permittivity ε0 = 8.854 . . . · 10−12 F/m by ke = 1/(4π ε0 ). Electron momentum and the radius of its circular orbit are related by 2π r = nλ = n

nh nh¯ h ⇒ p= = , p 2π r r

as explained in the previous example. A further relation between these two parameters can be established by noting that the centripetal force that acts on the electron should be identified with the Coulomb force: p2 e2 = ke 2 . me r r The last two equations can be used to express p and r in terms of the quantum number n. For instance, dividing the second equation by the first one, we find p; after substituting this p into the first equation, we find r. The result is pn =

ke me e 2 n2 h¯ 2 , rn = . nh¯ ke me e 2

2

h¯ The value of rB ≡ r1 = k m 2 = 0.529 Å is called Bohr radius. Substitution e ee of these expressions into the electron energy formula gives the quantized energy values:

E=−

1 Ry , n2

where 1 Ry =

ke2 me e4 2h¯ 2

≈ 13.606 eV

is the so-called Rydberg’s constant. When the electron performs a transition from a higher-energy level characterized by a quantum number m to a lower level with the quantum number n < m, it emits a photon of frequency f =

1 Ry Em − En = h h



1 1 − 2 n2 m



 ≈ (3.290 · 1015 Hz) ·

1 1 − 2 n2 m

 .

The radiation spectrum of hydrogen indeed consists of spectral lines, whose frequencies are described by this relation to a very high accuracy. This relation was established experimentally by Johannes Rydberg in 1888 and was explained using the above reasoning by Niels Bohr in 1913.

1.6 The Wave Function

11

The last formula for the frequency of a photon suggests that also the electron wave in the nth quantum state is endowed with the frequency fn = En / h, ωn = 2πfn = En /h. ¯

1.6 The Wave Function The success of Bohr’s model of hydrogen energy levels indicates that an electron in an atom really behaves as a wave. However, the version of quantum mechanics based on de Broglie’s wavelength expression is of very limited use. It can be applied only to very simple problems and describe systems with just one particle. It is of little help when the potential depends on more than one coordinate, when it changes along the path of the wave, or when the system has many particles that interact with each other, as they do in real life. To treat a broader spectrum of problems, an approach based on the wave equation is used. At the heart of this approach is the wave function of the particle, ψ, which depends both on space coordinate and time. It describes a certain oscillatory process that propagates in space (i.e., a wave) and contains information about the particle’s state of motion. Let us return to the electron moving on a circle of radius r around a stationary proton. Let us measure the position x along the circular orbit, see Fig. 1.3. The wave function of an electron depends on x and t. It should be a periodic function of x with the periodicity λ = h/p, and it should repeat itself every time the electron makes one full rotation. Hence, ψ(x + λ, t) = ψ(x, t), ψ(x + 2π r, t) = ψ(x, t). It then follows that 2π r = nλ, as stated in the previous section. The possible natural candidates for the wave function are the trigonometric functions: Fig. 1.3 The (real or imaginary part of the) wave function of an electron moving on a circular orbit

12

1 Principles of Quantum Mechanics

ψ(x, t) ∝ sin(kx − ωt) or ψ(x, t) ∝ cos(kx − ωt), where k = 2π/λ is the wave number and ω = E/h¯ is the angular frequency of the electron wave of energy E. However, there are insurmountable interpretation difficulties associated with these choices. We still do not quite know how ψ(x, t) is to be interpreted, but what we do know is that the absence of the particle means that its wave function is zero. The trigonometric functions above do turn to zero when their argument is an integer or a half-integer multiple of π . This means that there are some points in space, where the electron cannot be found, see Fig. 1.3. But there is nothing special about any point on the circular path of the electron wave. They are all identical. For this reason, neither candidate can be accepted as a wave function of an electron moving on a circle. There is a simple remedy to this problem. It is based on the trigonometric identity sin2 (θ ) + cos2 (θ ) = 1. Namely, we can treat the wave function as a mathematical object with two components, ψ(x, t) = (ψ1 (x, t), ψ2 (x, t)), ψ1 (x, t) ∝ cos(kx − ωt), ψ2 (x, t) ∝ sin(kx − ωt), and relate the presence of an electron to the magnitude squared of the wave function: |ψ(x, t)|2 = ψ12 (x, t) + ψ22 (x, t) = const. It is possible, in principle, to further develop quantum mechanics using the language of a two-component wave function. However, it is more convenient to treat it as a complex number,3 whose real and imaginary parts are ψ1 and ψ2 : ψ = ψ1 + iψ2 , ψ1 = Reψ, ψ2 = Imψ, i 2 = −1. This type of description is standard. It is equivalent to the two-component one. The “length squared” of ψ in the language of complex numbers is called the modulus squared: |ψ|2 = ψ ∗ ψ = (ψ1 − iψ2 )(ψ1 + iψ2 ) = ψ12 + ψ22 . How should it be interpreted? An electron is a particle described in the wave terms. The wave is a delocalized entity; hence, an electron wave is delocalized. The electron wave function ψ(x, t) does not carry information about the exact location of an electron. But if we perform a measurement of the electron’s position x, we will obtain some result. This result will be a random number uniformly distributed 3A

crash course in complex numbers is given in Appendix A.1. Those readers who did not encounter complex numbers previously are asked to read this appendix before proceeding with the main text.

1.6 The Wave Function

13

along the circle of length L = 2π r. The probability that a measurement of the electron’s position will yield a result anywhere between the positions x1 and x2 with 0 < x1 < x2 < L is, then, P (x1 < x < x2 ) =

x2 − x1 . L

This probability must be related to the modulus squared of the wave function. We write P (x1 < x < x2 ) = (x2 − x1 )|ψ(x, t)|2 with |ψ(x, t)|2 =

1 . L

We interpret |ψ(x, t)|2 dx as the probability to find an electron between two infinitely close points x1 = x and x2 = x + dx: dP (x) = |ψ(x, t)|2 dx =

dx . L

This means that |ψ(x, t)|2 has the physical meaning of the probability density. Note that the wave function is normalized to 1: 

L



L

dP (x) =

0

dx |ψ(x, t)|2 = 1,

0

meaning that the probability to find an electron anywhere is unity. Coming to the three-dimensional space r instead of one-dimensional space x, the wave function is complex-valued. It is expressed as a sum of its real and imaginary parts: ψ(r , t) = Reψ(r , t) + i Imψ(r , t). The probability to find the particle in a small volume d 3 r = dxdydz around the point r at the moment of time t is d 3 r |ψ(r , t)|2 . Suppose a particle is placed in a box of volume V . Because the total probability of finding the particle anywhere in this box is equal to one, the wave function must satisfy the normalization condition:  dx dy dz |ψ(r , t)|2 = 1. V

Occasionally, one has to consider a particle moving on a two-dimensional surface, say, in the (x, y)-plane, or performing a one-dimensional motion, say, along the x-axis. Then, the wave function would depend, in the former case, on the coordinates x, y and time t, and in the latter case, on the coordinate x and time t. The normalization condition will then be formulated as either a two-dimensional

14

1 Principles of Quantum Mechanics

  integral, dx dy |ψ(x, y, t)|2 = 1, or a line integral, dx |ψ(x, t)|2 = 1, respectively.

1.7 The Wave Function of a Free Particle The wave function of a free particle has the form of a plane wave,   ψ(r , t) = Aei(k·r −ωt) = A cos(k · r − ωt) + i sin(k · r − ωt) , characterized by the wave vector k and angular frequency ω. The prefactor A is to be determined from the normalization condition. The square of the wave function is independent of the position, |ψ(r , t)|2 = A2 , meaning that the probability density to find the particle is the same for any point of space. Here, we encounter a challenge: the integral of the probability density over the whole space of infinite volume is infinite. The standard way out of this difficulty is to consider the particle inside a cube of side length L and finite volume L3 with the periodic boundary conditions expressed as ψ(r + nL, t) = ψ(r , t), where n is a vector, all three of whose components are integers. This means that whenever the wave reaches one side of the cube, it reappears on the opposite side with the same value of the wave function. With this choice of the boundary condition, integration |ψ(r , t)|2 is to be performed over a finite volume L3 , giving  L3

d 3 r |ψ(r , t)|2 = A2 L3 = 1,

and thus A=

1 . L3/2

The plane wave is therefore described by the wave function ψ(r , t) =

1 i(k·  e r −ωt) . 3/2 L

1.8 Schrödinger’s Equation

15

Periodic boundary conditions imply that the wave vector can have only discrete values, 2π n. k = L At the end of the calculations, the limit L → ∞ is taken. This makes the wave vector k and momentum p = h¯ k continuous because the difference between two successive p-values  goes to zero.

1.8 Schrödinger’s Equation 1.8.1 Time-Dependent Schrödinger’s Equation The de Broglie expression for the wavelength λ = h/p and the expression for the magnitude of the wave number, k = 2π/λ, imply that momentum is p =   Similarly, the energy is related to the angular frequency as E = hω. hk/(2π ) = h¯ k. ¯ Then, the wave function of a free particle can be expressed in terms of momentum and energy as ψ(r , t) =

1 i(p· 1 e  r −Et)/h¯ = 3/2 ei(px x+py y+pz z−Et)/h¯ . 3/2 L L

Note that energy can be recovered from this expression as the time derivative: Eψ(r , t) = i h¯

∂ψ . ∂t

Likewise, the momentum can be recovered by differentiation with respect to space: px ψ(r , t) = −i h¯

∂ψ ∂ψ ∂ψ , py ψ(r , t) = −i h¯ , pz ψ(r , t) = −i h¯ . ∂x ∂y ∂z

The three spatial derivatives can be united into a single vector operator, called the gradient,  = ex ∂ + ey ∂ + ez ∂ , ∇ ∂x ∂y ∂z in terms of which the momentum vector is obtained as  r , t). pψ(  r , t) = −i h¯ ∇ψ(

16

1 Principles of Quantum Mechanics

We see that energy and momentum can be identified with the operators ∂  Eˆ = i h¯ , pˆ = −i h¯ ∇, ∂t which we denote with a hat in order to distinguish from the energy and momentum values E and p.  When these operators act on the wave function of a free particle, its energy and momentum values are obtained: Eˆ ψ(r , t) = E ψ(r , t), pˆ ψ(r , t) = p ψ(r , t).  again, we obtain Acting on both sides of the second expression with pˆ = −i h¯ ∇ the square of the momentum:  2 ψ, pˆ 2 ψ = p 2 ψ = −h¯ 2 ∇ where 2 2 2 2 = ∂ + ∂ + ∂ ∇ ∂x 2 ∂y 2 ∂z2

is called the Laplacian operator. The relation between the kinetic energy and the momentum of a free particle is p 2 . This same relation can be written using the derivatives: E = 2m i h¯

h¯ 2  2 ∂ψ =− ∇ ψ. ∂t 2m

This is Schrödinger’s equation for a free particle. Even though we have obtained it assuming the plane-wave form of ψ(r , t), it is valid for any type of wave function in free space. If the particle finds itself in some potential V (r ), then the energy expression should include its potential energy in addition to the kinetic energy, Eψ =

p 2 ψ + V (r )ψ, 2m

and expressing energy and momentum components in terms of the partial derivatives, we finally obtain the time-dependent Schrödinger equation: i h¯

∂ψ(r , t) h¯ 2  2 =− ∇ ψ(r , t) + V (r )ψ(r , t). ∂t 2m

1.9 Probabilistic Interpretation and the Collapse of the Wave Function

17

1.8.2 Time-Independent Schrödinger’s Equation To find the possible values of energy that a particle can have, the solution of the time-dependent Scrhödinger equation is written in the form ψ(r , t) = Ψ (r )e−iEt/h¯ with time-independent Ψ (r ). Substitution of this decomposition into the timedependent Schrödinger equation gives the time-independent version of this equation for a single particle: EΨ (r ) = −

h¯ 2  2 ∇ Ψ (r ) + V (r )ψ(r ). 2m

The solution of this equation with the boundary conditions appropriate for a given problem at hand yields the possible energies Eα that the particle can have, and the corresponding stationary wave functions, Ψα (r ). Both depend on a set of quantum numbers α = (α1 , α2 , . . .), which label the specific quantum state of the particle. The quantum state with the lowest energy found in the energy spectrum Eα is called the ground state.

1.9 Probabilistic Interpretation and the Collapse of the Wave Function The states of a particle moving in the positive and negative x-directions are described by the plane waves: 1 1 ψ→ (x, t) = √ ei(px−Et)/h¯ , ψ← (x, t) = √ ei(−px−Et)/h¯ L L 2 with p = nh L > 0 and E = p /(2m). Both wave functions, ψ→ (x, t) and ψ← (x, t), satisfy the time-independent Schrödinger equation for a free particle. Any linear combination of these two wave functions satisfies the same Schrödinger equation and therefore describes a possible quantum state of the particle. For example, consider the sum

1 ψsw (x, t) = √ (ψ→ (x, t) + ψ← (x, t)), 2

18

1 Principles of Quantum Mechanics

√ where the factor 1/ 2 comes from normalization of ψsw (x, t) to 1: 

L



L

dx |ψsw (x, t)|2 =

0

0

1 = 2

∗ dx ψsw (x, t) ψsw (x, t)



L

0

 dx |ψ→ | +

L

2

0

 dx |ψ← |

2

=

1 (1 + 1) = 1. 2

Here, we used the fact that 

L 0

∗ dx ψ← (x, t)ψ→ (x, t)

1 = L =

and similar with find

L 0



L

dx e 0

i2px/h¯

L

h¯ i2px/h¯

e =

i2pL x=0

L

h¯ h¯ ei2π nx/L

(ei2π n − 1) = 0 = i2pL i2pL x=0

∗ ψ dx ψ→ ← = 0. Using the expression

 ψsw (x, t) =

eiα +e−iα 2

= cos α, we

  px 2 e−iEt/h¯ , cos h¯ L

i.e., ψsw (x, t) describes a standing wave. Is the particle in the standing wave state moving to the right or to the left? To understand this, we apply the rule, according to which the momentum of a particle is to be found by differentiating its wave function with respect to the spatial coordinate. For the one-dimensional motion, this rule reads: pψ(x, ˆ t) = −i h¯

∂ψ(x, t) = pψ(x, t). ∂x

The problem with the standing wave is that the derivative    px 2 ∂ψsw (x, t) =− sin −i h¯ e−iEt/h¯ ∂x L h¯ is not given by a product of momentum p and the wave function ψsw (x, t). The reason is that the “momentum rule” applies to free particles only, whereas a standing wave appears if the particle is not free but is confined between two walls. It is moving to the right 50% of the time and to the left 50% of the time. In other words, if one measured the direction of its motion, one would get either the result “to the right” or “to the left” with the√probability of 50%. Note that the probability of 50% is the square of the factor 1/ 2 that multiplies both the right-propagating, ψ→ (x, t), and the left-propagating, ψ← (x, t), components of the standing wave ψsw (x, t) above.

1.9 Probabilistic Interpretation and the Collapse of the Wave Function

19

One can form an arbitrary combination of the right-propagating and the leftpropagating plane waves: ψ(x, t) = c→ ψ→ (x, t) + c← ψ← (x, t) with the coefficients c→ and c← such that |c→ |2 + |c← |2 = 1. For example, a more general expression for the standing wave ψsw (x, t) is eiθ→ eiθ← ψsw (x, t) = √ ψ→ (x, t) + √ ψ← (x, t) 2 2 with some real-valued phases θ→ and θ← . The probabilities of particular outcomes of a measurement of the particle’s direction of motion for this more general standing wave are P→ = |c→ |2 , P← = |c← |2 . Both are equal 1/2. Let us say, we measured the direction of propagation to be to the right. Is it possible for another measurement, performed immediately after the first one, to yield the result “to the left” with any probability? The answer is no. If two measurements performed immediately one after the other gave different momenta, p and −p, this would be at odds with the law of conservation of momentum. A particle cannot change its direction of motion, unless acted upon by a force. Same is true about the wave associated with the particle. In the wave function language, this means that a measurement induces a collapse of the original wave function ψsw (x, t) to either ψ→ (x, t) or ψ← (x, t) with the probabilities |c→ |2 and |c← |2 . The second measurement will yield the same momentum as the first one, provided that the two measurements are performed immediately one after the other. If the second measurement is performed after a finite time after the first one, then its result really depends on the external forces that may change the particle’s momentum. If such forces are present, e.g., because of the walls between which the particle is confined, the wave function of the particle will evolve from the plane wave back to the standing wave. As a further generalization of these statements, consider a wave function, which is a linear combination of many plane waves with momenta p1 , p2 , . . . : ψ(x, t) = where the momenta are

cn √ ei(pn x−En t)/h¯ , L n

20

1 Principles of Quantum Mechanics

pn = nh/L, n = 0, ±1, ±2, . . . , the coefficients cn are such that

|cn |2 = |c1 |2 + |c2 |2 + . . . = 1,

n

and the energies are En = pn2 /(2m). This time, the plane-wave contributions to ψ(x, t) differ not only in the direction, but also in the magnitude of their individual momenta pn . The parameters |c1 |2 , |c2 |2 , . . . are the probabilities that a measurement of the particle’s momentum will yield the results p1 , p2 , . . . , respectively. After a measurement that resulted in a particular momentum value pn , the particle’s wave function above collapses to the single-momentum wave function √1 ei(pn x−En t)/h¯ . L If there are no external forces acting on the particle, the particle will remain in that state indefinitely. All subsequent momentum measurements will yield the same result p = pn with probability 1. Otherwise, the wave function will evolve from the plane-wave state with the momentum pn to a more complicated sum of plane waves with different momenta. Now, suppose that we perform a momentum measurement many times, and after each measurement, we wait long enough for the wave function to evolve to the original state given by the sum over the plane waves above. Every time we measure the momentum, we will get a different number. But the average momentum resulting from a large number of such measurements is a well-defined value:

p =

|cn |2 pn ,

n

as |cn |2 is the probability to get the momentum value pn in a single measurement. The same average momentum can be obtained with the help of the momentum operator pˆ = −i h∂/∂x, see Sect. 1.8.1. Namely, ¯ 

p = −i h¯

L 0

dx ψ ∗ (x, t)

∂ψ(x, t) . ∂x

Indeed, multiplying ψ ∗ (x, t) =

c∗ ∂ψ(x, t) cn ipn i(pn x−En t)/h¯ = e √n e−i(pn x−En t)/h¯ and √ ∂x L L h¯ n n

together, we obtain ψ ∗ (x, t)

∂ψ(x, t) cn∗ cn ipn i2π(n −n)x/L −i(E  −En )t/h¯ n = e . e ∂x L h¯  n,n

1.10 Measurable and Unmeasurable in Quantum Mechanics

21

After integration over x from 0 to L, only the terms with n = n survive in the sum. Multiplication of the result with −i h¯ gives p. The above expression for the average momentum can be generalized to the threedimensional space, in which the average momentum is 

p  = −i h¯

 r , t). d 3 r ψ ∗ (r , t) ∇ψ(

1.10 Measurable and Unmeasurable in Quantum Mechanics The complex-valued wave function can be expressed in an equivalent way, viz., in terms of its modulus |ψ(r , t)| and phase θ (r , t)|: ψ(r , t) = |ψ(r , t)|eiθ(r ,t) ,

Imψ . |ψ| = (Reψ)2 + (Imψ)2 = ψψ ∗ , θ = tan−1 Reψ The arguments r, t are not written explicitly in the second line for the sake of brevity. With Euler’s formula, eiθ = cos(θ ) + i sin(θ ), the real and imaginary parts of the wave function are Reψ = |ψ| cos(θ ), Imψ = |ψ| sin(θ ). Out of the two parameters, |ψ| and θ , it is the former, |ψ(r , t)|, that has a tangible physical meaning of the square root of the probability density to find a particle. Because |eiθ(r ,t) |2 = 1 for any real-valued phase θ (r , t), the probability density does not depend on the phase. Only variations of the phase θ (r , t) in time and space lead to observable physical effects, but the phase itself cannot be measured in any experiment. Hence, the wave function ψ(r , t) is also not measurable, only its magnitude is. In other words, if two wave functions have different phases but the same magnitude, ψ1 = |ψ| eiθ1 , ψ2 = |ψ| eiθ2 , θ1 (r , t) = θ2 (r , t), then they are mathematically distinct, but physically equivalent. There is absolutely no way to determine experimentally which wave function is the correct one. This statement immediately encounters two objections. First, it is too selfcontradictory to be acceptable. An even more serious second objection is that this statement is not consistent with the time-dependent Schrödinger equation. Namely, if two wave functions ψ1 (r , t) = ψ(r , t) and ψ2 (r , t) == ψ(r , t) eiθ(r ,t)

22

1 Principles of Quantum Mechanics

are physically equivalent, then they should satisfy the same Schrödinger equation. In particular, we should have i h¯

h¯ 2  2 ∂ψ2 (r , t) =− ∇ ψ2 (r , t) + U (r ) ψ2 (r , t). ∂t 2m

But a simple substitution of ψ2 (r , t) = ψ(r , t) eiθ(r ,t) results in an equation for ψ(r , t) that would look similar to the already familiar Schrödinger equation if not for a few extra terms with the time and spatial derivatives of θ (r , t). To address both objections, we note that the statement is not more selfcontradictory than the assertion that the energy is defined up to an additive constant: it is the energy variations that are measurable in physical processes. Consider the electric field E as an example. It is derived from the electric potential φ(r ) as its spatial derivative:  r ) = −∇φ(  r ). E( The energy of a charge q in an electric field is qφ(r ). Adding an arbitrary constant φ0 to φ(r ) changes the energy by qφ0 , but it does not change the electric field  r ). Because it is the force q E that determines the  φ(  r ) = E(  r ) + φ0 ) = −∇φ( −∇( motion of the charge, the charge dynamics is independent of the constant φ0 . More generally, the dynamics of a charge q is determined by the electric and the  r , t), which are derivable from the scalar potential magnetic fields, E(r , t) and B(  r , t) as φ(r , t) and the vector potential A(   r , t) = ∇  r , t).  r , t) − ∂ A(r , t) , B(  × A( E = −∇φ( ∂t A simultaneous change of the scalar and vector potentials to φ(r , t) → φ(r , t) −

∂g(r , t)   r , t) + ∇g(  r , t) ; A(r , t) → A( ∂t

does not change the electric and magnetic fields, no matter how the scalar function g(r , t) is chosen. This property of the electromagnetic field is called the gauge invariance. The transformation of the scalar and vector potentials above is called the gauge transformation. Now, when we say that the particle finds itself in a potential U (r ), what we really mean is that the particle is charged and the potential is generated by an electric field: U (r ) = qφ(r ). To be fully consistent with electrodynamics, Schrödinger’s equation must involve not only the electric, but also the vector potential. It turns out that a multiplication of the wave function by a phase factor eiθ(r ,t) and a gauge transformation of the

1.11 Electron States in a Hydrogen Atom

23

 r , t) with a suitably chosen gauge function g(r , t) indeed potentials φ(r , t) and A( leave Schrödinger’s equation unchanged. We will not go into the details of this derivation. Likewise, we will not include the vector potential into consideration. But the two statements made in this section, namely, that the phase of the wave function is unmeasurable and that two wave functions that differ by phase only are physically the same, should be borne in mind.

1.11 Electron States in a Hydrogen Atom An electron in a hydrogen atom finds itself in a potential V (r ) = −ke

e2 . r

It turns out that with this potential, the time-independent Schrödinger equation can be solved exactly. The resulting stationary wave functions turn out to depend on three quantum numbers, usually denoted as n, l, and m. The principal quantum number, n, determines the energy of the electron, which turns out to be exactly the same as what we obtained in Sect. 1.5: En = −1 Ry/n2 . The principal quantum number assumes positive integer values: n = 1, 2, 3, . . . . The orbital quantum number, l, determines the angular momentum of the electron orbiting around the nucleus. It is given by

L = h¯ l(l + 1). For a given principal quantum number n, the orbital quantum number can assume n different values: l = 0, 1, . . . , n − 1. This result differs from what we obtained within the simplistic treatment of Sect. 1.5. There, we obtained the angular momentum values pr = nh, ¯ which are incorrect. The magnetic quantum number, m (not to be confused with the electron mass, me ), determines the projection of the orbital angular momentum on some selected coordinate axis, say, the z-axis: Lz = h¯ mz .

24

1 Principles of Quantum Mechanics

For a given orbital quantum number, the magnetic quantum number assumes 2l + 1 different values: m = l, l + 1, . . . , l − 1, l.

1.12 Spin In addition to the quantum numbers that characterize its motion in space, an electron also possesses its own internal degree of freedom, which is not related to the electron’s orbital motion. Associated with it is the electron’s intrinsic angular momentum called spin. The spin of a particle is an intrinsic property that does not change in time. It was explained by Paul Dirac in 1928 by combining the rules of quantum mechanics with special relativity. Spin angular momentum is characterized by an additional quantum number, s, which can assume only two values: s = 12 and s = − 12 . The projection of the electron spin angular momentum on some selected axes is Sz = hs. ¯ Associated with spin angular momentum is the magnetic moment of an electron, m,  which is  It manifests itself as an additional important in the presence of a magnetic field, B.  energy −m  · B. Other particles may have other spin values, either integer or half-integer. For instance, photons have spin s = 1; some particles of the meson family have spin s = 0 and others have spin s = 1; particles of the baryon family may have either spin 1/2 (e.g., protons and neutrons) or 3/2; gravitons have spin 2; Higgs bosons have spin 0, etc.

1.13 Degeneracy One should not confuse the concepts of energy level and quantum state. An energy level is a possible energy value that the system of interest can have according to the time-independent Schrödinger equation. The quantum state is specified by a set of quantum numbers α that label the system’s wave function Ψα (r ). Different quantum states may have different energies, or they may belong to the same energy level. The situation when the same energy level accommodates more than one quantum state is called degeneracy. The degree of degeneracy of a particular energy level is the number of different quantum states that belong to this energy level. In other words, it is the number of different sets of quantum numbers α such that Eα is the same. Consider a hydrogen atom as an example. Quantum states of an electron in a hydrogen atom are labeled by the hydrogen quantum numbers α = (n, l, m, s).

1.14 Indistinguishability of Quantum Particles

25

The energy does not depend on l, m, and s. The degree of degeneracy of the energy level characterized by the principle quantum number n will be denoted as gn . It is found as the number of possible combinations of l = 0, . . . , n − 1, m = −l, . . . , l, and s = 1/2, −1/2 that correspond to the same n-value: gn = 2

l n−1

1.

l=0 m=−l

The factor 2 comes from two possible spin values. The double sum runs over all possible values of l and m; every time either of this quantum number changes, we should increase the result by 1. Using the fact that l

1 = 2l + 1,

m=−l

we find, using the formula for arithmetic series, that n−1 gn = 2 (2l + 1) = 2n2 . l=0

The lowest energy level, n = 1, consists of 2 quantum states with l = 0, m = 0, and sz = ±1/2. This means that the ground state energy level of hydrogen is double degenerate. The next energy level, n = 2, has the degeneracy g2 = 8, i.e., 8 states have the energy E2 . These states are characterized by the following quantum numbers: l = 0, m = 0, and sz = ±1/2 (2 states), and l = 1, m = −1, 0, 1, and sz = ±1/2 (6 states).

1.14 Indistinguishability of Quantum Particles Consider the situation when we have more than one particle of the same kind, e.g., N electrons. In classical physics, each particle follows its own trajectory, and so it is possible, in principle, to follow the motion of any particle and to be certain that we are looking at the same particle on the trajectory. But in quantum physics, the concept of trajectory is meaningless because it is impossible to define the trajectory of a wave distributed over the whole of space. Impossibility to follow the motion of an individual particle implies the impossibility to label quantum particles, i.e., to distinguish them from one another. The state of N particles is described by an N-particle wave function, which depends on N coordinates and time, ψ(r1 , . . . , rN , t). It must be normalized to 1:  d 3 r1 . . . d 3 rN |ψ(r1 , . . . , rN , t)|2 = 1.

26

1 Principles of Quantum Mechanics

It evolves in time according to the time-dependent Schrödinger equation: i h¯

h¯ 2   2 ∂ψ(r1 , . . . , rN , t) 2 N =− ψ + V (r1 , . . . , rN )ψ, ∇1 ψ + . . . + ∇ ∂t 2m

 n2 = ∂ 2 + ∂ 2 + ∂ 2 , n = 1, . . . , N, and the N-particle potential energy where ∇ ∂xn ∂yn ∂zn V (r1 , . . . , rN ) includes an external potential and the potential energy of interaction between the particles. So far, the difference between the many-particle state and a single-particle state is just in the number of arguments and Laplacian operators. Mathematically, indistinguishability of quantum particles means that the wave function ψ(r1 , r2 , . . . , rN , t) and the one with an arbitrary permutation of the coordinates r1 , r2 , . . . , rN are physically equivalent. The wave function itself is unmeasurable, only its modulus is. Then, an interchange of any two coordinates gives a wave function that has the same modulus as the original one: 2

2

2

|ψ(. . . , ri , . . . , rj , . . . , t)|2 = |ψ(. . . , rj , . . . , ri , . . . , t)|2 for any pair of indices i and j . But this is only possible if the two wave functions differ by a multiplicative constant of unit modulus: ψ(. . . , rj , . . . , ri , . . . , t) = cψ(. . . , ri , . . . , rj , . . . , t), |c|2 = 1. From this, we can conclude that the constant is of the form c = eiθ , where θ is an arbitrary real number, implying infinitely many possible values of c. But actually, the spectrum of the possible c-values is much narrower. Indeed, performing an interchange of the coordinates ri and rj again, we recover the original wave function: ψ(. . . , ri , . . . , rj , . . . , t) = cψ(. . . , rj , . . . , ri , . . . , t) = c2 ψ(. . . , ri , . . . , rj , . . . , t). This means that the prefactor squared is one, c2 = 1, and therefore, the prefactor can only have two values: c = ±1.

1.15 Spin-Statistics Theorem There is an important result, called the spin-statistics theorem (Pauli, 1940):

1.16 Pauli’s Exclusion Principle

27

Particles with integer spin (i.e., s = 0, 1, 2, . . . ) follow a many-particle wave function that remains the same if any two coordinates are interchanged, e.g., for two particles ψ(r1 , r2 , t) = ψ(r2 , r1 , t). Such particles are called bosons. Particles with half-integer spin (i.e., s = 1/2, 3/2, 5/2, . . . ) follow a many-particle wave function that changes sign if any two coordinates are interchanged, e.g., for two particles ψ(r1 , r2 , t) = −ψ(r2 , r1 , t). Such particles are called fermions. The particles that are most relevant for the purposes of this book are electrons. Their spin is 1/2, and therefore, they are fermions.

1.16 Pauli’s Exclusion Principle Electrons are spin-1/2 fermions with an antisymmetric wave function. Now, suppose you have a system of two electrons, and assume that interaction between them is negligibly small. Both electrons find themselves in the same potential produced, say, by an atomic nucleus. The energy levels of the electrons can be found by solving the time-independent Schrödinger equation, and the solution will be characterized by some quantum numbers, which we denote collectively as α and β. That is, the energy of one electron is Eα , its stationary wave function is Ψα (r1 ), the energy of the other electron is Eβ , and its stationary wave function is Ψβ (r2 ). The net wave function of both electrons must be obtained as some combination of Ψα (r1 ) and Ψβ (r2 ). A simple product, Ψ (r1 , r2 ) = Ψα (r1 )Ψβ (r2 ), will respect the time-independent Schrödinger equation for two electrons. However, it is not an acceptable two-electron wave function because it does not change sign upon the interchange of r1 and r2 . An expression that does have this property is  1  Ψαβ (r1 , r2 ) = √ Ψα (r1 )Ψβ (r2 ) − Ψα (r2 )Ψβ (r1 ) = −Ψαβ (r2 , r1 ). 2 √ The prefactor 1/ 2 is necessary for the correct normalization to one. Now, if α and β are the same, we have 1 Ψαα (r1 , r2 ) = √ (Ψα (r1 )Ψα (r2 ) − Ψα (r2 )Ψα (r1 )) = 0. 2 The wave function of two fermions in the same quantum state is zero. This means that in a system of more than one fermion (e.g., electrons), only one fermion can occupy the same quantum state. In other words, a single-particle quantum state may be either occupied by only one fermion or empty.

28

1 Principles of Quantum Mechanics

1.17 Problems 1.17.1 Solved Problems Problem 1 A photon with wavelength 300 nm kicks an electron out of a metal. The energy needed to remove an electron from the metal is w = 3.5 eV. Determine de Broglie wavelength of this electron. Problem 2 An electron is moving in the xy-plane in the presence of a magnetic field B pointing in the z-direction. What are the possible values of the electron’s kinetic energy and magnetic moment? Problem 3 The wave function of an electron is given by ψ(x, t) = A sin(kx) e−b|x| eiωt with k = 1 Å−1 and b = 2 Å−1 . (a) Find the normalization constant A. Hint: Use Euler’s formula to evaluate the integral. (b) Determine the locations where the electron is most likely to be found. Problem 4 An electron is confined to the x-axis, where it is placed inside an infinite potential well of width L: V (x) =

 0 for 0 < x < L ∞ for x ≤ 0 and x > L.

By solving the time-independent Schrödingers equation −

h¯ 2 d 2 Ψ (x) = EΨ (x) for 0 < x < L 2me dx 2

with the boundary conditions Ψ (x = 0) = Ψ (x = L) = 0 and normalization L 2 0 dx |Ψ (x)| = 1, find all possible wave functions Ψ (x) and energies E that the electron can have. Problem 5 The wave function of a free electron moving in the x-direction is given by 1 ψ(x, t) = √ L

 √ 3 i(x/(0.2 nm)−ω1 t) 1 − i i(−x/(1 nm)−ω2 t) e − √ e 2 2 2

with the periodic boundary conditions ψ(x + L, t) = ψ(x, t).

1.17 Problems

29

(a) What are the angular frequencies ω1 and ω2 ? (b) What possible momentum values of this electron can be measured and what are the probabilities to measure those momentum values? (c) If many electrons are prepared in the state described by the wave function above, what is their average momentum? Problem 6 The quantum states of an isotropic two-dimensional simple harmonic oscillator of mass m and spring constant k depend on 2 quantum numbers, n1 and n2 , which can take on non-negative integer values 0, 1, 2, 3, . . . . The energy is En1 n2 = h¯ ω(n1 + n2 + 1) with the natural frequency ω =

√ k/m.

(a) Find the degeneracy gn of the nth energy level with energy hω(n + 1). ¯ (b) The quantum states of an isotropic three-dimensional simple harmonic oscillator of mass m and spring constant k depend on 3 quantum numbers, n1 , n2 , and n3 , which can take on non-negative integer values 0, 1, 2, 3, . . . . The energy is En1 n2 n3 = hω(n ¯ 1 + n2 + n3 + 3/2). + 3/2). Find the degeneracy gn of the nth energy level with energy hω(n ¯

1.17.2 Practice Problems Problem 1 A photon of wavelength λ = 85 nm is absorbed by a hydrogen atom thereby exciting it from the lowest energy ground state to the first excited state. The atom was initially at rest. The mass of hydrogen atom is 1.008 Da, where 1 Da (Dalton) = 1.6605 · 10−27 kg. (a) Use momentum conservation to find the final velocity of the hydrogen atom. (b) Use energy conservation to find the final velocity of the hydrogen atom. (c) Which answer, (a) or (b) above, is to be trusted? Why? Problem 2 The wave function of an electron is given by ψ(x, t) = A(ax − −1 x 2 )e−k|x| eiωt with k = 0.5 Å and a = 1 Å, and the value of the angular frequency ω is unimportant. ∞ (a) Let P+ = 0 dx|ψ(x, t)|2 be the probability to find the electron anywhere in 0 the positive-x region and P− = −∞ dx|ψ(x, t)|2 be the probability to find the electron anywhere in the negative-x region. Find the ratio P+ /P− . (b) Determine the normalization constant  ∞ A, including the units. Hint: You may want to use the integral formula 0 dxx n e−x = n!.

30

1 Principles of Quantum Mechanics

Fig. 1.4 Double slit experiment

Problem 3 Electrons of a given energy E are shot one by one onto a double slit, see Fig. 1.4. Assume the distance between the slits, d, and the distance from the slits to the screen, L, to be known. The screen is covered with a sensitive material that changes its brightness on the spots hit by electrons. Hence, after sufficiently many electrons are shot, a certain pattern is observed on the screen. Establish that pattern for L  d and L  x, where x is the distance on the screen from the symmetry axis. Consider two cases: (a) Assuming that electrons are classical particles, sketch the screen brightness I (x). (b) Assume electrons are plane waves, which interact with both slits simultaneously. Hence, each slit becomes a source of a partial wave, ψ1 and ψ2 , where the subscripts 1 and 2 label the slits. The electron wave function at the screen is ψ = ψ1 + ψ2 . Determine screen brightness I (x) ∼ |ψ(x, t)|2 up to a multiplicative constant.   Answer: I (x) ∼ 1 + cos k Ld x . Problem 4 An electron is confined to the xy-plane, where it is placed inside a square potential well of side length L: V (x, y) =

 0 for 0 < x < L and 0 < y < L ∞ otherwise.

The time-independent Schrödinger equation reads h¯ 2 − 2me



∂ 2 Ψ (x, y) ∂ 2 Ψ (x, y) + ∂x 2 ∂y 2

 = EΨ (x, y)

1.17 Problems

31

inside the square. The boundary conditions are Ψ (0, y) = Ψ (L, y) = Ψ (x, 0) = Ψ (x, L) = 0. Note that the wave function must be normalized according to 



L

L

dx 0

dy |Ψ (x, y)|2 = 1.

0

Find all possible wave functions Ψ (x) and energies E that the electron can have. Problem 5 The ground state wavefunction of a proton in a harmonic potential 2 2 V (x) = kx 2 /2 is given by Ψ (x) = Ae−x /(2σ ) . Assuming k = 1 N/m, use Schrödinger’s equation to find σ . Problem 6 Two non-interacting spin-1/2 particles find themselves in a simple harmonic potential V (x) = kx 2 /2. The energy of a single particle in the nth quantum state is En = hω(n + 1/2). Find the energies and degeneracies of the ¯ first 5 energy levels. Keep in mind that the two particles can have the same energy only if their spins are antiparallel. Answer: En = nhω ¯ and gn = n + 2n/2, for n = 1, 2, . . ., where · · ·  is the floor function, which equals the largest integer that does not exceed its argument. In particular, g1 = 1, g2 = 4; g3 = 5; g4 = 8; g5 = 9, etc.

1.17.3 Solutions Problem 1 The energy of the incident photon of wavelength 300 nm = 0.3 µm is hf =

1.24 = 4.13 eV. 0.3

Part of this energy, viz. w = 3.5 eV, goes into helping the electron get out of the metal. The rest of the photon energy is converted into the electron’s kinetic energy: EK = hf − w = 4.13 − 3.5 = 0.63 eV. The electron’s wavelength is λe =

150/0.63 = 15.4 Å.

Problem 2 In the presence of a magnetic field, an electron experiences a Lorentz force of magnitude

32

1 Principles of Quantum Mechanics

Fig. 1.5 Electron trajectory in a magnetic field

FL = evB. The direction of this force is perpendicular to both the velocity v and the magnetic  The Lorentz force is balanced by the centrifugal force, field B. FC =

me v 2 , r

acting in the opposite direction, so the electron moves in a circle, see Fig. 1.5. From the condition FL = FC , we find the first relation between the electron orbit radius r and its momentum p = mv: evB =

me v p me v 2 , eB = = . r r r

The second relation comes from the quantization condition that the circumference must accommodate an integer number of electron’s de Broglie wavelengths λ = h/p: h 2π r = nλ = n , n = 1, 2, 3, . . . . p It is convenient to use the reduced Planck constant h¯ = h/(2π ), in terms of which this condition reads rp = nh. ¯ From these equalities, we obtain p2 = nheB. ¯

1.17 Problems

33

Hence, the kinetic energy of the electron assumes discrete values En =

p2 eh¯ =n B = nμB B, 2me 2me

where the combination eh¯ 2me

μB =

is called Bohr’s magneton. A more precise quantum-mechanical treatment leads to the same result, but with n being an odd integer. The electron moving in a circle can be viewed as a current loop with current flowing in the clockwise direction. Such a loop possesses a magnetic dipole moment  Its μ pointing into the plane of the figure, i.e., in the direction opposite to B. magnitude is μ = I A, where I is the electric current due to the circular motion of our electron and A is the loop area, A = π r 2. We find the radius of the electron’s orbit from the equations obtained above. We get r2 =

nh¯ . eB

Hence, A=π

nh¯ . eB

The electric current I is the amount of charge that is transferred through an arbitrarily chosen cross section of the loop per unit time. The electron’s velocity is √ p nehB ¯ v= = , me me and its rotation period is T =

2π r . v

34

1 Principles of Quantum Mechanics

Every T time units, the charge transferred is −e. Hence, the magnitude of the current is √ e e2 B ev e nehB/m ¯ e I= , = = = √ T 2π r 2π me 2π nh/(eB) ¯ and the magnetic moment μ = IA =

he e2 B π nh¯ ¯ =n · = nμB 2π me eB 2me

is quantized in Bohr’s magnetons. Problem 3 (a) The normalization constant is found from the normalization condition 

−∞

dx |ψ(x, t)|2 = 1.

Probability density to find the electron at the position x |ψ(x, t)|2 = ψ ∗ (x, t)ψ(x, t) = A2 sin2 (kx)e−2b|x| . We can find A from the equation  A2

∞ −∞

dx sin2 (kx)e−2b|x| = 2A2



dx sin2 (kx)e−2bx ,

0

where we used the fact that the integrand is an even function of x, allowing us ∞ ∞ to replace −∞ with 2 0 . We evaluate the integral using Euler’s formulas: eikx = cos(kx) + i sin(kx), e−ikx = cos(kx) − i sin(kx), from which we obtain sin(kx) =

eikx − e−ikx . 2i

Plugging this result into the integral, we get 

2

2A

0

2  ikx  e − e−ikx A2 ∞  2ikx −2bx −2ikx e−2bx , dx e = − dx e −2 + e 2 0 (2i)2

1.17 Problems

35

where we used the fact that i 2 = −1. What  ∞ we now need to integrate are the exponential functions. Using the identity 0 dxe−px = p1 , where the real part of p is positive, we have  2

A

   1 A2 k 2 1 1 A2 1 b = − − = − 2 = 1. 2b 4(b + ik) 4(b − ik) 2 b b + k2 2b b2 + k 2

Finally, the normalization constant is 1 2b(b2 + k 2 ). k √ √ Numerically, A = 2 · 2 · (4 + 1) = 2 5 Å−1/2 . (b) The electron is most likely to be found at the position x that maximizes the probability density |ψ(x, t)|2 . We find these positions by differentiation: A=

d  2 2 A sin (kx)e−2b|x| = 0, dx as the expression for |ψ(x, t)|2 is given in part (a). Differentiation gives 2 sin(kx) cos(kx)k + sin2 (kx)(−2b)sign(x) = 0 ⇒ k cos(kx) = b sin(kx)sign(x), or simply sign(x) tan(kx) =

k . b

This equation determines the positions of maxima and minima of |ψ(x, t)|2 . The largest maxima, i.e., the positions where the particle is most likely to be found, are located at   k 1 . xmax = ± tan−1 k b

Problem 4 We look for the solution of Schrödinger’s equation in the form Ψ (x) = A sin(kx) + B cos(kx) with unknown coefficients A and B and the wave number k. Substitution of the second derivative

36

1 Principles of Quantum Mechanics

d 2 Ψ (x) = −k 2 (A sin(kx) + B cos(kx)) = −k 2 Ψ (x) dx 2 into Schrödinger’s equation gives −

h¯ 2 d 2 Ψ h¯ 2 k 2 = Ψ = EΨ, 2me dx 2 2me

allowing us to relate the wave number k to the energy E: h¯ 2 k 2 = E, k = 2me

√ 2me E . h¯

To find A and B, we use the boundary conditions and normalization. First, we note that Ψ (0) = A sin(0) + B cos(0) = 0 ⇒ B = 0, and hence, there is no cosine term in Ψ (x) = A sin(kx). The second boundary condition, Ψ (L) = A sin(kL) = 0, suggests that kL must be an integer multiple of π , kL = nπ, n = 1, 2, 3, . . . , because sin(nπ ) = 0. We do not include n = 0 because this would give Ψ (x) = 0 (no electron at all). We do not consider negative values of n because a wave function with negative n represents the same quantum state as the wave functions with positive n: the two such wave functions differ only by the sign. Now that we have established that k = nπ L , we find the energy in the quantum state n: En =

h¯ 2 k 2 h¯ 2 π 2 . = n2 2me 2me L

 LIt remains2 to determine the normalization constant A from the condition 0 dx |Ψ (x)| = 1, giving 

L

A2

dx sin2

0

 nπ x L

= 1.

The integral can be found using either the identity sin2 (θ ) = sin(θ ) = giving

eiθ −e−iθ 2i

, where θ =

nπ x L .

1−cos(2θ) 2

or the identity

The value of the integral turns out to be L/2,

1.17 Problems

37 2L

A

2

 =1 ⇒ A=

2 L

for all quantum numbers n. Problem 5 (a) The total wave function consists of two counterpropagating plane waves with the wave numbers k1 =

1 1 = 5 nm−1 , k2 = = −1 nm−1 0.2 −1

and the corresponding wave lengths found from λ1,2 =

2π k1,2 :

λ1 = 0.4 π nm = 4 π Å, λ2 = 2 π nm = 20 π Å. The energies corresponding to these wave lengths are found from λ1,2 =  150 eV·Å E1,2

2

. On the other hand, energy is related to the angular frequency by

E1,2 = hω ¯ 1,2 . Hence,  λ1,2 =

2

150 eV · Å hω ¯ 1,2

2

⇒ ω1,2

150 eV · Å = . hλ ¯ 21,2

Numerically, h¯ = 6.58 · 10−16 eV · s. Thus, 2

ω1,2 =

2.28 · 1017 Å · s−1 . λ21,2

After plugging in the values of λ1,2 (in Å), we get ω1 = 1.44 · 1015 s−1 , ω2 = 5.77 · 1013 s−1 . (b) The total wave function ψ(x, t) consists of two plane-wave functions, corresponding to wave numbers k1 and k2 : ψ(x, t) = c1 ψ1 (x, t) + c2 ψ2 (x, t) with ψ1,2 =

1 i(k1,2 x−ω1,2 t) e . L

The respective momentum values are found as p1,2 = hk ¯ 1,2 with h¯ = 1.055 · 10−34 J · s:

38

1 Principles of Quantum Mechanics

p1 = 5.275 · 10−25

kg · m kg · m , p2 = −1.055 · 10−25 . s s

The probabilities P1,2 to measure momenta p1,2 are related to the factors c1,2 that multiply the plane waves ψ1,2 as P1,2 = |c1,2 |2 . Numerically,  √ 2 2 1 1 − i2 3 3 1−i 1+i P1 = = = = 25%. = = 75%, P2 = √ · √ = 2 4 8 8 4 2 2 2 2 As expected, P1 + P2 = 1. (c) The average momentum is

p = P1 p1 +P2 p2 = (5.275·0.75−1.055·0.25)·10−25 = 3.69·10−25 kg·m/s.

Problem 6 (a) Keeping in mind the definition of degeneracy as the total number of combinations of quantum numbers that correspond to the same energy, we need to find the number of combinations of the non-negative integers n1 , n2 = 0, 1, 2, . . . such that their sum equals n: n1 + n2 = n. To each value of one of those numbers, say, n1 between 0 and n, there corresponds a single value of n2 = n − n1 . Hence, there are n + 1 combinations of n1 and n2 such that the sum of these numbers is n. The degeneracy of the nth energy level is n + 1: gn =

n

1 = n + 1.

n1 =0

(b) This time, we need to find the number of combinations of three non-negative integers n1 , n2 , n3 such that their sum has a fixed value n: n1 + n2 + n3 = n. Let one of these numbers, say, n1 , assume the values between 0 and n. The values of n1 larger than n are not allowed because the sum n1 + n2 + n3 will

1.17 Problems

39

also be larger than n. For each value of n1 , another number, say, n2 , may assume the values between 0 and n − n1 . Again, higher values of n2 are not allowed for the same reason. For each combination of n1 and n2 , the third quantum number has a fixed value n − n1 − n2 . The degeneracy is the number of combination of n1 between 0 and n and n2 between 0 and n − n1 . For each value of n1 , the number n2 assumes n − n1 + 1 possible values. The degeneracy is then gn =

n n−n 1 n1 =0 n2 =0

1=

n

(n−n1 +1) =

n1 =0

n

(n+1)−

n1 =0

n

n1 = (n+1)2 −

n1 =0

n

n1 =0

The last term is just the sum of an arithmetic series. It equals n n1 =0

n1 =

n(n + 1) . 2

Finally, gn = (n + 1)2 −

 n (n + 1)(n + 2) n(n + 1) = (n + 1) n + 1 − = . 2 2 2

n1 .

Chapter 2

Crystal Structure of Solids

2.1 Periodic Table of Elements We can now apply what we have learned about the energy levels of hydrogen, the concept of spin, and Pauli’s exclusion principle to understand the periodic table of elements (Mendeleev, 1869). We may consider the electrons in an atom as approximately non-interacting because they tend to avoid each other due to their Coulomb repulsion. Then, the one-electron states in an atom are affected by the positive point-like nucleus to a larger degree than by the remaining electrons. The conclusion is that if the atomic number Z is not too high, the electron quantum states in an atom will be similar to Hydrogen quantum states, i.e., they will be characterized by the principal quantum number n = 1, 2, . . ., orbital quantum number l = 0, 1, . . . , n, magnetic quantum number m = −l, . . . , l, and spin quantum number s = ±1/2, see Sect. 1.11. The single-electron states nlms (r ) are then to be filled from bottom up taking into account Pauli’s exclusion principle. When filling the table, one should keep in mind that the nth energy shell can accommodate 2n2 electrons, each occupying a state with its own values of l, m, and s. The common notation is to denote the orbitals with l = 0 by the letter s (not to be confused with spin); the orbitals with l = 1 are denoted with the letter p (not to be confused with momentum); the l = 2 orbitals are denoted with the letter d; the l = 3 orbitals with letter f. The electron orbitals for the first 10 elements are shown in Table 2.1. Consider silicon as an example, whose electron configuration is 1s2 2s2 2p6 3s2 2 3p . Its deepest shell with n = 1 can accommodate two electrons with l = m = 0 and opposite spins; hence, we have 1s2 . The second shell, n = 2, can accommodate 2 · 22 = 8 electrons. Those electrons can occupy an s-orbital with l = 0, which accommodates two electrons with opposite spins (hence 2s2 ) and three p-orbitals with l = 1 and m = 1, 0, 1, with two electrons on each, giving 2 · 3 = 6 electrons in the 2p-states (hence, 2p6 ). Thus, the n = 2 shell is completely filled. The electrons belonging to a partially filled shell are called the valence electrons. In Si, the valence © The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_2

41

42 Table 2.1 Electron orbitals for the first 10 elements of the periodic table

2 Crystal Structure of Solids H (Hydrogen), Z = 1 He (Helium), Z = 2 Li (Lithium), Z = 3 Be (Beryllium), Z = 4 B (Boron), Z = 5 C (Carbon), Z = 6 N (Nitrogen), Z = 7 O (Oxygen), Z = 8 F (Fluorine), Z = 9 Ne (Neon), Z = 10

1s1 1s2 1s2 1s2 1s2 1s2 1s2 1s2 1s2 1s2

(full shell) 2s1 2s2 2s2 2p1 2s2 2p2 2s2 2p3 2s2 2p4 2s2 2p5 2s2 2p6 (full shell)

electrons belong to the n = 3 shell. It contains 2 electrons with opposite spins in the s-state with l = m = 0, and two electrons in the p-state with l = 1. These two electron states can have any value of m = 1, 0, 1 and spin s = −1/2, 1/2, with at least one of these quantum numbers in the two states being different. If one considers atoms with a higher atomic number (Z > 18), i.e., with a higher number of electrons, then this simple scheme stops working because the approximation of non-interacting electrons does not apply anymore. Interaction between the electrons starts to play bigger role.

2.2 Chemical Bonding Chemical bonding can be understood based on the general premise that the system of electrons generally occupies the lowest energy state, called the ground state. When two or more atoms are brought together, the ground state of the electrons belonging to all these atoms will be modified, depending on the distance between the atomic nuclei. The ground state energy of the electrons may either increase or decrease if the atoms are close to each other. If the ground state energy increases, the atoms of interest will not form molecules, and if it decreases, they will bind together. Finding the ground state of a system consisting of several atoms is a difficult task, which can be tackled only numerically. But the general mechanisms that lead to qualitative understanding of atomic bonding can be described relatively easily. There are four basic binding mechanisms: Van der Waals Bonding Van der Waals bonding is the weakest one of all four, but van der Waals forces responsible for this type of bonding act between all neutral atoms and molecules. While atoms are electrically neutral, the center of mass of the negative electron charge randomly fluctuates in time around the center of mass of the positive nuclear charge. These quantum fluctuations generate a randomly fluctuating electric field around an atom, and this field slightly displaces the electron cloud in another atom, thereby polarizing the other atom. Of course, the second

2.3 Crystal Lattices

43

atom polarizes the first one as well. The mutual polarization is such that the two atoms tend to attract each other. The resulting interaction potential is known to decrease with the distance, d, between the two atoms as the sixth power, 1/d 6 . For the noble gases, whose energy shells are completely filled (He, Ne, Ar, Kr, Xe, Rn), van der Waals forces are the only forces that can bind those atoms together at low temperature and high pressure. Ionic Bonding Consider two atoms from the opposite ends of the period table. Atom A has all its inner energy shells filled, and the next partially filled shell contains only one electron (examples: A = Li, Na, or K). The other atom B lacks just one electron to have all its energy shells filled (examples: B = H, F, or Cl). In other words, the electron configuration of the atom A is the same as in some noble gas atom plus an extra electron; for the atom B, it is the same as some noble gas atom minus an electron from the outermost shell. When A and B are brought close to each other, it will be energetically favorable for the atom A to give its extra electron to the atom B, thus filling up all shells of both atoms. This turns A into a positive ion and B into a negative ion. The two ions attract each other electrostatically, so that they form a polar molecule AB. If there are macroscopically many atoms A and B, they will form an ionic crystal, such as the salts NaCl, KCl, NaF, LiBr, etc. Covalent Bonding Covalent bonding acts between both similar and dissimilar atoms. Each electron state characterized by the same quantum numbers n, l, and m can admit two electrons with opposite spins. In a covalent bond, the valence electrons are shared between atoms. The sharing of electrons allows each atom to attain the equivalent of a full outer shell. For example, a Si atom has 4 valence electrons in the n = 2 shell, which can accommodate 2n2 = 8 electrons. In crystalline silicon, each atom has 4 neighbors to share the valence electrons with, thus giving 4 + 4 = 8 electrons in the outer shell. A similar bonding mechanism acts in other important semiconductor materials. Metallic Bonding Metallic bonding is a mechanism by which not molecules, but crystals are formed. Each atom in a metal contributes its valence electrons to the atoms of the whole crystal, thereby binding them together. The valence electrons detach from their host atoms and become free to move within the crystal. These free electrons are responsible for the high electric conductivity of metals.

2.3 Crystal Lattices 2.3.1 Atomic Order in Solids If many atoms are brought together, then it can be energetically favorable for them to arrange themselves into a crystal, i.e., a pattern that periodically repeats itself

44

2 Crystal Structure of Solids

in space. If the size of the crystal lattice exceeds a few hundred micrometers, one speaks about a single crystal. A polycrystalline material consists of a large number of crystalline grains, whose linear size may vary from tens of nanometers to a few hundred micrometers. Note that the typical interatomic distance in a solid is several Angstroms, so that even a nanometer-sized grain contains thousands of atoms arranged periodically. Finally, an amorphous solid does not have any degree of crystalline order even on the length scales of a few nanometers.

2.3.2 Bravais Lattices A Bravais lattice is a periodic arrangement of structureless lattice points in space, such that every lattice point can be reached from any other lattice point by adding an integer number of the lattice translation vectors. The coordinate of a lattice point  and c, as can be expressed in terms of the three translation vectors, denoted as a , b, r = i a + j b + k c with integers i, j , and k. The translation vectors are not necessarily mutually orthogonal and do not necessarily have the same length. At a first glance, it might seem that the number of such possible lattices is huge. But from the point of view of the symmetry, this intuition is not quite correct. It turns out that there are only 14 three-dimensional Bravais lattices, named after a French crystallographer Auguste Bravais, who summarized them in 1850. Depending on the relation between the lengths of the translation vectors and the angles between them, 6 lattice families are possible, with the number of members in each family varying from one to four. The triclinic lattice is the least symmetric one, in which all translation vectors are of different lengths and all angles are arbitrary but not equal 90◦ (see Fig. 2.1a). The most symmetric is the cubic lattice, where all translation vectors are the same and all angles are 90◦ (see Fig. 2.1b). Lattice constants are the parameters that are needed to completely characterize the Bravais lattice. A triclinic lattice requires six lattice constants: three lengths a,

Fig. 2.1 Primitive cells of (a) a triclinic and (b) a cubic Bravais lattice

2.3 Crystal Lattices

45

b, and c, and three angles α, β, and γ . For a cubic lattice, only one lattice constant, the side length a, is needed. The difference between the members of the same family is that some of them may have additional lattice points not only in the corners, but also in the center, on the two opposite bases, or on all six bases. Then, the lattices are called body-centered, basecentered, and face-centered, respectively. If none of these possibilities are realized, the lattice is called simple. An exception is the hexagonal family, which can be of two types: simple and rhombohedral. All 14 Bravais lattices are described in standard textbooks on solid state physics and in numerous online resources; hence, we will not discuss this topic in much detail here.

2.3.3 Unit Cell, Primitive Cell, and Crystal Basis A unit cell is a geometric figure whose periodic repetition in space generates the whole lattice without empty spaces in between. Its choice is not unique: it may have many shapes and sizes. A unit cell of the smallest volume is called primitive. The shape of a primitive cell is also not unique, but its volume is fixed: it contains exactly one lattice point. Figure 2.2 illustrates these definitions on a two-dimensional oblique lattice, where the cells A and B are non-primitive, and the remaining cells C, D, and E are different choices of a primitive unit cell. Depending on the position of a lattice point, it may be shared by several unit cells. For example in the two-dimensional lattice from Fig. 2.2, the lattice points in the corners of cell A are shared by four unit cells; with three points inside the cell, this gives 4 × 1/4 + 3 = 4 lattice point per cell A. Cell B has four lattice points in the corners, each shared by four similar cells, and two lattice points on the opposite sides, each shared by two cells; altogether, this gives 4 × 1/4 + 2 × 1/2 = 2 lattice points per cell B.

Fig. 2.2 An oblique lattice with two possible choices of the non-primitive cells A and B and three primitive unit cells C, D, and E, the last of which is the Wigner–Seitz cell

46

2 Crystal Structure of Solids

In contrast, a primitive cell contains exactly one lattice point. Cells C, D, and E in Fig. 2.2 are primitive. A special type of a primitive cell is the so-called Wigner–Seitz cell, defined as a locus of all points in space that are closer to a given lattice point than to any other lattice point. A Wigner–Seitz cell is built by connecting a given lattice point to all its neighbor points with straight lines and then drawing planes perpendicular to each of those connecting lines. The Wigner–Seitz cell is enclosed inside the so-obtained planes around the selected lattice point. Cell E in Fig. 2.2 illustrates this procedure for a two-dimensional lattice. Not every periodic arrangement of points can have the smallest unit cell containing just one lattice point. Consider, e.g., the two-dimensional lattice from Fig. 2.3a. Here, the cell A contains one dot; however, this cell cannot cover the whole lattice by periodic repetition in the plane. The smallest unit cell that reproduces the whole lattice must contain two dots, such as cell B or C. In order to be able to describe this kind of lattices, we need to introduce an important concept of crystal basis. A lattice point itself is a structureless geometric entity; the basis is a structure associated with each lattice point. This structure may be, e.g., two points. For the lattice from Fig. 2.3a, this would be, e.g., one dot in the corner of cell C and the one inside this cell. Then, the lattice from Fig. 2.3a is a square lattice with the primitive cell C; its lattice points are endowed with a basis of two dots. In order to describe a real crystal, the basis of its Bravais lattice must contain information about the type, number, and mutual arrangement of atoms that occupy each lattice point. A crystal structure is completely determined by its Bravais lattice and by the basis. This is illustrated by a two-dimensional crystal structure in Fig. 2.3b, showing a square Bravais lattice and a basis consisting of two different atoms.

Fig. 2.3 (a) An example of a periodic arrangement of dots, in which the cell A with just one dot is not a primitive cell, because it is not a unit cell; cells B and C containing two dots are possible unit cells. (b) A hypothetical two-dimensional crystal structure, defined by its square Bravais lattice and the basis consisting of two atoms

2.3 Crystal Lattices

47

2.3.4 Volume Density and Atomic Packing Fraction Assume for simplicity’s sake that the basis is formed by just one atom. Then, the  and c, is v = a · (b × volume of its primitive cell, built on the primitive vectors a , b, c). The volume density of atoms is n=

1 1 = . v a · (b × c)

If, instead of a primitive cell, one works with a larger unit cell built on the translation  and c, then vectors a , b, n=

Ncell , a · (b × c)

where Ncell is the number of atoms per unit cell. The physical boundary of an atom is not well defined. Nevertheless, one can approximately view atoms in a crystal lattice as solid impenetrable spheres of such radii that neighboring spheres are just touching each other. For a lattice made of just one type of atoms, the atomic radius r is half the distance d between the neighboring atoms in it, or d = 2r. The lattice constant a and the atomic radius r are thus proportional to each other, a ∝ d = 2r, with the proportionality coefficient depending on the crystal structure. The concept of atomic radius is useful because it allows one to approximately predict the lattice constant of a material if the atomic radii of the components forming it are known. For example, the lattice constant of the diamond modification of carbon aC = 3.567 Å, from which the atomic radius of carbon can be found as rC = 0.772 Å with the interatomic distance dC = 1.544 Å. Silicon likewise forms diamond crystal lattice with the lattice constant aSi = 5.431 Å, which corresponds to the atomic radius rSi = 1.176 Å and interatomic distance dSi = 2.352 Å. From this, we can expect that in a diamond-like silicon carbide lattice SiC, the distance between the neighbor silicon and carbon atoms is dSiC = rC + rSi = 1.948 Å. The expected lattice constant of this structure is aSiC ≈ aSi × ddSiC = 12 (aSi + aC ) = Si 4.5 Å. This value is in reasonable agreement with the known measured value of aSiC = 4.36 Å, exceeding it by only 3%. Atomic packing fraction (AP F ) is the fraction of volume in a crystal occupied by the atoms, which are viewed as solid spheres that touch each other. Specific examples of its calculation will be given below.

48

2 Crystal Structure of Solids

2.4 Basic Cubic Structures Most semiconductor materials belong to the cubic crystal family, whose three members—the simple cubic (sc), body-centered cubic (bcc), and face-centered cubic (fcc)—and the related zincblende and diamond structures (see Fig. 2.4) are briefly reviewed here. The Simple Cubic (sc) The simple cubic (sc) lattice is the simplest member of the cubic family. The side length of its unit cell, a, is called the lattice constant. Because each atom of the primitive cell is shared by eight cells with a common corner, it contributes 1/8 of its volume to a given cell. Because there are 8 corners, there are 8 · 18 = 1 atoms per unit cell. The volume density of atoms is nsc =

1 . a3

Each atom in an sc lattice has 6 nearest neighbors. If each atom is viewed as a solid sphere that touches the neighbor spheres, its radius would be r = a/2 and its volume Vsphere = 43 π(a/2)3 . Since there is just one atom per primitive cell, the atomic packing fraction AP Fsc =

Vsphere π = = 0.52 = 52%. 3 6 a

The only material with this structure is polonium. Simple cubic structure is rarely found in nature because of its small atomic packing fraction, which is the lowest out of all structures of cubic family. To minimize the total energy of the crystal, atoms tend to come close together, thereby maximizing the AP F . The reason why polonium is an exception from this rule has to do with the specific configuration of its six valence electrons’ orbitals that favor bonding to six nearest neighbors. The Body-Centered Cubic (bcc) The body-centered cubic (bcc) lattice is obtained by placing an extra atom in the center of each cube of an sc lattice. The primitive cell of a bcc lattice can be built on the three vectors connecting a corner atom with

Fig. 2.4 (a) The basic cubic structures: simple cubic (sc), body-centered cubic (bcc), and facecentered cubic (fcc). (b) The zincblende/diamond structure (left) and a tetrahedron as its building block (right)

2.4 Basic Cubic Structures

49

three neighboring central atoms. The primitive cell does not have cubic symmetry and is therefore inconvenient to work with. Hence, the conventional unit cell of a bcc lattice is a cube with one atom in the center. One can think of it as an sc lattice with the basis consisting of two atoms: one in the cube corner and the other one in the center. Alternatively, one may view a bcc lattice as two sc lattices shifted with respect of each other along the main diagonal of the primitive cell by one-half of its length. Therefore, the volume density of a bcc lattice is nbcc =

2 a3

because there are 2 atoms per unit cell. Each atom in a bcc structure has 8 nearest neighbors. The atomic packing fraction AP Fbcc = 68% is notably higher than in the sc structure. Some metals form bcc lattices, such as chromium, molybdenum, tantalum, and tungsten. The Face-Centered Cubic (fcc) The face-centered cubic (fcc) lattice is formed by placing six atoms in the centers of the six faces of an sc lattice. The primitive cell of an fcc structure is built on the vectors connecting a corner atom with its three neighboring atoms on the faces. The primitive cell does not have cubic symmetry and is inconvenient to work with. The conventional cell of an fcc lattice is a cube with six atoms on its six faces. Each of the eight corner atoms is shared by 8 cells and therefore contributes 1/8 of its volume to a given unit cell. Each atom on the six faces contributes 1/2 of its volume to a given unit cell. The number of atoms per unit cell is therefore 1 1 8 · 8 + 2 · 6 = 4. The number of nearest neighbors of an atom in an fcc lattice is 12. The volume density of the atoms is then nfcc =

4 . a3

The atomic packing fraction AP Ffcc = 74%. This is the highest value of all cubic lattices. Another structure that has the same AP F is hexagonal closed-packed (hcp). Due to their high degree of packing, fcc and hcp structures are the ones favored by most metals. Specifically, materials with the fcc structure include aluminum, copper, nickel, gold, silver, and platinum.

50

2 Crystal Structure of Solids

Zincblende and Diamond Structures Zincblende and diamond structures can be described as two interpenetrating fcc lattices shifted with respect to each other along the main diagonal by 1/4 of the diagonal length. If the two lattices are made of the same type of atoms (e.g., C, Si, Ge, or α-Sn), the structure is a diamond. If the two fcc lattices are made of different atoms (e.g., GaAs, InSb, InAs, or ZnS), the structure is called zincblende, which is another name for zinc sulfide, ZnS. Note that the materials that prefer to form this structure are either non-metals (C, Si, As, S) or poor metals (Ga, In, Sb, Zn). The building block of this structure is formed by a tetragonal arrangement of atoms, see Fig. 2.4b. The conventional unit cell of a diamond or a zincblende structure is a cube. The number of atoms in this cell is 8, i.e., n = 8/a 3 . Each √ atom has 4 nearest neighbors. The distance between the neighboring atoms is a 3/4. The AP F = 34%. Not all semiconductors form diamond or zincblende structure. Examples are numerous: ZnSb, ZnAs, ZnO, BeO, CdSb, CdAs, etc. Some materials may assume more than one different crystal structure, called polymorphs. For example, ZnS, ZnSe, CdS, and CdSe may form zincblende or wurtzite lattices, whereas silicon carbide (SiC) has 250 different crystalline forms, zincblende being one of them.

2.5 Formation of Diamond Structure Quantum mechanics explains diamond structure as follows. Consider an element belonging to group IV of the periodic table, such as Si. All elements from group IV have 4 valence electrons, two in the s-state and two in the p-state. When many such atoms are brought together, a process called hybridization of orbitals occurs. In this process, one s-electron is promoted into a p-state, resulting in one s-orbital and three p-orbitals. Then, the s-orbital combines with the three p-orbitals to form four orbitals of the new type, the so-called sp3 hybrid orbitals. Each of the four sp3 -orbitals is elongated, with an angle of 109.5◦ formed between any two of them, see Fig. 2.5. Furthermore, each sp3 -orbital can be occupied by two electrons of opposite spins. Thus, when many group-IV atoms

Fig. 2.5 (a) Formation of an sp3 hybrid orbital. (b) A sketch of the electron density distribution in an sp3 hybrid orbital accommodating four electrons

2.6 Miller Indices

51

are brought together, they arrange themselves so that each atom has four nearest neighbors, thus forming tetragons, the building blocks of the diamond lattice. To understand the zincblende structure formed by atoms belonging to groups III and V (the III–V semiconductors), we note that an atom from group III (e.g., Ga) has 3 valence electrons, and an atom from group V (e.g., As) has 5 valence electrons. An As atom can give one of its electrons to a neighboring Ga atom, so that both atoms now have 4 valence electrons. Then, the sp3 -hybridization proceeds as described above. In a similar way, zincblende structure can be formed by some of the II-VI semiconductors, such as InSb, CdTe, etc. In these materials, a group-VI element gives two of its valence electrons to a group-II element, resulting in 4 valence electrons in the atoms of each type.

2.6 Miller Indices 2.6.1 Determination of Miller Indices Miller indices (William H. Miller, 1839) are a standard convenient method of indicating various crystallographic directions and planes in a given crystal lattice. To indicate a direction, a vector d in that direction has to be used. However, simply stating the components of d is not enough. One must also give a reference to a particular coordinate system and indicate how the crystal lattice is oriented relative to that system. In order to avoid the necessity of giving this additional information,  it is more convenient to express d in terms of the lattice translation vectors, a , b, and c. Depending on the convenience considerations, those vectors may or may not be primitive. The direction vector d may have any length. It is decomposed into the translation vectors d = i a + j b + k c, such that the three numbers i, j , and k are integers without a common denominator. The direction is then specified by placing these three integers into square brackets, [i j k]. If one of these numbers is negative, the corresponding Miller index is ¯ Figure 2.6a shows Miller indices for some denoted with an overbar, e.g., [1 1 1]. directions of a cubic lattice. Some crystallographic directions possess the same symmetry. To indicate the whole family of such symmetry-related directions, one representative member of this family is placed into triangular brackets. For instance, in a cubic lattice, one ¯ such family is 1 0 0, consisting of [1 0 0], [0 1 0], [0 0 1], [1¯ 0 0], [0 1¯ 0], and [0 0 1] directions.

52

2 Crystal Structure of Solids

Fig. 2.6 Several crystallographic (a) directions and (b) crystal planes with the Miller indices  and c are aligned with the coordinate axes indicated in the brackets. The translation vectors a , b, x, y, and z

To indicate a crystallographic plane, the following algorithm is used. First, the intercepts of the plane with the coordinate axes built on the translation vectors, a ,  and c, are expressed in terms of the lengths of these vectors as pa, qb, and sc. b, The numbers p, q, and s cannot be zero, i.e., the plane cannot go through the origin. Then, the numbers are inverted to give 1/p, 1/q, and 1/s. Each of these inverted numbers is multiplied by the smallest number, n, such that the triplet i = n/p, j = n/q, and k = n/s is formed by integers i, j , and k. Those integers are the Miller indices for the plane of interest. If one of the intercepts is infinite, then the corresponding Miller index is zero. Negative Miller indices are denoted with an overbar. Miller indices for planes are indicated in round brackets. Figure 2.6b shows Miller indices for several planes in a cubic lattice. A family of symmetry-related planes is indicated by placing Miller indices for one representative member of this family into curly brackets. For instance, for cubic lattices, the {1 0 0} family consists of (1 0 0), (0 1 0), (0 0 1), (1¯ 0 0), (0 1¯ 0), and ¯ planes. (0 0 1)

2.6.2 Miller Indices for Cubic Structures As stated earlier, it is convenient to treat bcc, fcc, and diamond/zincblende lattices as cubic, with several atoms per unit cell (2 in bcc, 4 in fcc, and 8 in diamond). A nice feature of cubic lattices is that a direction with Miller indices [i j k] is perpendicular to the plane with the same Miller indices (i j k). Let us find the distance between two successive (i j k) planes. We note that an (i j k) plane crosses the x-axis at the point x = na/ i, the y-axis at the point y = na/j , and the z-axis at the point z = na/k, see Fig. 2.7. Here, n is an integer. Then, the two vectors

2.7 Imperfections and Impurities in Solids

53

Fig. 2.7 An (i j k) plane of a cubic lattice

r1 =

na na na na ey − ex , r2 = ez − ex j i k i

belong to the (i j k) plane. On the other hand, a unit vector in the [i j k] direction is, by definition, i ex + j ey + kez e = . i 2 + j 2 + k2 Now, it is easy to verify that r1 · e = r2 · e = 0, and thus the unit vector in the [i j k] direction is perpendicular to the two non-parallel vectors in the (i j k) plane. This means that [i j k] direction is perpendicular to that plane, as stated. To find the distance between two (i j k) planes, we note that the closest such plane intersects the coordinate axes at the following points: the x-axis at the point x = (n + 1)a/ i, the y-axis at the point y = (n + 1)a/j , and the z-axis at the point z = (n + 1)a/k. Then, a vector n 1 n+1 aex − ex = aex d = i i i begins on the nth plane and ends on the (n + 1)st plane. The distance between the two planes is the projection of this vector onto a unit vector perpendicular to the (i j k) planes: d = d · e =

a i 2 + j 2 + k2

.

2.7 Imperfections and Impurities in Solids From the electrical properties’ point of view, single crystals are preferred over polycrystalline materials because the grain boundaries in the latter tend to deteriorate the electrical characteristics. However, even in a single crystal, deviations from perfect long-range order are possible for various reasons.

54

2 Crystal Structure of Solids

Fig. 2.8 (a) Point and (b) line defects in a crystal lattice

One obvious reason for such deviations is the unavoidable random thermal vibrations of atoms. However, the average positions around which the atoms vibrate do form a crystal structure. Other causes of deviations from perfect crystallinity are the formation of defects of various types. Point defects, see Fig. 2.8a, result in a local distortion of the crystal lattice. They may form as vacancies, i.e., missing atoms on same lattice sites, or as interstitial defects, where an atom occupies the space of the crystal structure at which no atom should be present. Other types of point defects are possible, e.g., Frenkel defects formed by closely located vacancy and interstitial defects. Impurity atoms are considered point defects as well. Line defects may extend over macroscopic distances. They appear as dislocations, which are of two main types: edge and screw dislocations, see Fig. 2.8b. In the former, one of the atomic planes terminates in the middle of the crystal, resulting in a “bending” of the adjacent planes around that half-plane. A screw dislocation is a bit harder to visualize, but basically it is a twisting of the crystal lattice. Other types of defects are planar defects (grain boundaries, stacking faults, or twin boundaries) and bulk defects such as cracks, pores, voids, or impurity precipitates.

2.8 Problems 2.8.1 Solved Problems Problem 1 Consider a two-dimensional honeycomb lattice formed by regular hexagons, see Fig. 2.9a. Can the hexagon corners serve as lattice points of a Bravais lattice? If no, how can they be grouped into the basis? What are the translation vectors of the Bravais lattice? What does the Wigner–Seitz cell look like?

2.8 Problems

55

Problem 2 Find the atomic packing fraction of a diamond lattice. Problem 3 A certain plain of a cubic lattice intersects the coordinate axes at the points x = 2a, y = −3a, and z = a, where a = 7 Å is the lattice constant. Find the distance between two neighboring planes of this family. Problem 4 Find the number of atoms per unit area in the (1 1 1) plane of a sc, bcc, and fcc lattices with the lattice constant a = 4 Å.

2.8.2 Practice Problems Problem 1 Find the atomic packing fraction of fcc and bcc lattices. Problem 2 GaAs forms the zincblende lattice with the density of 5.318 g/cm3 . The atomic masses of the atoms forming this structure are mGa = 69.7 and mAs = 74.9 amu (1 amu = 1.6605·10−27 kg). Determine the lattice constant of this structure and find its concentration of valence electrons that form the Ga–As bonds. Problem 3 Find the surface density of atoms (SDA), i.e., the number of atoms per cm2 , in the (110) plane of a diamond lattice with the lattice constant a = 5.65 Å. Problem 4 Consider a body-centered cubic lattice with the lattice constant a = 6 Å. What are the Miller indices of the plane shown in Fig. 2.9b? What is the surface density of atoms in that plane?

Fig. 2.9 (a) A honeycomb lattice from Problem 1. (b) A crystallographic plane in a bcc lattice from Problem 4

56

2 Crystal Structure of Solids

2.8.3 Solutions Problem 1 If we align one translation vector a along the lower side of the hexagon and another vector b at an angle of 120◦ to a , then a linear combination i a + j b will cover not only the corners, but also the centers of each hexagon. The hexagon centers are not the lattice points of this structure. Hence, the corners of the hexagons cannot be used as lattice points of a Bravais lattice. But two corners can be grouped together to form the basis of the Bravais lattice, see Fig. 2.10. The resulting lattice points form a hexagonal lattice with the lattice vectors shown in the figure. The original hexagons are Wigner–Seitz cells of this lattice. Problem 2 The diamond structure can be thought of as two fcc lattices shifted relative to each √ other along the longest diagonal of the unit cell by one-quarter of its length d = a √3, see Fig. 2.11. The distance between the nearest neighbor atoms is, then, d4 = a 43 . If the atoms are viewed as solid spheres of radius r that just touch each other, then the distance between the centers of the neighboring spheres is 2r = d/4, allowing us to relate the radius to the lattice constant as √ 3 . r=a 8 Now, let us count the number of atoms in a diamond structure unit cell. Each of its 8 corner atoms is shared by 8 cells; hence, each corner atom contributes 1/8 of its volume to a given cell. Each of its 6 atoms on the 6 faces is shared by 2 unit cells; Fig. 2.10 Lattice points of a hexagonal Bravais lattice

Fig. 2.11 Diamond (or zincblende) unit cell

2.8 Problems

57

hence, the face atoms contribute 1/6 of their volume to a given cell. Finally, there are 4 atoms that are completely inside a given cell, see Fig. 2.9. Hence, the total number of atoms in a unit cell is     1 1 +6· + 4 = 1 + 3 + 4 = 8. N =8· 8 2 The volume occupied by a single atom is V0 = occupied by all 8 atoms in a cell is Vatoms = NV0 =

4 3 3πr .

Hence, the volume

√ √ 3∼ 8 · 4 3 ( 3)3 3 πa = a π = 0.34 a 3 . 3 16 83

Since the unit cell volume is a 3 , the atomic packing fraction is AP F =

Vatoms = 0.34 = 34%. a3

Problem 3 We begin by finding the Miller indices of this plane. For this, we invert the intersection point coordinates divided by a: a 1 a 1 a = , =− , =1 x 2 y 3 z and multiply these three numbers by the smallest positive integer (= 6) that will turn them into integers. The resulting triplet is the Miller indices: (i j k) = (3 2¯ 6). The distance between two neighbor planes with the same Miller indices is (for cubic family lattices) given by 7 a =√ = 1 Å. d= 2 2 2 9 + 4 + 36 i +j +k Problem 4 Consider the sc lattice first with the (1 1 1) plane shown in Fig. 2.12. In this plane, the atoms √ form a triangular lattice consisting of equilateral triangles of side length d = a 2. Since each atom is shared by 6 triangles, there are 3/6 = 1/2 of an atom per triangle. It is less than 1 because a triangle is not a unit cell of this two-dimensional lattice. The unit cell is a rhombus (shaded area) of side length d and height h found using Pythagoras’ theorem: √  2 3 d 2 . h + =d ⇒ h=d 2 2 2

58

2 Crystal Structure of Solids

Fig. 2.12 Arrangement of atoms in the (111) plane of a sc lattice

Fig. 2.13 Arrangement of atoms in the (111) plane of a bcc lattice

The area of such a rhombus is √ √ 3 = a 2 3, A = dh = d 2 2

and, because there is just one atom per rhombus, the surface density of atoms is SDA =

1 1 1 −2 −2 = √ = √ Å = 3.61 · 10−2 Å = 3.61 · 1014 cm−2 . A a2 3 16 3

A unit cell of a bcc lattice contains an extra atom right in the center, see Fig. 2.13. However, and, perhaps, counterintuitively, this central atom does not happen to be in the (1 1 1) plane. The easiest way to see this is to imagine a (1 1 0) plane, which does contain that central atom. Since the (1 1 1) plane can be obtained by tilting the (1 1 0) around one of the cube’s edges, the (1 1 1) plane does not contain the central atom of the bcc unit cell. Therefore, the arrangement of atoms in this plane is exactly the same as in the sc lattice, with the same surface density of atoms 3.61 · 1014 cm−2 .

2.8 Problems

59

Fig. 2.14 Arrangement of atoms in the (111) plane of an fcc lattice

Finally, an fcc lattice has extra atoms located in the middle of each face. The arrangement of atoms in the (1 1 1) plane is the same as in the sc case, but with atoms in the middle of each side of the triangles, see Fig. 2.14. A unit cell (shaded 1 area in the figure) contains 1 + 4 · 2 + 1 = 4 atoms. This means that the SDA is 4 times as big as in the sc case: SDA = 4 · 3.61 · 1014 = 1.44 · 1015 cm−2 .

Chapter 3

Equilibrium Statistical Mechanics

3.1 Microstates and Macrostates Physical systems consist of a huge number of particles. The most complete information about the system is contained in the system’s microstate (microscopic state). In classical mechanics, the microstate is specified by a huge number of coordinates and velocities of all particles comprising the system. It evolves in time according to Newton’s second law. In quantum mechanics, the microstate is given by the collective wave function, which depends on all the system’s coordinates. It evolves in time according to the time-dependent Schrödinger equation. Information about the microstate is complete in the following sense: If the system is perfectly isolated from the rest of the Universe, then its microstate will evolve in time according to the system’s autonomous equations of motion. Then, the microstate at the initial moment of time determines the system’s microstate at any future time according to these equations. It is a hopeless task to solve the equations that govern the evolution of the system’s microstate. There are several reasons for this: 1. The initial microstate of the system is unknown. 2. The equations that govern the system’s microstate evolution are deterministic, but their solution is usually chaotic (random). This means that the tiniest deviation of the initial state will result in a completely different trajectory of the system. 3. The system is never completely isolated from the rest of the world. In particular, it is impossible to switch off gravity, or perfectly isolate the system from external electromagnetic waves. Those interactions cannot be completely accounted for. However, small, they affect the dynamics of the systems microstate, see the previous point. 4. Last but not least, the system may be simply too big to be treated theoretically. Solving 1030 or so equations of motion is practically impossible. Because of these reasons, the microstate changes in time in a random, unpredictable manner. © The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_3

61

62

3 Equilibrium Statistical Mechanics

Luckily, information about the system’s microstate is practically never required. What is of interest is a set of the coarse-grained macroscopic parameters that characterize the system as a whole, such as pressure, volume, energy, temperature, concentration of atoms, polarization, magnetization, etc. Because the system’s microstate changes randomly in time, we may introduce the probability pα to find the system in a microstate α, in which the system’s macroscopic parameter of interest, Y , has the value Yα . As the microstate changes, so does its property Y . These random changes are called fluctuations. A measurement of the parameter Y takes finite time tY . This time is of the same order of magnitude as the reaction time of the measuring device used. The time of measurement is many orders of magnitude longer than the characteristic time over which the system’s microstate changes. For instance, oscillation period of an atom in a solid is about 10−13 s, much shorter than the reaction time of any device. This means that during a measurement, the system visits an astronomically huge number of its microstates. The total amount of time it spends in a microstate α during the measurement can be estimated as tα = pα tY . When the system is in the microstate α, its property Y has the value Yα . The result of a measurement will be the time-averaged value of Y :

Y  =

1 Y α tα = Y α pα . tY α α

A macrostate of a system is specified by a relatively small number of the macroscopic parameters that describe some measurable property of the system. Those parameters can be either the control parameters that can be fixed by an experimentalist or they can be the average values of some fluctuating properties of the system. For example, if we consider a gas in a container, then the volume of the container V is part of the macrostate description. If the gas finds itself inside a cylinder with a movable piston, then the gas volume is not fixed; however, applying a constant pressure to the system fixes the average volume V , which must be used as a macrostate variable. Other examples of the macrostate variables are the number of particles, temperature, pressure, etc.

3.2 Thermal Equilibrium The microstate probabilities pα , in general, change with time. As an example, consider a container whose right half is initially filled with gas and the left half is empty. Very quickly the gas will distribute itself uniformly within the container. The initial state and the final state are characterized by different sets of microstate probabilities. Corresponding to this transient process from the initial to the final states, theaverage value of a physical parameter Y will also be time-dependent:

Y (t) = α Yα pα (t).

3.3 Postulate of Equal A Priori Probabilities

63

But if we wait long enough, the system will eventually enter a special macroscopic state, in which the probabilities pα do not change anymore. This state is called thermal equilibrium, or thermodynamic equilibrium. Suppose two systems, initially isolated from each other, are in equilibrium states. They do not need to have the same values of such parameters as temperature or pressure. Now, we bring the two systems in contact with each other, allowing them to exchange energy and particles. Then, energy will flow from the hotter system to colder one and atoms will migrate from the system with the higher pressure to the one with the lower pressure. Eventually, the two systems will come to equilibrium with each other, as their temperature and pressure will become equal. We may also consider a single system in some non-equilibrium initial state. As the system equilibrates, any non-uniformity of its temperature and pressure cause energy and particles to redistribute themselves inside the system until the system reaches equilibrium. In thermodynamic equilibrium, temperature and pressure are uniform. Also, in equilibrium, there is no transfer of energy and particles. One may think (erroneously) that in thermal equilibrium, energy and particles do not flow between different parts of the system. In fact, thermal equilibrium should not be imagined as something static. Rather, it is a dynamic state, in which different parts of the system do exchange particles and energy, but the fluxes of those quantities are perfectly balanced by the respective counterfluxes. As a result, no overall transport occurs and the average amount of energy and the average number of particles in each part of the system remains constant.

3.3 Postulate of Equal A Priori Probabilities Consider a system that is isolated to the best of our abilities. Its extensive properties—the volume V , the number of particles N, and the energy E—are held fixed and do not change in time. The microstate of the system, on the other hand, constantly changes. In each microstate α visited by the system, these extensive parameters have fixed values: Vα = V , Nα = N, Eα = E. The postulate of equal a priori1 probabilities is a drastic statement about the system’s dynamics in thermodynamic equilibrium. It states that in thermodynamic equilibrium all microstates which are consistent with the given fixed extensive parameter values are equally probable. Mathematically, this can be expressed as follows: If, for two microstates α and α  of an isolated system we have Vα = Vα  = V , Nα = Nα  = N, and Eα = Eα  = E, then pα = pα  . No rigorous proof of this statement exists. At the same time, all experimental evidence speaks in favor of this postulate. We accept simply because it successfully

1 The Latin expression “a priori” means “from the earlier.” It denotes those properties of an object that do not depend on the empirical evidence, but follow from common sense and logic.

64

3 Equilibrium Statistical Mechanics

explains all phenomena observed in the systems containing many particles. The success of statistical physics can be taken as an a posteriori2 proof that the postulate of equal a priori probabilities is correct.

3.4 Grand Canonical Distribution Consider a system, which can exchange energy and particles with a much bigger system called the heat bath. The energy E and the number of particles n in the system of interest is not fixed, because the system exchanges these parameters particles with the heat bath. The role of the heat bath is to maintain constant the average energy E and the average number of particles n in the system. If at some moment of time, the number of particles in the system is greater than n, then the particles are more likely to leave the system and enter the heat bath. If n < n, then the particles are more likely to enter the system from the heat bath; same applies to energy. To each number of particles, n, in the system, there corresponds a certain set of states α. The energy of the system with n particles in a state α is denoted as Enα . We assume that the properties of the system—namely, its quantum states and energies Enα —are known. The question that we attempt to answer here is: What is the probability pnα for the system to have n particles and be in the microscopic state α? At a first glance, we do not have enough information to answer this question. For instance, we do not know the nature of the heat bath and the mechanism of the system-bath coupling, which makes the energy and particle exchange between the two objects possible. But this question can be answered with the help of the postulate of equal a priori probabilities. Namely, if, for a fixed number of particles, n, two different microstates α and α  have the same energy, Enα = Enα  , then they are equally probable, pnα = pnα  , independent of the nature of the system. In other words, for a fixed number of particles n, the microstate probability pnα is simply the inverse of the total number of microstates with the energy Enα . This implies that the probability pnα can only depend on the number of particles n in the system and the energy Enα of the state α: pnα =

1 G(n, Enα ), Z

2 The Latin phrase “a posteriori” means “from the later” and refers to the statements that follow from experience or observation of the physical world.

3.4 Grand Canonical Distribution

65

where the function G(n, Enα ) is to be established, and the constant Z in the denominator is introduced in order to make sure that the total probability is normalized to one, pnα = 1, n

α

meaning that Z=

n

G(n, Enα ).

α

The constant Z is called the grand partition function. To find the function G(n, Enα ), we consider two identical systems that are coupled to the same heat bath. The two systems are sufficiently far away from each other to be statistically independent. The probability for one system to have n particles and to be in the state α is pnα . The probability for the other system to have n particles and to be in the state α  is pn α  . The combined probability for the first system to be in the state (n, α) and the other system to be in the state (n , α  ) is given by the product of the individual probabilities: pnα pn α  =

1 G(n, Enα )G(n , En α  ). Z2

On the other hand, this composite probability must depend on the total energy and the total number of particles in the two systems via the function G: pnα pn α  =

1 G(n + n , Enα + En α  ) ˜ Z

with the normalization constant Z˜ = G(n + n , Enα + En α  ). n

n

α

α

Equating the natural logarithms of the last two expressions for pnα pn α  , we conclude that the function G(n, Enα ) must be such that ˜ 2 ). ln G(n + n , Enα + En α  ) = ln G(n, Enα ) + ln G(n , En α  ) + ln(Z/Z But this is possible if and only if ln G(n, Enα ) depends linearly on both arguments, n and Enα . Hence, we introduce two parameters, A and B, to express the linear relation between the function G(n, Enα ) and its arguments: ln G(n, Enα ) = An + BEnα ⇒ G(n, Enα ) = eAn+BEnα .

66

3 Equilibrium Statistical Mechanics

Note that the condition Z˜ = Z 2 is then fulfilled automatically, because Z=

eAn+BEnα ,

Z˜ =

n

=

n

α

α

eAn+BEnα



eA(n+n )+B(Enα +En α )



eAn +BEn α = Z 2 .

n α 

Actually, it is customary to express the parameters A and B in terms of two other μ 1 parameters, denoted as T and μ: B = − kT and A = kT . Here, T is the temperature (measured in Kelvins), the parameter μ is called the chemical potential and, k = 1.3806 . . . · 10−23 J/K = 8.6173 . . . · 10−5 eV/K, is Boltzmann’s constant. We thus arrive at the standard expression for the grand canonical distribution for the system to have n particles and find itself in the state α: pnα

    μn − Enα 1 μn − Enα , Z= . = exp exp Z kT kT n α

The constants μ and T are determined from the requirements that the system has a given average number of particles and a given average energy:

n =

n

α

npnα , E =

n

Enα pnα .

α

As stated earlier, thermodynamic equilibrium state is the state of no microscopic currents, by means of which different parts of the system would exchange energy or particles. Consider now a spatially extended large system containing a very large number of particles. In this system, we focus on two small volumes ΔV , one around some point r and the other around a point r  . The average number of particles and the average energy in both small volumes must be the same, independent of the choice of their positions r and r  . But n and E are uniquely determined by the chemical potential μ and temperature T . Hence, we conclude that in thermodynamics equilibrium, the chemical potential μ and temperature T are constant everywhere inside a spatially extended system.

3.5 Fermi-Dirac Distribution

67

3.5 Fermi-Dirac Distribution In the previous discussion, we did not specify the nature of the system. Therefore, the main result obtained there—namely, the grand canonical distribution—is very general and applies to systems of any nature. In particular, consider electrons in a crystal. Assume that the interaction between electrons can be neglected. Hence, each electron may occupy a single-electron state α. Nothing can stop us from treating this quantum state as the system and to apply the grand canonical distribution to get its occupation probability. The energy of this system can be either the quantum state energy Eα if it is occupied by an electron, or 0 if it is empty: Enα = nEα , n = 0, 1. The number of electrons n in the state α can assume only two values, 0 and 1, according to Pauli’s exclusion principle. We can determine the average number of electrons in the state α by using the grand canonical distribution. If the state is empty, then n = 0, E0α = 0, and p0α = Z1 . If the state is filled with an electron, then n = 1, E1α = Eα , and p1α =

e(μ−Eα )/kT Z

. The average number of electrons in the state α state is, thus,

nα  = 0 · p0α + 1 · p1α = p1α =

1 (μ−Eα )/kT . e Z

The partition function is Z=

en(μ−Enα )/kT = 1 + e(μ−Eα )/kT .

n=0,1

Then

nα  =

e(μ−Eα )/kT 1 = . 1 + e(μ−Eα )/kT 1 + e(Eα −μ)/kT

This number, which is between 0 and 1, is the probability p1α that the state α is occupied. This formula is called the Fermi-Dirac distribution. The letter μ is a standard notation for the chemical potential adopted in thermodynamics. In solid-state physics, a different name and notation is used for the chemical potential. Namely, in solid-state physics, the chemical potential is called the Fermi energy and is denoted as EF : μ ≡ EF .

68

3 Equilibrium Statistical Mechanics

This is the convention that we also will be using. Hence, the probability of occupation of a particular quantum state α is given by the Fermi-Dirac distribution: f (Eα ) =

1 1 + e(Eα −EF )/kT

.

The probability for this state to be empty is given by a similar expression: 1 − f (Eα ) = 1 −

1 1 + e(Eα −EF )/kT

=

e(Eα −EF )/kT 1 = , 1 + e(Eα −EF )/kT 1 + e(EF −Eα )/kT

note the change of sign in the exponential function in the denominator. A plot of the Fermi-Dirac distribution vs. energy (with the state subscript α omitted) is shown in Fig. 3.1a. At E < EF , Fermi-Dirac distribution approaches the value 1; at E > EF , it goes to zero very quickly. The transition between these two extremes occurs near Fermi energy, at which the distribution assumes the value f (EF ) =

1 . 2

The width of the transition region depends on the temperature. At T = 0, the distribution f (E) is a sharp step going from the value 1 at E < EF to 0 at E > EF (dotted line). Increasing the temperature makes the transition of f (E) near E = EF from 1 to 0 more smooth.

Fig. 3.1 (a) Fermi-Dirac distribution at T = 0 (dashed line) and for three non-zero temperatures (solid curves). (b) Fermi-Dirac distribution at T = 0.1 EF (solid curve) and its Boltzmann approximation f (E) = e−(E−EF )/kT (dashed curve). The inset shows the same plot at E > EF with the logarithmic scale on the y-axis chosen for the ease of comparison of the curves

3.7 Fermi Energy at Low Temperatures

69

3.6 Boltzmann Approximation For energies exceeding EF by a few thermal energies kT , Fermi-Dirac distribution can be approximated by the so-called Boltzmann’s distribution, obtained by neglecting the 1 in the denominator: f (E) ≈ e−(E−EF )/kT . This approximation is valid for energies, at which e(E−EF )/kT is much bigger than 1. Typically, the term “much bigger” means “bigger by at least one order of magnitude,” i.e., e(E−EF )/kT > 10  1 ⇒ E − EF > kT ln(10) = 2.3 kT . The accuracy of Boltzmann approximation at large energies is seen in Fig. 3.1b showing Fermi-Dirac distribution and Boltzmann approximation at T /EF = 0.1. Boltzmann approximation is quite accurate in this case for E/EF > 1.2, see inset. The probability for a given state below Fermi energy to be empty (see Sect. 3.5) can be approximated in a similar way: 1 − f (E) =

1 ≈ e−(E−EF )/kT . 1 + e(E−EF )/kT

This approximation is valid provided that EF − E > kT ln(10) = 2.3 kT . At the room temperature T = 300 K, the thermal energy kT = 0.02585 eV, and we see that Boltzmann’s approximation applies if the Fermi energy differs from a particular energy E by at least 0.06 eV.

3.7 Fermi Energy at Low Temperatures Fermi energy depends on temperature. Its temperature dependence should be found from the condition that the sum of the occupation probabilities for all quantum states be the same as the total number of electrons N. This gives an equation for EF : α

f (Eα ) ≡

α

1 = N. 1 + e(Eα −EF )/kT

Fermi energy EF at any temperature can be determined from this equation, provided that the energies of the quantum states Eα are known. It is often convenient to take

70

3 Equilibrium Statistical Mechanics

the sum not over the quantum states, but over the energy levels En , each of which is degenerate and contains gn quantum states. In this formulation, Fermi energy is to be found from gn = N. (E 1 + e n −EF )/kT n At T > 0, the solution of this equation needs to be performed numerically or using analytical approximations. The resulting EF does not need to coincide with any energy level En of the system. At absolute zero temperature, all states with energy below Fermi level are occupied and all states above Fermi level are empty. Let us denote the energy of the highest occupied energy level at T = 0 as E1 and its degeneracy as g1 . If the number of particles N is known together with the energies and degeneracies of all energy levels of the system, then the highest occupied energy level is relatively easy to figure out. One just needs to fill all energy levels with particles, starting from the ground state and up, until all particles are exhausted. Let us also denote the energy and the degeneracy of the lowest energy level which is empty at T = 0 as E2 and g2 . In this section, we wish to find the Fermi energy at the thermal energy slightly higher than zero, but well below the energy difference between the lowest empty and the highest occupied levels, kT  E2 − E1 . We need to consider the cases of complete and partial occupancy of the highest occupied level at T = 0 separately: Case 1: n1 = g1 ; Case 2: n1 < g1 , where n1 is the number of electrons in the level E1 at T = 0 (Fig. 3.2).

Fig. 3.2 Occupancies of the levels E1 and E2 at (a) T = 0 and (b) T > 0. Filled circles represent occupied quantum states, empty circles are empty states. It is assumed that at T = 0, all states belonging to the level E1 and all levels below E1 are occupied, and all states belonging to the levels E2 and higher are empty

3.7 Fermi Energy at Low Temperatures

71

Case 1 At T  (E2 − E1 )/k, only the excitation of particles from the level E1 to the level E2 plays a role. In other words, the g1 particles that belonged to the level E1 at T = 0 get redistributed between the levels E1 and E2 at T > 0. In this case, the chemical potential at low temperatures is found from g1 g2 + = g1 , 1 + e(E1 −EF )/kT 1 + e(E2 −EF )/kT because there are n1 +n2 = g1 particles that belong to the levels E1 and E2 . Defining x = e(E1 −EF )/kT , ΔE = E2 − E1 , we have: g2 g1 + = g1 . 1+x 1 + xeΔE/kT Multiplying both sides by the product of the denominators and rearranging the terms, we obtain a quadratic equation x 2 g1 eΔE/kT + x(g1 − g2 ) − g2 = 0, whose solution reads g2 − g1 −ΔE/kT e + x= 2g1



(g2 − g1 )2 −2ΔE/kT g2 e + e−ΔE/kT . 2 g1 4g1

In view of the condition kT  ΔE, we can arrange the exponentials as e−2ΔE/kT  e−ΔE/kT  e−ΔE/(2kT ) . This allows us to neglect the first term in the square root relative to the second one, and then to neglect the first term in the right-hand side relative to the square root. Then, x ≡ e(E1 −EF )/kT =



g2 −(E2 −E1 )/(2kT ) e . g1

Solving this for the Fermi energy, we obtain: EF (T ) =

E1 + E2 kT g1 + ln . 2 2 g2

On heating, the Fermi energy shifts toward that energy level which has the lower degeneracy.

72

3 Equilibrium Statistical Mechanics

Fig. 3.3 (a) Same as in Fig. 3.2a, but this time with n1 < g1 . (b) Fermi-Dirac distribution at T > 0

Case 2 This time, we have n1 < g1 particles in the level E1 at T = 0. At T > 0, particles can get transferred from the level E1 to the higher level E2 but also from the lower level E0 < E1 to the level E1 , see Fig. 3.3a. That is, now we have g0 + n1 particles that get redistributed among three levels E0 , E1 , and E2 , where g0 is the degeneracy of the level E0 , which was completely filled at T = 0. Accordingly, Fermi level must be established from the equation g0 g1 g2 + + = g0 + n1 . 1 + e(E0 −EF )/kT 1 + e(E1 −EF )/kT 1 + e(E2 −EF )/kT A rigorous solution of this equation for EF is difficult, but still possible. But since we are interested in the temperatures T  E2 − E1 and E1 − E0 , we can simplify the calculations considerably with the following reasoning: The Fermi-Dirac occupation probability of a quantum state with the energy E, f (E) =

1 1 + e(E−μ)/T

,

makes a sharp transition from 1 to 0 at E = μ. At T = 0, the occupation probability of a quantum state belonging to the energy level 0 is f (E0 ) = 1; for the quantum states belonging to the level 2 it is f (E2 ) = 0; and for a quantum state belonging to the level E1 it is n1 /g1 , as n1 states out of g1 are occupied. Hence, at 0 < T  E1 − E0 and E2 − E1 , the occupation probabilities should not be very different from these values, see Fig. 3.3b. Therefore, we can approximate the equation that determines the chemical potential by setting the first term in the left-hand side to g0 and the third term to 0, giving g1 = n1 . 1 + e(E1 −μ)/T

3.8 Problems

73

Solving this for the chemical potential, we obtain: EF (T ) = E1 − T ln

g1 − n1 . n1

As the temperature increases, the Fermi-Dirac distribution broadens around the energy EF . The Fermi energy adjusts itself so as to maintain the occupation probability of any quantum state belonging to the level E1 equal to n1 /g1 , see Fig. 3.3b. If more than half of the states in the level E1 are filled, then (g1 −n1 )/n1 < 1 and the Fermi energy increases; for n1 < g1 /2, it decreases. If n1 = g1 /2, it stays equal to E1 same to the first order in T .

3.8 Problems 3.8.1 Solved Problems Problem 1 A certain disease is known to affect 1 in 10,000 people. The medical test for this disease is 99.9% accurate, i.e., the probability of a false results (no matter if positive or negative) is 0.1%. What is the probability that a person who got a positive result of that test actually has this disease? Problem 2 What is the smallest number of students in a class such that at least two students have birthdays on the same day with at least 50% probability? Assume that a year has 365 days, i.e., neglect leap years. Problem 3 Consider a gas of bosons at temperature T and chemical potential μ. What is the average number of bosons in some quantum state with energy E? Note that, like fermions, bosons are indistinguishable particles, but there is no restriction on the number of bosons in the same quantum state. Problem 4 The degeneracy of a particular energy level g = 6. The probability for a particular quantum state belonging to this level to be occupied by an electron is f = 0.1. What is the probability Pn for this level to have n electrons with n = 0, . . . , 6? What is the average number of electrons occupying this level? Problem 5 A particular energy level E has the degeneracy 6. What should be the energy difference ΔE = E − EF for this energy level to be empty with probability 1/3 at T = 300 K? Problem 6 A system consists of N = 15 non-interacting spin-1/2 particles with the single-particle energies Eij = ΔE · (i 2 + j 2 ), where ΔE = 1 eV and the quantum numbers i and j can assume the non-negative integer values 1, 2, 3, . . . . Determine the Fermi energy EF at zero temperature. Does the Fermi energy increase, decrease,

74

3 Equilibrium Statistical Mechanics

or stay the same as the system’s temperature is increased from zero? Answer these questions for N = 16 and N = 20 particles as well.

3.8.2 Practice Problems Problem 1 Three fair dices are rolled. Calculate the probabilities pn to obtain n dots on their faces, with n = 3, 4, . . . , 18. Problem 2 The energy of a harmonic oscillator with the natural frequency ω is quantized as En = hω(n + 1/2) with n = 0, 1, 2, . . .. At temperature T , what is the ¯ probability for the oscillator to be in the quantum state n? What is its average  energy n

E? You may need the formula for the sum of a geometric series, ∞ n=0 x = −1 (1 − x) , valid for |x| < 1. Problem 3 A particular energy level has the energy 0.04 eV above Fermi energy. It can accommodate at most 2 electrons of opposite spins. The temperature is 300 K with kT = 0.02585 eV. What is the probability for this level to be empty? What is the probability for it to be occupied by just one electron? By two electrons? Problem 4 The degeneracy of a particular energy level g = 100. Its energy is 0.1 eV above Fermi energy, EF , whose temperature dependence can be neglected. At what temperature will this energy level be occupied by at least one electron with 1% probability? Problem 5 A gas of N = 1000 electrons may occupy the energy levels En = hω(n+1/2) of a harmonic oscillator with the natural frequency such that hω ¯ ¯ = 1 eV and n = 0, 1, 2, . . .. Not more than two electrons can occupy the same energy level. Find the Fermi energy of this system at T = 0.

3.8.3 Solutions Problem 1 The wrong way of solving this problem is the obvious one: The probability to get a false positive result is 0.1%. The probability to be sick is then 100% − 0.1% = 99.9%. The right way is a bit more intricate. Let pS = 1/10 000 = 10−4 be the probability of having the disease and pF = 0.1% = 10−3 be the probability of getting a false test result. Suppose a large number N of people took the test, and NP people tested positive. This number consists of two groups: (1) the people who are actually sick and were tested correctly, and (2) the healthy people who got false positive results. The number of people in group 1 is given by the product of the

3.8 Problems

75

number of sick people, pS N, and the probability of test being correct, 1 − pF . Thus, N1 = (1 − pF ) pS N. The number of people in group 2 is the product of the total number of healthy people, N − NS = N(1 − pS ), and the probability that the testing went wrong, pF . Thus, N2 = (1 − pS ) pF N. The probability for a person with a positive test result to belong to group 1 (i.e., to be sick) is p=

N1 (1−pF ) pS 1 = = = (1−p N1 + N2 (1−pF ) pS + (1−pS ) pF 1 + (1−pSF))ppFS 1+

1 0.9999·10−3 0.999·10−4

,

which is 9.08%. The probability that a person with a positive test result is actually not sick is almost 91%. Problem 2 Let N be the number of students in the class. The probability P0 that all N students have birthdays on different days is P0 =

N −1  366 − N 365 − i 364 · ... · = . 365 365 365 i=1

We need to find the smallest N, at which 1 − P0 > 1/2, or P0 < 1/2, or N −1  i=1

1 365 − i < . 365 2

One can attack this problem numerically, e.g., by building an Excel table and calculating the value of the product in the left-hand side of this inequality for different values of N . A more elegant way to find the answer is to perform an analytical calculation. Taking the natural logarithm of both sides, N −1 i=1

ln

 N −1  365 − i i < − ln(2) ; < − ln(2). ln 1 − 365 365 i=1

The sum of the logarithms can be approximately found using the approximation ln(1 + x) ≈ x for |x|  1.

76

3 Equilibrium Statistical Mechanics

We assume that N  365, meaning that i/365  1 for i = 1, . . . , N − 1. We will have to check the validity of this assumption after obtaining the value of N . We have N −1 i=1

  N −1 N −1 i i 1 (N − 1)N 1 ≈− ln 1 − i=− =− , 365 365 365 365 2 i=1

i=1

where we recognized an arithmetic series to obtain the last equality. We now need to find the smallest N, for which 1 N(N − 1) > ln(2) ⇒ N(N − 1) > 2 · 365 · ln(2) ≈ 506. 365 2 We obtain N = 23. Problem 3 The probability to have n particles in a quantum state with the energy E is given by the grand canonical distribution: pn =

e−n(E−μ)/kT . Z

The value of the constant Z is such that the probabilities to have any number of particles add up to one: Z=

e−n(E−μ)/kT =

n=0

∞  n e−(E−μ)/kT = n=0

1 1 − e−(E−μ)/kT

,

where we used the sum of the geometric series formula, 1+x +x 2 +. . . = 1/(1−x) for |x| < 1, in the last equality. The average number of particles in this quantum state is

n =

npn =

n=0

∞

n=0 ne

−n

Z

, =

E−μ . kT

The numerator can be evaluating by noting that ∞ n=0

ne−n = −

∞ de−n n=0

d

=−

∞ d −n 1 d e− e =− =  2 . d d 1 − e− 1 − e− n=0

Dividing this result by Z = 1/(1 − e− ), we obtain:

3.8 Problems

77

n =

1 e− 1 = (E−μ)/kT . =  − 1−e e −1 e −1

This result for the average number of bosons in a particular quantum state is known as the Bose–Einstein distribution. It differs from the fermionic counterpart, the Fermi-Dirac distribution, in that the unity is subtracted from the exponential rather than added to it. When (E − μ)/kT is bigger than 1 by at least 2 or 3 times, the unity in the denominator can be neglected, and the Bose–Einstein distribution can be approximated with Boltzmann’s formula, n ≈ e−(E−μ)/kT . Problem 4 Each of the g = 6 states belonging to this energy level can be occupied with probability f = 0.1 and empty with probability 1 − f = 0.9. The probability for all states to be empty is P0 = (1 − f )g = 0.96 = 0.5314. The probability for the energy level to have exactly one electron is P1 = gf (1 − f )g−1 = 6 · 0.1 · 0.95 = 0.3543. Here, the factor f gives the probability for one state to be occupied, and the factor (1 − f )g−1 gives the probability for the remaining g − 1 states to be empty. Since there are g states that can be occupied, the product f (1 − f )g−1 is multiplied by g. The probability for the energy level to have exactly n electrons should be proportional to f n (1 − f )g−n . The first term in the product is the probability for some specific n states to be occupied and for the remaining g − n states to be empty. g The proportionality coefficient, denoted as Cn , is the number of ways to select n occupied states out of g available states: g

Pn = Cn f n (1 − f )g−n . The number of selections of n filled states out of g available states is called the binomial coefficient and is given by g

Cn =

g! . n!(g − n)!

Here is the explanation of this formula. Imagine two bins, one labeled “occupied” and the other labeled “unoccupied,” into which we put objects called “states.” These objects are labeled: 1, 2, 3, . . . , g. We put n states into the “occupied” bin, and the remaining g − n states into the “unoccupied” bin. We are interested in the number of such arrangements which are distinct. For example, an arrangement that puts states 1, 2, 3, . . . , n into the first bin is the same as the arrangement 2, 1, 3, . . . , n, as the two arrangements just differ by a permutation of the states 1 and 2 within the first “occupied” bin. Now, the total number of permutations of all states is g!.

78

3 Equilibrium Statistical Mechanics

Some of those permutations swap the states between bins, which results in a new arrangement, while some permutations just swap the states within the same bin, which does not result in a new arrangement. Hence, the total number of permutations needs to be divided by the number of permutations of n states in the “occupied” bin and by the number of permutations of g − n states in the “unoccupied” bin, i.e., by g n! and (g − n)!. The result is the expression for Cn above. In particular, C06 = C66 = 1, C16 = C56 = 6, C26 = C46 =

6! 6! = 15, C36 = = 20. 2!4! (3!)2

We obtain: P2 = 15 · 0.12 · 0.94 = 0.09842, P3 = 20 · 0.13 · 0.93 = 0.01458, P4 = 15 · 0.14 · 0.92 = 0.001215, P5 = 6 · 0.15 · 0.9 = 0.000054, P6 = 0.16 = 0.000001. The average number of electrons in this level is

n =

g

nPn = 0 · P0 + 1 · P1 + . . . + 6 · P6 ∼ = 0.6.

n=0

Problem 5 The probabilities for a particular quantum state to be occupied and to be empty are, respectively, f =

1 1 1 , 1−f =1− = . ΔE/kT ΔE/kT −ΔE/kT 1+e 1+e 1+e

The probability for all g = 6 quantum states belonging to this level to be empty is P0 = (1 − f )g =

1 . (1 + e−ΔE/kT )g

With P0 = 1/3, we can solve this equation to find ΔE: 1 1/g −1/g −1/g = P0 ⇒ 1 + e−ΔE/kT = P0 ⇒ e−ΔE/kT = P0 − 1. 1 + e−ΔE/kT

3.8 Problems

79

Taking the natural logarithm in both sides of the last equation, we finally obtain: −1/g

ΔE = −kT ln(P0

− 1).

At T = 300 K, the thermal energy is kT = 0.02585 eV. Plugging in all other numerical values, ΔE = −0.02585 ln((1/3)−1/6 − 1) = −0.02585 ln(31/6 − 1) = 0.0415 eV. Problem 6 Quantum states are labeled by three quantum numbers: i and j = 1, 2, . . . , and spin s = ±1/2. Each energy level characterized by a particular combination of the quantum numbers i and j can thus accommodate two particles of opposite spins. We form a table showing the energies and degeneracies of the lowest few energy levels: Level 1 2 3 4 5 6 7

(i, j ) (1, 1) (1, 2) and (2, 1) (2, 2) (1, 3) and (3, 1) (2, 3) and (3, 2) (1, 4) and (4, 1) (3, 3)

Degeneracy 2 4 2 4 4 4 2

Energy [eV] 2 5 8 10 13 17 18

The degeneracy of each level is obtained by multiplying by two the number of the (i, j ) combinations that result in the same energy, as there are two possible spin orientations. For N = 15, all particles end up in the first five levels at zero temperature: 2 + 4 + 2 + 4 + 3 = 15. The highest occupied energy level is filled with n5 = 3 particles and has the degeneracy g5 = 4. Because n5 < g5 , we have for the Fermi energy 5 EF = E5 − kT ln g5n−n = 13 eV + kT ln(3). It has the value of 13 eV at T = 0 5 and increases with temperature. For N = 16, all particles occupy the first five energy levels, as the sum of their degeneracies, 2 + 4 + 2 + 4 + 4 = 16, equals the number of particles. The highest occupied energy level is now completely filled: n5 = g5 = 4. The lowest empty energy level E6 has the degeneracy g6 = 4 and energy E6 = 17 eV. The Fermi g5 13+17 6 energy at low temperatures is given by EF = E5 +E + kT = 15 eV 2 2 ln g6 = 2 independent of temperature at low T . Finally, for N = 20, the particles occupy the first six energy levels (2 + 4 + 2 + 4 + 4 + 4 = 20) with the last one being completely filled: n = g6 = 4. The lowest empty energy level has g7 = 2 and E7 = 18 eV. The Fermi energy is EF = g6 E6 +E7 + kT 2 2 ln g7 = 17.5 eV + kT ln(2)/2, an increasing function of temperature with EF (T = 0) = 17.5 eV.

Chapter 4

Band Theory of Solids

4.1 Bloch’s Theorem In the absence of an external electric field, an electron in a solid interacts with the positively charged point-like nuclei located in the nodes of the crystal lattice, as well as with a huge number of other electrons. The positive nuclei and the negative electrons together produce an electrostatic potential, U (r ), which is periodic in space, having the periodicity of the crystal lattice. This means that a displacement by any translation vector d = i a + j b + k c of the lattice will not result in a change of the potential energy:  = U (r ). U (r + d) Of course, perfect periodicity of this potential is broken by the presence of defects, impurities, and the thermal vibrations of the crystal lattice. We assume that all these effects are weak, so that we can treat the potential U (r ) as periodic to sufficient accuracy. Now, we must solve the time-independent Schrödinger equation for one electron in a periodic potential: E(r ) = −

h¯ 2  2 ∇ (r ) + U (r ) (r ). 2m

We assume for simplicity that the crystal lattice has cubic symmetry. An infinite crystal is modeled as a large cube of side length L with the periodic boundary conditions imposed on the wave function: (r + eL) = (r ),

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_4

81

82

4 Band Theory of Solids

where e is a unit vector in the x-, y-, or z-direction. That is, we do the same trick as in Sect. 1.7, when we discussed the wave function of a free particle. In the special case of no potential, U (r ) = 0, the solution of the time-independent Schrödinger equation is a plane wave explained in Sect. 1.7: for U (r ) = 0 : (r ) =

1 i k·  e r, L3/2

where the wave vector k can have only discrete values, 2π (k1 ex + k2 ey + k3 ez ) k = L with all three components k1 , k2 , and k3 being integer numbers. When the periodic potential is present, the wave function should reflect its translational symmetry. But the wave function itself is not physically measurable, only its modulus squared is. Therefore, it should have the property:  = U (r ) = 0 : |(r + d)|  2 = |(r )|2 , for U (r + d) where d is a translation vector of the lattice. There is an important result about the wave function of an electron in a periodic potential, derived by Felix Bloch in 1928. Bloch’s theorem states that if the periodic potential U (r ) is present, then the solution of the time-independent Schrödinger equation takes the form of a modulated plane wave (r ) = nk (r ) =

1 i k·  e r unk (r ), L3/2

where the functions unk (r ) have the lattice periodicity,  unk (r ) = unk (r + d). In the absence of the periodic potential, they assume the value one: for U (r ) = 0 : unk (r ) = 1. The integer n is an additional quantum number that labels the wave functions (r ) = nk (r ). It is called the band index. The band index n and the wave vector k define Bloch states with the wave function nk (r ). The derivation of Bloch’s theorem is given in Appendix A.2. Here, we would like to point out that the Bloch wave function nk (r ) has the desired properties above.

4.2 Energy Bands

83

Namely, it becomes a plane wave in the absence of the periodic potential, and its modulus squared is periodic with the periodicity of the potential:  2 = |u  (r + d)|  2 = |u  (r )|2 = |  (r )|2 . for U (r ) = 0 : |nk (r + d)| nk nk nk

4.2 Energy Bands 4.2.1 Physical Origin of the Energy Bands Bands are formed by those Bloch states nk (r ) that are characterized by the same  To each wave vector k there value of the band index n, but different wave vectors k.  corresponds the energy En (k), which is a continuous function of k for a given value of the band index n. Following the wave–particle duality argument, we can identify the product h¯ k with the electron momentum p in the crystal; it is called the crystal momentum, or the quasimomentum.1 In this way, we find that a single energymomentum relation of a free electron gets replaced with many energy-momentum  that depend on the band index n and are more complicated than relations, En (h¯ k), p 2  = 2m . the simple quadratic formula for a free electron, Ef ree (p) e So far, the emergence of bands looks like a purely formal result that follows mathematically from Schrödinger’s equation with a periodic potential. Let us now try and understand the physical origin of the bands. The building block of a crystal is its primitive cell, see Sect. 2.3.3. A primitive cell is equipped with one or several atoms that form the basis of the crystal lattice. Now, imagine that we could somehow control the lattice constant a of the crystal without affecting the mutual arrangement of atoms inside each primitive cells. At large lattice constant, the primitive cells resemble isolated molecules, whereas at small a, they form the crystal, see Fig. 4.1a and b for a two-dimensional illustration. At large intercell separation a, the electron states in each cell are obtained by solving Schrödinger’s equation with the potential generated by those several nuclei that belong to a particular cell. Those electron states are discrete, i.e., they can be labeled with a quantum number, which we call n. Each such state can be filled with at most 2 electrons of opposite spins. The energy in the state n is denoted as En . If we now reduce the distance between the cells so that the electron wave functions of neighboring cells start to overlap, then the energies En will be affected by the neighboring atoms. Because electrons are indistinguishable, one cannot assign electrons to their host cells anymore. In other words, each electron starts to belong not to an individual cell, but to the whole crystal consisting of N cells. This implies that a single-cell state with a given set of quantum number n can

1 From

Latin quasi = apparent.

84

4 Band Theory of Solids

Fig. 4.1 (a) Periodic arrangement of primitive cells in space with the symmetry of the crystal lattice, but with the lattice so large that the intercell interaction is negligible. (b) An arrangement of the same primitive cells in a crystal. (c) Schematic illustration of the splitting of electron states into bands as the lattice constant is decreased

now be occupied by 2N electrons. But this is clearly impossible by Pauli exclusion principle, which allows only two electrons of opposite spins per state. In order to comply with Pauli’s exclusion principle and to accommodate all 2N electrons in a quantum state at the same time, each formerly single-cell state must broaden into N closely spaced substates with two electrons per substate, see Fig. 4.1c. Those substates form energy bands. Then, a new quantum number emerges, which allows one to distinguish between different substates within the same band. This quantum number is the wave vector k in the Bloch’s wave function  i.e., E = nk (r ). The energies now depends on two quantum numbers, n and k,  The number of possible k-states  in the same energy band must be equal to En (k). the number N of the primitive cells in the crystal.

4.2.2 The First Brillouin Zone Brillouin Zones In the beginning of Sect. 4.1 we said that each component of the wave vector k is given by an integer multiple of 2π/L, where L is the linear size of the crystal with periodic boundary conditions. Then, in the end of the last section, we stated that the  number of different k-values in each band equals the number of primitive cells in the crystal. The two statements apparently contradict each other. Indeed, the number of primitive cells, N, no matter how large, is still finite, whereas the number of integers is infinite. The contradiction is resolved by the fact that in each band, there is finite a collection of N different wave vectors k that result in physically distinct Bloch functions nk (r ). This collection of N physically distinct wave vectors is called the first Brillouin zone. All wave vectors outside of this collection yield the wave

4.2 Energy Bands

85

functions that are physically equivalent to those obtained from the wave vectors in the first Brillouin zone. They belong to other Brillouin zones: the second, the third, etc. Each Brillouin zone contains the same number N of wave vectors as the first one.

One-Dimensional Crystal To see how this works, consider a single electron in a one-dimensional model crystal obtained by a periodic arrangement of atoms along the x-axis. The electron finds itself in a periodic potential U (x + a) = U (x). The lattice constant of this crystal is a, the number of primitive cells (i.e., the number of periods of U (x)) is N , and the length is L = N a. The periodic boundary conditions mean that the wave function of an electron satisfies (x + L) = (x). According to Bloch’s theorem, it is given by the product 1 nk (x) = √ eikx unk (x), L √ where n is the band index, L serves the purpose of the plane-wave part

L L

ikx 2 normalization to one: 0 dx e√ = 0 dx L = 1, and the wave number is an L integer multiple of 2π/L, see Sect. 1.7: k=j

2π , j = 0, ±1, ±2, . . . . L

For most values of j , the plane-wave part of the Bloch function, viz., √1 eikx , L does not have the lattice periodicity. But notice what happens if k is increased by 2π a . Then, the plane-wave part becomes 1 i √ e L



k+ 2π a x

2π 1 = √ eikx ei a x . L

The function ei a x does have the periodicity of the lattice, because increasing x by 2π 2π a does not change its value: ei a (x+a) = ei a x in view of the fact that ei2π = 1, see Appendix A.1. Now, the function e

i 2π a x

1 i nk (x) = √ e L



k+ 2π a x

unk (x)

has the same modulus squared as nk (x); therefore, it is physically equivalent to nk (x), see Sect. 1.10. However, its plane-wave part has the wave number

86

4 Band Theory of Solids

k = k +

2π . a

This means that two Bloch states whose band index n is the same, but the wave numbers differ by 2π/a, are identical. This also implies that the energy En (k) is a periodic function of the wave number with the periodicity En (k + 2π/a) = En (k). Alternatively, we can express energy in terms of momentum p = h¯ k and state its periodicity as En (p + h/a) = En (p), as h = 2π h. ¯ The first Brillouin zone of a one-dimensional crystal consists of N wave numbers that have the smallest magnitude: 1st B.z. : k = j

2π N N π π with − < j < ; hence − < k < . Na 2 2 a a

In other words, the first Brillouin zone is a line of length 2π/a centered around k = 0. Here, we assumed N to be an odd number without loss of generality. The second Brillouin zone consists of the wave numbers in the range 2nd B.z : −2

π π π π π π < k < − and < k < 2 , or simply < |k| < 2 . a a a a a a

In general, the nth Brillouin zone is defined as nth B.z. : (n − 1)

π π < |k| < n . a a

To get an idea of the energy-momentum curves in the first Brillouin zone, we first take the effect of the lattice periodicity into account. For this, we take the energy-momentum curve of a free electron, E(p) = p2 /(2me ), see Fig. 4.2a, and periodically replicate it along the momentum axis with the periodicity 2π h/a ¯ corresponding to the wave number periodicity of 2π/a, see Fig. 4.2b. By combining different parts of parabolas, one can build periodic E(p) curves with the periodicity h2π/a. Those curves will have cusps at the odd or even integer multiples of h¯ π/a. ¯ Next, we take into account the periodic potential. Without going into detail of solving the corresponding Schrödinger’s equation, the main result of the periodic potential is rounding off of those cusps to produce smooth periodic energymomentum curves E(p) for all momenta in the so-called extended zone scheme, see Fig. 4.2c. Finally, keeping in mind that only the first Brillouin zone matters, we

4.2 Energy Bands

87

Fig. 4.2 (a) Energy-momentum relation of a free electron. (b) The graph from (a) is periodically repeated horizontally with the periodicity h2π/a. (c) The effect of the lattice potential U (x) is ¯ to round off the cusps of the energy-momentum curves belonging to different bands. (d) Energymomentum curves for the first 4 bands in the reduced zone scheme

restrict the momentum values to the range −hπ/a < p < h¯ π/a, corresponding to ¯ the reduced zone scheme, see Fig. 4.2d.

Band Gap The main result of the interaction between the electron and the periodic potential U (x) is rounding off of the cusps at the edges of the Brillouin zones and the development of the bandgaps. A band gap is the smallest energy interval that separates two bands. An electron in a crystal cannot have energy within the band gap, no matter what its momentum is.

88

4 Band Theory of Solids

This result is both extremely important from the point of view of semiconductor properties and quite counterintuitive. It is worthwhile to try and understand the origin of the bandgaps qualitatively. We start answering the band gap question by looking into the physical √ √ meaning of a Bloch state nk (x) = eikx unk (x)/ L. Its plane-wave part, eikx / L, is a wave that travels to the right if k is positive and to the left if k is negative. But a plane wave cannot exist alone in a periodic structure. Let us say, a primary plane wave propagates to the right. It gets reflected by the lattice potential to produce a secondary wave propagating to the left. The amplitude of the secondary wave depends on the potential U (x) and is, generally speaking, smaller than the amplitude of the primary wave. The secondary wave also gets reflected by the lattice potential to produce a tertiary wave that travels to the right, which also gets reflected to produce a wave traveling to the left, and so on. A Bloch state results from a superposition of all those forward- and back-propagating plane waves. The modulation function unk (x) describes this superposition. Now, consider what happens when k = π/a, i.e., the plane wave has the wavelength λ = 2π/k = 2a. Each period of the lattice now accommodates half of the wavelength a = λ/2 for the original wave and also for the forward- and backpropagating reflected waves. Those wave combine so as to form standing waves. The nodes of these standing waves, i.e., the points where |n,π/a (x)|2 = 0, correspond to zero probability to find an electron. The antinodes are located at the points where the electron is most likely to be found. By symmetry, either the nodes or the antinodes of these standing waves should coincide with the maxima of the potential U (x), see Fig. 4.3. If the standing wave nodes happen to be at maxima of the potential U (x), the energy of the standing wave will be lower; if the maxima of U (x) coincide with the standing wave antinodes, the energy of the wave will be higher. The energy difference between these two situations is the band gap. Fig. 4.3 A sketch of the periodic lattice potential U (x) (upper graph), and the electron probability density in the two possible standing waves that correspond to the wave number k = π/a

4.2 Energy Bands

89

Fig. 4.4 Band structure of silicon, germanium, and gallium arsenide, showing the energy vs. momentum curves for a few bands and for two crystallographic directions. The momentum is normalized to the momentum p0 of a free electron with the kinetic energy p02 /(2me ) = 1 eV

The Energy-Momentum Diagrams in Three Dimensions  In three-dimensional crystals, the first Brillouin zone consists of the k-vectors inside a certain polyhedron centered around k = 0. The shape of that polyhedron is chosen based on the symmetry of the crystal structure. Finding the electron energies vs. momentum for different bands in a crystalline solid is a hard mathematical and computational task. Nevertheless, the band structure calculations are performed routinely for many materials of practical significance. The structure of a few bands in Si, Ge, and GaAs is shown schematically in Fig. 4.4 as an example. It is seen the function En (p)  depends not only on the magnitude but also on the direction of p.  This is so, because the atoms of the crystal are arranged differently along the crystallographic directions that do not belong to the same family. For the p-vectors  that are oriented along the crystallographic directions of the same family, the En (p) curves are identical. The highest maximum and the lowest minimum of En (p)  at a fixed n are called the top and the bottom of the band, or the band edges. The energy difference between the top of a lower band and the bottom of a higher band is called the band gap, Eg . It has a typical value of the order of 1 eV. The band gap values of three representative semiconductors, Si, Ge, and GaAs, at T = 300 K are given in Appendix A.3. Due to the thermal expansion of the crystal lattice, the band gap depends weakly on temperature. The presence of a band gap plays an important role in the formation of the electronic properties of semiconductors.

Quasimomentum The momentum-like quantity p = h¯ k of an electron in a crystal is called quasimomentum, or the crystal momentum. Quasimomentum is in many respects similar to the kinematic momentum pkin = me v of a free electron. For example, the quasimomentum of an electron in a crystal is conserved, just like the kinematic momentum of a free electron does not change in time.

90

4 Band Theory of Solids

The introduction of the quasimomentum actually makes the discussion of electrons easier than in terms of the kinematic momentum pkin . For example, when an electric field E is applied to an electron, its kinematic momentum changes due to the electric field and due to the presence of the periodic potential U (r ). The quasimomentum, on the other hand, changes solely due to the electric field; the effect of the periodic potential is already taken care of in the energy-momentum  in a given band. relation En (h¯ k) An important difference between the two kinds of momenta, p and pkin , lies in the fact that the energy of an electron in a crystal is a periodic function of the quasimomentum, so that only p inside the first Brillouin zone are physically relevant. In a one-dimensional crystal, adding an integer multiple of 2π/a to the quasimomentum results brings the electron to a quantum state physically identical to the state with the quasimomentum p. In this book, we will omit the prefix “quasi” and will refer to p = h¯ k simply as momentum, keeping these differences from the kinematic momentum in mind.

4.2.3 Phase Velocity vs. Group Velocity Phase Velocity So far, we described an electron in a periodic potential as a Bloch wave. The full time-dependent Bloch wave function is (see Sect. 1.8.2) 

ψnk (r , t) = nk (r ) e−iωn (k)t = unk (r )

 1 i(k·  r −ωn (k)t)   = En (k) , e , ω ( k) n h¯ L3/2

 is the angular frequency corresponding to the energy En (k).  The phase where ωn (k) of the plane-wave part of this wave function,  θ (r , t) = k · r − ωn (k)t has a constant value at the point r given by r(t) = r0 +

 ωn (k) k t. 2  |k|

Indeed,  = k · r0 = const. θ (r (t), t) = k · r(t) − ωn (k)t The time-dependent position r(t) above describes motion from the starting point  k|  with the velocity r(0) = r0 in the direction of a unit vector k/|

4.2 Energy Bands

91

 = vph (k)

  En (p) En (k)  ωn (k) = , =   |p|  h| |k| ¯ k|

called the phase velocity. In the second equality, we switched from the description  in terms of the wave vector k to the one in terms of the momentum p = h¯ k. Even though the phase of the Bloch wave function moves with the velocity vph , this motion does not result in any observable effect. The reason is that the wave function is not a measurable quantity, only it modulus squared is. The probability density corresponding to the time-dependent state ψnk (r , t) is stationary: |ψnk (r , t)|2 =

1 |u  (r )|2 . L3 n k

The probability to find an electron is periodically modulated, but the electron remains delocalized in the following sense. The probability to find an electron inside a unit cell located at the point R is obtained by integrating the probability density  located at R:  over the volume of the unit cell Vcell (R))  = P (R)



 d r |ψnk (r , t)| = 3

 Vcell (R)

2

 d Vcell (R)

3r

|unk (r , t)|2

L3

= const.

Because the function unk (r ) has the periodicity of the crystal lattice, the integral does not depend on the location R of the unit cell. Hence, an electron can be found in any unit cell with the same probability.

Group Velocity The wave–particle duality principle says the same object may behave as a particle or as a wave, depending on the situation. Here, we will try to understand how electrons in a crystal can behave as particles. An object manifests its properties when it interacts with other objects. Electrons in a crystal interact with the crystal defects, with the thermal vibrations of the crystal lattice, and with other electrons. These interactions usually are more efficient for  than for others. This is similar some values of the wave vector k and energy En (k) to the interaction of a simple harmonic oscillator with an external force: it is most efficient if the force changes in time periodically with the natural frequency of the oscillator. Consider a group of Bloch states that belong to the same band n and whose wave vectors have the values close to k0 . These states are described by a collective wave function given by a linear combination φ(r , t) =

k

 ψ  (r , t) A(k) nk

92

4 Band Theory of Solids

 called the envelope function. This linear combination of with some function A(k), Bloch states is called the wave packet. The collective wave function φ(r , t) does not describe a state of definite energy.  which are Rather, it is a superposition of quantum states of many energies, En (k),  Because of that, φ(r , t) does not satisfy the selected by the envelope function A(k). time-independent Schrödinger equation. However, it satisfies the time-dependent Schrödinger equation i h¯

h¯ 2  2 ∂φ(r , t) =− ∇ φ(r , t) + U (r )φ(r , t). ∂t 2me

Therefore, φ(r , t) is a possible time-dependent state of an electron. Because the discrete wave vectors k are closely spaced, we can replace the sum by an integral and write  φ(r , t) =

 r −ωn (k)t)   u  (r ) ei(k· d 3 k A(k) . nk

We have absorbed the constant 1/L3/2 and whatever other constants arise in this replacement into the envelope function A(k − k0 ). Suppose a particular interaction is most efficient for the wave vectors around  some specific value k0 . Correspondingly, let us choose the envelope function A(k) such that it has a sharp peak at k = k0 and quickly decays to zero as the modulus of the difference |k − k0 | gets larger. To understand the behavior of the wave packet, let us consider the simpler case of a one-dimensional crystal; the insight that we will obtain in its analysis will be applicable to the three-dimensional crystals as well. Let us choose the envelope function to be a box of side 2k around the wave number k0 : A(k) =

 A0 if k0 − k < k < k0 + k, 0 otherwise.

The one-dimensional wave packet then becomes  φ(x, t) = A0

k0 +k

k0 −k

dk unk (x) ei(kx−ωn (k)t) .

For small k, the term unk (x) can be replaced with unk0 (x) and taken out of the integral, because k0 is not an integration variable. The angular frequency as a function of k can be approximated as a linear function: ωn (k) = ωn (k0 ) + ωn (k0 )(k − k0 ) + . . . , where ωn (k0 ) =

dωn (k)

. dk k=k0

With these replacements, we have

4.2 Energy Bands

93

 φ(x, t) = A0 unk0 (x)

k0 +k k0 −k



dk ei [kx−(ωn (k0 )+ωn (k0 )(k−k0 ))t] 

= A0 unk0 (x) e−i(ωn (k0 )−ωn (k0 ) k0 )t



k0 +k k0 −k



dk eik(x−ωn (k0 )t) .

In the second step, we moved the part of the exponential that does not depend on k outside the integral. The integration is easy to perform: 

k0 +k k0 −k

dk e

ik(x−ωn (k0 )t)

 eik(x−ωn (k0 )t)

k=k0 +k = i(x − ωn (k0 )t) k=k0 −k 



eik(x−ωn (k0 )t) − e−ik(x−ωn (k0 )t) i(x − ωn (k0 )t)    ik0 (x−ωn (k0 )t) sin k(x − ωn (k0 )t) = 2e , x − ωn (k0 )t 

= eik0 (x−ωn (k0 )t)

where we used Euler’s formula sin(θ ) = (eiθ − e−iθ )/(2i) in the last step, see Appendix A.1. Substitution of this result into the last expression for φ(x, t) gives φ(x, t) = 2 A0 unk0 (x) e

i(k0 x−ωn (k0 )t)

  sin k(x − ωn (k0 )t) . x − ωn (k0 )t

It gives the probability density to find an electron |φ(x, t)|2 = 4A20 |unk0 (x)|2 k 2 f (x, t), where   sin2 k(x − ωn (k0 )t) f (x, t) = . k 2 (x − ωn (k0 )t)2 If not for the function f (x, t), the probability density |φ(x, t)|2 would have been just a periodic function of space. The function f (x, t) makes all the difference. It has the maximal value2 f (xpeak (t), t) = 1 at xpeak (t) = ωn (k0 )t and decays to the left and to the right of that peak, simultaneously performing a few oscillations. But then the probability density |φ( x , t)|2 to find an electron is

2 Note

that lim→0

sin  

= 1.

94

4 Band Theory of Solids

Fig. 4.5 The function f (x, t) at times t0 = 0, t1 > 0, and t2 > t1

maximal at xpeak and decays to zero to the left and to the right of the peak. In other words, the electron is now localized at x = xpeak . It behaves as a particle. The behavior of the function f (x, t) at three different times is shown in Fig. 4.5. Its maximum moves with the velocity v=

dxpeak = ωn (k0 ), dt

called the group velocity. Remarkably, the group velocity is independent of the width k of the envelope function A(k). As a matter of fact, any other reasonable choice of A(k) yields the same group velocity value. The argument can be generalized to a three-dimensional crystal. In this case, the group velocity of a wave packet is a vector, whose components are given by vi =

  ∂ωn (k) ∂En (p) = , i = x, y, z, ∂ki ∂pi

where we used the relations En = hω ¯ n and p = h¯ k and dropped the subscript 0  in the wave vector k, around which the wave packet is centered. Note that for free classical particles with the standard energy-momentum relation E(p)  = p 2 /(2m), the velocity components are likewise given by vi = ∂E/∂pi = pi /m.

4.2.4 Bloch Oscillations Let us consider again a hypothetical one-dimensional crystal model with just one electron in the energy band n. Suppose that an external electric field E is applied to the crystal. The electron momentum p changes in time according to

4.2 Energy Bands

95

Fig. 4.6 Bloch oscillations of the quasimomentum in the presence of a constant electric field

dp(t) = −eE ⇒ p(t) = −eEt, dt assuming p(0) = 0. Eventually, p will reach the left edge of the first Brillouin zone at −hπ/a = −h/(2a). This state is physically identical to the one with the ¯ momentum +hπ/a = h/(2a). Hence, the momentum suddenly changes its value to ¯ h/(2a) and continues its linear decrease until it reaches the end of the Brillouin zone again. The electron momentum in the presence of a constant electric field performs saw-tooth-like oscillations with the amplitude h/(2a) and period h/(aeE), see Fig. 4.6. This periodic variation of the momentum is physically equivalent to its steady decrease p(t) = −eEt at all time in view of the equivalence of the Bloch states with momenta differing by h/a. Consider now what happens to the electron group velocity, given by v(t) = En (−eEt), in a one-dimensional crystal. Since the energy is a periodic function of p with the period h/a, the electron group velocity will perform oscillations around the value v = 0 with the period TB =

h . aeE

Also the position of the electron wave packet, 

t

x(t) =

dt  v(t  ) + x(0),

0

will be oscillating with the same period. This is a remarkable result that demonstrates the completely different behavior of an electron in a crystal from a free electron. A constant electric field accelerates a free electron, but an electron in a crystal performs oscillator motion, whose period depends on the crystal’s lattice constant. This effect is called Bloch oscillations.

96

4 Band Theory of Solids

Bloch oscillations are very hard to observe experimentally in real crystals. In order to perform at least one Bloch oscillation, an electron wave packet must remain unperturbed on the time scale of the order of TB . For the electric field strength E = 1 kV/cm and the lattice constant a = 4 Å, the period of Bloch oscillations has the value TB = 1.03 µs. This is many orders of magnitude longer than the characteristic collision time of an electron with quanta of lattice vibrations and with impurities in a crystal. Due to these collisions, the electron wave packet is destroyed well before it reaches the edge of the first Brillouin zone. But even in the absence of collisions, the wave packet gets destroyed for a different reason. Our derivation of the expression for the group velocity relied on the simplest linear approximation of the energy-momentum relation around the value p0 , the momentum of the wave packet: En (p) = En (p0 ) + En (p0 )(p − p0 ). A more accurate analysis should include higher-order terms in p−p0 . It shows that the wave packet width increases in time, which means that the wave packet eventually becomes delocalized. Nevertheless, Bloch oscillations have been observed in the so-called superlattices—artificial periodic structures with large lattice constant—at high electric fields.

4.3 Conduction Types of Solids 4.3.1 Band Filling and Electrical Conductivity After the band structure of a material is established, the electron states must be filled with electrons, with two electrons per state and 2N electrons per band, where N is the number of primitive cells. In doing so, the lower-energy bands will be completely filled. Naïve classical considerations would lead us to think (incorrectly) that the states with the lowest energy are characterized by zero electron velocity, and application of an electric field would lead to an overall velocity increase for those electrons, i.e., to an electric current.  and A completely filled band contains electrons with a non-zero wave number, k,  which may be very large in magnitude. In the absence of the momentum p = h¯ k, an electric field, there is no net current produced by the electrons in a completely filled band, because for each electron moving in one direction, the band contains another electron with the same magnitude of momentum, but moving in the opposite direction. Even in the presence of an electric field, a completely filled band produces zero contribution to the net electric current. A single electron is accelerated by an electric field, i.e., it changes its momentum. In a crystal containing many electrons, an electric field attempts to put each electron into a different momentum state in the same band. But if all those states are occupied, then Pauli exclusion principle disallows an electron to change its momentum in response to the electric field. Then,

4.3 Conduction Types of Solids

97

Fig. 4.7 Schematic illustrations of the energy-momentum diagrams of metals and semimetals. The shaded areas indicate the occupied states

the band will continue to contain the same number of electrons moving against and along the electric field, producing zero contribution to the electric current. It is only the bands that are partly filled that contribute to the electric current in response to an external electric field. The band theory allows one to understand the conductivity of conductors (metals and semimetals) and the lack thereof in insulators. The type of a given material is determined by its band structure and the location of Fermi energy at zero temperature. Note that the band structure diagrams that appear in this section do not refer to any particular materials and are given for illustration purposes only.

4.3.2 Metals and Semimetals In metals, such as Li, Au, Cu, etc., Fermi energy at zero temperature happens to be in the middle of one of the energy bands (Fig. 4.7). This means that the highest occupied band is filled only partly and contains both filled and empty states. If an electric field is applied to a metal, electrons in that partly filled band will change their momentum states, because there are empty states in the same band for its electrons to occupy while remaining in the same band. As a result, the field will create a disbalance of the electrons moving against and along the field, leading to the onset of an electric current. In semimetals, such as As, Sb, Bi, α-Sn, etc., the two highest bands that contain electrons at zero temperature overlap, and both are partly filled. As a result, both bands contribute to the electric current when an external electric field is applied.

4.3.3 Dielectrics and Semiconductors In dielectrics and semiconductors, Fermi energy at T = 0 happens to be inside the energy gap between two bands. As a result, the highest occupied band is completely

98

4 Band Theory of Solids

Fig. 4.8 Schematic illustrations of the energy-momentum diagrams of dielectrics and semiconductors

filled, while the next band is empty. Application of an electric field cannot change the momentum states of the electrons in the highest filled band, because there are no empty states in that band for the electrons to go to. Then, the electrons will not react to an applied electric field, and the material will not conduct electricity. The difference between the dielectrics and semiconductors is in the size of the energy gap, Eg , separating the highest filled band from the lowest empty band, see Fig. 4.8. In semiconductors, the band gap is of the order of 1–4 eV, whereas in dielectrics it exceeds 5 eV. Because of this, the lowest empty band in dielectrics remains empty even at the temperature of a few hundred Kelvin, whereas in semiconductors, some electrons can go into it from the highest occupied band at the room temperature.

4.4 Conduction and Valence Bands In semiconductors, the tail of the Fermi-Dirac distribution at T > 0 extends into the upper band that is empty at zero temperature, but becomes partly filled at T > 0. This band gets a non-negligible amount of free electrons which can change their momenta in response to an external electric field. Such electrons contribute to the electric conductivity and are called conduction electrons. The band where they “live” is called the conduction band. Because Fermi-Dirac distribution decreases exponentially with energy at its tail, conduction electrons occupy the bottom part of the conduction band. The band from which the electrons were promoted at non-zero temperature is called the valence band. This band was completely filled at zero temperature, but at a non-zero temperature, some electrons from the upper part, or the top, of the valence band move into the conduction band. As a result, the top of the valence band lacks a non-negligible number of electrons. Because empty states exist in the valence band at T > 0, this band also contributes to the electric current in response to an external electric field. Semiconductors in which the top of the valence band is at the same wave vector as the bottom of the conduction band are called direct-band gap semiconductors.

4.5 Holes

99

Fig. 4.9 Schematic illustrations of the energy-momentum diagrams in direct-band gap vs. indirect-band gap semiconductors. The shaded areas indicate the states occupied with electrons at T > 0

The typical example of direct-band gap semiconductors is GaAs. If the top of the valence band happens at a different momentum than the bottom of the valence band, the material is called an indirect-band gap semiconductor, the typical example being Si. Figure 4.9 illustrates this distinction. The band gap of a semiconductor is measured experimentally by studying the optical absorption of light. Namely, the light with the photon energy hf exceeding the band gap energy Eg can promote electrons from the valence band to the conduction band and is, therefore, absorbed by the material. On the other hand, if the photon energy is below Eg , the light will pass through the material. A measurement of the light frequency fedge at the absorption edge gives the band gap energy Eg = hfedge .

4.5 Holes The contribution to the net current caused by an electric field from a particular band is proportional to the sum of the velocities that correspond to those states of this band which are filled with an electron: Iband ∝ −e vp . filled states p

Note that the sum of velocities over all states, both filled and empty, from the same band is exactly zero. This is so, because to each state in the band with a particular velocity value there corresponds a state with the opposite velocity:

100

4 Band Theory of Solids

vp =

all states p

vp +

filled states p

vp = 0.

empty states p

Thus,

vp = −

filled states p

vp ,

empty states p

and the expression for the current contribution from a given band can be rewritten as (note the sign change in front of e) Iband = e

vp .

empty states p

The number of empty states in the valence band of a semiconductor is usually much smaller than the number of the filled states. It is for this reason that the second expression for Iband as the sum over the empty states is more preferable to use than the first one. Each empty state p in the valence band can be interpreted as a state filled with an imaginary particle, or a quasiparticle, of positive charge e and velocity vp . These quasiparticles are called holes. While a hole means the absence of an electron in a particular momentum and spin state in a band, holes do behave like real particles. Their introduction makes the discussion of semiconductors much easier, whereas the discussion involving only electrons would be excessively cumbersome. Therefore, the picture that we will adopt is this: There are two charge carriers in a semiconductor, the negatively charged electrons in the conduction band and the positively charged holes in the valence band. The probability fh that a particular state p with the energy E(p)  in the valence band is occupied by a hole is just the probability that it does not contain an electron. Because state occupation probability by electrons is given by the Fermi-Dirac distribution, fe (E), fh (E) = 1 − fe (E) = 1 −

1 1 = . 1 + e(E−EF )/kT 1 + e−(E−EF )/kT

The Fermi-Dirac distribution for holes, fh (E), looks almost the same as that for electrons, fe (E), except for the sign in front of the energy difference E − EF in the exponential. We can interpret this observation by stating that hole energies, E (h) (p),  have the sign opposite to electron energy in the same quantum state p,  up to an additive constant E: E (h) (p)  = −E (e) (p)  + E, see Fig. 4.10. The additive constant should be chosen such that holes and electrons have the same Fermi level:

4.6 Effective Mass Tensor

101

Fig. 4.10 Electron and hole energy-momentum curves

(h)

(e)

(e)

EF = −EF + E = EF , that is, (e)

E = 2EF . In this way, the Fermi-Dirac distribution for holes looks formally the same as for electrons: fh (E (h) ) =

1 (h)

(h) 1 + e(E −EF )/kT

.

We will always give energy from the electrons’ perspective and omit the superscript (e) by default. If we wish to indicate energy from the holes’ viewpoint, we will attach the superscript (h) to the respective energy.

4.6 Effective Mass Tensor In classical physics, the mass of an object is the proportionality coefficient between its acceleration and the force acting on it, a = F /m. Alternatively, it is a coefficient that relates the object’s kinetic energy and momentum, EK = p 2 /(2m). For electrons and holes in a crystal, the role of the momentum is played by the  and an applied force results in its change at a rate quasimomentum p = h¯ k, dpi = Fi , i = x, y, z. dt

102

4 Band Theory of Solids

The role of the kinetic energy is played by the dispersion relation E(p)  = E (e) (p)  (h) and E (p)  for electrons in the conduction band and holes in the valence band, respectively. Let us focus on the electrons for now. The ith component of an electron’s group velocity is vi =

∂E(p)  . ∂pi

The acceleration of an electron then has the ith component ai =

∂ 2 E(p) ∂ 2 E(p) d ∂E(p)   dpj  dvi = = = Fj . dt dt ∂pi ∂pi ∂pj dt ∂pi ∂pj j =x,y,z

j =x,y,z

The coefficients that multiply the force components in the sum play the role of the inverse mass of an electron in a semiconductor. It is called the effective mass tensor. In contrast to the usual mass of a free electron me , the effective mass depends on momentum and is a 3 × 3 matrix. It is marked with a star to distinguish from the free electron mass. The components of its inverse are related to the second derivative of the energy-momentum relation: ai =

 j =x,y,z

1 ∗ me (p) 



 Fj , ij

1 ∗ me (p) 

 = ij

 ∂ 2 E(p) . ∂pi ∂pj

We will be interested in the situations when the electrons’ momenta do not differ much from the momentum pC at the minimum of the conduction band. Then, the effective mass tensor is evaluated at a particular momentum p = pC ; as such, it has constant components independent of p.  The next simplification has to do with a convenient choice of the coordinate axes. At not too big deviations |p − pC | from the band minimum, the surface of constant energy E(p)  = const in the momentum space has the form of an ellipsoid, see Fig. 4.11a. Aligning the coordinate axes with its principal axes makes the matrix (1/m∗e )ij diagonal, i.e., its elements with i = j become zero. Hence, the effective mass has only three non-zero components: 1 ≡ m∗e,i



1 m∗e

 = ii



∂ 2 E(p) , i = x, y, z. ∂pi2 p=  pC

This definition is valid only for a particular choice of the coordinate axes; any other choice will give non-zero values of m∗e,ij with i = j . In many semiconductors with ellipsoidal constant-energy surfaces, including Si and Ge, two components of the effective mass tensor are the same (Fig. 4.12a). They are called the transverse (subscript t) effective masses. The remaining third component, which is different, is called the longitudinal (subscript l) effective mass:

4.6 Effective Mass Tensor

103

Fig. 4.11 (a) Constant-energy surface in the momentum space near the bottom of the conduction band; note that p = p − pC . (b) A sketch of the band structure of a semiconductor with two hole branches: heavy and light

Fig. 4.12 Constant-energy surfaces in the momentum space near the bottom of the conduction band of (a) Ge and (b) of GaAs

m∗e,x = m∗e,y = m∗e,t , m∗e,z = m∗e,l . The numerical values of the transverse and longitudinal effective masses are usually given as ratios to the free electron mass me . Depending on the material, the ratios m∗e,t and m∗e,l range from a few percent to a few. The values of the effective mass components in three representative semiconductors are given in Appendix A.3. In GaAs, which is a direct-band gap semiconductor, the constant-energy surface is a sphere centered at p = 0; hence, all three effective mass components are the same in this semiconductor (Fig. 4.12b). The effective mass of a hole m∗h in many semiconductors is not a matrix, but an ordinary number, because the constant-energy surface in the valence band happens to be a sphere centered at p = 0 at small p. The hole effective mass is found as the  in the valence band near the valence band maximum: curvature of the E(p)

104

4 Band Theory of Solids

p2 1 d 2 E(p)

E(p) = EV − , =− . 2m∗h m∗h dp2 p=0 The minus sign in front of the second derivative takes care of the fact that hole energy is measured down. The valence band in many semiconductors consists of two branches that meet at p = 0, see Fig. 4.11b. Corresponding to these two branches are the two types of holes, designated as heavy and light, with the effective masses m∗hh > m∗lh . The heavy and light holes effective masses in Si, Ge, and GaAs are given in Appendix A.3. As with the electrons, they typically range from a few percent of a free electron mass to a few free electron masses. A quasiparticle is a useful concept to describe particle-like elementary excitations in solids. Examples of quasiparticles are numerous and include the quanta of lattice vibrations (phonons), magnetization spin waves (magnons), bound electron– hole states (excitons), to name but a few. The conduction electrons and holes with the properties described in this chapter exist only inside the crystal, but not as free particles. For that reason, they are not real particles, but quasiparticles. In the rest of this book the term “electrons” will mean quasielectrons near the bottom of the conduction band; all other quasielectrons are irrelevant for our purposes.

4.7 Problems 4.7.1 Solved Problems Problem 1 Show explicitly that a linear combination of Bloch states ψnk (r , t), viz.,  ψ  (r , t), φ(r , t) = A(k) nk k

satisfies the time-dependent Schrödinger equation, i h¯

h¯ 2  2 ∂φ(r , t) =− ∇ φ(r , t) + U (r ) φ(r , t). ∂t 2me

Problem 2 Consider a wave packet formed by the plane waves in one dimension:  φ(x, t) =

−∞

dk A(k)

ei(kx−ω(k)t) . √ L

The angular frequency depends on the wave number according to the free-particle energy-momentum relation:

4.7 Problems

105

ω(k) =

hk E(hk) ¯ 2 ¯ = , h¯ 2m

where m is the particle’s mass. The envelope function is a Gaussian peak centered at k = k0 and having the width σk , viz., A(k) = A0 e−(k−k0 )

2 /(2σ 2 ) k

.

(a) Find the particle’s probability density |φ(x, t)|2 by performing a integration over k. L (b) Find the constant A0 from the normalization condition 0 dx |φ(x, t)|2 = 1. ∞ √ 2 Hint: use the identity −∞ dk e−α(k−κ) = π/α, where α is an arbitrary complex number with Re α > 0 and κ may be complex-valued as well. Problem 3 The energy-momentum dispersion relations near the edges of the two bands of a hypothetical one-dimensional semiconductor read conduction band :

E(p) = A eγ

valence band :

E(p) = B cos2 (πp/p0 )

cos(2πp/p0 )

with positive constants A = 3 eV, B = 1.5 eV, γ = 0.2, and p0 such that 1 eV.

p02 2me

=

(a) Is it a direct-band gap or an indirect-band gap semiconductor? (b) Determine the band gap and the Fermi energy at T = 0 relative to the top of the valence band. (c) Express the electron and hole effective masses in terms of the free electron mass, i.e., as ratios m∗e /me , m∗h /me . (d) Assuming the Fermi energy to be in the middle of the band gap, what is the probability for the lowest energy state in the conduction band to be filled with an electron at T = 300 K?

4.7.2 Practice Problems Problem 1 An electron in a one-dimensional lattice with periodicity a finds itself in a Bloch state nk (x) = √1 eikx unk (x) with unk (x + a) = unk (x). Its average L momentum is  dnk (x) ∗ ,

p = −i h¯ dx nk (x) dx see Sect. 1.9. Show that p = hk. ¯

106

4 Band Theory of Solids

Problem 2 Imagine a one-dimensional semiconductor with just one electron in the conduction band. A constant electric field E is applied to the sample. The assumed energy-momentum relation in the conduction band is E(p) = −E0 cos(ap/h). ¯ The electron’s wave function is not a pure Bloch state, but a wave packet of finite width. How does the group velocity of the electron evolves as it undergoes Bloch oscillations? What happens to its position?

4.7.3 Solutions Problem 1 The time derivative of the wave packet wave function multiplied by i h¯ is i h¯

∂ψ  (r , t) ∂φ(r , t)  = . A(k) i h¯ nk ∂t ∂t k

Each time-dependent Bloch function satisfies the time-dependent Schrödinger equation, i h¯

∂ψnk (r , t) h¯ 2  2 =− ∇ ψnk (r , t) + U (r ) ψnk (r , t). ∂t 2me

Hence, ∂φ(r , t)  = i h¯ A(k) ∂t k

=−



h¯ 2  2 − ∇ ψnk (r , t) + U (r ) ψnk (r , t) 2me

h¯ 2  2   ψ  (r , t) A(k) ψnk (r , t) + U (r ) A(k) ∇ nk 2me k

=−



k

h2

¯ 2 ∇ φ(r , t) + U (r )φ(r , t). 2me

Problem 2 (a) The wave function is given by the integral A0 φ(x, t) = √ L



  (k − k0 )2 h¯ 2 k t dk exp − + i kx − . 2m 2σk2 −∞



4.7 Problems

107

The argument of the exponential function is transformed so as to complete the square:   (k − k0 )2 h¯ 2 k t − i kx − 2m 2σk2 =

k 2 − 2k0 k + k02 2σk2

− ikx + i

h¯ 2 tk 2m

   k02 h¯ k0 1 2 t k + i − k + ix + m σk2 σk2 2σk2    k0 + ixσk2 k02 1 1 h¯ 2 k − 2k = +i t + h¯ 2 h¯ 2 2 σk2 m 1+im σk t 1+im σk t ⎛ ⎞   2  2  k0 + ixσk2 k0 + ixσk2 k02 1 1 h¯ ⎝ ⎠. = k− +i t − + h¯ 2 h¯ 2 h¯ 2 2 σk2 m 1+im σk t 1+im σk t 1+im σk t 1 = 2



Performing integration over k, we obtain  A0   2π φ(x, t) = √  1 h¯ t L σ2 + i m k

⎡  ⎞⎤  ⎛ 2 k0 + ixσk2 k02 1 1 h ¯ ⎠⎦ × exp ⎣ +i t ⎝ − h¯ 2 h¯ 2 2 σk2 m 1+im σk t 1+im σk t  !  (k0 + ixσk2 )2 1 A0 σk 2π = √ exp − k02 h¯ 2 h¯ 2 2σk2 σk t 1+im σk t L 1+im ⎛ ⎞  h¯ 2 k0 t σk2 x 2 − 2ik0 x + i m A0 σk 2π ⎠.  = √ exp ⎝− h¯ 2 h¯ 2 σk t L 1+im 2 1+im σk t Particle probability density is |φ(x, t)|2 = φ ∗ (x, t)φ(x, t) = 

1 exp − 2

A20  L

2π 1 σk2

+

h¯ 2 2 2 σ t m2 k

h¯ 2 k0 t σk2 x 2 − 2ik0 x + i m h¯ 2 1+im σk t

+

h¯ 2 k0 t σk2 x 2 + 2ik0 x − i m h¯ 2 1−im σk t

! .

108

4 Band Theory of Solids

After some algebra, the expression in the square brackets simplifies to

[. . .] = 2σk2

 x− 1+

h¯ k0 m t

2

h¯ 2 4 2 σ t m2 k

,

so that the particle probability density is ⎛ |φ(x, t)|2 =

A20 L

 1 σk2

+

h¯ 2 2 2 σ t m2 k



⎜ exp ⎝−σk2

x−

1+

h¯ k0 m t

2 ⎞

h¯ 2 4 2 σ t m2 k

⎟ ⎠.

This is a Gaussian distribution, ⎛  2 ⎞ √ h¯ k0 x − t m 2π ⎜ ⎟ exp ⎝− |φ(x, t)|2 = ⎠. L σx (t) 2σx2 (t) A20

The peak of this distribution is located at x = h¯ k0 m . Its width

h¯ k0 m t;

it moves with the velocity

    1 1 h¯ 2 2 2  σx (t) = + 2 σk t . 2 σk2 m Initially (at t = 0), the width of the probability density is σx (0) = √

1 2σk

.

The broader the distribution of the wave numbers that comprise the wave packet, the better it is initially localized in the x-direction. However, the probability distribution |φ(x, t)|2 becomes broader and broader in time. At large times it behaves as hσ ¯ k σx (t) = √ t. 2m Its rate of spreading is proportional to the width of the wave packet σk in the k-space.

4.7 Problems

109

(b) Integrating the probability density and using the integral formula, we obtain 

A2 1 dx |φ(x, t)| = 0 2π 3/2 = 1 ⇒ A0 = 3/4 L π −∞



2

L . 2

Without the constant A0 , the probability density is written as ⎛  2 ⎞ hk ¯ 0t x − m 1 ⎟ ⎜ |φ(x, t)|2 = √ exp ⎝− ⎠. 2 2σx (t) 2π σx (t)

Problem 3 (a) To establish the type of this hypothetical semiconductor, we need to find the energy minimum in the conduction band and energy maximum in the valence band. Let us begin with the conduction band. Since exponential is an increasing function of its argument, the minimum of EC (p) is found at that momentum p, at which cos(2πp/p0 ) has the minimal value of −1. This happens at p = pC,min = p0 /2. Let us look at the valence band. The maximum of EV (p) is found at p = pV ,max = 0. Since pC,min = pV ,max , this is an indirect-band gap semiconductor. (b) The band gap energy is the difference between the minimal energy in the conduction band and the maximal energy in the valence band: Eg = EC (pC,min ) − EV (pV ,max ) = A e−γ − B = 3 · e−0.2 − 1.5 = 0.956 eV. At T = 0, the Fermi energy is right in between the band gap: EF (T = 0) − EV = Eg /2 = 0.478 eV. (c) To find the carriers’ effective masses, we need to differentiate EC (p) near its minimum and EV (p) near its maximum twice and use the formulas m∗e = Let us do it:

1

d 2 EC

dp p=pC,min

, m∗h = −

1

d 2 EV

dp p=pV ,max

.

110

4 Band Theory of Solids

   2π dEC 2πp γ cos(2πp/p0 ) · = Ae · γ · − sin dp p0 p0   2π γ A γ cos(2πp/p0 ) 2πp , =− e sin p0 p0



 

d 2 EC

2π γ A 2πp γ cos(2πp/p0 ) 2π

= − · e · cos .

2 p0 p0 p0 dp p=p0 /2 p=p0 /2 We did not write the term proportional to sin(2πp/p0 ), which appears after differentiating the exponential function, because this term goes to zero after substitution p = p0 /2. With cos(2πp/p0 )|p=p0 /2 = cos(π ) = −1 we have:

d 2 EC

1 (2π )2 γ A −γ = ∗ = e .

2 me dp p=p0 /2 p02 This gives the electron effective mass m∗e =

p02 eγ . 4π 2 γ A

With p02 /(2me ) = C = 1 eV, we find p02 = 2me C. Hence, the ratio of electron effective mass to the free electron mass can be finally found: m∗e =

2me Ceγ 4π 2 γ A

m∗e Ceγ . = me 2π 2 γ A

Numerically, m∗e (1 eV) · e0.2 = 0.103. = me 2 · π 2 · 0.2 · (3 eV) Now, we perform a similar calculation for the valence band near its maximum at p = 0. We have:       πp π π dEV πp 2πp sin = − B sin , = −B · 2 cos dp p0 p0 p0 p0 p0 where we used the identity 2 sin(θ ) cos(θ ) = sin(2θ ). Taking the second derivative at p = 0,



 d 2 EV

1 π B 2π 2πp

= − = − cos m∗h p0 p0 p0 p=0 dp2 p=0

4.7 Problems

111

=−

p02 2π 2 B ∗ . ⇒ m = h 2π 2 B p02

As in the electron case, we plug in p02 = 2me C, where C = 1 eV, and obtain m∗h =

m∗h me C C ⇒ = 2 . 2 me π B π B

Numerically, m∗h 1 = 0.0675. = 2 me π · 1.5 (d) The probability for the lowest energy state in the conduction band to be occupied by an electron is given by the value of the Fermi-Dirac distribution f =

1 . 1 + e(EC −EF )/kT

Since the Fermi energy is in the middle of the band gap, we have EC − EF = Eg /2 = 0.478 eV. At T = 300 K, the thermal energy is kT = 0.02585 eV. The probability f has the numerical value f =

1 1 + e0.478/0.02585

= 9.32 · 10−9 .

Part II

Semiconductors in and out of Equilibrium

Chapter 5

Semiconductors in Equilibrium

5.1 Density of States We are now ready to calculate the equilibrium electron concentration in the conduction band, n0 , and equilibrium concentration of holes in the valence band, p0 . The notation comes from the sign of the respective charges: negative for electrons and positive for holes. The subscript 0 indicates thermal equilibrium. We will see later on in this chapter that equilibrium charge carrier concentration can be affected by adding various impurities that may also alter the band structure of the material, provided that impurity concentration is high. Here and in the following, we assume this not to be the case, i.e., impurity concentration is insufficient to change the band structure. Let us start with the electrons. The most general expression for the concentration of the conduction electrons is n0 =

2 f (E(p))  , L3 p∈C.B. 

where the sum is over all momentum states p in the conduction band (C.B.), E(p)  is the electron energy in the conduction band as a function of electron momentum, and the prefactor 2 comes from the two possible spin orientations, ±1/2. The result is divided by L3 , the volume of the semiconductor, assumed to be a cube of side length L with periodic boundary conditions. Evaluation of this sum is difficult because the dependence E(p)  is quite complicated and because Fermi–Dirac distribution f (E) is not easy to deal with. We can overcome both difficulties by making use of the fact that because f (E) decreases exponentially strongly with energy above Fermi energy, only the low-energy states in the conduction band are populated with appreciable probability. Hence, we can approximate the energy–momentum relation with a quadratic function

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_5

115

116

5 Semiconductors in Equilibrium

E(p)  = EC +

i=x,y,z

1 (pi − pC,i )2 , 2m∗e,i

where EC is the energy at the conduction band minimum and pC is the momentum at which this minimum occurs. The coordinate axes are chosen such that only the diagonal components of the effective mass matrix are non-zero (see Sect. 4.6). The value of the Fermi–Dirac distribution depends on the momentum p via the energy E(p).  Therefore, it is convenient in the expression for n0 to convert the sum over momenta into the sum over energies in the conduction band. Furthermore, the typical spacing between two neighboring momentum states is of the order of h/L, which is a very small number if L is macroscopically large. Then, instead of a sum, we can use an integral over energies:  n0 =

dE gC (E) f (E) . EC

The density of states, gC (E), is a function that tells us how many momentum and spin states are there in the conduction band per energy interval from E to E + dE in a unit volume. This number is gC (E) dE. The functional form of gC (E) can be established arithmetically by performing dimensional analysis. The unit of any physical parameter is some combination of mass (measured in kg), time (measured in s), and length (measured in m). For instance, the dimension of energy is [E] = J = kg m2 s−2 in SI units. The dimension of Planck’s constant is [h] = kg m2 s−1 , and, obviously, the dimension of the effective mass is [m∗e ] = kg . The density of states in the conduction band depends on these three parameters. The energy should be counted from the conduction band edge, i.e., we should be writing E − EC instead of just E. The density of states should be proportional to the combination γ gC (E) ∝ (E − EC )α m∗β e h

with the exponents α, β, and γ that are yet to be found. In terms of these exponents, the dimension of the density of states is

5.1 Density of States

117

[gC (E)] = (kg m2 s−2 )α kgβ (kg m2 s−1 )γ = kgα+β+γ m2(α+γ ) s−(2α+γ ) . By its very definition, the dimension of the density of states—that is, the number of states per unit energy per unit volume—is the inverse of the product of energy and volume: [gC (E)] = [E −1 ]m−3 = kg−1 m−5 s2 . Hence, the exponents α, β, and γ must be such that α + β + γ = −1 , 2(α + γ ) = −5 , −(2α + γ ) = 2 . Solving these three equations for the three unknowns gives their values α=

3 1 , β = , γ = −3 . 2 2

Then, the density of states in the conduction band is, up to an unknown constant C, √ ∗3/2 E − EC me gC (E) = C . h3 The non-dimensional number C cannot be established within the dimensional analysis. Neither does the dimensional analysis answer the question about the relevant effective mass m∗e , which should be some combination of the components of the effective mass tensor m∗e,i with i = x, y, z. To figure out the constants C and m∗e , a more rigorous treatment is needed. We first find the total number N(E) of the conduction band states whose energy is below a given value E. The possible momentum values of an electron are given by p = Lh n, where n is a vector whose all three components are integers. In the momentum space, each momentum state occupies a cube of volume  = (h/L)3 . To find N (E), we need to find the number of such cubes inside an ellipsoid defined by (py − pCy )2 (pz − pCz )2 (px − pCx )2 + + =1, 2m∗e,x (E − EC ) 2m∗e,y (E − EC ) 2m∗e,z (E − EC ) see Fig. 4.11a. The volume of this ellipsoid is1

1 An

ellipsoid with the major axes oriented in the x-, y-, and z-directions is defined by an equation 2 2 + yb2 + cz2 = 1 with the parameters a, b, and c being half the distance between the opposite poles of the ellipsoid in the x-, y-, and z-directions. The volume of an ellipsoid is V = 43 π abc. x2 a2

118

5 Semiconductors in Equilibrium

Fig. 5.1 Constant-energy surfaces in the momentum space near the bottom of the conduction band of (a) Si, (b) Ge, and (c) GaAs. Note that in the case of Ge, each of the eight valleys is shared by two Brillouin zones; as a result, the number of valleys in the first Brillouin zone of Ge is νC = 4

(E) =

4 π (2(E − EC ))3/2 m∗e,x m∗e,y m∗e,z . 3

The number of the conduction band states of energy below E is obtained by dividing (E) by . The result needs to be multiplied by 2 to account for two possible spin orientations and by the number νC of the equivalent energy minima in the conduction band. For example, in silicon, νC = 6; in Ge, νC = 4; in GaAs, νC = 1, see Fig. 5.1. Hence, N(E) = 2νC

L3 8νc (E) = 3 π (2(E − EC ))3/2 m∗e,x m∗e,y m∗e,z .  h 3

The density of states per unit energy interval per unit volume is obtained by differentiating this quantity with respect to energy: √

8 2π νC m∗e,x m∗e,y m∗e,z 1 dN(E) gC (E) = 3 = E − EC . L dE h3 The concentration of holes is obtained by integrating over those states in the valence band (V .B.) that are empty: p0 =

 EV 2 (1 − f (E( p))  = dE gV (E) (1 − f (E)) . L3 −∞ p∈V  .B.

The hole density of states in the valence band is found by a similar analysis as for electrons, but with two modifications. First, we focus on the materials in which there is only one energy maximum in the valence band at p = 0, and where the hole effective mass is an ordinary number (see Sect. 4.6), i.e., m∗h,x = m∗h,y = m∗h,z . Second, we take into account the existence of two kinds of holes, the heavy and the

5.2 Equilibrium Carrier Concentration

119

light, with the effective masses m∗hh and m∗lh . Adding the density of states for the two kinds of holes together, we have the total density of states in the valence band   8π (m∗hh )3/2 + (m∗lh )3/2 gV (E) = EV − E . h3

5.2 Equilibrium Carrier Concentration Boltzmann approximation for the Fermi–Dirac distribution is expected to hold quite well because, typically, the energy difference between EF and the band edges EC , EV , is of the order of a few tenths of eV. At the same time, at room temperature T = 300 K, we have kT = 0.02585 eV, which is much smaller than EC − EF and EF − EV . With Boltzmann’s approximation f (E) ≈ e−(E−EF )/kT , 1 − f (E) ≈ e(E−EF )/kT and our expressions for the densities of states in the conduction and valence bands, the expression for the electron concentration becomes  n0 =

dE gC (E) f (E) EC

 8 2π νC m∗e,x m∗e,y m∗e,z h3

dE

E − EC e−(E−EF )/kT .

EC

The integral is evaluated by changing the integration variables from E to x = (E − EC )/kT : 

dE

E − EC e−(E−EF )/kT = (kT )3/2 e−(EC −EF )/kT

EC

dx

x e−x

0

√ = (kT )3/2



π −(EC −EF )/kT e , 2

where the x-integration is performed in Appendix A.4. This gives, finally, n0 = NC e

−(EC −EF )/kT

, NC =

4 2νC (π kT )3/2 m∗e,x m∗e,y m∗e,z h3

.

120

5 Semiconductors in Equilibrium

The parameter NC is called the electron effective density of states. This formula can be interpreted physically as the product of the concentration NC of the conduction 1 band states available for electrons and the probability of f (E) = (EC −EF )/kT ≈ 1+e

e−(EC −EF )/kT for a particular state near the bottom of the conduction band to be occupied. The concentration NC of the available states is approximately the concentration of states whose energy does not exceed the energy EC at the bottom of the conduction band by more than the thermal energy kT . Hence, NC must increase with kT . Also, NC must depend on the curvature of the energy–momentum curve near the conduction band minimum: the lower the curvature (i.e., the higher the effective mass m∗e ), the flatter the band near the bottom, and the more states it offers for the electrons to occupy. Hence, NC also increases with the effective mass m∗e . A similar treatment for holes gives the concentration p0 = NV e

(EV −EF )/kT

√   4 2(π kT )3/2 (m∗hh )3/2 + (m∗lh )3/2 , NV = . h3

The parameter NV is called the hole effective density of states. The physical meaning of this formula is similar to that of the electron counterpart, except now we need to count the unoccupied states near the top of the valence band. The probability of a state at E = EV to be empty (i.e., to be occupied by a hole) is 1 − f (EV ) = 1 −

1 1 + e(EV −EF )/kT

=

e(EV −EF )/kT 1 = (E −E )/kT −(E 1+e V F 1 + e V −EF )/kT

≈ e−(EV −EF )/kT . The total concentration of holes is a sum of the heavy and light holes’ concentrations. The contribution of each hole species is proportional to the respective effective mass raised to the power 3/2. The typical values of the effective densities of states at room temperature T = 300 K are of the order of 1017 . . . 1020 cm−3 , depending on the material. Because the effective densities of states depend on temperature in proportion to T 3/2 , its knowledge at some particular reference temperature T0 , say, T0 = 300 K, is sufficient to determine them at any other temperature as  NC,V (T ) = NC,V (T0 )

T T0

3/2 .

The values of the effective densities of states at T0 = 300 K for Si, Ge, and GaAs can be found in Appendix A.3.

5.3 Energy Probability Distribution

121

5.3 Energy Probability Distribution The function

Pe (E) = C E − EC e−(E−EF )/kT with E > EC used above has the physical meaning of the energy probability distribution of electrons in the conduction band. The parameter C is the normalization constant, whose value is determined by the normalization condition 

 dE P (E) = C

EC

dE

E − EC e−(E−EF )/kT = 1 .

EC

The integral has been evaluated previously; with this result, C=√

2 e(EC −EF )/kT , π(kT )3/2

and thus Pe (E) = √

2 E − EC e−(E−EC )/kT . 3/2 π (kT )

This function is shown in the right panel of Fig. 5.2. By setting the derivative to zero, we find that the most probable electron energy is

dPe (E)

kT . = 0 ⇒ Em = EC +

dE E=Em 2 It is also useful to find the average electron energy relative to the conduction band edge:

Fig. 5.2 Hole (left) and electron (right) energy probability distribution

122

5 Semiconductors in Equilibrium

 Eavrg = EC +

dE (E − EC ) Pe (E)

EC

2 = EC + √ π (kT )3/2



dE (E − EC )3/2 e−(E−EC )/kT .

EC

We change the integration variable to x = (E − EC )/kT , giving 2 Eavrg = EC + √ kT π



dx x 3/2 e−x .

0

√ The integral with respect to x is evaluated in Appendix A.4; its value is 3 π /4. Hence, the average electron energy is Eavrg = EC +

3kT . 2

The result for holes is similar. Hole energy probability distribution is Ph (E) = √

2 EV − E e−(EV −E)/kT for E < EV . 3/2 π (kT )

Note that hole energy here is measured from the electron’s perspective. The most probable and average energies of a hole are below the valence band edge by the amounts kT /2 and 3kT /2, respectively, see Fig. 5.2, left panel.

5.4 Density of States Effective Mass vs. Conductivity Effective Mass 5.4.1 Density of States Effective Mass It is convenient to combine the effective mass components into a single parameter, called the density of states (DOS) effective mass, m∗e,DOS and m∗h,DOS , in terms of which the electron and hole densities of states are given by gC (E) =

4π(2m∗e,DOS )3/2 4π(2m∗h,DOS )3/2 E − E , g (E) = EV − E C V h3 h3

and the effective densities of states are √ √ 4 2(π kT m∗e,DOS )3/2 4 2(π kT m∗h,DOS )3/2 NC = , NV = . h3 h3

5.4 Density of States Effective Mass vs. Conductivity Effective Mass

123

The electron and hole DOS effective masses are given by m∗e,DOS = νC (m∗e,x m∗e,y m∗e,z )1/3 = νC (m∗e,t )2/3 (m∗e,l )1/3 , 2/3  m∗h,DOS = (m∗hh )3/2 + (m∗hl )3/2 . 2/3

2/3

In the electron expression, we used the fact that two effective mass components are equal to the transverse effective mass and the third one equals the longitudinal effective mass, as discussed in Sect. 4.6.

5.4.2 Conductivity Effective Mass Electrons In silicon, which is an indirect-band gap semiconductors, the conduction band has six equivalent valleys, see Fig. 5.1a. To each constant-energy ellipsoid, we can attach its own three coordinate axes aligned along its principal axes. A particular crystallographic direction, say, [1 0 0], is now aligned with the x-axes of two valleys, the y-axes of two other valleys, and the z-axes of the remaining two valleys. From the point of view of electric properties of the material, we are interested in the reaction of the electrons in all six valleys to the electric field. Therefore, if an electric field E is applied, say, in the [1 0 0] direction, the acceleration of an electron should be averaged over all six valleys. This gives the average acceleration in the [1 0 0] direction a[1 0 0] = −eE[1 0 0]

1 3



1 1 1 + ∗ + ∗ ∗ me,x me,y me,z

 .

Same is true about the two other crystallographic directions, [0 1 0] and [0 0 1]. Therefore, on average, an electron responds to an electric field according to  ∗ a = −eE/m e,cond where the conductivity effective mass is defined by 1 m∗e,cond

1 = 3



1 1 1 + ∗ + ∗ ∗ me,x me,y me,z

 .

In other indirect-band gap semiconductors, such as germanium, there are eight constant-energy surfaces oriented along the 8 directions of the 1 1 1 family, see Fig. 5.1b. Nevertheless, the rule to obtain the average conductivity effective mass

124

5 Semiconductors in Equilibrium

turns out to be the same as in silicon. The conductivity effective mass of Si and Ge is, then, m∗e =

(m∗e,l )−1

3 + 2(m∗e,t )−1

because m∗e,x = m∗e,y = m∗e,t and m∗e,z = m∗e,l . In GaAs, a direct-band gap semiconductor, Fig. 5.1c, conductivity effective mass is the same as the density of states effective mass, m∗e,cond = m∗e,DOS = m∗e . Holes It is clear from the discussion of Sect. 5.2 that the fractions of heavy and light holes among all holes are (m∗hh )3/2 (m∗lh )3/2 p0,hh p0,lh = , = , ∗ ∗ ∗ p0 p0 (mhh )3/2 + (mlh )3/2 (mhh )3/2 + (m∗lh )3/2 where p0,hh and p0,lh are the equilibrium heavy and light hole concentrations, respectively. In the electric current measurements, one does not distinguish the currents produced by each hole type. Rather, one measures the total current produced by both heavy and light holes. Therefore, the accelerations of both holes due to an  viz., external electric field E, ahh =

eE eE , a  = , lh m∗hh m∗lh

should be averaged according to their contributions to the net hole concentrations. We thus obtain the average hole acceleration ah = ahh

p0,hh p0,lh eE + alh = ∗ , p0 p0 mh,cond

where the hole conductivity effective mass is m∗h,cond =

(m∗hh )3/2 + (m∗lh )3/2 . (m∗hh )1/2 + (m∗lh )1/2

5.4 Density of States Effective Mass vs. Conductivity Effective Mass

125

5.4.3 Thermal Velocity Before we proceed, it is instructive to address the question about the typical group velocity of an electron and a hole at a given temperature T . By “typical,” we mean that the kinetic energy of a particle equals the average thermal energy, Eavrg , which is above the conduction band edge or below the valence band edge by the amount 3kT /2, see Sect. 5.3. Let us consider the electrons first. For the quadratic energy–momentum relation (see Sect. 5.1), the group velocity components are vi =

∂E pi − pC,i = , i = x, y, z . ∂pi m∗e,i

The electron energy near the bottom of the conduction band can then be expressed in terms of the group velocity components as E( v ) = EC +

m∗e,i vi2 i

2

.

The thermal velocity is defined as the velocity of an electron whose energy exceeds the conduction band edge energy by 3kT /2. More precisely, its three components are given by the identities 2 m∗e,i ve|th,i

2

=

kT , 2

and the thermal velocity of an electron is then ve|th =

2 2 2 ve|th,x + ve|th,y + ve|th,z .

Combining the last two equations together and recalling the definition of the electron conductivity effective mass, we have  ve|th =

3kT . m∗e,cond

Similarly, we define the thermal velocities of the heavy and light holes as  vhh|th =

3kT , vlh|th = m∗hh



3kT . m∗lh

126

5 Semiconductors in Equilibrium

Their combination according to the relative contribution of the two kinds of holes to the total hole concentration gives vh|th

p0,hh p0,lh = vhh|th + vlh|th = p0 p0



3kT . m∗h,cond

In the rest of this book, we will omit the subscripts DOS and cond in the effective masses m∗e and m∗h . Which effective mass type is meant will be clear from the context of the discussion.

5.5 Intrinsic Semiconductors Intrinsic semiconductors are materials without impurities. In intrinsic semiconductors, each electron that gets promoted into the conduction band leaves behind exactly one hole in the valence band. Therefore, the concentrations of electrons and holes are exactly the same. To emphasize that the semiconductor is intrinsic, the carrier concentrations, as well as the Fermi energy, carry the subscript i. Using the results obtained in the previous section, we can figure out the concentration of charge carriers n0i = NC e−(EC −EF i )/kT , p0i = NV e(EV −EF i )/kT and the intrinsic Fermi energy, EF i . Namely, by setting n0i = p0i ≡ ni , we obtain an equation for EF i , which is easily solved: EF i =

m∗ kT NV 3kT EC + EV EC + EV + ln + ln h∗ . = 2 2 NC 2 4 me

In the second equality, we used the relation between the effective densities of states and the effective masses of the two charge carriers. At zero temperature, the intrinsic Fermi energy is located exactly in the middle of the band gap. As the temperature increases, it shifts toward the conduction band if NV > NC (m∗h > m∗e ) or toward the valence band if NV < NC (m∗h < m∗e ). This is similar to the result obtained in Sect. 3.7, which predicts that the Fermi level shifts toward the state of the lower degeneracy as the temperature goes up. Here, the role of the state degeneracy is played by the effective densities of states. Substitution of the result for EF i into the expression for the electron (or hole) concentration, we obtain the intrinsic carrier concentration:

5.6 Doping and Extrinsic Semiconductors

ni = n0i = p0i =

127

NC NV e−Eg /(2kT ) .

√ The prefactor NC NV is typically of the order of 1017 − 1020 cm−3 . In semiconductors with Eg of about 1 eV at room temperature, kT = 0.0259 eV, intrinsic concentration is of the order of 107 − 1011 cm−3 . On the other hand, in the materials even with a relatively small band gap value, say, Eg = 3 eV and NC ∼ NV ∼ 1019 cm−3 , the intrinsic carrier concentration is about 7 · 10−7 cm−3 . One would need a cube of about 1 m side length to have just one free electron in it. To have a measurable concentration of conduction electrons, such a material would need to be heated up above its melting temperature.

5.6 Doping and Extrinsic Semiconductors One can control the concentration of conduction electrons and holes by adding the so-called shallow impurities that can be easily turned into positive or negative ions. This procedure is called doping. Doping can be performed in several ways, such as ion implantation or diffusion. Donors are dopants that give electrons to the lattice. An example of donor doping is adding elements from column V of the periodic table to Si. Group-V elements, such as arsenic or phosphorus, have 5 valence electrons, whereas in Si lattice, bonds are formed by 4 valence electrons. This means that one of the valence electrons of a donor atom does not participate in chemical bonding with the neighboring Si atoms and is therefore relatively loosely attached to its host. It can be easily removed from the donor impurity and become a free conductance electron. It cannot go into the valence band because almost all Bloch states in the valence band are occupied. After losing its electron, the donor atom turns into a positively charged ion. Acceptors are dopants that catch the host lattice electrons, thereby creating holes in the lattice. An example of acceptor doping is adding elements from the third column of the periodic table to Si. Group-III elements, such as boron or gallium, have three valence electrons, i.e., they are one electron short of forming a covalent bond with the four neighboring Si atoms. To make up for this deficiency, an acceptor impurity may take an electron from the host lattice, thereby becoming a negatively charged ion and creating a hole in the material. That electron comes from the valence band because the conduction band has much fewer electrons than the valence band. In III–V semiconductors, e.g., GaAs, a group-IV element, such as Si or Ge, may act as either a donor or an acceptor impurity, depending on which lattice atoms it substitutes. This is called the amphoteric doping. The concentration and the type of the charge carriers in this case depend on the technological details of doping procedure. A compensated semiconductor is the one where both donor and acceptor impurities are present.

128

5 Semiconductors in Equilibrium

We will assume that the concentration of the impurity atoms is at least several orders of magnitude smaller than the concentration of the host atoms. That is, the doping is too weak to change the band structure of the material. Instead, the impurity atoms will introduce additional energy levels within the band gap. They will also change the Fermi energy by affecting the concentrations of electrons and holes in the material. Charge carriers whose concentration is the larger are called majority carriers; charge carriers with the lower concentration are called minority carriers. If the majority carriers are electrons, a semiconductor is said to be of n-type; if the majority carriers are holes, it is a p-type semiconductor: n-type: n0 > ni > p0 = n2i /n0 , p-type: p0 > ni > n0 = n2i /p0 .

5.7 Impurity Energy Levels Consider donors first. All but one valence electron of a donor impurity is taking part in chemical bonding, whereas the remaining electrons are relatively loosely bound to its host. We can view the neutral donor atom as a positive ion with an electron bound to it. The binding energy of the electron to the impurity ion can be found in exact same way as the electron energy levels in hydrogen (see Sect. 1.5), but with two modifications. First, the electron mass must be replaced by the conductivity effective mass, me → m∗e . Second, calculation of hydrogen energy spectrum was performed in vacuum, whereas a donor ion and an extra electron find themselves in a semiconductor medium. The two charges interact directly via own electric field. They also polarize the medium, and the polarized medium generates an additional electric field that affects the interaction between the two charges. This additional field weakens the electron–ion interaction as compared to the interaction in vacuum. This weakening can be accounted for by modifying the Coulomb interaction energy: U (r ) = −

ke e 2 .  r

The parameter  is called the dielectric constant, or the relative permittivity, of the medium. Its typical semiconductor value is of the order of 10, see Appendix A.3. 2 Hence, our second modification is to replace e2 → e . For an electron in the ground state of a hydrogen atom, ionization energy is defined as the energy necessary to promote the electron to vacuum:

5.7 Impurity Energy Levels

Ei = 1 Ry =

129

ke2 me e4 2h¯ 2

= 13.6 eV .

In a semiconductor, ionization energy is the energy necessary to promote an extra electron from the bound state with a donor atom to the bottom of the conduction band. In other words, it is the energy difference between the bottom of the conduction band and the donor energy level. By making the two replacements just described, we find the donor ionization energy in a semiconductor to be Edi = EC − Ed =

ke2 m∗e e4 2h¯ 2  2

=

m∗e /me Ry . 2

Here, Ed is the donor energy level, which lies below the conduction band edge by donor ionization energy, Ed = EC − Edi (Fig. 5.3). Given that, typically, m∗e /me varies from about 0.05 to 2 and  is between 10 and 20, we find that the typical value of donor ionization energy is of the order of 0.02 . . . 0.2 eV. For instance, for silicon, we obtain Edi = 0.0258 eV. This value is identical to the thermal energy at room temperature, kT = 0.0259 eV. Based on this estimate, we conclude that at room temperature, a large part of donor atoms is ionized. It is also instructive to determine the typical distance between the extra valence electron and the donor impurity ion. In hydrogen, the Bohr radius of the electron h¯ 2 orbit in the ground state (n = 1) is rB = k m 2 . With the replacements described e ee above, we find that in a semiconductor, the radius of the first Bohr orbit is rd =

 h¯ 2   = rB ∗ ≈ (0.53 Å) ∗ . me /me me /me ke m∗e e2

Numerically, the electron orbit radius in a semiconductor is about 10 nm, which is ca. 20 lattice constants. Fig. 5.3 Donor and acceptor levels relative to the conduction and valence band energies

130

5 Semiconductors in Equilibrium

With respect to the acceptor impurities, the results are quite similar. A neutral acceptor atom in the crystal lattice can be viewed as a bound state of a negatively charged ion and a hole orbiting around it. Therefore, the ionization energy Eai of an acceptor level Ea , that is, the energy necessary to remove this hole from the atom into the valence band, is Eai = Ea − EV =

ke2 m∗h e4 2h¯ 2  2

=

m∗h /me Ry , 2

and the radius of the hole orbit around an acceptor atom is ra =

 h¯ 2  = rB ∗ . mh /me ke m∗h e2

The calculations performed in this section are approximate. They neglect the tensorial character of the effective mass and do not distinguish between heavy and light holes. In addition, they do not account for the interaction between the extra electron (or hole) attached to the donor (or acceptor) ion with its other electrons. But, in spite of their crude nature, these calculations give the right order of magnitude of the ionization energy, which has to be measured experimentally. Some values of the ionization energies for Si, Ge, and GaAs are given in Appendix A.3.

5.8 Statistics of Donors and Acceptors Let Nd be the concentration of donor atoms, Nd0 the concentration of neutral donors, and Nd+ the concentration of donors that have given an electron to the lattice and became positive ions. Obviously, Nd = Nd0 + Nd+ . To find Nd+ and Nd0 , we use the grand canonical distribution derived in Sect. 3.4. A donor impurity can exist either as a positive ion or as a neutral atom with an extra electron orbiting around it. That electron has two possible spin orientations: either spin up (↑) or spin down (↓). It is reasonable to assume that when a donor captures an electron, that electron exists in the ground state and has the energy Ed ; in other words, we neglect the excited states of the electron. Denoting the number of extra electrons attached to the donor as n, we have three possibilities: n = 0; n = 1 and s =↑; n = 1 and s =↓, where s stands for spin. The probability for a donor to have n = 0 or 1 valence electrons is given by the grand canonical distribution with the chemical potential μ being identical to Fermi energy EF :

5.8 Statistics of Donors and Acceptors

Pn =

131

1 (EF −Ed )n/kT , Z = 1 + gd e(EF −Ed )n/kT , gd = 2 . e Z

The donor degeneracy factor gd = 2 in the expression for Z comes from two possible spin orientations. The probability for a donor atom to be ionized, i.e., not have an extra electron, corresponds to n = 0. This probability is just the fraction of ionized donors, P0 = Nd+ /Nd . Therefore, the concentration of ionized donors is Nd+ =

Nd . 1 + gd e(EF −Ed )/kT

The concentration of donors that are not ionized is Nd0 = Nd − Nd+ =

1+

Nd 1 (Ed −EF )/kT gd e

.

In view of the relations Ed = EC − Edi , n0 = NC e−(EC −EF )/kT , we can rewrite the exponential as e(EF −Ed )/kT = e(EF −EC +Edi )/kT =

n0 Edi /kT e , NC

giving Nd+ =

Nd , Nd0 = 1 + gd Nn0C eEdi /kT 1+

Nd 1 NC −Edi /kT gd n0 e

.

The expressions relating the concentration of ionized acceptor atoms, Na− , and neutral acceptor atoms, Na0 , to the total acceptor concentration, Na , can be obtained by making two modifications in the results for obtaining the donors. First, donor degeneracy factor must be replaced with the acceptor counterpart, gd → ga . Similar to the donor case, the acceptor ground state can be occupied with either a heavy or a light hole of spin 1/2 or −1/2. The total number of combinations of hole spin and “heaviness” is ga = 4 . Second, we should keep in mind that the hole energies are measured downward, with E (h) = −E + E, see Sect. 4.5. Then, the difference between donor level and Fermi energies must be replaced with

132

5 Semiconductors in Equilibrium (h)

Ed − EF → Ea(h) − EF = −Ea + EF , where Ea is the acceptor level energy. After making these replacements, we obtain the concentrations of negatively charged and neutral acceptor impurities: Na− =

1 + ga

Na (E e a −EF )/kT

, Na0 =

1+

Na 1 (EF −Ea )/kT ga e

.

In view of the relations Ea = EV + Eai , p0 = NV e−(EF −EV )/kT , we can rewrite these expressions in an equivalent form: Na− =

Na , Na0 = 1 + ga NpV0 eEai /kT 1+

Na 1 NV −Eai /kT ga p0 e

.

5.9 Mass Action Law The expressions for n0 and p0 in Sect. 5.2 contain one unknown parameter, the Fermi energy EF . But note that the product of the two concentrations does not depend on the Fermi energy. Indeed, multiplication of these results gives n0 p0 = NC NV e−(EC −EV )/kT = NC NV e−Eg /kT . In the second equality, we used the fact that EC − EV = Eg , the band gap energy. Doping of a semiconductor is an efficient way to control the concentrations of electrons and holes. The expressions for the equilibrium concentrations derived in Sect. 5.2 still hold in doped as well as intrinsic semiconductors, with the difference between the two being in the location of the Fermi energy EF . The electron and hole concentrations can be written in a different form, which does not involve the effective densities of states NC,V and the Fermi energy. For this, we add and subtract the intrinsic Fermi energy to the arguments in the exponential functions: n0 = NC e−(EC +EF i −EF i −EF )/kT , p0 = NV e(EV −EF i +EF i −EF )/kT . But NC e−(EC −EF i )/kT = NV e(EF i −EV )/kT = ni . We thus have n0 = ni e(EF −EF i )/kT , p0 = ni e(EF i −EF )/kT .

5.10 Charge Neutrality Equation

133

With these expressions, we can rewrite the mass action law as n0 p0 = n2i . The product of electron and hole concentrations is the intrinsic concentration squared for any level of doping. The mass action law tells us that the concentration of one type of carriers uniquely determines carrier concentration of the other type. Because this law is derived using Boltzmann approximation, it holds provided that Fermi energy is separated from the edges of the conduction and valence bands by at least a few kT .

5.10 Charge Neutrality Equation At a first glance, doping of a material with, say, donors should not affect the concentration of holes, p0 , which should remain equal the intrinsic concentration. Donor doping should increase the concentration of electrons, n0 , from the value ni to the value ni + Nd+ , where Nd+ is the concentration of ionized doping. This intuition is wrong. Donor doping provides electrons not only to the conduction band, but also fills the empty states in the valence band, whose energy is smaller than the donor level, EV < Ed . As a result, not only the electron concentration increases, but also hole concentration gets reduced due to donor doping. Same is true about acceptors. Acceptor impurities not only take electrons from the valence band, thereby creating more holes, but they also capture the conduction electrons, thereby decreasing their concentration. The relation between the equilibrium carrier concentrations n0 and p0 on the one hand and between the ionized impurity concentrations Nd+ and Na− on the other hand is slightly more complex. Because the material must be electrically neutral, the concentration of positive charges must be exactly balanced by the concentration of negative charges. The positive charges are mobile holes and immobile donor ions. The negative charges are mobile conduction electrons and immobile acceptor ions. We thus arrive at the charge neutrality equation: n0 + Na− = p0 + Nd+ , or, explicitly, ni e(EF −EF i )/kT +

1 + ga

Na (E e a −EF )/kT

= ni e(EF i −EF )/kT +

1 + gd

Nd (E e F −Ed )/kT

.

134

5 Semiconductors in Equilibrium

This equation contains only one unknown: the Fermi energy EF . Once it is found, electron and hole concentrations can be determined using the expressions obtained earlier, viz., n0 = ni e(EF −EF i )/kT and p0 = ni e(EF i −EF )/kT . An exact analytical solution of the charge neutrality equation can also be obtained, in principle, by introducing a variable x = e(EF −EF i )/kT , which then will have to be found from a fourth-degree equation of the form x 4 +ax 3 +bx 2 +cx+d = 0 with the coefficients a, b, c, and d being some combinations of the parameters Na , Nd , ni , gd , ga , e(EF i −Ed )/kT , and e(Ea −EF i )/kT . A general solution of a fourth-degree equation exists, but it is too complex to be of practical utility; hence, it will not be considered. Another option is to solve the charge neutrality equation numerically. But the most instructive approach is to focus on a few practically relevant special limit cases, referred to as ionization regimes, in which analytical approximations for the Fermi energy and the carrier concentrations can be obtained.

5.11 Ionization Regimes 5.11.1 Complete Ionization The simplest and the most important practically is the regime when the overwhelming majority of the impurity atoms are ionized. This regime is realized when the energy differences EF − Ea and Ed − EF exceed thermal energy, kT , by some reasonably large amount, say, by a factor of 3 or more. Then, e(Ea −EF )/kT and e(EF −Ed )/kT are both much smaller than 1, and we can approximate Nd+ =

Nd Na ≈ Nd , Na− = ≈ Na 1 + gd e(EF −Ed )/kT 1 + ga e(Ea −EF )/kT

by neglecting the exponentials in the denominators of both expressions. Our charge neutrality condition then reads n0 + Na = p0 + Nd . From the mass action law, we can express p0 =

n2i , n0

resulting in a quadratic equation for n0 : n0 + Na =

n2i + Nd ⇒ n20 + (Nd − Na )n0 − n2i = 0 . n0

5.11 Ionization Regimes

135

The solution of this equation is Nd − Na + n-type: n0 = 2

 

Nd − Na 2

2 + n2i , p0 =

n2i . n0

From the point of view of numerical accuracy, these expressions work the best when the doping is of n-type, Nd > Na . But consider what happens in the extreme opposite case Na  ni , Nd . Then, the terms ni and Nd are negligibly small relative to Na , leaving us with n0 ≈ − N2a + N2a = 0 and p0 = n2i /n0 → ∞. Hence, in the opposite case of p-type doping, Na > Nd , it is more advantageous to use a mathematically equivalent, but numerically a different set of formulae: Na − Nd + p-type: p0 = 2





Na − Nd 2

2 + n2i , n0 =

n2i . p0

In particular, when doping of just one type is present with the concentration much higher than intrinsic concentration, the following simple results hold: for Nd  ni  Na : n0 = Nd , p0 =

n2i ; Nd

for Na  ni  Nd : p0 = Na , n0 =

n2i . Na

The relations above are derived under the assumption that the energy differences between donor level and Fermi energy, as well as between Fermi energy and acceptor level, are large compared to kT . To check if these assumptions hold true, we need to find Fermi energy. For this, we can use the relations like n0 = NC e−(EC −EF )/kT = ni e(EF −EF i )/kT , and p0 = NV e(EV −EF )/kT = ni e(EF i −EF )/kT . From these, we find several equivalent expressions for Fermi energy in a doped semiconductor: EF = EC − kT ln

NC n0 NV p0 = EF i + kT ln = EV + kT ln = EF i − kT ln . n0 ni p0 ni

It follows from the second equality that for n-type doping, n0 > ni > p0 = n2i /n0 , Fermi energy lies above the intrinsic Fermi energy, EF > EF i . Increasing the donor concentration raises Fermi energy. Likewise, the last equality shows that for p-type doping, Fermi energy is below the intrinsic Fermi energy, EF < EF i , and increasing the acceptor concentration lowers Fermi energy. We can now establish the condition under which all impurities are ionized. Let us focus on the n-type semiconductor for definiteness. In order for almost all donors to be ionized, Nd+ ≈ Nd , we must have

136

5 Semiconductors in Equilibrium

gd e(EF −Ed )/kT  1 . Adding and subtracting the conduction band energy EC in the argument of the exponential and keeping in mind that EC − Ed = Edi , we rewrite this as gd e(EF −EC +EC −Ed )/kT = gd e(EF −EC )/kT eEdi /kT  1 . But e(EF −EC )/kT = n0 /NC ≈ Nd /NC under the complete ionization assumption and for Nd  ni . We conclude that the complete donor ionization assumption holds true, provided that gd eEdi /kT

Nd e−Edi /kT  1 ⇒ Nd  NC . NC gd

Similarly, for acceptor doping, the condition of complete acceptor ionization, Na− ≈ Na , is fulfilled if Na  NV

e−Eai /kT . ga

At the room temperature and at typical values of impurity ionization energies, the ratios e−Edi /kT /gd and e−Eai /kT are of the order of 0.1. Then, the full ionization of impurities is achieved if the impurity concentrations Nd,a do not exceed a few percent of the effective densities of states NC,V . As the temperature is lowered, however, the exponential terms in the numerator, e−Edi /kT and e−Eai /kT , quickly go to zero. Also the effective densities of states decrease on cooling as NC,V ∝ T 3/2 . This means that the complete ionization assumption breaks down at low temperatures.

5.11.2 Intrinsic Regime Intrinsic carrier concentration, ni (T ), increases with temperature, whereas the doping concentrations, Na and Nd , are temperature-independent. Hence, when the temperature exceeds a certain value, denoted as Ti , intrinsic concentration becomes much greater than the difference of the impurity concentrations, ni  |Nd − Na |. a Then, the difference Nd − Na can be neglected in the expression n0 = Nd −N + 2  2 Nd −Na + n2i , and charge carrier concentrations become approximately equal 2 the intrinsic concentration: n0 (T ) ≈ p0 (T ) ≈ ni (T ) =

NC (T )NV (T )e−Eg /(2kT ) .

5.11 Ionization Regimes

137

It increases with temperature. Let us now establish the temperature Ti , at which the complete ionization regime ends and the intrinsic regime begins. At this temperature, intrinsic concentration should be comparable to the magnitude of the difference Nd −Na , which we assume to be non-zero:

ni (Ti ) = |Nd − Na | , or NC (Ti )NV (Ti )e−Eg /(2kTi ) = |Nd − Na | . Rearranging the terms in this equation, we find kTi =

ln

Eg NC (Ti )NV (Ti ) (Nd −Na )2

.

Recalling that NC,V (T ) = NC,V (T0 )(T /T0 )3/2 , where the reference temperature is usually taken to be T0 = 300 K, we finally have an equation, from which Ti can be found: \$

Ti = ln

Eg /k NC (T0 )NV (T0 ) (Nd −Na )2

 3 % . Ti T0

One can solve this equation for Ti analytically using the so-called Lambert W function.2 Alternatively, an iterative solution can be performed, namely, starting with Ti = T0 and plugging in this value into the right-hand side of the last equation to obtain a better estimate for Ti , which is again plugged in into the right-hand side to get a new Ti . This procedure is repeated until the results converge. In practice, only two or three iterations are sufficient to find Ti to a good accuracy. For the typical semiconductors and typical doping levels, the intrinsic regime begins at Ti exceeding the room temperature by a few hundred Kelvins.

5.11.3 Carrier Concentration in a Semiconductor with One Type of Doping at Not Too High Temperatures Consider the case when only one type of doping impurities—assume for definiteness donors—is present. Let us focus on the practically interesting case when the temperature is small enough for the intrinsic concentration to be negligible in comparison to the concentration of the ionized donors: Na = 0 , Nd+ (T )  ni (T ) at T < Ti .

2 Lambert’s

function W (x) is the solution of W (x)eW (x) = x.

138

5 Semiconductors in Equilibrium

We do not assume complete ionization. In view of the above inequality, the concentration of the conduction electrons is given by n0 = Nd+ =

1 + gd

Nd (E e F −Ed )/kT

to a very good accuracy. Because n0 = NC e(EF −EC )/kT , we obtain an equation, from which Fermi energy can be found: NC e(EF −EC )/kT =

1 + gd

Nd (E e F −Ed )/kT

.

Denoting x = e(EF −EC )/kT , we rewrite our equation in terms of this new variable: NC x = 1+xg NedEdi /kT . d Multiplying both sides by the denominator of the right-hand side, we obtain a quadratic equation for x: NC x(1 + xgd eEdi /kT ) = Nd . Its solution reads  x=

e−2Edi /kT Nd −E /kT e−Edi /kT di + e − . gd NC 2gd 4gd2

By the very definition of x, Fermi energy and electron concentration can be immediately expressed in terms of x as EF = EC + kT ln x , n0 = NC x , p0 =

n2i . NC x

Here, the hole concentration follows from the mass action law. The case when only acceptor-type impurities are present with Na (T )  ni (T ), Nd = 0 can be treated analogously and is left for the reader as an exercise.

5.11.4 Electron Freeze-Out Regime At the thermal energies kT below the impurity ionization energy, only a fraction of the impurity atoms are ionized, and this fraction decreases to zero as the temperature is decreased. This ionization regime is called the freeze-out regime.

5.11 Ionization Regimes

139

Let us consider for simplicity the case when only donor impurities are present. Then, we can use the formula for n0 obtained in the previous section. In that formula, further approximations can be made. First, we note that under the square root, we have e−2Edi /kT Nd −Edi /kT  e at kT  Edi . 2 gd NC 4gd This is so, because the ratio Edi /kT  1 is a large number, implying that e−Edi /kT  1, and hence e−2Edi /kT  e−Edi /kT . As for the prefactor Nd /(gd NC ), it is also large in view of the fact that NC (T ) ∝ T 3/2 decreases on cooling, and hence, Nd /(2NC (T )) increases. The expression for electron concentration then simplifies to  n0 (T ) = NC (T )

Nd e−Edi /kT e−Edi /(2kT ) − gd NC (T ) 2gd

 .

By the same reasoning, we can neglect the second term in this expression relative to the first one and obtain  Nd NC (T ) −Edi /(2kT ) n0 (T ) = e . gd The Fermi energy in the freeze-out regime is given by EF = EC −

kT Nd Edi + ln 2 2 gd NC

as can be obtained from the expression n0 = NC e(EF −EC )/kT and the approximate formula for n0 just obtained. Note that in the limit of zero temperature, Fermi energy goes to the limit EF → EC −

EC + Ed Edi = as T → 0 2 2

in full agreement with our observation made earlier that at zero temperature, Fermi energy is just in between the highest occupied state (donor level) and the lowest unoccupied state (conduction band edge), see Sect. 3.7. We can establish the temperature Tf that separates the freeze-out regime from the complete ionization regime. At this temperature, the two contributions under the square root in the expression for n0 from the previous section must be equal: e−2Edi /kTf Nd e−Edi /kTf . = gd NC (Tf ) 4gd2

140

5 Semiconductors in Equilibrium

Taking the natural logarithm of both sides and rearranging the terms, we obtain kTf =

ln

Edi NC (Tf ) 4gd Nd

with  NC (Tf ) = NC (T0 )

Tf T0

3/2 ,

T0 = 300 K being the standard reference temperature. Thus \$

Tf = ln

Edi /k  3/2 % .

NC (T0 ) 4gd Nd

Tf T0

This equation can be solved analytically using Lambert’s W -function or iteratively by first setting, e.g., Tf = T0 (or any other reasonable first guess, e.g., Tf = 0.1Edi /k), and then obtaining the next improved result for Tf according to its righthand side until convergence is reached.

5.12 Numerical Determination of Fermi Energy and Carrier Concentrations One possible way to find EF , n0 , and p0 from the charge neutrality equation, n0 + Na− = p0 + Nd+ , and mass action law, p0 = n2i /n0 , is as follows. Assume for definiteness that the semiconductor is of n-type. Then, by applying this same procedure used to treat the complete ionization regime, we find the electron and hole concentrations    + + −  N − Na− 2 Nd − Na n2 d + n0 = + n2i , p0 = i 2 2 n0 and the Fermi energy ⎛ + ⎜ Nd

EF = EC + kT ln ⎝

− Na−

2NC

⎞    + 2  N − Na− 2 n ⎟ d + + i2 ⎠ . 2NC NC

The expressions for Nd+ and Na− have been established earlier in Sect. 5.8.

5.12 Numerical Determination of Fermi Energy and Carrier Concentrations

141

The right-hand side of the last equation contains the ionized impurity concentrations, which themselves depend on the Fermi energy. This equation can be solved iteratively. Starting with some initial trial value of Fermi energy, one can determine Nd+ and Na− corresponding to this initial value of EF ; upon substitution of the ionized impurity concentrations so obtained into the last equation, one finds a new, more accurate estimate for EF , which is again used to find better estimates for Nd+ and Na− . This procedure can be repeated many times until the desired accuracy is achieved. In practice, the number of iterations is of the order of 10. For a p-type semiconductor, the same procedure can be performed, but with the interchanged n0 ↔ p0 and Nd+ ↔ Na− . Shown in Fig. 5.4 are the results of numerical and analytical calculations of the Fermi energy and carrier concentrations in a hypothetical semiconductor with the parameters indicated in the figure caption. For these parameters, the intrinsic temperature can be found to be Ti = 562 K, and the freeze-out temperature is Tf = 112 K. These two temperatures are marked by vertical lines in the figure. The agreement between the analytical and numerical results at 0 < T < Ti is smaller than the line thickness.

Fig. 5.4 The results of numerical calculations of the Fermi energy and electron and hole equilibrium concentrations in a hypothetical n-type semiconductor with the band gap Eg = 1 eV, the effective densities of states at T0 = 300 K taken to be NC (T0 ) = NV (T0 ) = 1019 cm−3 , donor concentration Nd = 1015 cm−3 , donor ionization energy Edi = 0.05 eV and degeneracy factor gd = 2, and no acceptors, Na = 0

142

5 Semiconductors in Equilibrium

It is seen that Fermi energy, measured relative to the top of the valence band, monotonically decreases with temperature and finally saturates at T > Ti at the level of 0.5 eV, i.e., in the middle of the band gap. As for the charge carrier concentrations, three regimes can be distinguished. (1) At low temperatures T < 100 K, thermal energy is insufficient to ionize impurity atoms, and let alone to promote electrons from the valence to the conduction band. As a result, the freeze-out of conduction electrons occurs, where both electron and hole concentrations go to zero on cooling. (2) In the temperature range between about 100 K and 500 K, the majority electron concentration has a plateau at the level n0 = Nd = 1015 cm−3  ni , whereas the minority hole concentration is much smaller than this value. This regime corresponds to complete ionization of donors. (3) At even higher temperatures, T > 500 K, intrinsic carrier concentration becomes comparable to and eventually starts to dominate over Nd on heating. In this intrinsic regime, characterized by the inequality ni (T )  Nd , we have n0 ≈ p0 ≈ ni , independent of the doping level.

5.13 Problems 5.13.1 Solved Problems Problem 1 The effective density of states has the dimension of inverse length cubed. Find a combination of the density of states effective mass m∗e,h , thermal energy kT , and Planck’s constant h that has the same dimension as the effective density of states, and compare it with the result obtained in Sect. 5.2. Problem 2 The density of states in the conduction band is gC (E) = 4π(2m∗e )3/2 √ E − EC . The total number of states (per unit volume) in the h3 conduction band in an energy interval between EC and EC + E is ZC (E) =  EC +E dE gC (E). Find the number of conduction band states in a unit volume EC with energies less than EC + kT . Compare it to the effective density of states in the conduction band by finding its ratio to NC =

2(2π m∗e kT )3/2 . h3

Problem 3 The temperature dependence of the band gap in Si is given by Eg = −4

eV/K 2 1.166 eV − 4.77·10 T . At T = 300 K, the intrinsic carrier concentration in Si T +636 K 10 −3 is 10 cm . Find ni at 400 K.

Problem 4 The DOS effective mass of holes in a hypothetical intrinsic semiconductor is ten times larger than that of the electrons. The band gap is 1 eV, independent of temperature. At T = 300 K, the intrinsic concentration is 109 cm−3 .

5.13 Problems

143

(a) Find the difference EF i − EV at 300 K. (b) Find the effective densities of states NC and NV at 300 K. (c) At what temperature is Fermi energy 0.6 Eg above the valence band edge? Problem 5 A Si sample is doped with boron (ionization energy Eai = 45 meV, degeneracy = 4) at Na = 1016 cm−3 . Take into account the temperature dependence of the band gap. The semiconductor parameters needed to solve the problem can be found in Appendix A.3. Problem 6 A p-type semiconductor has the band gap Eg = 0.8 eV, the electron and hole effective masses are the same, and ni = 2 · 109 cm−3 . The temperature is T = 300 K and Nd = 0. At what concentration of acceptors will Fermi energy be above the valence band edge by E = 0.2 eV? Problem 7 A compensated semiconductor with the intrinsic carrier density ni (300 K) = 1010 cm−3 and Eg = 0.9 eV is doped with Nd = 1016 cm−3 donors and Na = 1012 cm−3 acceptors. Determine Fermi energy relative to the intrinsic Fermi energy at T = 200 K in the complete ionization limit.

5.13.2 Practice Problems Problem 1 Derive the hole concentration p0 and the respective effective density of states NV following the same steps as for electrons in Sect. 5.2. Problem 2 At T = 300 K, the effective density of electron states in a semiconductor is 1020 cm−3 . What is the effective density of states at 200 K and at 400 K? Problem 3 Estimate electron concentration (= hole concentration) in an intrinsic semiconductor with Eg = 0.7 eV and in a dielectric with Eg = 7 eV at 300 K. Take a reasonable value for NC and NV , e.g., 1019 cm−3 . Problem 4 The concentration of holes in a p-type semiconductor (no donors) exceeds the concentration of electrons by 25 times. Find the ratio of the concentration of ionized acceptors to the intrinsic concentration. Problem 5 A Si sample is doped with a donor impurity at Nd = 1017 cm−3 . At the temperature T = 30 K, electron concentration in this sample was measured to be n0 = 1012 cm−3 . Find the impurity ionization energy Edi . Hint: n0 = Nd+  ni  p0 at 30 K. Problem 6 A compensated semiconductor with the band gap of 0.8 eV is doped with equal concentrations of donors and acceptors. The respective ionization

144

5 Semiconductors in Equilibrium

energies are Edi = 0.05 eV and Eai = 0.02 eV. Find the Fermi energy relative to the top of the valence band, EF − EV , in this material at absolute zero temperature.

5.13.3 Solutions Problem 1 For definiteness, let us focus on the conduction electrons; the discussion of holes is similar. To express NC in terms of m∗e and kT , we consider the units in which these parameters are measured (we use SI units in this problem): [NC ] = m−3 , [m∗e ] = kg , [kT ] = J =

kg · m2 . s2

We may also need Planck’s constant, measured in [h] = J · s =

kg · m2 . s

We express NC as a product NC ∝ (m∗e )α (kT )β hγ with unknown α, β, and γ and a non-dimensional prefactor. The dimension of this product is  [NC ] = kgα ·

kg · m2 s2

β  γ kg · m2 · = kgα+β+γ m2(β+γ ) s−(2β+γ ) . s

It must be equal to m−3 . Hence, we must have α + β + γ = 0 , 2(β + γ ) = −3 , 2β + γ = 0 . Subtracting the third equation from the second, we get γ = −3. Substitution of this value of γ back into the second equation gives β = 3/2. Finally, substitution of these values of β and γ into the first equation gives α = 3/2. Hence, up to a non-dimensional constant NC ∝

(m∗e kT )3/2 . h3

Problem 2 Substitution of the formula for gC (E) into the definition of ZC (E) gives

5.13 Problems

145

ZC (E) =

4π(2m∗e )3/2 h3



EC +E

dE EC

8π(2m∗e )3/2 E − EC = E 3/2 . 3h3

For E = kT , we have ZC (kT ) =

8π(2m∗e kT )3/2 . 3h3

The ratio of this parameter to NC has the value ZC (kT ) 8π · 23/2 /3 4 = = √ = 0.752 . NC 2(2π )3/2 3 π This is close to 1. This result confirms that the effective density of states can be interpreted as the concentration of states in the conduction band whose energies are higher than EC by approximately one thermal energy kT . Problem 3 The intrinsic carrier concentration is given by ni (T ) =

NC (T )NV (T ) e−Eg (T )/(2kT ) ,

where the effective densities of states in the conduction and valence bands are proportional to T 3/2 . We need to recalculate the square root of their product, √ NC (T )NV (T ) ∝ T 3/2 from the reference temperature T0 = 300 K to a different temperature T :

NC (T )NV (T ) =



T NC (T0 )NV (T0 ) T0

3/2 .

Likewise, we need to recalculate the exponential in the expression for ni : e−Eg (T )/(2kT ) = e−Eg (T0 )/(2kT0 ) eEg (T0 )/(2kT0 )−Eg (T )/(2kT ) . Multiplying these two expressions together, we find  ni (T ) = ni (T0 )

T T0

3/2 eEg (T0 )/(2kT0 )−Eg (T )/(2kT ) .

It remains to plug in the numbers. We start with the band gap at T0 = 300 K and T = 400 K: Eg (300 K) = 1.166 −

4.77 · 10−4 3002 = 1.120 eV , 300 + 636

146

5 Semiconductors in Equilibrium

Eg (400 K) = 1.166 −

4.77 · 10−4 4002 = 1.092 eV . 400 + 636

Next, we find the thermal energy at T = 400 K, given that kT0 = 0.02585 eV: kT = 0.02585 ·

400 = 0.03447 eV . 300

Finally, we determine the intrinsic concentration at 400 K: ni (400 K) = 1010 (400/300)3/2 e1.120/(2·0.02585)−1.092/(2·0.03447) = 5.21 · 1012 cm−3 .

Problem 4 (a) Intrinsic Fermi energy happens to be exactly in the middle of the band gap only if the electron and hole effective masses are the same; this is not the case in most semiconductors. When the effective masses are different, we have a general expression EF i =

m∗ EC + EV 3kT + ln h∗ , 2 4 me

from which it follows that EF i − EV =

m∗ Eg 3kT + ln h∗ . 2 4 me

Numerically, EF i − EV = 0.5 + 0.75 · 0.02585 · ln(10) = 0.545 eV . (b) We know that the effective density of states is proportional to the effective mass of the charge carriers in the respective band raised to the power 3/2: NC ∝ (m∗e )3/2 , NV ∝ (m∗v )3/2 . Knowing that holes are 10 times as heavy as the electrons, we can find the ratio of the effective densities of states as NC = NV



m∗e m∗h

3/2 .

On the other hand, the expression for ni contains the product NC NV : n2i = NC NV e−Eg /kT ⇒ NC NV = n2i eEg /kT .

5.13 Problems

147

Multiplying the last two equations together, we obtain the effective density of states in the conduction band:  NC2 =

m∗e m∗h

3/2

 n2i eEg /kT ⇒ NC =

m∗e m∗h

3/4 n2i eEg /(2kT ) .

The expression for NV is obtained by interchanging electron and hole effective masses:  NV =

m∗h m∗e

3/4 n2i eEg /(2kT ) .

Numerically, NC =

109 · e0.5/0.02585 = 4.47 · 1016 cm−3 , 103/4

NV = 103/4 · 109 · e0.5/0.02585 = 1.41 · 1018 cm−3 . (c) In the second formula from the solution to part (a), we set EF i − EV = cEg , where c = 0.6: cEg =

m∗ Eg 3kT + ln h∗ . 2 4 me

Solving this for kT , we find the thermal energy corresponding to the temperature at which the Fermi level is higher than the valence band energy by a desired amount: kT =

4 c − 1/2 Eg . m∗ 3 ln h∗ me

Numerically, this is kT =

0.1 4 · (1 eV) · = 0.05791 eV . 3 ln(10)

To convert thermal energy into temperature, we divide it by 0.02585 eV and multiply by 300 K: T =

0.05791 · 300 = 672 K . 0.02585

148

5 Semiconductors in Equilibrium

Problem 5 The concentration of ionized acceptors is given by a general formula Na− =

1 + ga

Na (E e a −EF )/kT

,

which can be transformed into x=

Na− 1 1 = = . (E −E +E −E )/kT E /kT Na 1 + ga e a V V F 1 + ga e ai e(EV −EF )/kT

In the second exponential in the denominator, we recognize the concentration of holes: p0 = NV e(EV −EF )/kT . So, we can write e(EV −EF )/kT =

p0 NV

x=

, giving

1 1 + ga eEai /kT

p0 NV

.

On the other hand, N− p0 = a + 2





Na− 2

2 + n2i .

It is reasonable to assume that at low temperatures, the concentration of ionized acceptors greatly exceeds the intrinsic concentration, Na−  ni , allowing us to approximate p0 = Na− = xNa to a good accuracy. Then, substitution of this expression into the expression for x just obtained gives x=

1 1 + ga NNVa eEai /kT x

=

Na Eai /kT 1 , A = ga e . 1 + Ax NV

This is a quadratic equation for the fraction of ionized acceptors, x: 1 Ax + x − 1 = 0 ⇒ x = − + 2A 2



1 1 + . 2 A 4A

The possibility of a negative sign in front of the square root has been discarded because x must be positive. It remains to plug in the numbers.

5.13 Problems

149

(a) At T = 200 K, kT = 0.02585 · 200/300 = 0.01723 eV. The effective density of states in the valence band at this temperature is 

200 NV (200 K) = NV (300 K) 300

3/2

= 1.116 · 1019 cm−3 .

This gives the parameter A to be 1016 · e0.045/0.01723 = 0.04883 . 1.116 · 1019

A=4·

Using this value, we find x = 0.955, i.e., 95.5% of acceptors are ionized. (b) At T = 50 K, kT = 0.02585 · 50/300 = 0.004308 eV. The effective density of states in the valence band at this temperature is  NV (50 K) = NV (300 K)

50 300

3/2

= 1.395 · 1018 cm−3 .

This gives the parameter A to be A=4·

1016 · e0.045/0.004308 = 986.3 . 1.395 · 1018

Using this value, we find x = 0.0313, i.e., 3.13% of acceptors are ionized. Problem 6 Since m∗e = m∗h , the intrinsic Fermi level lies exactly in the middle of the band gap, i.e., EF i − EV =

Eg = 0.4 eV . 2

We wish to have EF − EV = 0.2 eV , which implies that EF i − EF = 0.2 eV . We can figure out the concentration of holes at this value of the Fermi energy: p0 = NV e(EV −EF )/kT = NV e(EV −EF i +EF i −EF )/kT = ni e(EF i −EF )/kT , where we used the one of the previously obtained expressions for the intrinsic concentration, ni = NV e(EV −EF i )/kT . Numerically,

150

5 Semiconductors in Equilibrium

p0 = 2 · 109 · e0.2/0.02585 = 4.583 · 1012 cm−3 . This value is much bigger than ni . From this, we conclude that to a good accuracy p0 = Na− = Na , as practically all acceptors are ionized at 300 K. Hence, Na = 4.58 · 1012 cm−3 . Problem 7 First, we find the intrinsic concentration at T = 200 K from its value at T0 = 300 K:  ni (T ) = ni (T0 )

T T0

3/2

Eg

e 2kT0

E

g − 2kT

 = ni (T0 )

T T0

3/2

Eg

e 2kT0

 T 1− T0

.

Numerically,  ni (200 K) = 1010 ·

200 300

3/2

0.9

e 2·0.02585



300 1− 200

= 9.031 · 105 cm−3 .

This number is much smaller than the difference Nd − Na . Hence, in this n-type semiconductor, the concentration of electrons is to a very good accuracy n0 = Nd − Na = 9.999 · 1015 cm−3 . Electron concentration is related to the intrinsic concentration by n0 = NC e−(EC −EF )/kT = NC e−(EC −EF i +EF i −EF )/kT = ni e(EF −EF i )/kT , where we used one of the previously obtained expressions for the intrinsic concentration, ni = NC e−(EC −EF i )/kT . We obtain EF − EF i = kT ln

n0 . ni

Numerically, EF − EF i = 0.02585 ·

9.999 · 1015 200 · ln = 0.399 eV . 300 9.031 · 105

Chapter 6

Carrier Concentration and Electric Potential

6.1 Electron and Hole Concentrations in a Non-uniform Electric Potential If the electric potential φ(r ) inside a semiconductor is non-uniform, the charge carrier concentrations will differ from the values n0 and p0 obtained in the previous chapter. The reason is simple: the mobile charge carriers get redistributed in the  r ) produced by the spatial material in response to the electric field E = −∇φ( inhomogeneity of the potential. An overall motion of the charge carriers means that they are not in thermal equilibrium. In this chapter, we assume that the semiconductor is not a part of a closed circuit; hence, the electric current due to a redistribution of electrons and holes eventually stops, and the system comes to a new equilibrium state. Electrons tend to migrate from the regions with the lower electric potential to the regions with the higher potential. Likewise, holes migrate from the high-potential to the low-potential regions. As the charge carriers move from one region to another, they leave behind the ionized impurities. As a result, an internal disbalance of positive and negative charges is created, which itself produces an internal electric field. The internal field counteracts the external field, so that the total electric field in the material eventually becomes zero and further migration of the free charge carriers stops. This reasoning shows that the electric potential inside the semiconductor and the distribution of charge carriers affect each other, which makes finding the new equilibrium state a non-trivial task. We begin by establishing the effect of a non-uniform potential φ(r ) on the carrier concentrations. We mentally divide the material into small volume elements V such that the electric potential in each element is approximately constant. The local concentration of electrons and holes is defined as the ratio of their average number in each element to the volume V of that element.

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_6

151

152

6 Carrier Concentration and Electric Potential

The energy of a charged particle due to the presence of an electric potential φ(r ) is qφ(r ). That is, the energy of an electron near the top of the conduction band changes from EC to EC − eφ(r ), and the energy of a hole (from the holes’ (h) (h) perspective) near the top of the valence band changes from EV to EV + eφ(r ). We can repeat the derivation from Sect. 5.2 to obtain the local concentrations of electrons and holes at a point r with the result n0 (r ) = NC e−(EC −EF −eφ(r ))/kT , p0 (r ) = n2i /n0 (r ) = NV e(EV −EF −eφ(r ))/kT . It should be borne in mind that the electric potential is defined up to an arbitrary constant. If the potential is uniform, φ(r ) = const, this constant should be set to zero, as the carrier concentrations should be given by the expressions from Sect. 5.2 in this case. It is expedient to cast the expressions for n0 (r ) and p0 (r ) into a form that is independent of the choice of that constant. Namely, the electron and hole concentrations at a point r are related to their values at some reference point r0 by n0 (r ) = n0 (r0 ) e(φ(r )−φ(r0 ))/Vth , p0 (r ) = p0 (r0 ) e−(φ(r )−φ(r0 ))/Vth . Here, in order to avoid using the letter e in the meaning of the elementary charge and the base of an exponential (e.g., writing eeφ(r )/kT is a bit clumsy), we have introduced the thermal voltage Vth =

kT . e

At the room temperature T = 300 K, it has the value Vth = 0.02585 V.

6.2 Poisson’s Equation A non-uniform distribution of electric charges inside a semiconductor due to, e.g., a non-uniform doping profile, results in an onset of an internal electric field, E(r ),  r ). The electric field depends related to an electrostatic potential as E(r ) = −∇φ( on the distribution of the charges inside the material. Poisson’s equation relates the electric potential to charge density. It is the familiar Gauss law expressed in the form of a differential equation. For the sake of simplicity, we focus here on a special case when the electric charge density depends on the x-coordinate only and is uniform in the yz-plane: ρ = ρ(x). Consider a thin slab of thickness x and base area A perpendicular to the x-axis, see Fig. 6.1. By Gauss’ theorem, the electric field flux through its surface equals the charge inside the slab divided by the product 0 , where  is the relative dielectric constant of the material, 0 = 8.854 · 10−14 F/m is the permittivity of

6.2 Poisson’s Equation

153

Fig. 6.1 Gaussian surface inside a semiconductor is a cylinder; the electric field flux through it arises due to a non-uniform distribution of electric charge in the x-direction

vacuum, and  is the relative permittivity of the material: 

d A · E =

A

 x+x x

dx  ρ(x  ) . 0 

As the electric field has only the x-component, the flux through the slab is given by E(x + x)A − E(x)A. For very small x, we can neglect the x-dependence of the electric charge density inside the slab; hence, the total charge contained inside the slab is ρ(x)Ax. We thus have E(x + x)A − E(x)A =

ρ(x)A x . 0 

Dividing both sides by the slab volume A x and taking the limit x → 0, we have dE(x) ρ(x) E(x + x) − E(x) = = . x→0 x dx 0  lim

Because the electrostatic potential is non-uniform in the x-direction only, we have E(x) = −

dφ(x) . dx

Hence, we arrive at Poisson’s equation: d 2φ ρ(x) . =− 2 0  dx In a semiconductor, the charge density is a sum of the positive charge densities of holes and ionized donors and the negative charge densities of electrons and ionized acceptors: ρ(x) = e(p0 (x) + Nd+ (x) − n0 (x) − Na− (x)) . For the sake of generality, we allowed the doping concentrations to depend on the coordinate x. In equilibrium, the local concentrations of carriers depend on the

154

6 Carrier Concentration and Electric Potential

potential, as established in Sect. 6.1. Because of that, Poisson’s equation is nonlinear: d 2φ e  + −φ(x)/Vth φ(x)/Vth − p = − (x )e + N (x) − n (x )e − N (x) , 0 0 0 0 a d 0  dx 2 where x0 is a reference point, where the potential has the value φ(x0 ) = 0. Its exact solution in a one-dimensional geometry will be presented in the end of this chapter. But also approximate solutions can be obtained when the surface potential is small compared to thermal voltage and when it is large, but not too high. These approximations are discussed below.

6.3 Approximate Solution of Poisson’s Equation 6.3.1 Problem Formulation Consider a thick semiconductor slab with a flat boundary in the yz-plane extending in the positive x-direction. The semiconductor finds itself in thermal equilibrium at the temperature sufficiently high for complete ionization of all doping impurities. For definiteness, we assume that the semiconductor is of p-type, as in Fig. 6.2a, with all acceptors ionized and no donors: Na− ≈ Na  ni , Nd = 0 . The behavior of the electrostatic potential is described by Poisson’s equation d 2 φ(x) e =− (p0 (x) − n0 (x) − Na ) 2 0  dx with p0 (x) = Na e−φ(x)/Vth , n0 (x) =

n2 n2i = i eφ(x)/Vth . p0 (x) Na

The electrostatic potential on the surface has a fixed value φS , and very far away from the surface, it is zero. The value of the surface potential is maintained by an external voltage applied to a metal electrode. In order to prevent the current from flowing, that electrode is separated from the semiconductor by a thin insulating layer, see Fig. 6.2. Note that due to the presence of this insulating layer and due to the fact that the metal and the semiconductor have different work functions, the voltage applied to the metal electrode differs from the value φS . In this chapter, we will simply assume φS to be given.

6.3 Approximate Solution of Poisson’s Equation

155

Fig. 6.2 The development of a depletion layer near when (a) a positive bias is applied to the surface of a p-type semiconductor and (b) a negative bias is applied to the surface of an n-type semiconductor

We wish to find out how the electrostatic potential φ(x) decreases from the initial value φ(0) = φS to the value far from the surface φ(∞) = 0 . Furthermore, because there is no electric field at infinity, we have a further condition dφ

=0.

dx x=∞

6.3.2 Debye Screening First, let us focus on the situation when the surface potential is small compared to the thermal voltage. Then, we can approximate   φ(x) p0 (x) = Na e−φ(x)/Vth ≈ Na 1 − Vth  n2 and neglect the electron concentration n0 (x) ≈ Nia 1 + φ(x) relative to the hole Vth and acceptor concentrations. This allows us to linearize Poisson’s equation with respect to φ(x)/Vth as d 2 φ(x) eNa φ(x) = φ(x) = 2 , 2 0 Vth dx λD

156

6 Carrier Concentration and Electric Potential

where we introduced the so-called Debye length  λD =

0 Vth . eNa

The general solution of the linearized Poisson equation reads φ(x) = Ae−x/λD + Bex/λD . Due to the boundary condition φ(∞) = 0, we have to set B to zero. Next, considering the boundary condition at x = 0, we find that the parameter A is, then, the surface potential φS , yielding φ(x) = φS e−x/λD . We see that the free charge carriers (holes in this case) redistribute themselves in the material in response to the external potential in such a way that the electric potential in the material quickly goes to zero. This phenomenon is called screening.

6.3.3 Depletion Approximation A simple approximate expression for the potential φ(x) in the semiconductor can be obtained if the surface potential φS has the same sign as the majority charge carriers, i.e., φS > 0 for a p-type semiconductor (Fig. 6.2a) and φS < 0 for an n-type semiconductor (Fig. 6.2b). In this case, the majority carriers are pushed away from the surface. On the other hand, we assume that the magnitude of the surface potential is not large enough to attract a considerable amount of the minority carriers. As a result, a region is formed near the surface, where neither the majority nor the minority carriers compensate the uniform charge of the dopant ions. The charge density inside this region is close to the charge density of the dopants. It is negative in a p-semiconductor and positive in an n-semiconductor. This region is called the depletion region or the space-charge region (SCR). Within the depletion approximation, the boundary of the SCR is viewed as sharp. That is, the true (but unknown) distribution of the electric charge density is approximated by a box distribution:  ρ(x) ≈

−eNa

for x ≤ xd ,

0

for x > xd ,

where xd is the yet unknown width of the depletion region, see Fig. 6.3. With this approximation for the charge density, Poisson’s equation

6.3 Approximate Solution of Poisson’s Equation

157

Fig. 6.3 (a) Schematic illustration of the hole concentration vs. the coordinate x (solid lines) and the depletion approximation for p0 (x) (shaded area). (b) Schematic illustration of the charge density vs. coordinate (solid line) and its depletion approximation (shaded area)

 eNa d 2 φ(x) 0  = dx 2 0

for x ≤ xd for x > xd

is easy to solve both inside and outside the SCR. It should be borne in mind that the solutions of Poisson’s equation obtained in the two regions, x ≤ xd and x > xd , must coincide at the boundary of the SCR, x = xd . Integrating Poisson’s equation once with respect to x, we have  eNa (x − xd ) dφ(x) = 0  dx 0

for x ≤ xd for x > xd

.

It is 0 at x > xd because the electric field −dφ/dx must vanish at x → ∞. The integration constant in the expression for dφ/dx for x ≤ xd is chosen so as to make sure that the derivative dφ/dx is continuous at x = xd . One more integration gives  φ(x) =

eNa 20  (x

0

− xd )2

for x ≤ xd , for x > xd .

Note that φ(x) is continuous at the SCR boundary x = xd . We now can determine the width xd of the depletion region from the surface value of the potential: eNa xd2 φ(0) = = φS ⇒ xd = 20 

 20  φS . eNa

This completes the derivation. Keeping in mind that the electric field induced in the semiconductor is E(x) = −dφ(x)/dx, we conclude that it decreases linearly from the maximal value

158

6 Carrier Concentration and Electric Potential

Fig. 6.4 Electric potential and electric field in the semiconductor obtained within the depletion approximation

 eNa xd = E(0) = 0 

2eNa φS 0 

at x = 0 to zero at x = xd , see Fig. 6.4. For an n-type semiconductor with φS < 0, a similar analysis gives the same formulae, but with the acceptor concentration replaced by the donor concentration, Na → Nd , and the opposite sign of φ(x):  φ(x) =

eNd − 2 (x − xd )2 0

for x ≤ xd

0

for x > xd

 , xd =

20  |φS | . eNd

Combining the results for the p- and n-type semiconductors together, we express the electric potential in the depletion region as    x 2 20  φ(x) = φS 1 − , xd = |φS | , xd eNdop where Ndop = Nd or Na depending on the semiconductor type.

6.3.4 Validity Range of the Depletion Approximation Let us now determine more precisely the validity range of the depletion approximation. As stated earlier, for this approximation to be valid, the concentration of both majority and minority carriers must be much smaller than the doping concentration. Assuming for definiteness the semiconductor to be p-type, we demand that p0 (x)  Na and n0 (x)  Na for x < xd .

6.3 Approximate Solution of Poisson’s Equation

159

The charge carrier concentrations are related to the electric potential by p0 (x) = p0 (∞)e−φ(x)/Vth = Na e−φ(x)/Vth , n0 (x) = n0 (∞)eφ(x)/Vth =

n2i φ(x)/Vth e , Na

where we used the general formulas from Sect. 6.1 and the fact that Na  ni , which allows us to approximate to a good accuracy p0 (∞) = Na and n0 (∞) = n2i /Na . We thus arrive at two conditions: eφ(x)/Vth  1 , eφ(x)/Vth 

Na2 n2i

within the depletion region x < xd . It is clear that the first condition cannot be fulfilled at all values of x < xd . Indeed, as the coordinate increases from 0, the potential φ(x) decreases and eventually reaches the value of a few Vth at some coordinate x0 :   x0 2 φ(x0 ) = φS 1 − = KVth , xd where K ∼ 2 or 3. The depletion approximation actually becomes poor at    KVth x > x0 = xd 1 − . φS Note that x0 < xd . In order for the validity range of this approximation to be broad, x0 must be only slightly smaller than xd , which is only possible if φS  Vth . This is the first validity criterion of the approximation. As usual, the strong inequality  means that the surface potential must exceed the thermal voltage by at least 10 times. However, the surface potential cannot be too large because otherwise the second condition, e−φS /Vth 

Na2 , n2i

will be violated. Thus, the depletion approximation is valid if the surface potential has the value within the range Vth  φS < 2Vth ln

Na . ni

160

6 Carrier Concentration and Electric Potential

It should be much higher than the thermal voltage, but smaller than the so-called threshold potential φT = 2

EF i − EF Na = 2Vth ln e ni

by at least a few multiples of the thermal voltage. For an n-type semiconductor with φS < 0, a similar condition can be derived. To summarize, both for n- and p-semiconductors, the depletion approximation is valid, provided that Vth  |φS | < 2Vth ln

Ndop , ni

where the doping concentration Ndop is either Nd or Na , depending on the semiconductor type. This double inequality can only be fulfilled if the doping level is sufficiently large. Namely, we must have 2Vth ln

Ndop  Vth ⇒ Ndop  ni . ni

More precisely, Ndop must exceed the intrinsic concentration by at least a few hundred times. If the magnitude of the surface potential exceeds the threshold potential φT , an inversion layer is formed near the semiconductor surface. In the inversion layer, the concentration of the minority carriers exceeds the doping level. As a result, the conductivity of the inversion layer is comparable to or may even exceed the conductivity of the bulk semiconductor. The depletion approximation cannot be applied to describe this effect, and one must resort to the exact solution of Poisson’s equation.

6.4 Band Diagrams and Band Bending In thermal equilibrium, Fermi level must be constant everywhere in the semiconductor. The non-uniformity of the carrier concentrations n0 (x) and p0 (x) in the presence of an x-dependent potential φ(x) implies that the position of the band edges EV and EC relative to the Fermi level EF depends on the coordinate x. Namely, the valence band edge gets closer to the Fermi level in the direction of the hole concentration increase, and the conduction band edge gets closer to EF in the direction of the electron concentration increase. Mathematically, EC (x) = EC − eφ(x) , EV (x) = EV − eφ(x) ,

6.5 Electric Potential in a Semiconductor from Poisson’s Equation

161

Fig. 6.5 Band bending in an n-type semiconductor when the surface potential φS is (a) negative and (b) positive

where EC and EV (without the explicit x-dependence) are the band energies far from the surface, where the electric potential is zero. This is conveniently depicted in an energy band diagram, which shows how the important energy levels change with the spatial coordinate x. Figure 6.5 exemplifies the energy band diagrams of an n-type semiconductor with the negative and positive surface potential. If the surface potential is positive, the semiconductor bands bend down near the surface. If the surface potential is negative, the bands bend up. The size of band bending is e|φS |. The direction of band bending has to do with the fact that the electron energy in the presence of the electric potential is shifted by the amount −eφ(x). The energy band diagram does not have to be perfectly scale-accurate; however, it must show the relative arrangement of the important energies in a semiconductor. For example, if the semiconductor is of n-type, its Fermi level EF far from the surface must be higher than the intrinsic Fermi level EF i ≈ (EC + EV )/2; in other words, EF must be closer to the conduction band edge than to the valence band edge. In a p-type semiconductor, EF must be closer to the valence band than to the conduction band. Note that the position of the intrinsic Fermi level bends together with that band edges EC (x), EV (x). If the intrinsic Fermi level EF i (x) crosses the semiconductor Fermi energy EF , this means that the conductivity type of the semiconductor changes from the p- to the n-type at the point of crossing where EF i (x) = EF .

6.5 Electric Potential in a Semiconductor from Poisson’s Equation 6.5.1 Exact Solution of Poisson’s Equation Because the right-hand side of Poisson’s equation strongly depends on the unknown electrostatic potential, its analytical solution may seem a formidable task even for complete ionization. Yet, Poisson’s equation can be solved analytically under the complete ionization conditions.

162

6 Carrier Concentration and Electric Potential

For the sake of brevity of the formulae, we still assume that Na− ≈ Na  ni and Nd = 0. But the method developed here applies to arbitrary doping levels with both donor and acceptor impurities. It is convenient to cast Poisson’s equation, formulated in the beginning of Sect. 6.3, into a non-dimensional form. Let us introduce the non-dimensional potential y(x) and the non-dimensional coordinate t according to y(x) =

x φ(x) , t= . Vth λD

Here, λD is Debye length defined in Sect. 6.3.2. It is also expedient to define the non-dimensional threshold potential from Sect. 6.3.4 as yT =

φT Na EF i − EF N2 , eyT = 2a . = 2 ln =2 Vth ni kT ni

With these definitions, Poisson’s equation is conveniently written in the nondimensional form:  d 2 y(t) −y(t) y(t)−yT = − e − e − 1 dt 2 with the boundary conditions y(0) = yS =

φS dy (t = ∞) = 0 . , y(∞) = Vth dt

Poisson’s equation is reminiscent of a Newtonian equation of motion for a unitmass particle with position y(t) in a potential V (y): d 2y dV (y) . =− 2 dy dt The potential is obtained by integration: dV (y) = e−y − ey−yT − 1 ⇒ V (y) = −e−y − ey−yT − y . dy This mechanical analogy allows us to use the law of energy conservation. Namely, multiplying both sides of the “equation of motion” with the “velocity” dy/dt, we obtain     dy d 2 y d 1 dy 2 dy dV (y) ⇒ =− + V (y) = 0 . dt dt 2 dt dy dt 2 dt

6.5 Electric Potential in a Semiconductor from Poisson’s Equation

163

At any moment of time, the total “energy” of the particle 1 E= 2



dy dt

2

1 + V (y) = 2



dy dt

2

− e−y − ey−yT − y

is a constant. The value of the “energy” E can be established from the boundary condition at t = ∞, where y = 0 and dy/dt = 0: E = −1 − e−yT . Substitution of this expression into the definition of “energy,” we conclude that 1 2



dy dt

2

− e−y − ey−yT − y = −1 − e−yT ,

and thus the velocity is given by   dy = −sign(φS ) 2 y + e−y − 1 + e−yT (ey − 1) . dt The correct sign in front of the square root must be opposite to the sign of the surface potential φS . If φS > 0, then the potential should be decreasing to 0 with distance from the surface, and thus dy/dt < 0. If φS < 0, then the potential should be increasing with distance, and thus dy/dt > 0. The last equation can be written in the equivalent form dy dt = −sign(φS )  . −y 2 y + e − 1 + e−yT (ey − 1) Integrating this from t = 0, where y = yS , to some arbitrary t and the corresponding y(t) gives 1 t = −sign(φS ) √ 2



y(t) yS

dy 

.   y  + e−y − 1 + e−yT (ey − 1)

Finally, let us convert this result from the non-dimensional variables y and t into the dimensional ones, φ and x: λD x = √ sign(φS ) 2



φS /Vth φ(x)/Vth

dy

. −y y + e − 1 + e−yT (ey − 1)

This completes the solution of Poisson’s equation. The integral in this solution must be evaluated numerically. Instead of the x-dependent potential φ(x), we have the coordinate x at which a given value of the electrostatic potential φ is realized. That

164

6 Carrier Concentration and Electric Potential

is not a problem: all that needs to be done is to plot the independent variable φ on the vertical axis and the dependent variable x(φ) on the horizontal axis. Even though the solution obtained in this section is mathematically exact, it still relies on Boltzmann’s approximation for the carrier concentrations. Therefore, it cannot be applied when the magnitude of the surface potential gets too large. More precisely, the Fermi energy must differ from the band edge energies EC (x) = EC − eφ(x) and EV (x) = EV − eφ(x) by at least a few thermal energies both inside of the material and on the surface. Assuming this to be the case far from the surface, we must have EC − eφS − EF > eVth , EV − eφS − EF > eVth . If these conditions do not hold true, one cannot use Boltzmann’s approximation for the charge carrier concentrations.

6.5.2 Numerical Results The field effect refers to the possibility to control the concentration and the sign of the charge carriers near the surface of a semiconductor using an electric field. The field effect is at the heart of metal–oxide–semiconductor field effect transistor (MOSFET) operation, so let us discuss it in detail. For definiteness, let us consider a p-type Si semiconductor doped with Na = 1015 cm−3 acceptors at room temperature T = 300 K. Using the parameters from Appendix A.3, we find for this doping level the threshold potential and the Debye length  Na = 0.603 V , λD = φT = 2Vth ln ni

0 Vth = 0.129 µm . eNa

Suppose that we can control the value of the electrostatic potential φS on its surface, and we wish to investigate how the potential φ(x) and the charge density ρ(x) = e(p0 (x) − n0 (x) − Na− ) , p0 (x) = Na e−φ(x)/Vth , n0 (x) =

n2i , p0 (x)

change with the coordinate x. This is achieved by solving Poisson’s equation, as discussed in Sect. 6.5.1. The behavior of the electrostatic potential (normalized to the threshold value) and electric charge density ρ(x) is shown in Fig. 6.6a– d. The upper plot of each part of this figure is the potential normalized to the threshold value, φ(x)/φT , vs. the distance measured in the units of Debye length, x/λD . The lower plot shows the charge density normalized to the magnitude of the

6.5 Electric Potential in a Semiconductor from Poisson’s Equation

165

charge density of the acceptors, ρ(x)/(eNa ). Depending on the value of the surface potential, the following kinds of behaviors are observed: (a) At the surface potential φS = 0.01φT = 0.006 V, electron concentration near n2

the surface has the value n0 (0) = Nia eφS /Vth ≈ 1.25 · 105 cm−3 , much smaller than acceptor concentration. The hole concentration near the surface is very close to the acceptor concentration, p0 (0) = Na e−φS /Vth ≈ 7.9 · 1014 cm−3 . This allows using the Debye screening approximation from Sect. 6.3.2; in fact, the curve φ(x) = φS e−x/λD in this case is practically indistinguishable from the numerical curve from Fig. 6.6a. (b) Increasing the surface potential to the value φS = 0.5 φT = 0.3 V results in a formation of the space-charge region with the charge density of the acceptor background, −eNa , and thickness of about xd ≈ 0.623 μm ≈ 4.8λD . Inside the depletion region with constant charge density, the potential decreases approximately quadratically. At x > xd , the potential exhibits an exponential tail, where φ(x) ∝ e−x/λ . (c) At the surface potential equal to the threshold value, φS = φT , the size of the depletion region slightly increases as compared to plot (b). More importantly, right at the surface, a very thin layer appears, where the charge density is twice the charge density in the rest of the depletion region. The reason for this is clear: at this value of surface potential, electron concentration near the surface is the same as acceptor concentration, n0 (0) = Na . On the other hand, hole concentration near the surface is equal to the electron concentration in the bulk, p0 (0) = Na e−φT /Vth = n2i /Na . Because the concentrations of electrons and holes near the surface are inverted relative to their bulk values, this thin electronenriched layer is called the inversion layer. (d) At even higher surface potential φS = 1.2φT , the potential φ(x) inside the inversion layer initially decreases from the initial value φS to the threshold value φT . This part of the plot corresponds to the electron-rich inversion layer, marked by a very large negative charge density ρ(x). Near the point x where the potential reaches the value φT , the inversion layer ends and the depletion region begins. Its width and charge density are the same as at the threshold surface potential value from panel (c). That is, after the surface potential reaches the threshold value, the width of the depletion region saturates at the value  xdT =

20  φT , eNa

as obtained by solving Poisson’s equation using the depletion approximation and setting φS to φT . A further increase of φS does not affect the depletion region width, which still remains equal xdT .

166

6 Carrier Concentration and Electric Potential

Fig. 6.6 The electric potential normalized to the threshold value φT = 0.603 V and the charge density normalized to the magnitude of the acceptor charge density ρa = eNa = 1.602 · 10−4 C/cm3 in p-type Si doped at Na = 1015 cm−3 for different values of the surface potential: (a) φS = 0.01φT ; (b) φS = 0.5φT ; (c) φS = φT ; (d) φS = 1.2φT

6.6 Problems

167

6.6 Problems 6.6.1 Solved Problems Problem 1 The surface of a p-Si sample doped at Na = 1016 cm−3 contains trapped positive charges. Their surface concentration is η = 1011 cm−2 , i.e., the surface charge density is eη = 1.602 · 10−8 C/cm2 . The potential far from the surface is zero. What is the depletion region width xd and the value of the surface potential? Is the depletion approximation applicable to answer this question? Problem 2 Same as in Problem 1, but this time η = 1012 cm−2 . Is the inversion layer formed near the surface of the sample? If yes, what is its surface charge density and the number of electrons per unit area? Problem 3 Formulate Poisson’s equation to find the electric potential in an intrinsic semiconductor with the boundary conditions φ(0) = φS and φ(∞) = 0. How does this equation simplify for |φS |  Vth ? Find the Debye length of intrinsic silicon at T = 300 K. Problem 4 The value of the surface potential on an n-type Si sample with Nd = 1017 cm−3 is φS = −0.5 V. At what distance xi from the surface are electron and hole concentrations equal, p0 (xi ) = n0 (xi ) = ni ? Hint: Use the depletion approximation to answer this question.

6.6.2 Practice Problems Problem 1 The surface of a p-Si sample doped at Na = 1016 cm−3 contains an unknown number η of positive charges per unit area. At what concentration η of those charges does an inversion layer start to form on the surface of the sample? What is the electric field value in the semiconductor right at the surface at this concentration of surface charges? Problem 2 The potential on the surface of an n-Si sample with Nd = 5 · 1015 cm−3 is φS = −0.75 V. The temperature is 300 K. At this value of the surface potential, an inversion layer exists at the surface. Find the voltage drop across the inversion layer. Problem 3 Consider an n-type Si sample with Nd = 1016 cm−3 . At what value of the surface potential φS are the electron and hole concentrations near the surface equal?

168

6 Carrier Concentration and Electric Potential

Problem 4 Formulate and solve Poisson’s equation to find the electric potential φ(x) in an intrinsic semiconductor with  ∞the dtboundary conditions φ(0) = φS and φ(∞) = 0. You may need the identity x sinh(t) = − ln (tanh(x/2)).

6.6.3 Solutions Problem 1 The threshold value of the surface potential is φT = 2Vth ln

Na 1016 = 2 · 0.02585 · ln = 0.7221 V . ni 8.59 · 109

The maximal surface charge density of the depletion layer can be found by assuming the surface potential to be at the threshold value:  −eNa xdT = eNa =

20  φT = − 20 eNa φT eNa

2 · 8.854 · 10−14 · 11.7 · 1.602 · 10−19 · 1016 · 0.7221

= −4.896 · 10−8 C/cm2 . Since this number exceeds in magnitude the value of eη, we can conclude that the inversion layer is not formed at the surface, and the depletion approximation is valid. The surface charge density (i.e., charge per unit area) of the depletion region is given by the product of the volume charge density and the depletion region width, −eNa xd . It should perfectly compensate the surface charge density due to the trapped charges. We thus have eNa xd = eη ⇒ xd = η/Na = 1011 /1016 = 10−5 cm = 0.1 µm . The depletion region is maintained by the surface potential found from the formula xd =

20  eNa φS ,

giving

φS =

eNa xd2 1.602 · 10−19 · 1016 · 10−10 = = 0.0773 V . 20  2 · 8.854 · 10−14 · 11.7

Problem 2 As established in the solution to the previous problem, the magnitude of the maximal surface charge density in the depletion region is eNa xdT = 4.896 · 10−8 C/cm2 . This is below the surface charge density of the trapped charges, eη = 1.602 · 10−7 C/cm2 . Therefore, the depletion region alone cannot ensure the charge

6.6 Problems

169

neutrality. The number −eNa xdT found above is the surface charge density of the depletion region. Let ηi be the concentration of electrons per unit area in the inversion layer. The surface charge density of the inversion layer, −eηi , is found from the charge neutrality eη − eNa xdT − eηi = 0 ⇒ −eηi = eNa xdT − eη ; − eηi = 4.896 · 10−8 − 1.602 · 10−7 = −1.112 · 10−7 C/cm−3 . The corresponding surface concentration of electrons is ηi =

1.112 · 10−7 = 6.94 · 1011 cm−2 . 1.602 · 10−19

Problem 3 In an intrinsic semiconductor, the charge density is ρ(x) = e(p0 (x) + n0 (x)) , where the carrier concentrations in the presence of the potential φ(x) are given by p0 (x) = ni e−φ(x)/Vth , n0 (x) = ni eφ(x)/Vth . Hence, ρ(x) = eni (e−φ(x)/Vth − eφ(x)/Vth ) = −2eni sinh(φ(x)/Vth ) . Poisson’s equation reads d 2 φ(x) 2eni sinh(φ(x)/Vth ) . = 0  dx 2 At small values of its argument |x|  1, the hyperbolic sine can be approximated as sinh(x) ≈ x; hence, for small potential |φ(x)|  Vth , we can write d 2 φ(x) 2eni φ(x) = φ(x) = 2 , 2 0 Vth dx λD where the Debye length  λD =

0 Vth . 2eni

At T = 300 K in Si, ni = 8.59 · 109 cm−3 , so

170

6 Carrier Concentration and Electric Potential

 λD =

8.854 · 10−14 · 11.7 · 0.02585 = 3.12 · 10−3 cm = 31.2 µm . 2 · 1.602 · 10−19 · 8.59 · 109

Problem 4 The value of the electric potential at this point is defined by the condition Nd eφ(xi )/Vth =

n2i −φ(xi )/Vth ni e ⇒ φ(xi ) = Vth ln . Nd Nd

On the other hand, the potential depends on the coordinate x as  20  |φS | . eNd

φ(x) = φS (1 − x/xd ) , xd = 2

At the point x = xi , we must have   xi 2 ni φS 1 − = Vth ln xd Nd

 ⇒ xi = xd 1 −

 Vth ni ln φS Nd

 .

Numerically, 

2 · 8.854 · 10−14 · 11.7 · 0.5 = 8.04 · 10−6 cm = 80.4 nm , 1.602 · 10−19 · 1017    0.02585 7 · ln 10 = 7.01 nm . xi = 80.4 · 1 − 0.5 xd =

Chapter 7

Generation–Recombination Processes

7.1 Recombination Mechanisms The electron and hole concentrations n0 and p0 do not change in time in the state of thermal equilibrium. Nevertheless, even in equilibrium, electrons constantly get promoted from the valence band into the conduction band and return into the valence band. Excitation of the electrons from the valence band into the conduction band results in the generation of electron–hole pairs; recombination is an elementary process, in which a conduction electron re-enters the valence band where to occupy an empty state that we call a hole. The state of thermal equilibrium is by no means static. It is a dynamic state, in which generation and recombination processes perfectly balance each other. Domination of one of these two processes would mean an increase or a decrease of the electron and hole concentrations. Generation dominates over recombination if the initial concentrations of the charge carriers was below the equilibrium values n0 and p0 . In the opposite case, recombination proceeds at a higher rate until equilibrium is established. During an electron–hole recombination event, energy and momentum must be conserved. Note that the vast majority of conduction electrons occupy the states at the bottom of the conduction bands, whereas the majority of holes “live” near the top of the valence band. This means that the energy released in a recombination event is slightly greater than the band gap energy Eg by an amount of the order of the thermal energy kT , see Sect. 5.3. The momentum released in a recombination event depends on the band structure of the semiconductor. In the direct-band gap semiconductors, the momentum at the bottom of the conduction band is the same as at the top of the valence band, so that the electron and hole have very close momentum values before the recombination. This means that very little momentum is released after they recombine. In the indirect-band gap semiconductors, where the band edges happen to be at different momenta, the momentum released has an appreciable value. © The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_7

171

172

7 Generation–Recombination Processes

Both the energy Eg and the momentum released in a recombination event must be carried away by a third particle. This third particle can be a photon, a phonon, another electron, or a hole. It should be borne in mind that the momentum of a massless photon of energy hf = Eg , namely, pph = h/λ = hf/c = Eg /c, is much smaller than momentum of a massive particle of the same kinetic energy, ppart =

2mEg . Indeed, the ratio of the photon-to-particle momentum is pph /ppart = Eg /(2mc2 ). For the lightest massive particle, an electron, the so-called rest energy is me c2 ≈ 511 keV, whereas the typical band gap in a semiconductor Eg ≈ 1 eV. Hence, the momentum ratio is about pphot /pe ≈ 10−3 . An important conclusion can be drawn from this estimate. If the momentum released in a recombination event is small, then photons are much more likely to participate in the recombination. If the initial state of an electron in the conduction band and its final state in the valence band differ significantly not only in energy, but also in momentum, then the probability of a photon emission is much lower. Recombination in semiconductors can proceed according to the four main mechanisms: Radiative recombination , in which an electron recombines with a hole with an emission of a photon. This mechanism is the dominant one in the direct-band gap semiconductors (see Fig. 7.1a), such as GaAs, the extra energy is carried away by a photon. In the indirect-band gap semiconductors, such as Si, radiative recombination is also possible, but much less likely than in the direct-band gap semiconductors. The reason is that it must be accompanied by a release of a phonon which would carry away the momentum difference between the initial electron state at the bottom of the conduction band and the final state at the top of the valence band (see Fig. 7.1b). The more particles are involved in a process, the less probable it is; hence, radiative recombination in the indirect-band gap semiconductors plays a minor role as compared to other mechanisms that follow. Auger recombination is an example of a non-radiative mechanism, in which the energy and momentum released in a recombination event are carried away by another electron from the conduction band or by another hole from the valence band, see Fig. 7.2a and b, respectively. The charge carrier that absorbs the energy and momentum initially has high energy. It gives up very quickly its excess energy to the lattice.

Fig. 7.1 Radiative recombination in the (a) direct-band gap and (b) indirect-band gap semiconductors. The filled circles represent electrons in the conduction band; the empty circles represent holes in the valence band

7.2 Charge Carrier Dynamics

173

Fig. 7.2 Two types of an Auger process, in which either (a) an electron or (b) a hole absorbs the energy and momentum released in a recombination event. This particle then quickly dissipates the extra energy ∼ Eg by giving it away to the lattice

Trap-assisted Shockley-Read-Hall (SRH) recombination is a non-radiative recombination event assisted by the so-called deep impurities, or traps. The donors and acceptors are shallow impurities in the sense that their energies, Ed,a , are close to the band edges. In contrast, the traps are deep impurities whose energy Et is close to the middle of the band gap. Usually, they are metal atoms of various types, such as Fe, Cu, Ni, Cr, Au, Pt, etc. The deep impurities can capture conduction electrons, which then can go into the valence band, i.e., recombine with holes. The energy Eg is released in two smaller portions, first due to electron capture by a trap (energy released = EC − Et ), and then due to the recombination of the trapped electron with a hole (energy released = Et − EV ). During a SRH recombination event, it is the trap atom that first absorbs the excess energy and momentum, and then dissipates it into the crystal in the form of phonons. Surface recombination proceeds according to the SRH mechanism just described, but with the traps located on the surface of the semiconductor. Not all atoms on the surface have their valence electrons paired up with those of the neighbor atoms. Therefore, many surface atoms have unsaturated dangling bonds that can capture conduction electrons. In addition, surfaces may have a large number of defects and impurity atoms that can serve as traps as well. Radiative and Auger recombination processes cannot be controlled externally by increasing the degree of purity of the material. They are sometimes called intrinsic recombination mechanisms. In contrast, SRH and surface recombination rates can be reduced by increasing the purity of the material, by surface passivation, and by heavy doping of the semiconductor near the surface. They are referred to as extrinsic recombination mechanisms.

7.2 Charge Carrier Dynamics 7.2.1 Generation and Recombination Rates Under the non-equilibrium conditions, the carrier concentrations, n and p, differ from their equilibrium values, n0 and p0 . The deviations of the respective con-

174

7 Generation–Recombination Processes

centrations from the equilibrium values are termed the excess electron and hole concentrations: n = n − n0 , p = p − p0 . Normally, a semiconductor is electrically neutral, implying that n = p. Apart from thermal activation of electrons from the valence to the conduction band, excess charge carriers can be produced by an external agent, e.g., by illuminating the semiconductor with light. After an external generation process is switched off, the excess concentration n will decay to zero. In this section, we would like to describe the process of generation and equilibration of the excess carriers mathematically. For the sake of simplicity, we will assume the semiconductor to be uniform, i.e., the excess concentration n to be position-independent. Let us denote the generation rate of electrons and holes as G. It is the number of electrons and holes generated in a unit volume per unit time; hence, it is measured in [G] = cm−3 s−1 . Because electrons and holes are produced in pairs, their generation rates are the same, and we do not need to introduce separate generation rates for electrons and holes. The total generation rate or electron–hole pairs, Gtot , consists of two contributions: the thermal generation, Gth , which is acting in thermal equilibrium, and excess non-thermal generation, G, which is due to an external perturbation, such as light: Gtot = Gth + G. The thermal generation at the rate Gth originates from the energy exchange between the valence band electrons with the lattice vibrations and electromagnetic waves that exist within the semiconductor. It cannot be switched on or off. In contrast, the nonthermal generation is usually induced and can be controlled by an experimentalist. In principle, the generation rate may depend on the excess concentration n, but only if n becomes very large, e.g., comparable to the effective densities of states in the valence and conduction band. Indeed, at the excess concentration this high, most of the Bloch states near the top of the valence band are empty, and most states near the bottom of the conduction band are occupied by electrons. Both of these factors make further generation of excess electron–hole pairs more difficult.

7.2 Charge Carrier Dynamics

175

Here, we will focus on the usual case when n  NC , NV . Then, the generation rate Gtot is independent of the excess carrier concentration n. We also introduce the recombination rate R as the number of recombination events that happen in a unit volume per unit time, i.e., it is measured in [R] = cm−3 s−1 , just like the generation rate. In contrast to the generation rate, the recombination rate R does depend on the excess concentration n. The more carriers are present, the more recombination events should take place in a unit volume per unit time. Hence, the recombination rate R(n) increases with the excess concentration. Assuming a uniform distribution of excess carriers in the semiconductor, the rate of change of the excess carrier concentration is given by the difference of the generation and the recombination rates: dn = Gtot − R(n) = G + Gth − R(n). dt In thermal equilibrium, charge carriers are generated only due to the thermal excitation. Furthermore, there are no excess carriers. Hence, thermal equilibrium is defined by the conditions G = 0 and n = 0. Furthermore, in thermal equilibrium, the concentration of carriers does not change in time. Hence, the time derivative

dn

= Gth − R(0) = 0. dt G=0,n=0 The thermal generation rate is exactly equal the recombination rate at zero excess concentration: Gth = R(0).

In the out-of-equilibrium case, it is convenient to combine the thermal generation rate and the recombination rate into a single parameter, called the net recombination rate: U (n) = R(n) − Gth = R(n) − R(0). The net recombination rate is positive if the recombination processes dominate over thermal generation at n > 0. It is negative if n < 0, in which case thermal generation dominates. In thermal equilibrium, n = 0 and U (0) = 0. The recombination rate is actually a sum of several contributions due to different recombination mechanisms operative in the volume of a semiconductor. As discussed above, these are the radiative recombination (subscript r), the Auger

176

7 Generation–Recombination Processes

recombination (subscript A), and the Shockley-Read-Hall recombination mechanism (subscript SRH ). The net recombination rate for each of these recombination channels is given by the difference Ur (n) = Rr (n) − Rr (0), UA (n) = RA (n) − RA (0), USRH (n) = RSRH (n) − RSRH (0).

7.2.2 Recombination Time Approximation Consider a situation when some non-thermal generation mechanism was present initially, but was switched off at t = 0. Let us find out how the non-equilibrium excess concentration n(t) decays to zero at t ≥ 0. Since at t ≥ 0 we have G = 0, the equation that governs the equilibration of charge carriers is dn = Gth − R(n) = −U (n). dt Let us assume that the excess concentration is so small that we can linearize the net recombination rate near the point U (0) = 0 as U (n) = U  (0)n + . . . ≈

n for n  n0 + p0 τ

and neglect the higher-order terms. Of course, when we say that n is small, we should also answer the question: small compared to what? As will be shown below in this chapter, the excess concentration should be much smaller than the majority carrier concentration. The parameter 1 ≡ τ=  U (0)



−1

dU (n)

dn n=0

is called the recombination time, or the lifetime of the charge carriers. Within the relaxation time approximation, the excess carrier concentration is an exponentially decaying function of time: Within this approximation, we can write n dn =− ⇒ n(t) = n(0)e−t/τ . dt τ Typically, several recombination channels act simultaneously in the material: the radiative, SRH, and Auger recombination. Then, the net recombination rate is the sum of the contributions from all recombination channels,

177

U (n) = Ur (n) + UA (n) + USRH (n), all of which depend on n. Taking the derivatives of all three recombination rates at n = 0, we obtain the expression for the total recombination time 1 1 1 1 + + , = τ τr τA τSRH where τr , τA , and τSRH are the recombination times due to each individual channel. The net lifetime τ is smaller than the smallest recombination time present. If an external non-thermal generation mechanism is acting, e.g., due to the illumination of the material with light, then G > 0, and the equation for the excess concentration assumes the form dn n =− + G, dt τ provided that n is not too big to invalidate the recombination time approximation for U (n). Starting from some initial value n(0), the excess concentration will then evolve according to   n(t) = n(0)e−t/τ + Gτ 1 − e−t/τ , until it reaches a steady state with dn = 0, n = Gτ, dt after which it will not change. The electron and hole concentrations in the steady state are given by n = n0 + Gτ, p = p0 + Gτ.

7.3 Radiative Recombination A single radiative recombination event involves an electron and a hole and does not require a third particle to take place. Therefore, the number of radiative recombination events that happen in a unit volume per unit time is proportional to the electron and hole concentrations: Rr = Bnp. The proportionality constant B is called the radiative recombination coefficient. It is measured in

178

7 Generation–Recombination Processes

[B] = cm3 /s. In Si (an indirect-band gap semiconductor), it has the value of BSi ≈ 4.7 · 10−15 cm3 /s at 300 K, whereas in GaAs (a direct-band gap semiconductor), it is five orders of magnitude higher, BGaAs ≈ 7 · 10−10 cm3 /s. By writing n = n0 + n and p = p0 + n, we can express the radiative recombination rate in terms of the excess carrier concentration n: Rr (n) = B(n0 + n)(p0 + n) = Bn0 p0 + B(n0 + p0 )n + Bn2 . The net radiative recombination rate is Ur (n) = Rr (n) − Rr (0) = B(n0 + p0 )n + Bn2 . By taking its derivative with respect to n at n = 0, we find the radiative recombination time τr =

1 Ur (0)

=

1 . B(n0 + p0 )

Observing that the net recombination rate can be written as Ur (n) = n τr + 2 Bn , we conclude that the radiative recombination time description is a good approximation provided that the first term is much bigger than the second term, i.e., n  n0 + p0 . In the opposite limit, n  n0 + p0 , the net radiative recombination rate increases as the second power of n: Ur = Bn2 .

7.4 Auger Recombination When an electron and a hole recombine, the energy and momentum released can be transferred to either another electron or to another hole. Hence, Auger recombination involves three particles and may proceed via two channels, depending on whether it is an electron or a hole that carries away the energy. Let us denote the electron-assisted Auger recombination rate as RA,e and the hole-assisted rate as RA,h . The Auger recombination rate is RA = RA,e + RA,h .

7.4 Auger Recombination

179

The rate of an Auger process involving two electrons and a hole is proportional to the hole concentration and to the square of electron concentration: RA,e = Ce n2 p. Similarly, RA,h = Ch np2 . The proportionality constants Ce and Ch are called the Auger recombination coefficients. They are measured in [Ce ] = [Ch ] = cm6 /s and their typical value is of the order of 10−30 cm6 /s in a number of semiconductors, including Si and GaAs. As before, we write n = n0 + n and p = p0 + n to express the Auger recombination rate in terms of the excess carrier concentration n: RA,e (n) = Ce (n0 + n)2 (p0 + n) = Ce n20 p0 + Ce (n20 + 2n0 p0 )n + Ce p0 n2 + Ce n3 , RA,h (n) = Ch p02 n0 + Ch (p02 + 2n0 p0 )n + Ch n0 n2 + Ch n3 . The net recombination rates UA (n) are obtained by subtracting the values RA,e (0) = Ce n20 p0 and RA,h (0) = Ch p02 n0 from the respective expressions: UA (n) = UA,e (n) + UA,h (n), UA,e (n) = Ce (n20 + 2n0 p0 )n + Ce p0 n2 + Ce n3 , UA,h (n) = Ch (p02 + 2n0 p0 )n + Ch n0 n2 + Ch n3 . Taking the derivative of the sum of these two expressions at n = 0, we find the Auger recombination time to be τA =

Ce (n20

1 1 = . 2 2 2 + 2n0 p0 ) + Ch (p0 + 2n0 p0 ) Ce n0 + Ch p0 + 2(Ce + Ch )n2i

If the material is of n-type, the electron-mediated Auger recombination process dominates, and if it is of p-type, the hole-assisted Auger mechanism is more efficient. Correspondingly,

180

7 Generation–Recombination Processes

τA ≈

⎧ ⎨

1 Ce n20 ⎩ 12 Ch p0

if n0  ni  p0 , if p0  ni  n0 .

The recombination time approximation is valid under the condition that the linear term in the expression for UA (n) is much higher than the quadratic and cubic terms, i.e., Ce (n20 + 2n0 p0 ) + Ch (p02 + 2n0 p0 )  (Ce p0 + Ch n0 )n + (Ce + Ch )n2 . The right-hand side of this strong inequality monotonically increases with n. Hence, this inequality is fulfilled for n much smaller than the value at which the two sides of the inequality become equal. We thus arrive at the condition  n 

Ce n20 + Ch p02 + 2n0 p0 (Ce + Ch ) Ce p0 + Ch n0 (Ce p0 + Ch n0 )2 + − . C e + Ch 2(Ce + Ch ) 4(Ce + Ch )2

In an n-type semiconductor, we can neglect all terms in the right-hand side that contain p0 and obtain

n  n0

Ch C e + Ch



 1+4

⎧ Ce ⎪ ⎪ ⎨2 Ch n0 if Ch  Ce ;

Ce (Ce + Ch ) − 1 ≈ 2n0 if Ce  Ch ; ⎪ Ch2 ⎪ ⎩n if C ≈ C . 0

e

h

For a p-type semiconductor, the condition is similar, but with n0 replaced by p0 and the coefficients Ce and Ch interchanged:

n  p0

Ce C e + Ch



⎧ Ch ⎪ ⎪ ⎨2 Ce p0 if Ce  Ch ; Ch (Ce + Ch ) 1+4 − 1 ≈ 2p0 if Ch  Ce ; ⎪ Ce2 ⎪ ⎩p if C ≈ C . 

0

e

h

For an intrinsic semiconductor, the recombination time approximation is justified for n  ni , irrespective of the relation between the Auger coefficients Ce and Ch .

7.5 Shockley-Read-Hall (SRH) Recombination 7.5.1 Electron and Hole Capture and Emission by the Traps Suppose the material contains deep impurity atoms, or traps, with the energy Et and concentration Nt . Let us denote the concentration of those traps that are filled

181

Fig. 7.3 An illustration of electron capture, electron emission, hole capture, and hole emission by a trap

with an electron as Nt . We focus on the case when the trap concentration is too small to affect the charge neutrality. We furthermore assume that a trap atom can accommodate not more than just one electron. The four possible exchange processes may happen between a trap and the valence and conduction bands. They are schematically shown in Fig. 7.3, in which the filled circles represent electrons and empty circles represent holes: Electron capture (ec) is a transition of an electron from the conduction band to the trap level. The rate of this process is proportional to the concentration of empty traps, Nt − Nt , and to the non-equilibrium electron concentration n. Denoting the proportionality constant as cec , the rate of electron capture is Rec = cec (Nt − Nt )n. Electron emission (ee) is a back-transition of an electron from a trap into the conduction band. The rate of this process is proportional to the concentration of filled traps, Nt , with the proportionality constant cee : Ree = cee Nt . Hole capture (hc) is a transition of an electron from a trap into the valence band. The rate of hole capture is proportional to the concentration of holes and the concentration of traps filled with an electron: Rhc = chc Nt p. Hole emission (he) is a transition of an electron from the valence band to a trap. Its rate is proportional to the concentration of empty traps: Rhe = che (Nt − Nt ). The emission processes can be interpreted as generation and the capture processes as recombination of charge carriers.

182

7 Generation–Recombination Processes

7.5.2 The Principle of Detailed Balance The rate constants of the four processes, cec , cee , chc , and che , are not independent. Rather, they are related to each other by the principle of detailed balance. The idea behind this principle is that in thermal equilibrium, the rate of each elementary process is equal to the rate of the reverse process. That is, electron capture rate exactly equals electron emission rate, and hole capture and emission processes proceed at the same rate as well. In thermal equilibrium (subscript 0), the probability for a trap to be occupied by an electron is given by the Fermi-Dirac distribution: ft =

1  , Nt0 = Nt ft . 1 + e(Et −EF )/kT

Strictly speaking, the exponential factor should be multiplied by the trap degeneracy factor gt = 2 due to the two possible spin orientations of the captured electron. We absorb this factor into the definition of the trap energy, which we write as Et = Et0 + kT ln gt , where Et0 is the true energy of the trap. Because in equilibrium the rates of direct and reverse processes are the same, Rec0 = Ree0 with n = n0 , p = p0 , we have: cec Nt (1 − ft )n0 = cee Nt ft . Dividing both sides by ft Nt , we can express the electron emission rate constant as cee = cec (ft−1 − 1)n0 = cec e(Et −EF )/kT ni e(EF −EF i )/kT = cec ni e(Et −EF i )/kT . In the same manner, from the condition Rhc0 = Rhe0 we find che = chc ni e(EF i −Et )/kT . Hence, instead of four rate constants, we need only two capture constants: ce ≡ cec and ch ≡ chc , where we dropped the subscript c as superfluous. The out-ofequilibrium capture and emission rates for electrons and holes are: Rec = ce (Nt − Nt )n, Ree = ce ni e(Et −EF i )/kT Nt ,

183

Rhc = ch Nt p, Rhe = ch ni e(EF i −Et )/kT (Nt − Nt ). The electron and hole capture coefficients have the dimension [ce,h ] = cm3 /s. They must be proportional to the thermal velocity of the charge carriers, see Sect. 5.4.3,  ve,h|th =

3kT , m∗e,h

as the faster the charge carriers move, the more often they collide with the traps. Hence, ce,h = σe,h ve,h|th . The proportionality constants σe,h are called the capture cross section of electrons and holes. The capture cross sections depend on the probability that a collision between a respective charge carrier and a trap will result in the carrier capture. The capture cross section has the dimension of area and its typical value ranges from 10−18 to 10−14 cm2 .

7.5.3 The Net SRH Recombination Rate The concentration of filled traps, Nt , is related to the non-equilibrium electron and hole concentrations, n and p. To establish this relation, we note that, due to electric neutrality, the net electron SRH recombination rate, Ue = Rec − Ree , must be the same as the net hole recombination rate, Uh = Rhc − Rhe . Using the expressions for the rates Rec , Ree , Rhc , and Rhe from the previous section, we have * + * + ce (Nt − Nt )n − ni e(Et −EF i )/kT Nt = ch Nt p − ni e(EF i −Et )/kT (Nt − Nt ) .

184

7 Generation–Recombination Processes

Solving this equation for Nt , we find: Nt = Nt

ce n + ch ni e(EF i −Et )/kT . ce (n + ni e(Et −EF i )/kT ) + ch (p + ni e(EF i −Et )/kT )

Finally, substitution of this result into the net recombination rate, we find after some simple algebra: USRH = Ue = Uh = Nt

ce ch (np − n2i ) . ce (n + ni e(Et −EF i )/kT ) + ch (p + ni e(EF i −Et )/kT )

This formula can be written in a more compact form by introducing the characteristic concentrations n1 = ni e(Et −EF i )/kT , p1 = ni e(EF i −Et )/kT . It is convenient to divide the numerator and the denominator by the product Nt ce ch and to introduce the electron and hole capture times τe =

1 1 1 1 = , τh = = , Nt ce Nt σe vth e Nt ch Nt σh vth h

where we used the expressions for the capture coefficients in terms of the capture cross √ sections. It is seen that the recombination times decrease with temperature as 1/ T . The net SRH recombination rate is USRH =

np − n2i . τh (n + n1 ) + τe (p + p1 )

Recalling that n = n0 + n and p = p0 + n, as well as keeping in mind the mass action law, n0 p0 = n2i , the SRH recombination rate is written in an equivalent form USRH =

n(n0 + p0 + n) . τh (n0 + n1 ) + τe (p0 + p1 ) + (τe + τh )n

7.5.4 SRH Recombination Time At small excess concentrations, n  n0 + p0 the excess recombination rate is proportional to n:

USRH ≈

185

n , τSRH

and the SRH recombination time is given by τSRH =

τh (n0 + n1 ) + τe (p0 + p1 ) . n0 + p0

Consider what happens if one type of charge carriers, say, electrons, dominates. Note that the parameters n1 and p1 are of the similar order of magnitude as the intrinsic concentration, because Et is close to the middle of the band gap. Then, we can neglect the small concentrations, which are defined by the inequality n0  n1 ∼ p1 ∼ ni  p0 = n2i /n0 . This gives the SRH recombination time τSRH ≈ τh . More generally, τSRH ≈

 τh

if n0  ni  p0

τe

if p0  ni  n0

.

The SRH recombination time tends to the value of the capture time of the minority carriers: holes in an n-semiconductor and electrons in an p-semiconductor. This may seem a bit counter-intuitive, but is relatively easy to understand as follows. Suppose, the semiconductor is of n-type, and so most traps are occupied by electrons. A trapped electron is likely to return back to the conduction band in an n-type semiconductor, because its valence band does not have many holes. Since recombination means transition of an electron from a trap to the valence band (or, equivalently, hole capture by an occupied trap), recombination time is determined by the hole capture process. A similar argument applies if a semiconductor is of p-type. Another important observation is that at the excess concentration higher than all other concentrations found in the general formula for USRH , we have USRH ≈

n for n  n0 , p0 , ni , n1 , p1 . τe + τh

This has the familiar form of the excess concentration to the recombination time ratio. We see that, in contrast to the radiative and Auger mechanisms, the recombination time approximation recovers its validity in the case of SRH recombination also at large excess concentrations, but with a different recombination time τSRH = τe + τh . Its value is of the same order of magnitude as τSRH in the small-n limit. It is for this reason that the SRH recombination is often described within the relaxation time approximation, viz. USRH ≈ n/τSRH , both at low and high excess concentrations, with a constant τSRH independent of n.

186

7 Generation–Recombination Processes

7.6 Surface Recombination So far, we assumed an infinite semiconductor, whereas a real-life semiconductor device has a surface. As a result of an abrupt termination of the material, new electron states appear on the surface, called the surface states. They have energies within the band gap. Hence, they act as the centers where recombination can proceed according to the SRH mechanism. In addition, a semiconductor surface usually contains defects and impurities, which likewise act as recombination centers. Surface recombination proceeds via the SRH mechanism. Let us assume for simplicity that surface traps are uniformly distributed in a thin surface layer of thickness δx with the concentration Nt , which differs from the trap concentration far from the surface. The number of recombination events that happen inside this layer per unit time is 

dN dt

 = U A δx, surf

where A is the surface area, N is the total number of the excess charge carriers inside the surface layer, and the net recombination rate U is given by the SRH expression. Hence, 

dN dt

 = Nt surf

ce ch (np − n2i ) A δx ce (n + n1 ) + ch (p + p1 )

with n1 = ni e(Et −EF i )/kT , p1 = ni e(EF i −Et )/kT , as before. Denoting the surface concentration of traps as ηt = Nt δx, [ηt ] = cm−2 , and keeping in mind that np − n2i = (n0 + n)(p0 + n) − n0 p0 = (n0 + p0 + n)n, we write the rate of change of the excess carrier concentration as 

dN dt

 = AS, surf

where we introduced the so-called surface recombination velocity

7.7 Quasi-Fermi Energies

S = ηt

187

ce ch (n0 + p0 + n) . ce (n0 + n1 ) + ch (p0 + p1 ) + (ce + ch )n

It is the same for both electrons and holes. In the limits of small and large excess concentrations n, surface recombination velocity is S(n → 0) = ηt

ce ch (n0 + p0 ) ce ch . , S(n → ∞) = ηt ce (n0 + n1 ) + ch (p0 + p1 ) ce + ch

The two limit values are of the same order of magnitude, allowing us to conclude that the surface recombination velocity depends relatively weakly on the excess concentration n near the surface. It is often an acceptable approximation in modeling various semiconductor devices to take the surface recombination velocity as a constant independent of the excess concentration. An implicit assumption made in this discussion is that the surface traps are characterized by a single energy level. In reality, this is not the case: surface trap energies are distributed close to the middle of the band gap. Because it is difficult to control the physico-chemical process on the surface, the surface recombination velocity has to be measured experimentally rather than calculated theoretically. Surface recombination is an undesirable effect in the technological applications. Reduction of the surface recombination rate is achieved by surface passivation, i.e., deposition of a thin passive layer on the semiconductor surface. For example, Si surface is usually passivated by Si3 N4 or SiO2 . Surface passivation is an important step in semiconductor technology, especially in the design of solar cells. Surface passivation cannot be performed underneath the metal contacts, because a non-conducting passivating layer would prevent the current to be collected from the semiconductor device. In that case, an alternative method of reducing the surface recombination can be used. The idea is that recombination requires both electrons and holes; hence, prevention of one type of charge carriers from coming to the surface would drastically decrease the surface recombination rate. Doping the surface region with the same type of impurities as the bulk, but at a much larger concentration, achieves just that: it prevents the minority carriers from coming close to the surface and to recombine with the majority carriers.

7.7 Quasi-Fermi Energies Suppose that the non-equilibrium conditions are created in a semiconductor by an external perturbation, such as illumination of the material by light. The material then strives to restore equilibrium by two main mechanisms: (1) scattering of electrons and holes by the lattice vibrations, defects, and each other, and (2) the generationrecombination processes. Each of these mechanisms is characterized by its own characteristic rate. It turns out that, usually, equilibration within the electron and hole subsystems proceeds

188

7 Generation–Recombination Processes

much faster than equilibration between them. This is so, because the recombination time is typically much longer than the scattering time. As a result, electron and hole subsystems are close to equilibrium within themselves, but they are far from equilibrium with each other. This means that the occupation probabilities of the momentum states for electrons and holes are given by the equilibrium Fermi-Dirac distributions. However, because the concentration of particles is intimately related to their Fermi energy, we conclude that electron and hole subsystems must be characterized by different Fermi energies, denoted as EF e and EF h . That is, electron and hole occupation probabilities of some momentum state p are given by fe (E(p))  =

1  F e )/kT 1 + e(E(p)−E

, fh (E(p))  =

1  1 + e(EF h −E(p))/kT

,

where the energy E(p)  belongs to the conduction band in the electron case, and in the case of holes, it belongs to the valence band. To emphasize the fact that the system is not in equilibrium, the individual electron and hole Fermi energies are called quasi-Fermi energies, or imrefs.1 The electron and hole quasi-Fermi energies are related to their non-equilibrium concentrations by the general formulae from Sect. 5.1, but with n0 and p0 replaced with n and p:  n=

EC

 dE gC (E) fe (E), p =

EV

−∞

dE gV (E) fh (E).

If Boltzmann approximation is valid, then these expressions simplify to n = NC e−(EC −EF e )/kT = ni e(EF e −EF i )/kT , p = NV e(EV −EF h )/kT = ni e(EF i −EF h )/kT , where EF i is the intrinsic Fermi energy. The mass action law generalizes to np = n2i e(EF e −EF h )/kT . After switching off the external perturbation, a semiconductor material will tend towards the equilibrium state, where electron and hole imrefs are equal to each other. In that state, the earlier obtained equilibrium version of the mass action law, n0 p0 = n2i , is restored.

1 Singular: imref. This word is derived from the name Fermi spelled backwards, and is sometimes interpreted as “imaginary reference.”

7.8 Problems

189

190

7 Generation–Recombination Processes

zero with the recombination time τeff . The recombination time depends on the thickness W of the slab. At W = 1 µm, it is measured to be 0.2 µs, whereas at W = 10 µm, it is 0.5 µs. The effective recombination time depends on the sample thickness due to the surface recombination. Based on this information, express the effective recombination time τeff in terms of the bulk recombination time τ and the surface recombination velocity S. Find τ and S from the data provided.

7.8.2 Practice Problems Problem 1 It is possible to use the recombination time approach not only at low but also at high excess carrier concentration n by formulating its dynamics as n dn =− dt τ (n) with the recombination time τ (n) that depends on n. Write down the expressions for τ (n) for the cases of radiative and Auger recombination channels. Problem 2 At T = 300 K, the radiative recombination coefficient in Si is B = 4.7 · 10−15 cm3 /s, and Auger recombination coefficients are Ce = 1.1 · 10−30 cm6 /s and Ch = 0.3 · 10−30 cm6 /s. Its intrinsic concentration is ni = 8.59 · 109 cm−3 . (a) At what excess carrier concentration will the net Auger recombination rate be the same as the net radiative recombination rate in intrinsic silicon? (b) At what excess carrier concentration will the net Auger recombination rate be the same as the net radiative recombination rate in p-Si doped at 1015 cm−3 acceptors? Problem 3 The excess charge carriers are generated by light at a rate G in a doped semiconductor with given values of the carrier concentrations n0 and p0 , a constant SRH lifetime τSRH , and a given radiative recombination coefficient B. (a) Neglecting Auger recombination, express the excess carrier concentration n in the steady state in terms of these parameters. (b) Same as in (a), but using the recombination time approximation in the radiative recombination term. (c) In order for the recombination time approximation to be valid, the excess generation rate must be much smaller than a certain value. Establish this value by comparing your results from parts (a) and (b).

7.8 Problems

191

7.8.3 Solutions Problem 1 The excess concentration changes in time according to dn(t) = Ur (n) = −B(n0 + p0 + n(t))n(t). dt To solve this equation, we first rewrite it as dn(t) = −B dt (n0 + p0 + n(t))n(t) and integrate the right-hand side over time from 0 to t. This corresponds to the integration of the left-hand side from the initial excess concentration n(0) to the value n(t): 

n(t) n(0)

dn = −B t. (n0 + p0 + n )n

 1 To perform the integration, we use an identity (a+x)x = a1 x1 − us to rewrite the integral as a sum of two simpler integrals 1 n0 + p0



n(t) n0

dn − n



n(t) n0

dn n0 + p0 + n

1 a+x

, which allows

 = −B t.

Each of the two  integrals can be evaluated using the standard formula for the antiderivative dx/)x + a) = ln(x + a): 1 n0 + p0

  n(0) n0 + p0 + n(0) ln − ln = −B t. n(t) n0 + p0 + n(t)

By multiplying both sides by n0 + p0 and then exponentiating, we obtain n(0) n0 + p0 + n(t) 1 = et/τr , τr = . n(t) n0 + p0 + n(0) B(n0 + p0 ) Solving this for the excess concentration n(t), we get:    −1 n(t) n(0)  t/τr t/τr = e e + −1 . n(0) n0 + p0 The time dependence of the so-obtained excess concentration is shown in Fig. 7.4a. We see that at a finite n(0) value, the relaxation time approximation

192

7 Generation–Recombination Processes

Fig. 7.4 The time dependence of the excess concentration in a semiconductor where only the radiative recombination mechanism is operative with (a) linear scale and (b) logarithmic scale chosen on the vertical axis

overestimates the values of n(t) at t > 0. The lower the initial excess concentration n(0), the closer the curves are to the one obtained within the relaxation time approximation. Increasing n(0) results in a faster decay of n(t) to zero than the single-exponential curve n(t)/n(0) = e−t/τr . Nevertheless, at large times, the logarithm of the excess concentration decreases with time with the same slope equal to 1/τr for all initial concentration values, see Fig. 7.4b. Problem 2 We begin by assuming that the recombination time approximation is valid with the recombination time:  τ=

1 τSRH

1 1 + + τr τA

−1

with the SRH recombination time τSRH = 1 ms. The radiative recombination time τr =

1 1 = −12 = 10−3 s = 1 ms. BNd 10 · 1015

Because n0 = Nd = 1015 cm−3  p0 , the Auger recombination is mediated by the electrons. The respective recombination time τA =

1 1 = −29 = 0.1 s = 100 ms. 2 10 · 1030 Ce Nd

The hole Auger recombination process can be neglected. The net lifetime is, then τ = (1 + 1 + 0.01)−1 = 0.498 ms.

7.8 Problems

193

To find the excess carrier concentration, we equate the generation rate to the recombination rate, approximated as n = G ⇒ n = Gτ = 0.498 · 10−3 · 1015 = 4.98 · 1011 cm−3 . τ This number is much smaller than the doping level of 1015 cm−3 , which means that the relaxation time approximation is indeed valid. The difference between the electron and hole quasi-Fermi energies is found from (Nd + n)(p0 + n) ≈ Nd n = n2i e−(EF e −EF h )/kT , giving EF e − EF h = kT ln

Nd n = 0.02585 · ln(4.98 · 106 ) = 0.398 eV. n2i

The excess carrier concentration at time t = 1 ms after switching off the illumination is n(t) = n(0) e−t/τ = 4.98 · 1011 e−1/0.498 = 6.69 · 109 cm−3 . Problem 3 We begin by writing the generalization of the mass action law (n0 + n(t))(p0 + n(t)) = n2i eEF (t)/kT , from which the difference of the quasi-Fermi energies is obtained: EF (t) (n0 + n(t))(p0 + n(t)) = ln kT n2i   (n0 + p0 )n(0) −t/τ n2 (0) −2t/τ = ln 1 + e + e . n2i n2i Here, we used the identity n0 p0 = n2i and employed the expression n(t) = n(0)e−t/τ obtained within the relaxation time approximation. In the case (a), we have n0 = p0 = ni , giving     EF (t) n(0) −t/τ n(0) −t/τ n2 (0) −2t/τ . e + e e = 2 ln 1 + = ln 1 + 2 kT ni ni n2i In the case (b), we neglect the terms proportional to p0 and n2 (0) in the natural logarithm, giving

194

7 Generation–Recombination Processes

Fig. 7.5 The time dependence of the ratio EF (t)/EF (0) for several values of the parameter x, see main text

    n0 n(0) −t/τ EF (t) n(0) −t/τ = ln 1 + e e = ln 1 + , kT p0 n2i where we used the mass action law in the second equality. Let us denote the ratio of the initial excess carrier concentration to ni (case (a)) or to p0 (case (b)) as x:  x=

n(0)/ni case (a), n(0)/p0 case (b).

Then, in both cases, EF (t) ln(1 + x e−t/τ ) = . EF (0) ln(1 + x) This dependence for several values of x is shown in Fig. 7.5. For x  1, the term xe−t/τ  1 for all values of t. Using the approximation ln(1 + ) ≈  for ||  1, we have EF (t) 1 + xe−t/τ ≈ for x  1. EF (0) 1+x In the opposite limit x  1, the difference of the quasi-Fermi levels initially decreases linearly as

7.8 Problems

195

EF (t) ln(xe−t/τ ) t ≈ =1− for x  1 and t < τ ln x, EF (0) ln x τ ln x and then enters the exponential decrease. Problem 4 The SRH recombination rate USRH =

np − n2i τh (n + n1 ) + τe (p + p1 )

with n1 = ni e(Et −EF i )/kT and p1 = ni e(EF i −Et )/kT is maximal when the denominator is minimal. The denominator can be written as τh (n + n1 ) + τe (p + p1 ) = τh n + τe p + τh ni e(Et −EF i )/kT + τe ni e(EF i −Et )/kT    τh (Et −EF i )/kT τe −(Et −EF i )/kT √ = τh n + τe p + ni τe τh e + e τe τh   1 τh Et − EF i √ . + ln = τh n + τe p + 2ni τe τh cosh kT 2 τe τh 1 √ In the last step, we expressed τh /τe as e 2 ln τe and used the definition of a hyperbolic cosine, cosh(x) = (ex + e−x )/2. The denominator is minimal when the hyperbolic cosine has the smallest value of 1 at

Et = EF i +

τh kT ln . 2 τe

Because cosh(x) increases exponentially fast when the magnitude of its argument |x|, the most active recombination centers are the ones whose energy is close to the intrinsic Fermi level. Problem 5 The excess carriers are lost due to the recombination in the bulk and on the surface of the sample. Let N = AW n be the total number of excess charge carriers in the sample of surface area A and thickness W . Within the relaxation time approximation, it decreases according to dN(t) N (t) =− − 2SAn, dt τ where the factor of 2 takes care of the fact that the sample has two surfaces. So,

196

7 Generation–Recombination Processes

AW

dn n n , = −AW − 2SAn = − dt τ τeff

from which equation we express the effective recombination time in terms of the bulk recombination time and the surface recombination velocity: 1 τeff

=

1 S +2 . τ W

From the numerical data, namely, τeff (W = 1 µm) = 0.2 µs and τeff (W = 10 µm) = 0.5 µs, we obtain a system of two equations, 5 µs−1 =

1 1 + (2 µm−1 )S, 2 µs−1 = + (0.2 µm−1 )S. τ τ

We find: S = 1.67 µm/µs = 167 cm/s, τ = 0.6 µs.

Chapter 8

Carrier Transport

8.1 Flux and Electric Current Density It is of fundamental importance in semiconductor device theory to know how much electric charge is transferred from one part of the device to another by electrons and holes. In the following discussion, we will adopt the particle-based rather than the wave-based picture, i.e., we will treat electrons and holes as classical particles with the conductivity effective masses m∗e and m∗h and charges −e and e, respectively. Consider electrons in a physically small volume V centered at a position r, see Fig. 8.1. By “physically small,” we mean that its linear size is much smaller than all other characteristic dimensions of the system, but still large enough to contain many electrons at the local concentration n(r , t), which is practically constant inside V . Note that we dropped the subscript 0 in the electron and hole concentrations, as now these systems are not in equilibrium. Each electron inside V has its own group velocity, vj . We can perform an arithmetic averaging over all velocities of the electrons contained in V and thus obtain the average velocity: ve (r , t) =

1 vj . n(r , t)V j

Here, summation is performed over all electrons in V , n(r , t)V is the number of electrons in V , and vj is the group velocity vector of the j th electron. In general, electron concentration and average velocity depend on time and spatial coordinates. We choose V to be a small cylinder with the cross-sectional area A and length L inside a semiconductor, see Fig. 8.1. We orient the axis of this cylinder along the mean velocity ve and define a small time interval t according to L = | ve |t .

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_8

197

198

8 Carrier Transport

Fig. 8.1 Flow of electrons in a semiconductor

The cylinder contains N = nV = n A | ve |t electrons. Each of those electrons moves with its own individual velocity, but on average, all electrons move toward the cylinder’s base with the velocity ve . Then, the number of electrons that traverse the area A in time t will be just N . When divided by the product A · t, this gives us the electron flux density 1 je (r , t) = n(r , t) ve (r , t) = vej . V j

It is a vector whose magnitude is the number of electrons that traverse a unit surface area oriented perpendicular to the particles’ flow per unit time. Its direction coincides with the direction of the average electron flow at the point r at time t. The hole flux density, vh (r , t) , jh (r , t) = p(r , t) is defined in exact same manner, where p(r , t) is the local hole concentration at the position r and time t, and vh (r , t) is the average velocity of a hole. The product of the flux density by the charge of the respective carriers, ve (r , t) , Jh (r , t) = ejh (r , t) = ep(r , t) vh (r , t), Je (r , t) = −eje (r , t) = −en(r , t) is the electric current density of electrons and holes. The net current density, J = Jh + Je = e(jh − je ) , is a vector pointing in the direction of the overall electric charge transfer. Its magnitude gives the amount of charge transferred per unit time through a unit area oriented perpendicular to the direction of the overall charge flow.

8.3 Drift Current

199

8.2 Diffusion Current If electrons are distributed non-uniformly in a semiconductor material, they will tend to move from a region of higher concentration to a region of lower concentration. The degree of non-uniformity of the concentration is measured by the spatial derivatives of n(r , t), namely, ∂n/∂x, ∂n/∂y, and ∂n/∂z. All three partial derivatives can be combined into a single vector, the gradient, which was already introduced in the discussion of Schrödinger’s equation in Sect. 1.8.1:  r ) = ∂n ex + ∂n ey + ∂n ez . ∇n( ∂x ∂y ∂z The gradient points in the direction of the largest increase of electron concentration. Diffusion is described by the so-called Fick law. It says that the particles flow  i.e., in the direction of the largest concentration in the direction opposite to ∇n, decrease. The magnitude of the diffusive flux density is proportional to the concentration gradient. This law applies to any type of particles, including electrons and holes in a semiconductor. Hence, the diffusion flux densities of electrons and holes are  , jh|diff = −Dh ∇p  . je|diff = −De ∇n The proportionality constants, De and Dh , are called the electron and hole diffusion coefficients. The diffusion coefficient is measured in the units of [De,h ] = cm2 /s . The corresponding electric current density of electrons and holes is  , Jh|diff = eDh ∇p  . Je|diff = eDe ∇n

8.3 Drift Current  a free electron in vacuum would be moving Under the action of an electric field E,  e . In an ideal defect-free crystal at absolute with the acceleration ae = −eE/m zero temperature, an electron would undergo Bloch oscillations, as explained in Sect. 4.2.4. Consider now what happens when an electric field E acts in a real semiconductor.

200

8 Carrier Transport

Fig. 8.2 (a) Motion of a charge carrier with no electric field in the sample. (b) Electron and hole drift in an electric field

An electron in a real material constantly experiences collisions with lattice vibrations (phonons), defects, impurity atoms, and other electrons and holes. These collisions result in sudden changes in the electron’s direction of motion, but the average velocity of an electron is zero in the absence of an electric field, see Fig. 8.2a. When an electric field E is applied, the electron gets accelerated by it. However, as a result of collisions, the electron loses the energy acquired from the electric field. Effectively, the field is accelerating the electron only within a short time interval between two successive collisions, see Fig. 8.2b. Same applies to holes. We denote the average value of the collision time for the two types of charge carriers as τe and τh . Due to its acceleration by the field between the collisions, a charge carrier acquires a regular non-zero velocity component, called the drift velocity. It is given by the product of the electron’s acceleration due to the electric field and the characteristic time between the collisions of an electron or a hole: e  Eτe = −μe E , μe = eτe /m∗e , m∗e e  ∗ = ah τh = ∗ Eτ h = −μh E , μh = eτh /mh . mh

ve|drf = ae τe = − vh|drf

Note that ve|drf is oriented against the electric field because the charge of an electron is negative. Hole drift velocity vh|drf is oriented along the electric field. The proportionality constants μe and μh that relate the drift velocity and the electric field are called electron and hole mobilities. Mobility is measured in the units of [μe,h ] = cm2 /(V · s) . Electron and hole drift flux densities are je|drf = −nμe E , jh|drf = pμh E ,

8.4 Conductivity and Resistivity

201

and the respective electric current densities are Je|drf = eμe nE , Jh|drf = eμh pE .

8.4 Conductivity and Resistivity If a voltage V is applied to a semiconductor slab of length L and cross-sectional area A = wd, see Fig. 8.3a, current I will be flowing through it. The ratio of the applied voltage to the current is known as resistance; according to Ohm’s law, it is a voltage-independent constant: R = V /I . The voltage is related to the electric field according to V = LE . On the other hand, the current is given by the product of the electric current density and the cross-sectional area of the sample: I = AJdrf , where the drift current density is Jdrf = Je|drf + Jh|drf = e(μe n + μh p)E , see Sect. 8.3. Combining these expressions, we arrive at the resistance formula R=

L L L = = ρ, A(μe n + μh p) Aσ A

which clearly shows that the resistance depends on the geometry of the sample through the ratio L/A, and on its material properties via the parameters σ = e(μe n + μh p) , ρ = σ −1 =

1 , e(μe n + μh p)

known as the conductivity and resistivity of the material. If excess carriers are not injected into the semiconductor, one can replace in these expressions the nonequilibrium concentrations n and p with the equilibrium counterparts n0 and p0 .

202

8 Carrier Transport

8.5 Current–Voltage Measurements 8.5.1 Photoconductivity The measurements of the current–voltage curves provide a great deal of information about the concentration and mobilities of the charge carriers. They can also be used to measure their recombination rates. This can be done by first injecting excess carriers into the semiconductor by, e.g., illumination, and then observing its return to equilibrium after switching off the excess carrier generation process. A practical way to measure the net recombination time is to measure the time-dependent conductivity of the semiconductor sample of interest: σ (t) = e(n(t)μe + p(t)μh ) , where μe , μh are the electron and hole mobilities. Since n(t) = n0 + n(t) and p(t) = p0 + n(t), the total conductivity has the time-dependent and the timeindependent parts: σ (t) = σ0 + σ (t) , where σ0 = e(n0 μe + p0 μh ) , σ (t) = en(0)(μe + μh )e−t/τ . If the non-thermal generation mechanism is photogeneration, i.e., the generation of charge carriers by light, then the parameter σ is called photoconductivity. Taking the natural logarithm of the ratio σ (t) to the initial value σ (0) = n(0)(μe + μh ), we immediately find: ln

t σ (t) =− . σ (0) τ

That is, the natural logarithm of the photoconductivity as a function of time is a straight line with the slope −1/τ .

8.5.2 Hall Effect Let us focus for the sake of simplicity on a situation when the charge carriers of one type dominate in the sample; that is, either electron or hole contribution to the conductivity can be neglected. Consider what happens when, in addition to the electric field in the x-direction, E = ex V /L, a magnetic field B = Bez is applied

8.5 Current–Voltage Measurements

203

Fig. 8.3 (a) Motion of electrons and holes due to the electric field generated by the applied voltage. (b) Same as in (a), but in the presence of a magnetic field B applied perpendicular to the sample, which is assumed to be a p-type semiconductor. (c) Same as in (b), but for an n-type semiconductor sample

perpendicular to the sample in the z-direction, see Fig. 8.3b and c. A magnetic field creates a force that acts on a charge q = e or −e moving with the drift velocity vdrf = ve|drf or vh|drf : Fm = q vdrf × B . If the majority charge carriers are holes, q = +e, then their flow coincides with the direction of the electric current I , Fig. 8.3b. If the majority carriers are electrons, q = −e, then their flow is against the electric current, Fig. 8.3c. In either case, the magnetic force Fm acting on a majority carrier points in the negative y-direction. As a result, the majority carriers get deflected toward the same side of the sample. This side accumulates positive or negative charge if the semiconductor is of p- or n-type, respectively, see Fig. 8.3b and c. The opposite side gets depleted of the majority carriers and therefore also gets charged up. The charge on the opposite sign is due to the ionized impurities—negative acceptors in a p-type and positive donors in an n-type semiconductor. The process of charge build-up stops when the accumulated charges generate an electric field whose force on the majority carriers exactly balances the magnetic force, F e = Fm . As a result, a potential difference develops between the two opposite sides of the sample. It is called the Hall voltage. Its polarity immediately signals the sign of the majority charge carriers, see Fig. 8.3b and c. The magnitude of the Hall voltage allows finding their concentration. Indeed, the electric field in the y-direction and the force produced by this field on a majority carrier are |Ey | = |VH |/w , |Fe | = e|VH |/w .

204

8 Carrier Transport

This force must be equal in magnitude of the magnetic force |Fm | = e|vdrf |B. Let us assume for definiteness that the majority carriers are holes. Neglecting the contribution of the minority electrons to the total current, the drift velocity of the majority holes can be found from I = wdJh|drf = wdevh|drf p ⇒ vh|drf =

I , wdep

and thus the magnetic force is |Fm | =

IB . wdp

The condition |Fm | = |Fe | gives the concentration of holes: p=

IB . ed|VH |

If the sign of the Hall voltage reveals that the majority carriers are electrons, then their concentration is given by an exact same formula n=

IB . ed|VH |

8.6 Temperature and Doping Level Dependence of Mobility Collisions are responsible for the electrons’ transitions from one momentum state to another. Usually, several collision mechanisms are operative, namely, scattering of electrons and holes by the lattice vibrations (phonons), scattering by the impurities, and scattering by the lattice defects. Note that all these mechanisms result in the deviation of the atomic arrangement in a semiconductor from a perfect periodic order. The frequency of phonon scattering, νphonon , increases with the temperature. The respective scattering time τphonon = 1/νphonon is decreasing with T . Thus, if only phonon scattering mechanism were present, the mobility μ ∝ τphonon would be decreasing with temperature. Experimental measurements performed on semiconductor samples where the phonon scattering is the dominant one (i.e., the impurity concentration is low) suggest that τphonon ∝ T −α , where the exponent α is close to 2; e.g., α ≈ 2.2 in silicon. Impurity scattering frequency, νimpurity , increases with the concentration of the ionized impurities, NI = Nd+ + Na− ,

8.7 Einstein’s Relation

205

Table 8.1 Electron and hole mobility parameters of silicon as a function of temperature, measured in Kelvins Parameter μ0 [cm2 /(V·s)] μ1 [cm2 /(V·s)] N0 [cm−3 ] α

Electrons 88 (300 K/T )0.57 1252 (300 K/T )2.33 1.26 · 1017 (T /300 K)2.4 0.88 (300 K/T )0.146

Holes 54.3 (300 K/T )0.57 407 (300 K/T )2.23 2.35 · 1017 (T /300 K)2.4 0.88 (300 K/T )0.146

and decreases with temperature. The reason for the temperature decrease is that the higher the temperature, the higher the thermal velocity of electrons and holes and the less time they spend interacting with the ionized impurities. Therefore, the probability that this interaction will result in a change of the charge carrier’s momentum decreases with T . When several scattering mechanisms are present, the total scattering frequency is the sum of the contributions from each mechanism, e.g., ν = νphonon + νimpurity for thermal and impurity scattering. As for the time of scattering, we have τ −1 = −1 −1 τphonon + τimpurity . The mobility is, then, μ = m∗ (νphonone+νimpurity ) for electrons and holes. It decreases both with NI and with T . Various empirical fitting expressions for electron and hole mobilities exist. Here, we reproduce the one that has been suggested for silicon and describes the electron and hole mobilities as a function of both impurity concentration and temperature:1 μ = μ0 +

μ1 . 1 + (NI /N0 )α

The temperature dependence of the parameters μ0 , μ1 , N0 , and α is indicated in Table 8.1.

8.7 Einstein’s Relation The diffusion coefficient is a parameter that tells us how quickly an initially nonuniform distribution of charge carriers spreads out through the sample. Mobility, on the other hand, relates the average velocity of a charge carrier to the applied electric field. At a first glance, De,h and μe,h are independent of each other because they describe completely different processes. Yet, there is a simple relation between them, which was originally discovered by Einstein in 1905. As in Sect. 6.1, we place a piece of semiconductor in a non-uniform electric potential φ(r ), which causes a redistribution of charge carriers inside the material.

1 N.D. Arora, J.R. Hauser, and D.J. Roulston, “Electron and hole mobilities in silicon as a function of concentration and temperature”, IEEE Trans. Electron Dev., ED-29, 292–295 (1982).

206

8 Carrier Transport

 which, in turn, results A non-uniform potential produces an electric field, E = −∇φ, in a drift of charge carriers with the respective flux densities je|drf = −μe n0 (r ) E  On the other hand, the non-uniformity of electron and hole and jh|drf = μh p0 (r ) E. concentrations results in the diffusion of these charge carriers with the flux densities  0 (r ) and jh|diff = −Dh ∇p  0 (r ). The total flux densities je|diff = −De ∇n  − De ∇n  0 = μe n0 ∇φ(  r ) − De ∇n  0 (r ) , je (r ) = je|drf + je|diff = −μe En  r ) − Dh ∇p  0 (r ) jh (r ) = −μh p0 ∇φ( must be zero in equilibrium. This is only possible if  r ) = De ∇n  r ) = Dh ∇p  0 (r ) , −μh p0 (r )∇φ(  0 (r ) . μe n0 (r )∇φ( Note that     0 (r ) ∇n  ln n0 (r ) = ∇φ(r ) , ∇p0 (r ) = ∇  ln p0 (r ) = − ∇φ(r ) , =∇ n0 (r ) Vth p0 (r ) Vth as follows from the expressions for n0 (r ) and p0 (r ) from Sect. 6.1. Combining the last two equations, we obtain Einstein’s relation: μe =

De Dh , μh = . Vth Vth

While mobility is relatively easy to measure experimentally, the diffusion coefficient is not. Einstein’s relation allows finding the diffusion coefficient from the knowledge of mobility. Einstein’s relation is approximate because it relies on Boltzmann’s approximation for the charge carriers concentrations. It breaks down if the Fermi energy differs from the conduction or valence band edge by less than a few thermal energies kT .

8.8 Continuity Equation As electrons and holes move inside the semiconductor under the action of an electric field E(r ), they get generated and recombine. Hence, the respective concentrations n(r , t) and p(r , t) change both in time and in space. Continuity equation is the balance equation that relates the rate of change of the concentration to the flow of particles, as well as their generation and recombination. Here, we will focus, for the sake of simplicity, on the one-dimensional flow of electrons in the x-direction. We assume that generation and recombination rates depend on the x-coordinate only and are constant in the yz-plane at a given x. The derivation for holes is completely analogous. Consider a small cylinder of length

8.8 Continuity Equation

207

Fig. 8.4 Electron flow in a semiconductor

x and the base area A, see Fig. 8.4. The cylinder is oriented in the x-direction, which is the direction of the average particle flow. Its volume is V = Ax, and it contains N = nV electrons. We assume that x is sufficiently small for the concentration n(x) to be practically constant inside the cylinder. The number of electrons inside this cylinder changes in time for two reasons: (i) electrons flow into and out of the cylinder through its two bases, and their inflow and the outflow do not necessarily balance each other; (iii) electrons get generated and recombine inside the cylinder with the generation and recombination rates not necessarily equal each other. Mathematically, the balance of these factors can be expressed as dNe = dt



dNe dt



 −

in

dNe dt



 +

out

dNe dt



 −

gen

dNe dt

 . rec

The generation and recombination contributions are 

dNe dt



 = G A x ,

gen

dNe dt

 = R A x . rec

As for the in- and outflow of the electrons, it is related to the respective current densities:     dNe dNe = je (x)A , = je (x + x)A . dt dt in out Note that, in contrast to the concentration, we cannot assume that electron current density is constant inside the cylinder. Had we set je (x) = je (x + x), then the inand outflow contributions would have mutually canceled. Collecting all terms, we rewrite the balance equation as ∂n(x, t) Ax = je (x)A − je (x + x)A + G(x)Ax − R(x)Ax . ∂t e (x) e (x) = ∂j∂x in the limit Dividing both sides by Ax and recalling that je (x+x)−j x x → 0, we arrive at the continuity equation for electron concentration; the hole counterpart is obtained analogously:

208

8 Carrier Transport

∂n ∂je ∂p ∂jh =− +G−R , =− +G−R . ∂t ∂x ∂t ∂x Note that the current density consists of drift and diffusion contributions: je,h = je,h|drf + je,h|diff , je|drf = −μe nE , jh|drf = μh pE , je|diff = −De

∂n ∂p , jh|diff = −Dh . ∂x ∂x

8.9 Problems 8.9.1 Solved Problems Problem 1 An n-type silicon sample at T = 300 K has the conductivity of 16 ( · cm)−1 . (a) Determine the donor concentration and the electron mobility using the empirical expressions for mobility from Sect. 8.6. (b) What is the diffusion coefficient of electrons and holes in this sample? Problem 2 Consider a semiconductor with donor doping concentration Nd (x) = (1014 cm−3 ) ex/(1 μm) that increases with x. Find the electric field and electrostatic potential distribution inside this semiconductor. Problem 3 When a Si sample is illuminated by a lamp, its conductivity is measured as 66.6 −1 cm−1 . After illumination is switched off, the conductivity becomes 33.3 −1 cm−1 after 0.1 µs and 9.1 −1 cm−1 after 2 µs. Determine the following parameters: the net recombination time in the sample.

8.9.2 Practice Problems Problem 1 A Si sample is doped with donors at Nd = 1017 cm−3 and acceptors at Na = 1018 cm−3 . The temperature is 300 K. Using the mobility vs. impurity concentration formula from Sect. 8.6, determine the conductivity and the resistivity of this sample.

8.9 Problems

209

Problem 2 A silicon sample is acceptor-doped at Na = 1017 cm−3 . The photoconductivity of this sample is found to decay as σ (t) ∝ e−t/(0.1 ms) . Find its Shockley–Read–Hall recombination time. Problem 3 The geometric parameters of a semiconductor sample at T = 300 K are: d = 20 µm, w = 300 µm, and L = 1 mm. When the voltage of 0.1 V is applied, the current of 0.3 mA flows through the sample. A magnetic field of B = 0.1 T is applied in the z-direction, and the measured Hall voltage is VH = 20 mV such that the resulting Hall electric field points in the positive-y-direction. Determine the conductivity type, the majority carrier concentration, and the majority carrier mobility in this sample.

8.9.3 Solutions Problem 1 (a) Since it is an n-type semiconductor, it is reasonable to assume that n0 ≈ Nd  ni  p0 , and hence, the dominant contribution to the conductivity comes from the electrons. Hence, we approximate σ = e(μe n0 + μh p0 ) = eμe Nd . Using the expression from Sect. 8.6,  μ0 +

μ1 1 + (Nd /N0 )α

 Nd =

16 σ = . e 1.6 · 10−19

We solve this equation iteratively. First, we rewrite it as Nd =

σ/e μ0 +

μ1 1+(Nd /N0 )α

=

1020 88 +

1252 1+(Nd /1.26·1017 )0.88

.

Then, starting with some initial value of Nd , say, Nd = 1017 cm−3 , we use the right-hand side expression to calculate an improved estimate, which is again plugged in into the right-hand side. This procedure is repeated until convergence is reached. The final result turns out to be Nd = 1.5 · 1017 cm−3 . Electron mobility is then found to be μe = 666 cm2 /(V · s).

210

8 Carrier Transport

(b) Electron diffusion coefficient is found using Einstein’s relation: De = μe Vth = 666 · 0.02585 = 17.2 cm2 /s . Hole mobility at Nd = 1.5 · 1017 cm−3 is μh = 54.3 +

407 1 + (1.5 · 1017 /2.35 · 1017 )0.88

= 297.5 cm2 /(V · s) .

Hole diffusion coefficient is, then, Dh = μh Vth = 297.5 · 0.02585 = 7.69 cm2 /s .

Problem 2 Since Nd (x)  ni at x > 0, the electron concentration n0 (x) = Nd (x) increases with x. This means that the electrons should diffuse in the negative-xdirection with the diffusion particle current density je|diff = −De

dn0 (x) dNd (x) = −De . dx dx

But a small displacement of the negative electrons relative to the positive donor ions results in an onset of an electric field in the negative-x-direction. This field pulls the electrons to the right, so that there is no electron flow in the material. The drift current produced by this field, je|drf = −Eμe n0 (x) = −Eμe Nd (x), perfectly compensates the diffusion current: je|drf + je|diff = −Eμe Nd (x) − De

dNd (x) =0. dx

From this, we find the electric field: E =−

De 1 dNd d ln Nd = −Vth , μe Nd dx dx

where we used Einstein’s relation, De = μe Vth , and the fact that d ln Nd /dx = Nd−1 dNd /dx. Since d ln Nd /dx = 1 μm−1 = 104 cm−1 , the electric field is E = −0.02585 · 104 V/cm = −259 V/cm .

8.9 Problems

211

Since the electric field is related to the potential as E =−

dφ(x) , dx

we can conclude that the potential increases with x as     V V · x = 258.5 ·x . φ(x) = 0.02585 µm cm Problem 3 In order to find Nd and τ , we thus need to fit the experimental σ (t) curve with an exponential function: σ (t) = σ0 + σ (0) e−t/τ , σ0 = eμe Nd , σ (0) = e(μe + μh )n(0) , where σ0 is the conductivity in equilibrium (no radiation), and σ (0) is the photoconductivity. From the experiment, we know that σ (t) decreases by a factor of 2 in the first 0.1 µs. This implies that τ is of the order of 0.1 µs as well. After 2 µs, the exponential factor e−t/τ should be negligibly small (note that e−2/0.1 = e−20 = 2 · 10−9 ), so we can set to a good accuracy σ (2 μs) = σ0 = 9.1 −1 cm−1 . From the experimental data, we find that at t = 0, σ (0) = σeq + σ0 = 66.6 −1 cm−1 , from which we find the photoconductivity σ (0) = σ (0) − σeq = 66.6 − 9.1 = 57.5 −1 cm−1 . We finally find τ by using the conductivity at t = 0.1 µs: τ =−

t ln

σ (t)−σeq σ0

=−

0.1 ln

33.3−9.1 57.5

= 0.1155 μs .

Part III

Semiconductor Devices

Chapter 9

Metal–Semiconductor Contact

9.1 Reasons to Study Metal–semiconductor contact is worth studying for several reasons. First, to collect a signal from a semiconductor device, one needs to attach a metal wire to it; in this case, one is interested in having a good ohmic contact with low contact resistance for both bias directions. Second, as we shall see later, metal–semiconductor contact can also act as a diode, i.e., let the current flow in only one direction. Such diodes, called Schottky diodes, can be preferred for some applications over the semiconductor pn junction diodes discussed later on in this book. The third reason is that understanding the physics of a metal–semiconductor contact, especially the energy band diagrams, will prepare us to analyze a more complicated system, the metal–oxide–semiconductor field effect transistor.

9.2 Energy Band Diagram The minimal energy necessary to remove an electron from a piece of metal is called the metal work function. It is the difference between the energy of an electron at rest just outside the metal—the so-called vacuum level—and the Fermi energy of a metal. We will denote the work function as eψm , a product of the elementary charge e and the parameter ψm that is measured in Volts: eψm = Evac − EF . Its typical value is about 4–6 eV, depending on the material. We define the work function in a semiconductor in the same manner, i.e., as the difference between the vacuum and the Fermi energy,

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_9

215

216

9 Metal–Semiconductor Contact

Fig. 9.1 The energy band diagram of (a) a metal, (b) a semiconductor, and (c) a metal– semiconductor contact

eψs = Evac − EF , see Fig. 9.1a and b showing the energy band diagrams of a metal and a semiconductor that are not in contact with each other. In addition, we define the electron affinity eχ as the energy difference between the vacuum level and the conduction band edge, eχ = Evac − EC . Electron affinity ranges between 3 and 4.5 eV, depending on the material. A metal and a semiconductor in contact will exchange their electrons so as to bring their Fermi energies to a common level. The Fermi level in a metal lies inside its conduction band, and therefore, the number of free electrons in a metal is in many orders of magnitude higher than the number of conduction electrons and holes in a semiconductor. For this reason, the change of the Fermi level in the metal will be negligibly small as compared to the change of the Fermi level in the semiconductor. In other words, semiconductor Fermi level will line up with the metal Fermi level, whereas the metal Fermi energy will practically remain the same. The vacuum level of the metal and the semiconductor must be the same at the point of contact. At the same time, electron affinity and the band gap of the semiconductor must be the same both in the bulk and near the semiconductor– metal interface. Indeed, these parameters depend on the band structure of the semiconductor and do not depend on band filling. These three observations—common Fermi level, the same vacuum level at the contact, and the constant values of the semiconductor electron affinity and band gap—necessarily imply that semiconductor bands are bent near the interface with the metal, see Fig. 9.1c showing band bending for ψs < ψm . Generally speaking, bands can bend both up and down, depending on the mutual relation between metal work function and semiconductor work function in the bulk. If semiconductor work function is higher than the metal work function, semiconductor bands bend down; otherwise, they bend up.

9.2 Energy Band Diagram

217

While the electron affinity and band gap are the same in the semiconductor bulk and near the interface, the semiconductor work function is position-dependent due to band bending. So is the energy difference between the Fermi level and the band edges of the semiconductor. This leads to a change of the majority carrier concentration in the semiconductor bulk and near the interface. Even the type of the majority carriers may differ in the bulk and near the contact plane. For instance, in the case shown in Fig. 9.1c, the semiconductor is of the ntype in the bulk, but the concentration of holes exceeds the electron concentrations near the surface. This can be understood as follows. Because the semiconductor work function is smaller than the metal work function, it is easier for electrons to move over from the semiconductor into the metal than from the metal into the semiconductor. The semiconductor near the metal will then be depleted of the conduction electrons, resulting in the appearance of a space-charge region created by the positively charged donor ions near the contact. The electrons that entered the metal from the semiconductor side, in turn, will create excess negative charge in the metal. This access charge exists as a surface charge at the metal–semiconductor interface. Strictly speaking, it also results in band bending in the metal, but the size of this bending is negligibly small as compared to the semiconductor counterpart. Band bending in the semiconductor results in an onset of the built-in voltage, which we define as the magnitude of the difference of work functions of the two materials: Vbi = |ψm − ψs | . Assuming the bulk of the semiconductor to be grounded, the value of the electric potential on the semiconductor surface is φS = −Vbi if ψm > ψs , see Fig. 9.1c. An electron on the metal side with the energy equal to EF will “see” a sharp potential barrier that prevents it from entering the semiconductor conduction band. This barrier is called the Schottky barrier. By inspecting the diagram in Fig. 9.1c, we see immediately that its height is given by eφB = eψm − eχ . This expression is sometimes called the Schottky–Mott rule. The metal work function ψm and the semiconductor electron affinity χ are bulk properties of the materials, whereas φB is the property of the metal–semiconductor interface. In real life, Schottky barrier height is given by the Schottky–Mott rule only approximately. It is also affected by other surface properties of the two materials in contact, in particular, by surface chemistry and the presence of surface defects. Therefore, in practice, Schottky barrier has to be measured experimentally.

218

9 Metal–Semiconductor Contact

9.3 SCR Capacitance The potential distribution in the semiconductor is described by Poisson’s equation, see Sect. 6.2: d 2 φ(x) e =− (p0 (x) − n0 (x) + Nd ) . 0  dx 2 We solve it using the depletion approximation explained in Sect. 6.3.3. That is, we approximate the charge density as zero outside the depletion region of width xd and as eNd inside the depletion region 0 < x < xd . The solution of Poisson equation reads  eNd − 2 (x − xd )2 for 0 < x < xd , 0 φ(x) = 0 for x > xd . Employing the boundary condition, φ(0) = −Vbi , we immediately find the depletion region width  xd =

20 Vbi . eNd

If an external bias V is applied to the metal relative to the semiconductor, we have to replace Vbi with Vbi − V in this expression:  xd =

20 (Vbi − V ) . eNd

A change of the voltage V by an amount dV results in a change of the SCR width by  0  dxd dV = − dV . dxd = dV 2eNd (Vbi − V ) This results in a change of the SCR charge by  dQ = −eNd A dxd = The capacitance per unit area is

0  eNd AdV . 2(Vbi − V )

9.4 Ohmic Contact

219

Fig. 9.2 The inverse square of the capacitance per unit area of a SCR formed in an n-type semiconductor in contact with a metal with ψm > ψs as a function of the applied voltage

 1 dQ = C = A dV 

0  e0 Nd = . 2(Vbi − V ) xd

This expression can also be obtained from a formal definition of a parallel-plate capacitance of thickness xd , namely, C = 0xA . d This result offers a practical method to determine the built-in voltage Vbi experimentally. Indeed, we note that the inverse capacitance squared, 1 2 = (Vbi − V ) , 2 e0 Nd C depends linearly on the applied voltage V . The slope of this straight line is − e02Nd . The built-in voltage can be found as the intercept of this straight line with the horizontal axis, see Fig. 9.2.

9.4 Ohmic Contact For signal collection from a semiconductor device, it is desirable that the contact between the semiconductor and the metal wire had a small resistance for both directions of bias. Such contacts are called ohmic. There are two ways to produce an ohmic contact: (1) using metal–semiconductor combination that would have little or no Schottky barrier and (2) employing the tunneling effect. Option 1 If the semiconductor is of n-type, then one can use a metal with the work function smaller than the semiconductors, ψm < ψs . This will cause the semiconductor bands to bend down. When no voltage is applied, the energy band diagram looks like the one in Fig. 9.3a. The band bending occurs because some electrons leave the metal into the semiconductor, creating a surface layer of an increased conduction electron concentration on the semiconductor side. Application of a positive voltage to the semiconductor will make it easier for even more electrons to be transferred from the metal into the semiconductor. Application of a positive voltage to the metal will pull electrons from the semiconductor into the metal

220

9 Metal–Semiconductor Contact

Fig. 9.3 An ohmic contact between a metal and (a) an n-type and (b) a p-type semiconductor

Fig. 9.4 (a) Tunneling of a wave packet through a potential barrier of finite width and height. (b) Realization of a tunneling barrier by heavy donor doping of an n-type semiconductor near the interface with a metal

because there is no potential barrier at the metal–semiconductor interface. Thus, current will flow with little resistance for both bias polarities. If the semiconductor is of p-type, then one can use a metal whose work function is higher than that of the semiconductor, ψm > ψs . This will cause the semiconductor bands to bend up, creating a thin hole-enriched layer near the interface with the metal, see Fig. 9.3b. Application of a positive bias to the semiconductor will cause the majority holes to move toward the metal, and, at the same time, it will cause the electrons from the metal to flow into the semiconductor. After entering the semiconductor, those electrons will recombine with the holes, with the overall effect of electric current flowing from the semiconductor to the metal with little resistance. Application of a positive bias to the metal, on the other hand, will attract electrons from the semiconductor valence band into the metal; this is equivalent to the flow of holes away from the metal. Option 2 When a massive classical object of some kinetic energy E hits a potential barrier of height VB > E, it bounces back. In quantum mechanics, however, this is not necessarily the case. At the most fundamental level, all objects are waves described by their wave function. When such a wave meets an obstacle, the wave function cannot instantaneously become zero at the position of the barrier. It smoothly decays to zero inside the barrier but remains finite even on the other side of the barrier. This is so even when the barrier height exceeds the particle’s kinetic energy. This means that a particle, such as an electron, has a small, but finite probability to tunnel through the barrier to the other side, see Fig. 9.4a. Tunneling probability is the larger the thinner the barrier and the smaller its height.

9.5 Rectification in a Metal–Semiconductor Contact

221

Now, a strong doping of a thin layer of an n-type semiconductor with donors will create additional band bending near the surface. The width of the SCR is inversely proportional to the square root of the doping concentration and can be made, therefore, very small. This makes it possible for electrons to tunnel from metal to semiconductor and back, see Fig. 9.4b. That is, electrons will be able to move both ways between the metal and the semiconductor via tunneling mechanism.

9.5 Rectification in a Metal–Semiconductor Contact 9.5.1 Metal/n-Type Semiconductor Junction Qualitative Considerations Let us derive the current–voltage relation of a junction formed by an n-type semiconductor with a metal of a higher work function, ψm > ψs , see Fig. 9.1c. This contact is rectifying, as the following reasoning shows. Application of a positive bias to the metal attracts the majority electrons from the semiconductor into the metal, which results in a large current in the forward direction. On the hand, application of a negative bias to the metal prevents the majority electrons to enter the metal from the semiconductor. Furthermore, the electrons of the metal likewise are not able to enter the semiconductor because of the high and sharp Schottky barrier they encounter at the metal–semiconductor boundary. Hence, the current in the reverse direction is small. It is not exactly zero because a small fraction of the metal electrons do have energy exceeding eφB . Assume zero bias. Electrons attempting to go from the metal into the semiconductor meet a high and sharp Schottky barrier eφB , whereas the conduction electrons attempting to go in the opposite direction have to overcome a much shallower barrier eVbi due to the built-in voltage, see Fig. 9.1c. Electron fluxes from the metal into the semiconductor and from the semiconductor into the metal must perfectly balance each other in equilibrium at zero applied voltage: jm→s (0) + js→m (0) = 0 . The reason why the two fluxes balance each other in spite of the big difference between the sizes of the two barriers, eφB and eVbi , is because the concentration of electrons in the metal greatly exceeds the majority electron concentration in the semiconductor. Our goal is to find the total electron flux and the electric current density j (V ) = jm→s (V ) + js→m (V ) , J (V ) = −ej (V )

222

9 Metal–Semiconductor Contact

when a voltage V is applied to the metal side, whereas the semiconductor is grounded. Qualitatively, the rectification effect of the metal–semiconductor contact results from the different dependence on the applied voltage V of the potential barrier that electrons need to overcome to enter the semiconductor from the metal side and vice versa. Namely, the external voltage V has practically no effect on the height of Schottky barrier eφB . This, in turn, implies that the electron flux density from the metal into the semiconductor is practically independent of V : jm→s (V ) ≈ jm→s (0) = −js→m (0) = jS . Here we denoted the so-called saturation flux density as jS = −js→m (0). As for the semiconductor side, application of a positive bias to the metal lowers the barrier by eV , see Fig. 9.5a, thereby exponentially increasing the number of electrons that can enter the metal from the semiconductor per unit time. This concentration gets enhanced by a factor eV /Vth . We therefore expect that the electron flux into the metal should be js→m (V ) = js→m (0)eV /Vth = −jS eV /Vth . The current–voltage (or J − V ) curve is thus expected to have the form J (V ) = −ejs→m (V ) − ejm→s (V ) = ejS eV /Vth − ejS = JS (eV /Vth − 1) , where JS = ejS is the reverse saturation current density, calculated below. The graph of this function is shown in Fig. 9.5b. A passive1 element, in which the current to flow for one polarity of bias with very little current for the reverse polarity, is called

Fig. 9.5 (a) The energy band diagram of a metal contact with an n-type semiconductor when a positive voltage is applied to the metal. (b) Qualitative behavior of the current–voltage curve of a rectifying contact between a metal and an n-type semiconductor. (c) Electronic symbol of a Schottky diode

1A

passive element is the one that does not require an external power source.

9.5 Rectification in a Metal–Semiconductor Contact

223

a diode. Specifically, a diode based on a metal–semiconductor contact is called the Schottky diode. Its electronic symbol is depicted in Fig. 9.5c.

9.5.2 Reverse Saturation Current Density of a Schottky Diode To obtain the reverse saturation current density, we need to estimate the number of electrons that enter the metal from the semiconductor side per unit area per unit time when a voltage V is applied. Let us first consider a simpler case of a classical gas in a solid container. The gas has density n, atomic mass m, and temperature T , corresponding to thermal energy kT . The number of particles j incident on the wall of the container per unit surface area per unit time should be expressible in terms of m, kT , and n. We can figure out this expression by analyzing the dimensions of the parameters involved, which are [n] = L−3 ; [kT ] = M · L2 /T2 ; [m] = M . Here, L, T, and M stand for the dimensions of length, time, and mass, respectively. We need to combine the parameters n, kT , and m so as to get the right dimension of j , namely, [j ] = 1/(L2 · T). The only such combination is  j = bn

kT , m

where the non-dimensional prefactor b cannot be established by dimensional analysis. The kinetic theory of gases gives the value  kT 1 . b= √ ⇒ j =n 2π m 2π We can use this result to obtain the semiconductor-to-metal particle current density by replacing the particle mass m with electron conductivity effective mass m∗e and particle concentration n with the concentration n∗ of those electrons that are capable of overcoming the energy barrier e(Vbi − V ) that stands on their way into the metal. In order to be able to get out of the semiconductor, a conduction electron must have the energy not less than EB = EC + e(Vbi − V ) = (EC + eVbi ) − eV = EF + eφB − eV . We used the fact that

224

9 Metal–Semiconductor Contact

EC + eVbi = EF + eφB , as follows from the energy band diagram at zero bias. The concentration of conduction electrons with the energy above EB is then n∗ =



dE g(E) f (E) ≈ NC e−(eφB −eV )/kT = NC e−(φB −V )/Vth ,

EB

where g(E) and f (E) are electron density of states and Fermi–Dirac distribution; we used Boltzmann approximation to evaluate the integral. As obtained earlier (see Sect. 5.2), the effective density of states in the conduction band is NC =

2(2π m∗e kT )3/2 . h3

Modifying our expression for the particle flux density, j , we obtain the electron flux density from the semiconductor to the metal as 

 kT = NC 2π m∗e

js→m (V ) = n

kT e(φB −V )/Vth . 2π m∗e

The saturation electron flux density is therefore jS =

4π m∗e k 2 T 2 −φB /Vth e . h3

As for electric current density, J (V ) = JS (eV /Vth −1), we get the reverse saturation current density JS = AT 2 e−φB /Vth , where A=

4π m∗e k 2 e m∗ = (120.2 A · cm−2 · K−2 ) · e 3 me h

is the so-called Richardson constant.2 In semiconductors, the typical value of Richardson’s constant A is about 100 A/(K2 ·cm2 ). With the typical Schottky barrier height of ca. 0.7 eV, we find that at room temperature, the reverse saturation current density JS is of the order of 10−5 A/cm2 .

2 It is named after Owen Richardson, who developed this theory to describe thermionic emission of electrons from metals into vacuum in the early 1900s (Nobel Prize 1928).

9.5 Rectification in a Metal–Semiconductor Contact

225

Fig. 9.6 A junction formed by a metal and a p-type semiconductor of the larger work function, eψs > eψm , (a) at zero applied voltage and (b) when a negative bias is applied to the metal. (c) The J − V curve of this junction

9.5.3 Metal/p-Type Semiconductor Junction The energy band diagram of a junction formed by a metal and a p-type semiconductor with a higher work function at zero applied voltage is shown in Fig. 9.6a. Due to the work function difference, ψm < ψs , the semiconductor bands are bent down near the interface. The built-in voltage is Vbi = ψs − ψm . The Schottky barrier is now measured from the metal Fermi level to the valence band edge in the junction plane. For an ideal diode, it is given by eφB = eχ + Eg − eψm , as can be verified by inspecting the energy band diagram. Application of a negative bias to the metal, Fig. 9.6b, pushes the electrons from the metal into the semiconductor and pulls the holes from the semiconductor into the metal; the two types of charge carriers meet and recombine at the metal–semiconductor boundary. This results in an appreciable current through the structure in the negative-x direction. This current should increase in magnitude with increasing the negative voltage. On the other hand, application of a positive bias to the metal side prevents electrons from leaving the metal into the semiconductor and prevents the majority holes from coming to the metal from the semiconductor. The current, however, is not exactly zero, even when the positive voltage applied to the metal is large. A large positive voltage pulls the electrons from the metal–semiconductor interface into the volume of the metal, simultaneously generating holes on the semiconductor side

226

9 Metal–Semiconductor Contact

immediately near the junction plane. Those holes then move into the semiconductor bulk, resulting in a small positive current. This process can be described as injection of holes from the metal into the semiconductor. The current–voltage curve of this diode looks qualitatively like the one in Fig. 9.6c. The analytical form of the current–voltage relation is similar to the one obtained earlier for a rectifying junction formed by a metal and an n-type semiconductor, except for the signs in front of the current and the voltage: J (V ) = JS (1 − e−V /V th ) . The expression for the saturation current is similar to the one obtained earlier, but with the electron conductivity effective mass replaced by the hole counterpart: JS = AT 2 e−φB /Vth , A =

4π m∗h k 2 e m∗h −2 −2 = (120.2 A · cm · K ) · . me h3

9.6 Non-ideality Effects The J − V relation obtained in Sect. 9.5.2 describes an ideal Schottky diode and does not account for some important effects that take place in the real metal– semiconductor contacts. One such effect overlooked by this theory is that the barrier height “seen” by electrons impinging on the metal from the semiconductor side is actually lower than the value used in the calculations. To understand this, let us consider the junction formed by a metal and an n-type semiconductor, see Fig. 9.5a, under a forward bias. Consider a conduction electron inside the space-charge region near the metal– semiconductor interface. The ionized donors produce the electric potential in the space-charge region (see Sect. 6.3.3): 

x φSCR (x) = (Vbi − V ) 1 − xd



2 , xd =

20 (Vbi − V ) . eNd

In addition, the electron also interacts with the electrons of the metal. This interaction can be effectively described by the method of image charges. Namely, the force produced on the electron by the metal is the same as the force between this electron of charge −e and its image charge +e located at a distance x on the other side of the metal–semiconductor interface, see Fig. 9.7a: Fim (x) = −

e2 1 e2 = − . 4π 0  (2x)2 16π 0 x 2

9.6 Non-ideality Effects

227

Fig. 9.7 (a) An electron (charge −e) at a distance x from a metal surface interacts with the metal so as if there were an image charge e at a distance x on the other side of the semiconductor–metal interface. (b) The total electric potential is a sum of the SCR-generated contribution, φSCR (x), and the image charge potential φim (x)

The image-charge force can be expressed as the negative derivative of the imagecharge electric potential multiplied by the electron charge, −e: Fim (x) = e

dφim (x) e , φim (x) = − . dx 16π 0 x

The total potential in which the electron finds itself is, thus, φtot (x) = φSCR (x) + φim (x) , see Fig. 9.7b. It is seen that it has a maximum, whose height is smaller than the value Vbi − V obtained without taking the image charge into account. The barrier height reduction φ can be obtained by approximating φSCR (x) ≈ (Vbi − V )(1 − 2x/xd ); this approximation is valid provided that the maximum of the total potential φtot (x) is not too far from the surface. The result of this calculation is  φ(V ) =

e3 Nd (Vbi − V ) 8π 2 (0 )3

1/4 .

We see that the barrier height decrease depends on the applied voltage. The result is that the reverse saturation current density is increased relative to its ideal-junction value by a factor eφ(V )/Vth : JS = AT 2 e−φB /Vth eφ(V )/Vth . Actually, this value of the saturation current density is also not quite accurate for several reasons:

228

9 Metal–Semiconductor Contact

(i) A further effect neglected by the theory is that electrons with the energy greater than the barrier height are incident onto the interface with the metal from the semiconductor side does not necessarily make it into the metal. In fact, they can be reflected back into the semiconductor, even though their energy is higher than the barrier that prevents them from entering the metal. This is a purely quantum effect that has to do with the wave nature of electrons; it cannot be explained within the classical framework. (ii) What is even more important, the electrons with the energy lower than the barrier height can still make it through the barrier due to the quantum tunneling effect. (iii) The theory developed above neglects the recombination of electrons and holes in the space-charge region and also the surface recombination on the semiconductor boundary. (iv) There is a thin dielectric layer that separates the metal and the semiconductor. While the electrons can tunnel through this layer, there is also a finite potential difference across this layer, which affects the value of the Schottky barrier height. All these non-ideality effects result in a deviation of the experimental current– voltage curve from the ideal one obtained here. The ideal J − V curve describes the real-life devices only qualitatively correctly. In order to fit the experimental J − V curves of a real Schottky diode, the ideal-diode relation is modified by introducing the so-called ideality factor n: J (V ) = JS (eV /(nVth ) − 1) . The ideality factor n is usually of the order of 1 − 2, but it can also be outside of this range.

9.7 Problems 9.7.1 Solved Problems Problem 1 Consider a junction formed by p-Si doped at Na = 1015 cm−3 and some metal at T = 300 K. The semiconductor is grounded. Silicon parameters can be found in Appendix A.3. What should the metal work function be in order for the voltage applied to the metal electrode to be the same as the surface potential on the semiconductor? Draw the energy band diagram at zero voltage V , V > 0, and V < 0. Problem 2 A junction is formed by silicon and a golden electrode with the work function eψm = 5.1 eV. Determine the type (donors or acceptors) and the

9.7 Problems

229

Fig. 9.8 Two Schottky diodes connected (a) in parallel and (b) in series

minimal concentration of the dopants in order for an inversion layer to form in the semiconductor near the surface. Problem 3 Two identical ideal Schottky diodes are connected in parallel, with one in forward and the other in reverse direction, see Fig. 9.8a. Assume the reverse saturation current IS of each diode to be known. Derive and sketch the current– voltage relation, I (V )/IS vs. V /Vth , of this circuit.

9.7.2 Practice Problems Problem 1 Derive the value of the barrier lowering φ from Sect. 9.5.2. Problem 2 When a positive bias of 0.5 V is applied to the metal side of a metal– silicon junction, the junction has the capacitance of 0.25 pF. A bias of 1.5 V results in a capacitance of 0.05 pF. The junction area A = 10−5 cm2 , and the temperature T = 300 K. (a) Is the semiconductor of p- or n-type? What is the smallest value of the applied voltage at which the space-charge region in the semiconductor starts to appear? Is the metal work function higher or lower than the semiconductors? (b) What is the doping level of the semiconductor? (c) What is the value of the metal work function? Problem 3 When a positive forward bias of 0.1 V is applied to an ideal Schottky diode at T = 350 K, a current density J = 5.32 · 10−10 A/cm2 is measured. The bias of 0.5 V results in the current density of 3.18 · 10−4 A/cm2 . (a) What is the reverse saturation current density of this junction? (b) Determine the height of Schottky barrier. Problem 4 Two identical ideal Schottky diodes are connected in series, one in the forward and the other in the reverse direction, see Fig. 9.8b. Assume the reverse saturation current, IS , of each diode to be known. Derive the current–voltage curve I (V ) of this circuit. Plot the ratio I /IS vs. the ratio V /Vth .

230

9 Metal–Semiconductor Contact

9.7.3 Solutions Problem 1 In order for the surface potential to be exactly equal to the voltage applied to the metal, band bending must be absent in the semiconductor. The size of band bending, which is the built-in voltage, is zero only if the metal work function is the same as the semiconductor work function. Therefore, we must have eψm = eψs = Evac − EF = Evac − EC + EC − EF = eχ + EC − EF . The energy difference EC − EF can be found from the electron concentration: n0 =

n2i = NC e−(EC −EF )/kT , Na

giving EC − EF = kT ln

Na NC 1015 · 3.2 · 1019 = 0.02585 ln = 0.871 eV . (8.59 · 109 )2 n2i

The metal work function must be eψm = 4.05 + 0.871 = 4.92 eV . The energy band diagrams of this contact for V = 0, V > 0, and V < 0 are shown in Fig. 9.9. Problem 2 Let us assume that the majority carriers in the semiconductor are electrons. Referring to Fig. 9.1c, we can express the difference Evac,m − EF in two ways:

Fig. 9.9 The energy band diagram of a contact formed by a p-type silicon and a metal with ψm = ψs at zero, positive, and negative voltage applied to the metal

9.7 Problems

231

ψm = Vbi + χ +

EC − EF . e

The inversion layer starts forming when the concentration of holes near the surface equals the concentration of electrons far from the surface. Hole concentration near the surface is related to its value in the bulk via p0,surf = p0 eVbi /Vth =

n2i Vbi /Vth e . n0

From the condition p0,surf = n0 , we obtain (see also Sect. 6.3.4) Vbi = 2Vth ln

n0 . ni

Next, the difference between the conduction band energy and the Fermi energy is related to the electron concentration by (see Sect. 5.2) EC − EF NC = Vth ln . e n0 Substitution of the expressions for Vbi and (EC − EF )/e gives ψm = 2Vth ln

n0 NC n0 NC + χ + Vth ln = χ + Vth ln . ni n0 n2i

From this, we find the electron concentration: n0 =

n2i (ψm −χ )/Vth e . NC

Taking the parameters from Appendix A.3, we find its numerical value n0 =

(8.59 · 109 )2 (5.1−4.05)/0.02585 e = 1.01 · 1018 cm−3 . 3.2 · 1019

We see that n0  ni , which is consistent with our assumption that the semiconductor is of n-type. If we assumed that it were of p-type, then we would have had to use the energy band diagram from Fig. 9.6a; a similar reasoning would have brought us to a conclusion that n0  ni , which is inconsistent with the assumption about the conductivity type of the semiconductor. Hence, the semiconductor must be doped with donors at Nd = 1.01 · 1018 cm−3 . Problem 3 The total current I is the sum of currents through the upper, I1 , and the lower, I2 , diodes,

232

9 Metal–Semiconductor Contact

Fig. 9.10 The current–voltage curve of a circuit, in which two diodes are connected in parallel, see Fig. 9.8a

I = I1 + I2 . Since the diodes are in parallel, the same voltage V is applied to both of them. The upper diode is in the forward direction; hence, I1 (V ) = IS (eV /Vth − 1) . The lower diode is reverse-biased: if V is large and positive, the current through the lower diode is IS , and if V is large and negative, I2 ∝ −IS e−V /Vth . More generally, I2 (V ) = −IS (e−V /Vth − 1) . Adding the two currents together, I (V ) = IS (eV /Vth − e−V /Vth ) = 2IS sinh This relation is plotted in Fig. 9.10.

V I (V ) V ⇒ = 2 sinh . Vth IS Vth

Chapter 10

Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

10.1 MOSFET Schematics and Operation Principle A MOSFET is a workhorse of integrated electronics and is at the heart of every digital circuit. It is a building block of a charge coupled device (CCD). To name but a few of its other applications, it is used to store information and perform logical operations in digital electronics, to amplify and generate ac-signals in analog circuits, and to convert analog signals into digital ones. A schematics of an enhancement-mode MOSFET with an n-channel, or nMOSFET, is shown in Fig. 10.1a. It is based on a p-type substrate, with the terminal attached to it called the body (B). The body is usually grounded. In the upper part of the substrate, there are two heavily doped n+ -regions, with the source (S) and drain (D) terminals. They are separated by an insulating oxide layer, on top of which there is a metal electrode, called the gate (G). In Si-based circuits, the insulating layer is usually formed by SiO2 (silicon dioxide), hence the name of the device. The electrodes can be made of a metal, but also they can be made of heavily doped semiconductor. The idea of an n-MOSFET operation is that by applying a positive voltage to the gate, one affects the value of the electric potential on the semiconductor surface underneath the oxide layer. Once the gate voltage reaches a certain threshold value, VT , the electric potential on the semiconductor surface becomes equal to the threshold potential φT = (EF i −EF )/(2e), at which an electron-rich inversion layer is formed, as discussed in the end of Sect. 6.3.4. The inversion layer connects the source and the drain, allowing electric current to flow between these two electrodes. Likewise, one may use an n-type substrate with the p+ -type source and drain regions. Then, application of a sufficiently large negative voltage to the gate will result in a formation of a hole-enriched inversion layer. This kind of a MOSFET is called the p-MOSFET in the enhancement mode. The electronic symbols of an enhancement-mode n- and p-MOSFETS are shown in Fig. 10.1a.

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_10

233

234

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

Fig. 10.1 (a) The structure of an enhancement-mode n-MOSFET and its electronic symbol; in a p-MOSFET, whose electronic symbol is shown to the right, the substrate is of n-type, and the heavily doped regions under the source and drain electrodes are of the p+ -type. (b) The sketch of a depletion-mode n-MOSFET and its electronic symbol. The depletion-mode p-MOSFET has the same structure, but with the n-type substrate, the p+ -type source and drain regions, and a holeenriched inversion layer underneath the oxide

The action of a MOSFET is thus reminiscent of a faucet, where a small variation in the turning angle of the valve has a large effect on the water flow. Note that the oxide layer is absolutely necessary for MOSFET operation. Indeed, if one had a metal gate electrode deposited directly on the semiconductor surface, it would have been impossible to control surface conductivity by the gate voltage simply because the surface would already have been connecting the source and the drain at all voltages. A great advantage of MOSFET technology is its flexibility. It is possible to have the parameters of the device such that the inversion layer is present even at zero gate voltage; then, one would need to apply a certain threshold voltage to the gate in order to switch the inversion layer off. A MOSFET with the pre-existing electronrich inversion layer at zero gate voltage is termed an n-MOSFET in the depletion mode, see Fig. 10.1b. One can also build a depletion-mode p-MOSFET if one uses an n-type body and two p+ -type source and drain electrodes. The electronic symbols of depletion-mode n- and p-MOSFETs are shown in the same figure.

10.2 Qualitative Description of MOSFET I − V Curve

235

Fig. 10.2 (a) The current–voltage curves of an enhancement-mode n-MOSFET, connected as shown in panel (b), for different values of the gate voltages. The dotted curve separates the region where ID increases with VD from the region where ID is constant

10.2 Qualitative Description of MOSFET I − V Curve Consider an enhancement-mode n-MOSFET with the body and the source electrodes grounded, a voltage VD applied to the drain and a current ID measured. Its I − V curve for different values of the gate voltage VG is shown in Fig. 10.2. At a fixed gate voltage exceeding the threshold value, VG > VT , the drain current ID initially increases linearly with the drain voltage. The initial slope (the conductance) dID /dVD of the ID vs. VD curve increases as the gate voltage VG is increased. The reason for this is clear: the higher the gate voltage, the thicker the inversion layer, and hence the lower its resistance. Interestingly, when the drain voltage attains a certain value VDsat , the drain current reaches saturation. It remains constant upon further increase of the drain voltage above VDsat -value. The saturation drain voltage increases with the gate voltage. Let us try and understand the current saturation. In order for an inversion layer to form, it is necessary for the potential difference V between the semiconductor surface underneath the oxide layer and the gate to be greater than some threshold voltage VT . But when a voltage VD is applied to the drain, the value of the local potential at a given point underneath the oxide will depend on the distance x from the source. It will change from V (0) = 0 at x = 0 to V (L) = VD at x = L, where L is the drain-to-source distance, see Fig. 10.3. The potential difference between the gate and a point x in the inversion channel is then given by V (x) = VG − V (x).

236

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

If the inversion channel connects the drain and the source, then V changes from the highest value VG at x = 0 to the lowest value VG − VD at x = L. Increasing the drain voltage VD results in a decrease of V (L) = VG − VD . As long as V (L) is above the threshold level, the inversion channel is still connecting the drain and the source, and the current is still increasing upon further increase of the drain voltage, albeit not as sharply as in the beginning of the I − V curve. But at some point, the drain voltage reaches the value VDsat = VG − VT , at which the local potential difference at x = L equals V (L) = VT . Then, the existence of the inversion channel cannot be supported near the drain anymore, although it still can exist at some distance away from it. This causes the phenomenon called the pinch-off, see Fig. 10.3. At pinch-off, the inversion channel ends at some distance L from the drain. The distance L increases with VD starting from the value L = 0 at VD = VDsat . It might come as a surprise that the drain current does not go to zero after the pinch-off, even though the inversion channel is not in contact with the drain anymore. Rather, the current saturates and does not change upon further increase of the drain voltage. This is so, because, after the pinch-off, the potential difference between one end of the inversion layer at x = 0 and the other end at x = L − L remains constant and equals VDsat . For VD greater than the saturation value VDsat by not too much, the distance L should be much smaller than L, which implies that the inversion channel resistance R is approximately independent of VD . Hence, also the current in the inversion layer should be equal to IDsat = VDsat /R independent of VD . The current ID = IDsat at VD > VDsat is carried by the electrons that move from the rightmost edge of the inversion layer to the drain through the space-charge region around the drain. Our next task is to find the threshold gate voltage VT at which the inversion layer develops and to derive an analytic expression for the I − V curve of a MOSFET.

Fig. 10.3 Inversion layer at VD > VDsat

10.3 Quantitative Description of a MOSFET I − V Curve

237

10.3 Quantitative Description of a MOSFET I − V Curve Let us consider the situation when a thin inversion channel is formed, i.e., the gate voltage exceeds the threshold value, VG > VT , and the drain voltage is below the pinch-off value, VD < VDsat . As we go along the inversion channel in the xdirection, the potential difference V (x) between a point x in the channel and the source at the origin increases from V (x = 0) = 0 to V (x = L) = VD . The local electric field in the inversion layer, E(x) = −

dV (x) , dx

acts in the negative-x-direction. It pulls the electrons from the source to the drain. On average, the electrons in the inversion layer move with the drift velocity, which depends on x: ve|drf (x) = −μe E(x) = μe

dV (x) , dx

where μe is the electron mobility in the inversion channel. Note that it is appreciably smaller than electron mobility far away from the surface because the scattering of the electrons by the surface is an additional mechanism that slows them down. This mechanism is not operative in the semiconductor bulk. Let ηi (x) be the surface concentration of the electrons in the inversion layer. It depends on the distance x from the source, being maximal at x = 0 and gradually decreasing to ηi (L) as the inversion layer gets thinner. The corresponding surfacecharge density is −eηi (x). It is supported by the local potential difference across the oxide layer above the threshold voltage VT , V (x) − VT = VG − V (x) − VT . The threshold voltage must be subtracted from V (x) because there is no inversion layer at V (x) < VT ; the inversion layer only starts to be formed at V (x) = VT . The surface-charge density −eηi (x) is given by  (VG − VT − V (x)), −eηi (x) = −Cox

where  = Cox

0 ox tox

is the unit area capacitance of the insulating oxide layer between the gate electrode and the MOSFET body. The thickness of this oxide layer is tox , and its relative dielectric constant is ox .

238

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

The value of the electric current at a position x is given by I (x) = −eW ηi (x) ve|drf = W eηi (x) μe

dV dV  = W Cox . (VG − VT − V (x)) μe dx dx

Indeed, dq = −eW ηi (x)dx is the total electron charge contained between x and x + dx. This charge is moving with the average velocity ve|drf = dx/dt, resulting in the current I (x) = dq/dt above. Note that for a positive drain voltage VD , the electrons are drifting in the positive x-direction, so that the current I (x) is negative. Now, due to charge conservation, the current must be constant at all values of x. Its value is equal to the drain current, ID = −I (x) for all x. We choose the minus sign so as to make the drain current have the same sign as the drain voltage. Thus,  ID = W Cox (VG − VT − V (x))μe

dV . dx

We multiply both sides of this equation by dx and integrate its left-hand side over x from x = 0 to x = L, giving ID L. Its right-hand side is integrated over the voltage  ((V − V )V − from the value V (x = 0) = 0 to V (x = L) = VD , giving W Cox G T D 2 VD /2). We thus obtain the current–voltage curve before saturation is reached:  ID (VD ) = Kn 2(VG − VT )VD − VD2 for VD < VDsat , where the combination Kn =

 W μe Cox 2L

is called the conduction parameter of an n-MOSFET. Note that ID = 0 at VD = 0, as one would expect. This ID (VD ) curve represents a parabola with a maximum at VD = VDsat = VG − VT , as can be verified by differentiation. If VD > VDsat , this relation would predict a decrease of ID with VD . But the analytical considerations presented above are invalid if VD exceeds the saturation value VDsat because we are now in the pinch-off regime, in which the inversion layer does not connect the source and the drain anymore. Rather than starting to decrease, the current saturates at the value IDsat = ID (VDsat ) = Kn (VG − VT )2 for VD > VDsat . The current–voltage curve of a p-MOSFET is the same as of an n-MOSFET, with the only difference being that the conduction parameter Kn has to be replaced with Kp =

 W μh Cox , 2L

where μh is the hole mobility near the surface.

10.4 Determination of the Threshold Voltage

239

10.4 Determination of the Threshold Voltage 10.4.1 Energy Band Diagram of a MOS Structure at Zero Gate Voltage The inversion layer in the p-semiconductor is formed when the potential on its surface underneath the oxide reaches the threshold value φT = 2Vth ln

Na EF i − EF =2 , ni e

at which electron concentration near the surface becomes equal to hole concentration in the bulk. Semiconductor surface potential is controlled by the voltage on the gate electrode separated from the semiconductor by a thin dielectric (e.g., SiO2 ) layer. We need to figure out the threshold gate voltage VT , at which the surface potential attains the value φT . Solving this problem requires a careful analysis of the energy band diagram of the metal–oxide–semiconductor system when a voltage VG is applied to the gate, while the source, the drain, and the body are grounded. Let us forget about the source and the drain for the moment and consider the energy bands in the p-type substrate when zero voltage is applied to the gate, see Fig. 10.4, showing the metal–oxide–semiconductor (MOS) structure in panel (a) and its energy band diagram at zero bias in panel (b). Drawing the energy band diagram of a MOS structure is based on the same principles as in the simpler metal– semiconductor case. In particular, metal and semiconductor in equilibrium must have the same Fermi energy. This is so because maintaining zero voltage between the gate and the body of a MOS structure requires connecting the two objects by a wire through which the gate and the body can exchange electrons. This electron exchange renders the Fermi energies in the gate and the substrate to be the same.

Fig. 10.4 (a) A metal–oxide–semiconductor (MOS) capacitor with zero voltage between the substrate and the gate and (b) the energy band diagram of this structure

240

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

Next, the vacuum energy level must be continuous throughout the MOS structure. Just as in the case of a metal–semiconductor contact, this implies band bending in the semiconductor and oxide layers. More precisely, because there are no free charge carriers in the oxide, a potential difference Vox develops across it due to the band bending in the semiconductor and also due to the surface charges that are trapped on the oxide surface (we will discuss them later). Band bending in the semiconductor results in the onset of a surface potential φS . The energy difference between the vacuum level and Fermi energy in the metal is the metal work function, eψm . Electron affinity in the semiconductor bulk—that is, the energy difference between the semiconductor conduction band edge and the vacuum energy—is denoted as eχ . The work function in the semiconductor is then eψs = Evac,s − EF s = eχ + EC − EF .

10.4.2 Energy Band Diagram of a MOS Structure for Non-zero Gate Voltage Consider now what happens when a positive bias VG is applied to the gate. This leads to a shift of all energy levels in the gate down by the amount eVG , e.g., the new Fermi level in the metal is now EF m = EF s − eVG . At the same time, the energy differences between the metal Fermi level EF m and the vacuum level, eψm , remain the same as in the zero-bias case. Because the semiconductor is grounded, all the bulk energy levels and energy differences (EF s , EF i , EC , EV , Evac,s , and eχ ) remain the same as in the zero-bias case. But at the semiconductor–oxide interface, the size of the band bending will be affected by the voltage VG applied to the gate. The size of the semiconductor band bending near the surface is quantified by the surface potential eφS , which equals the difference between the characteristic energies (such as Evac,s or EF i ) in the bulk and near the surface, see Fig. 10.5b. When the gate voltage reaches the threshold value, VG = VT , the surface potential becomes φ S = φT = 2

EF i − EF , e

and an inversion layer starts to form. A useful relation between all these characteristic energies can be established by considering the difference between the vacuum energy and the semiconductor Fermi level in the bulk. On the one hand, it is just the semiconductor work function eψs = EC − EF + eχ ,

10.4 Determination of the Threshold Voltage

241

Fig. 10.5 (a) A metal–oxide–semiconductor (MOS) capacitor with a non-zero voltage between the substrate and the gate and (b) the energy band diagram of this structure

see the right part of Fig. 10.5b. The same energy difference can be expressed in terms of the metal properties, the potential drop across the oxide, and the band bending parameter, namely, eψs = eψm − eVG + eVox + eφS , see the left part of Fig. 10.5b. Equating the two expressions, we have eψm − eVG + eVox + eφS = EC − EF + eχ , or VG = ψm + Vox + φS − χ −

EC − EF . e

This relation can be written in several equivalent forms. For instance, previously, we have obtained an expression for the intrinsic Fermi energy EF i =

Eg kT NV EC + EV EC + EV + ln = EC − . ≈ 2 2 NC 2 2

Given that the effective densities of states NV and NC are of the same order of magnitude, the ratio NV /NC is of the order of unity, and thus the logarithmic term can be neglected. Then VG = ψm − χS + Vox + φS +

Eg EF − EF i − . e 2e

242

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

10.4.3 Oxide Voltage An oxide layer of thickness tox has the capacitance per unit area  Cox =

0 ox , tox

where ox is the relative dielectric constant of the oxide. A voltage Vox across the oxide layer is associated with the surface charges on its opposite sides. The gate (metal) acquires a charge per unit area Qm , which has the same sign as the oxide voltage polarity. The charge developed in the semiconductor underneath the oxide layer has the surface density Qs = −Qm . It equals in magnitude to the surface-charge density on the metal side because the whole structure must be electrically neutral. Thus, by the definition of capacitance, the voltage across the oxide is given by Vox =

Qm Q tox = − s = − Q .  Cox Cox 0 ox s

The semiconductor surface-charge density consists of three contributions: 1. The negative charge of the ionized acceptors is in the depletion region underneath the oxide. The surface-charge density of the depletion region is  Qd = −eNa xd , xd =

20  φS . eNa

Here, xd is the width of the depletion region, as derived earlier (see Sect. 6.3.3). 2. The negative charge is due to the electrons in the inversion layer. We denote the respective surface-charge density as Qi . 3. During the semiconductor surface oxidation process, additional positive charge is formed at the Si/SiO2 interface due to the charge carriers trapped by the surface states, trapped ions of various types, charged defects, etc. The magnitude of the respective surface-charge density Qss (the subscript ss stands for “semiconductor surface”) depends on the technological conditions and is fixed. Thus, in general, the voltage drop across the oxide layer is Vox = −

QS eNa xd + Qi − Qss = .   Cox Cox

10.4 Determination of the Threshold Voltage

243

Fig. 10.6 The energy band diagram of an enhancement-mode n-MOSFET when the flat-band voltage is applied to the gate

10.4.4 Flat-Band Voltage The general relation between the gate obtained in the end of Sect. 10.4.2 involves the surface potential φS , which determines the magnitude of band bending and, accordingly, the width of the depletion region. The flat-band voltage is defined as that value of the gate voltage VG = VF B for which the band bending is zero, i.e., φS = 0, see Fig. 10.6. Then, there is no depletion region under the oxide layer, i.e., xd = 0 under the flat-band conditions. Recalling that the inversion layer is formed after the depletion region reaches its maximal size, we immediately realize that also Qi = 0. Then, the oxide voltage under the flat-band conditions is determined just by the trapped surface-charge density, VoxF B = −

Qss ,  Cox

and the flat-band value of the gate voltage is VF B = ψm − χ −

Eg Q EF i − EF Q − − ss = ψm − ψs − ss . e 2e Cox Cox

This is just the difference between the metal and semiconductor work functions minus the oxide voltage due to the trapped surface charges. For an n-channel MOSFET, the flat-band voltage is negative because the semiconductor work function, eψs = eχ + EF i − EF +

Eg , 2

exceeds the metal counterpart, and because the charge Qss on the semiconductor– oxide interface is positive.

244

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

When an arbitrary voltage is applied to the gate, it can be expressed as VG = VF B +

eNa xd + Qi + φS .  Cox

10.4.5 Threshold Voltage When the gate voltage VG increases to the threshold value VT , the electrostatic F potential at the semiconductor–oxide interface becomes φS = φT = 2 EF i −E . At e this value of the surface potential, the space-charge region underneath the oxide reaches its maximal width   0  2 0  xdT = 2 φT = (EF i − EF ). eNa e Na A further increase of VG above VT results in an increase of the inversion-layer surface-charge density, but not in an increase of the depletion region. At the threshold voltage VG = VT , the inversion layer just starts to be formed but is not quite there yet. Therefore, we can set at the threshold Qi = 0. The oxide voltage is then VoxT =

eNa xdT − Qss .  Cox

We thus have an expression for the threshold gate voltage VT = VF B +

eNa xdT EF i − EF . +2  Cox e

This expression can be written in other equivalent forms. For example, using the formula for the flat-band voltage, we have VT = ψm − χ +

Eg eNa xdT − Qss EF i − EF − . +  Cox e 2e

We have considered the case of an n-MOSFET here. Derivation of these relations for a p-channel MOSFET, and also for the case when, instead of a metal, a heavily doped p- or n-type semiconductor is used as a gate electrode, can be performed in a similar manner.

10.5 Capacitance–Voltage Measurements

245

10.5 Capacitance–Voltage Measurements A great deal about the MOS structure can be learned from the capacitance–voltage measurements, in which the capacitance between the body and the gate electrodes is measured as a function of the gate voltage. Such measurements are performed by biasing the gate with a dc-voltage VG and measuring the current produced by a weak ac-voltage v(t) = v0 sin(ωt); this current equals i(t) =

dv dQ =C = Cv0 ω cos(ωt), dt dt

where C=

dQ dQ/dt = dv/dt dv

is the MOS capacitance and Q is the charge on the metal electrode. To exclude the influence of the MOS geometry, we will evaluate the capacitance per unit area, C  = C/A, where A = W L, see Fig. 10.3. As before, we focus on the n-MOSFET, i.e., the body is of p-type. Let us assume for now that the frequency ω of the ac-voltage is sufficiently small for the charge carriers in the semiconductor to be able to react to the time-dependent electric field. Three regimes can be distinguished. Accumulation regime, in which the gate voltage is below the flat-band value: VG < VF B . At the typical doping levels Na > 1014 cm−3 , the semiconductor body behaves as a poor conductor, and therefore, it remains under zero potential. Application of a gate voltage below the flat-band value results in an accumulation of holes in a very thin surface layer underneath the oxide, see Fig. 10.7a. The thickness of this layer is of the order of Debye screening length, see Sect. 6.3.2. Since the voltage drop occurs

Fig. 10.7 The MOS structure in the (a) accumulation, (b) depletion, and (c) inversion regime

246

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

mostly across the oxide, the capacitance of the structure equals to that of the oxide layer:  C  (V ) = Cox =

0 ox . tox

Depletion regime, in which the gate voltage is high enough for the depletion region to form near the surface, but insufficient for the formation of the inversion layer, see Fig. 10.7b: VF B < VG < VT . The depletion region width and capacitance per unit area depend on V as  xd =

20 (V − VF B ) 0  , Cd = = eNa xd

 eNa 0  . 2(V − VF B )

The net capacitance now consists of the oxide and the depletion region capacitances connected in series: 1 1 1 =  +   C Cox Cd

⇒ C =

 C Cox d .  + C Cox d

Since Cd decreases with V , so does the total capacitance at VG > VF B . The depletion regime ends when the gate voltage reaches the threshold value, at which an inversion layer forms near the surface. The minimal capacitance per unit area is then   C C  eNa 0   0 ox dT   Cmin =  .  , CdT = x = Cox + CdT 2φT d Inversion regime, in which the gate voltage exceeds the threshold value, VG > VT , resulting in a formation of the inversion layer. Because the whole structure must be electrically neutral, the charge per unit area on the metal electrode, Q = Q/A, is a sum of the magnitudes of inversion-layer charge, Qi = Qi /A, and the charge of the depletion region, QdT = −exdT Na . Thus, Q = exdT Na + |Qi |.

10.5 Capacitance–Voltage Measurements

247

Fig. 10.8 The capacitance–voltage curve of a MOS structure at (a) low-frequency driving, (b) high-frequency driving, and (c) intermediate-frequency driving

20 φT The depletion region has the maximal width xdT = corresponding eNa to the threshold value of the surface potential. Therefore, it does not increase with increasing VG . On the other hand, the charge of the inversion layer grows exponentially strongly with the gate voltage, so that at VG exceeding VT by a small amount, the inversion-layer contribution starts to dominate over the depletion region contribution: Q ≈ |Qi |. Correspondingly, the voltage drop across the depletion region can be neglected, i.e., the main voltage drop occurs across the oxide layer,  , as in the accumulation regime: and the measured capacitance is C  (V ) = Cox  . Q ≈ |Qi | ⇒ C  ≈ Cox

The capacitance–voltage curve for slow driving is sketched in Fig. 10.8a. So far, we assumed that the frequency ω is sufficiently low for the semiconductor charge carriers to react to the time-dependent voltage v(t). The slowest component of the semiconductor charge is the inversion layer, which is formed due to the generation–recombination processes. If the frequency ω is much higher than the inverse recombination time, then the charge density in the inversion layer is unable to follow the temporal variations of the gate voltage. As a result, the inversion layer becomes a thin static charged sheet. Even though it may have an appreciable surface-charge density Qi , it practically does not change in time, making very little contribution to the capacitance C =

dQd /dt dQi /dt + . dv/dt dv/dt

 , see Fig. 10.8b at As a result, the measured capacitance saturates at the value Cmin high frequencies. At the intermediate frequencies, the capacitance at V > VT saturates at some   , which increases as the frequency is decreased, see value between Cmin and Cox Fig. 10.8c.

248

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

10.6 Problems 10.6.1 Solved Problems Problem 1 Determine the flat-band and the threshold voltage of a Si-based nMOSFET with the base doping level Na = 1015 cm−3 , SiO2 insulator of thickness 100 nm and the dielectric constant 3.9. The trapped surface-charge density is 1011 cm−2 . The temperature is 300 K. As the gate electrode polycrystalline n+ -Si is used with the Fermi level higher than the conduction band energy by 0.05 eV, you may assume that the electron affinity of the gate electron is the same as of the MOSFET body. Problem 2 Same as in Problem 1, but this time it is a p-MOSFET, i.e., the body is n-type with the same doping concentration Nd = 1015 cm−3 , and the gate is made of the heavily doped p+ -Si with the Fermi level 0.05 eV below the valence band edge. Problem 3 The experimental capacitance–voltage curve of a Si-based MOSFET is sketched in Fig. 10.9a. Its oxide layer is SiO2 with the dielectric constant ox = 3.9. The gate metal work function is eψm = 4 eV. The temperature is 300 K. Based on this information, determine the following: (a) (b) (c) (d)

Is this a p-MOSFET or an n-MOSFET? What is the oxide layer thickness? What is the semiconductor doping level? What is the surface concentration of trapped charges in the semiconductor– oxide interface?

Problem 4 For an enhancement-mode n-MOSFET biasing shown in Fig. 10.9b, sketch the current–voltage curve, ID vs. VDS , for VGD = 0, 0.5 VT , VT , and 2 VT .

Fig. 10.9 (a) The capacitance–voltage curve of some MOS structure in Problem 3. (b) The biasing of an n-MOSFET in Problem 4

10.6 Problems

249

10.6.2 Practice Problems Problem 1 A MOS capacitor is formed by an n+ -Si/SiO2 /n-Si structure at T = 300 K. The substrate is grounded. The n+ -Si, used as a gate electrode, is doped so heavily that its Fermi energy is above the conduction band edge by E = 0.05 eV. The n-type silicon body is doped at Nd = 1017 cm−3 . The SiO2 layer has thickness tox = 200 nm and a relative dielectric constant of ox = 3.9. On the interface with n-Si, it carries the trapped charges of surface density Qss = 6 · 10−9 C/cm2 . The properties of Si are given in Appendix A.3. Draw the energy band diagram of the structure when a positive voltage VG is applied to the gate. Use this diagram to express the applied gate voltage VG in terms of the characteristic energies, Eg , E, EF EF i , eφS , and eVox . Find the flat-band voltage and the threshold voltage of the device. Problem 2 A p-MOSFET for which W/L = 7, where W is the device width, and L is the source-to-drain distance; the oxide thickness and dielectric constant are tox = 50 nm and ox = 3.9, and the hole mobility near the surface μh = 70 cm2 /(V · s. The device is to be used as a controlled resistor. (a) Calculate the surface-charge density in the inversion channel that is required for the MOSFET resistance between the source and the drain to be 10 k at low (sat) values of VD  VD . Note that at small drain voltage, the inversion-layer surface-charge density Qi is independent on the coordinate x. (b) What gate voltage in excess of the threshold voltage, V = VG − VT , is necessary to maintain the inversion surface-charge density found in part (a)?

10.6.3 Solutions Problem 1 We consider a MOS structure, whose energy band diagrams at zero and positive gate voltage V are shown in Figs. 10.4b and 10.5b, respectively. The work function of the “metal” n+ -Si eψm = eχ − E, E = 0.05 eV. We can directly apply the results obtained in Sects. 10.4.4 and 10.4.5. Namely, the flat-band voltage is given by VF B = ψm − χ −

Eg Q EF i − EF − − ss e 2e Cox

250

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

=−

Eg E EF i − EF Q − − − ss . e e 2e Cox

The second term in the right-hand side of this expression can be evaluated as p0 = Na = ni e(EF i −EF )/kT ⇒

EF i − EF Na = Vth ln e ni

= 0.02585 ln

1015 = 0.3015 V. 8.59 · 109

The oxide layer capacitance per unit area is  Cox =

0 ox 8.854 · 10−14 · 3.9 = = 3.453 · 10−8 F/cm2 . tox 10−5

The voltage drop across the oxide is then VoxF B = −

Qss 1.602 · 10−19 · 1011 =− = −0.4639 V.  Cox 3.453 · 10−8

The flat-band voltage is VF B = −0.05 − 0.3015 −

1.12 − 0.4639 = −1.375 V. 2

We now go on to the threshold voltage VT = VF B +

eNa xdT EF i − EF . +2  Cox e

At threshold, the potential on the semiconductor surface has the threshold value φT = 2

EF i − EF = 2 · 0.3015 = 0.603 V. e

The voltage drop across the oxide layer is now due to not only trapped charges, but also due to the charges of ionized acceptors in the depletion region. The depletion region width has the maximal value  xdT =

 0  2 φT = eNa

8.854 · 10−14 · 11.7 · 0.603 = 0.8831 µm. 1.602 · 10−19 · 1015

The contribution of the SCR to the voltage drop across the oxide is

10.6 Problems

251

Fig. 10.10 The energy-band diagram of a p-MOSFET at (a) VG = 0 and (b) VG < 0

eNa xdT 1.602 · 10−19 · 1015 · 0.8831 · 10−4 = = 0.4097 V.  Cox 3.453 · 10−8 Collecting everything together, we find the threshold voltage to be VT = −1.375 + 0.4097 + 0.603 = −0.362 V. Problem 2 The energy band diagram of the structure at zero and at a negative gate voltage is shown in Fig. 10.10. Because the Fermi level of the gate p+ -Si electrode is below the valence band edge by the amount E = 0.05 eV, its work function, eψm = eχ + Eg + E = 4.05 + 1.12 + 0.05 = 5.22 eV, exceeds the work function of the n-type body, eψs = eχ + EC − EF = eχ + EC − EF i + EF i − EF = eχ + = 4.05 + 0.56 − 0.02585 ln

Eg Nd − kT ln 2 ni

1015 = 4.308 eV. 8.59 · 109

Consider the energy difference between the metal vacuum and the semiconductor Fermi levels. On the one hand, Evac,m − EF s = eψm − eVG , and on the other hand, Evac,m − EF s = −eVox − eφS + eψs . Note that VG , Vox , and φs are all negative. From these two equations, we express the applied voltage in terms of everything else:

252

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

VG = ψm − ψs + Vox + φS . The same relation was obtained for a n-MOSFET in Sect. 10.4.2. In the flat-band  = −0.4639 V, as established in the situation, φS,F B = 0 and Vox,F B = −Qss /Cox previous problem. Hence, VF B = 5.22 − 4.308 − 0.4639 = 0.4481 V. To get the threshold voltage, we need to replace the surface potential with the threshold value φT = −2Vth ln

Nd = −0.6031 V. ni

The depletion region width at threshold is  xdT =

20 |φT | = 0.8832 µm, eNd

and the voltage drop across the oxide layer is VoxT =

−eNs − eNd xdT  Cox

= −1.602 · 10−19

1011 + 1015 · 0.8832 · 10−4 = −0.8739 V, 3.453 · 10−8

 was found in the previous problem. where the numerical value of Cox We can find finally the threshold voltage:

VT = ψm − ψs + VoxT + φT = 5.22 − 4.308 − 0.8739 − 0.6031 = −0.565 V. Problem 3 (a) The measured capacitance–voltage curve shows that the capacitance at V > −0.5 V is higher than the capacitance at V < −5 V. This means that a large negative voltage V < −5 V must be applied to the gate to create an inversion layer. We conclude that the majority carriers in the MOSFET body are electrons, i.e., this is a p-MOSFET with the flat-band and the threshold voltage values of VF B = −0.5 V, VT = −5 V.  = 11.5 nF/cm2 . From this value, we (b) The capacitance of the oxide layer is Cox can find the oxide thickness as

10.6 Problems

253

 Cox =

0 ox 0 ox 8.854 · 10−14 · 3.9 ⇒ tox =  = = 0.3 µm. tox Cox 11.5 · 10−9

 (c) The minimal capacitance Cmin = 8.4 nF/cm2 is formed by the oxide layer, √ and the depletion region at its maximal width xdT = 20 |φT |/(eNd ), where φT = 2Vth ln(Nd /ni ) is the threshold surface potential. We have

1  Cmin

=

C C 1 1 11.5 · 8.4  = 31.16 nF/cm2 . +  ⇒ CdT =  ox min =   Cox CdT Cox − Cmin 11.5 − 8.4

The SCR capacitance per unit area at the threshold surface potential is   CdT

0  = = xdT

0 eNd . 4Vth ln(Nd /ni )

To find the donor concentration from this equation, we rearrange the terms as Nd =

2 4Vth CdT Nd . ln 0 e ni

An iterative solution of this equation starts with a reasonable initial value of Nd , say, Nd = 1018 cm−3 . Its substitution into the right-hand side gives a new value Nd = 1.12 · 1016 cm−3 , which is then substituted again into the right-hand side to further improve the accuracy of the result. This procedure is repeated until convergence is reached, giving the value Nd = 8.34 · 1015 cm−3 . (d) The flat-band voltage is given by VF B = ψm − ψs −

Qss ,  Cox

where the metal work function is known, and the semiconductor work function is ψs = χ +

Eg EF − EF i EC − EF =χ+ − e 2e e

= 4.05 + 0.56 − 0.02585 · ln

8.34 · 1015 = 4.254 V. 8.59 · 109

We obtain  Qss = Cox ·(ψm −ψs −VF B ) = 11.5·10−9 (4−4.254+0.5) = 2.83·10−9 C/cm2 .

254

10 Metal–Oxide–Semiconductor Field Effect Transistor (MOSFET)

This corresponds to the concentration of charges of Qss /e = 1.76 · 1010 cm−2 .

Problem 4 If VG and VD were independent parameters, the current–voltage curve of a MOSFET would depend on the relation between these voltages (see Lecture Notes for details): ⎧ ⎪ VG < VT , ⎪ ⎨0 for   ID (VD ) = Kn 2(VG − VT )VD − VD2 for VD < VG − VT , ⎪ ⎪ ⎩K (V − V )2 for V ≥ V − V . n

G

T

D

G

T

That is, the current is zero in the sub-threshold regime; it increases with VD in the sub-saturation region; and it is constant IDsat = Kn (VG − VT )2 in the saturation regime. For the connection in Fig. 10.9b, the gate and the drain voltages are not independent. Rather, they differ by a fixed amount set by the battery: VG = VD + VDG . The minimal gate voltage required for the current to flow is VT ; otherwise, there is no inversion layer. The current is guaranteed to be zero for VG = VD + VDG < VT , or VD < VT − VDG . At VD ≥ VT − VDG , the current will be increasing with VD according to whether the gain-to-drain voltage is below or above the threshold voltage. If VGD = VG − VD < VT , we are in the saturation regime, in which ID (VD ) = Kn (VG − VT )2 = Kn (VD + VGD − VT )2 . In particular,  for VGD = 0 : ID (VD ) =

for VGD = 0.5 VT : ID (VD ) = and

0 Kn (VD − VT

for VD < VT )2

for VD > VT

 0 Kn (VD − 0.5 VT

,

for VD < 0.5 VT )2

for VD > 0.5 VT

,

10.6 Problems

255

Fig. 10.11 The current–voltage curves of an n-MOSFET from Fig. 10.9b for different values of the gate-to-drain voltage, as indicated near each curve

 for VGD = VT : ID (VD ) =

0

for VD < 0

Kn VD2

for VD > 0.

If VGD = VG − VD > VT , we are in the sub-saturation regime, in which   ID (VD ) = Kn 2(VG − VT )VD − VD2 = Kn 2(VD + VGD − VT )VD − VD2 = Kn (VD2 + 2VD (VGD − VT )). In particular,  for VGD = 2 VT : ID (VD ) =

0

for VD < −VT

Kn VD (VD + 2VT )

for VD > −VT

.

The ID (VD ) curves for all these cases are shown in Fig. 10.11 with the VGD voltage indicated at each curve.

Chapter 11

PN Junction Diode

11.1 The Structure of a pn Junction A pn junction diode is fabricated by letting the doping impurities, say, acceptors, diffuse into a, say, donor-doped substrate. After that, good ohmic contact electrodes must be deposited onto the resulting n- and p-regions, see Fig. 11.1a. For the ease of the discussion, a pn diode is usually schematically represented as an elongated structure, see Fig. 11.1b. Its electronic symbol is shown in Fig. 11.1c. It is immediately obvious that the current–voltage curve of this device should be non-linear. Indeed, if a positive bias is applied to the p-region relative to the n-region, then the majority holes will be pushed from the p-side into the n-side, the majority electrons from the n-side will easily flow into the p-side, and we will have a large current through the structure. If the polarity of bias is reversed—minus to the p-side and plus to the n-side—then it will be the minority electrons in the p-side that will be pushed into the n-side, and minority holes in the n-side that will go to the p-side, meaning that the current will be small. The asymmetry of the current–voltage curve opens the possibility to use a pn junction, e.g., to convert an ac-voltage into a dc-voltage. Other uses of pn diodes are numerous; we will discuss their optoelectronic applications later on. Apart from electrons and holes that are free to move, there are also stationary positively charged donor ions in the n-region and negatively charged acceptor ions in the n-region. They create the charged background that balances the respective charge densities of electrons and holes inside the quasi-neutral p- and n-regions (p-QNR and n-QNR, see Fig. 11.1b). At the interface between the n- and p-type semiconductors, electrons from the n-side and holes from the p-side recombine with each other, and therefore, the interface region contains only a negligibly small concentration of electrons and holes. But it has positively charged donor ions on the n-side and negatively charged acceptor ions on the p-side, forming a kind of capacitor. In other words, the interface region becomes the space-charge region

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_11

257

258

11 PN Junction Diode

Fig. 11.1 (a) The structure of a “real-life” pn junction diode, (b) its schematic representation showing the two quasi-neutral regions (QNRs) separated by the space-charge region (SCR), and (c) the electronic symbol of a pn diode

(SCR) or depletion region. The total charges of the two sides of SCR are equal in magnitude but opposite in sign, so that its total charge is zero. When analyzing the pn junction diode, we will make the following assumptions. We will consider a step homojunction, in which the host lattice in the p- and n-sides is the same and the doping profile is sharp, i.e., the concentration of donors is Nd on the n-side and zero on the p-side, and the concentration of acceptors is Na on the p-side and zero on the n-side. We will assume complete ionization of the impurities with ni  Nd and Na . Finally, we will use the depletion approximation to describe the SCR.

11.2 The Energy Band Diagram of a pn Junction at Zero Bias Consider the case of zero bias. In thermal equilibrium, the Fermi energy must be uniform throughout the pn structure. But on the p-side, EF is closer to the valence band edge, and on the n-side, it is closer to the conduction band edge. This implies that the energy bands must bend in the SCR to maintain the uniformity of Fermi energy, see figure showing the energy band structure of a pn junction at zero bias. Physically, the bands are bent because the electrons from the n-part of the diode diffuse into the p-part, where they recombine with the holes. Vice versa, the holes from the p-side diffuse into the n-side and recombine with the electrons there. As a result, only the positively charged donor ions and negatively charged acceptor ions remain on the two sides of the junction in the SCR. Hence, the SCR represents a charged capacitor with a built-in voltage, Vbi , developed across it. The magnitude of Vbi can be established from the following considerations. In the presence of a non-uniform electric potential in a semiconductor, the electron concentration is given by n0 (x) = n0n eφ(x)/Vth , n0n = Nd ,

11.2 The Energy Band Diagram of a pn Junction at Zero Bias

259

where n0n = Nd is the electron concentration in the n-part, assumed to be grounded. From this, we conclude that electron concentrations in the p-region are given by n0p = Nd e−Vbi /Vth . On the other hand, by the mass action law, n0p =

n2i , p0p = Na , p0p

where p0p = Na is the majority hole concentration in the p-region far away from the SCR boundary. Combining these two expressions for n0p , we find Nd e−Vbi /Vth =

n2i Na Nd ⇒ Vbi = Vth ln . Na n2i

If the two sides of the junction are connected by a conducting wire, the builtin voltage will not cause an electric current to flow through it. The existence of such a current would contradict the law of energy conservation. The physical reason why the built-in voltage cannot produce an current is that there would be additional semiconductor band bending in the metal–semiconductor contact regions on the pand n-sides, see Fig. 11.2a. These two contact regions will be characterized by their own values of the built-in voltage, so that the three built-in voltages, which add up to zero with the built-in voltage in the pn junction region.

Fig. 11.2 (a) A pn diode at zero bias (top) and its energy band diagram (bottom). (b) A pn diode under a non-zero bias (top), together with the electric potential and electric field distribution within the structure (bottom)

260

11 PN Junction Diode

For the same reason, touching the two ends of a pn diode with two terminals of a voltmeter will show zero voltage, not Vbi . The built-in voltage can be found by measuring the voltage-dependent capacitance, similar to the metal–semiconductor case.

11.3 PN Junction Under an External Bias Consider what happens when a bias V is applied to the p-side of a pn diode, see Fig. 11.2b. A forward bias, V > 0, reduces the potential barrier that prevents the majority carriers from entering the opposite side of the junction, whereas a reverse bias, V < 0, increases this barrier. We will focus on the practically interesting case when the applied bias is smaller than the built-in voltage, V < Vbi , meaning that the SCR exists in the pn structure. In the less interesting opposite case, V > Vbi , the diode will behave more or less according to Ohm’s law. Because the QNRs have a considerable number of mobile charge carriers, the voltage drop across them is negligible. But this is not so in the SCR, which is depleted of the free charge carriers. Hence, the voltage drop V occurs practically completely across the SCR. To find out how the potential changes in the diode, we adopt the depletion approximation, see Sect. 6.3.3. Namely, we assume that there are no free charge carriers in the SCR, which has abrupt boundaries at x = −xp and x = xn , see Fig. 11.2b. Outside of the SCR (i.e., at x < −xp and x > xn ), the charge density ρ(x) is zero, and inside the SCR, it is approximated by  ρ(x) =

−eNa

at − xp < x < 0

eNd

at 0 < x < xn

.

Within the depletion approximation, we must impose the boundary conditions for the SCR boundaries: φ(−xp ) = V − Vbi , φ(xn ) = 0,

dφ dφ (x = −xp ) = (x = xn ) = 0. dx dx

With these boundary conditions, the solution of Poisson’s equation reads  φ(x) =

eNa 2 20  (x + xp ) + V eNd (x − xn )2 − 2 0

− Vbi

at − xp < x < 0 at 0 < x < xn

.

11.3 PN Junction Under an External Bias

261

The first derivative of the electric potential is related to the electric field:  − eNa (x + xp ) dφ(x) E(x) = − = eN0  d dx 0  (x − xn )

at − xp < x < 0 at 0 < x < xn

.

It remains to determine the SCR boundaries, xn and xp . First, we note that electric field must be continuous at x = 0, i.e., E(x = 0) must have the same value if one uses the upper and lower expressions for E(x). This immediately gives Na xp = Nd xn . This equality expresses the fact that the net charge of the negatively ionized acceptors in the left part of the SCR must be compensated by the positive charge of ionized donors in its right part, so that the SCR is electrically neutral. In addition, the potential must be continuous at x = 0, i.e., φ(x = 0) must have the same value if one uses either expression for φ(x). This gives eNa 2 eNd 2 xp + V − Vbi = − x . 20  20  n Solving the two equations for two xp and xn , we obtain  xp =

0 (Vbi − V ) Nd 2 , xn = e(Na + Nd ) Na

 2

0 (Vbi − V ) Na . e(Na + Nd ) Nd

The total width of the SCR is, then,  w = xp + xn =

0 (Vbi − V ) Na + Nd 2 = e Nd Na

 2

0 (Vbi − V ) , eN

where 1 1 1 Nd Na = + ⇒ N= . N Nd Na Nd + Na The maximal (in magnitude) built-in electric field is realized at x = 0. It is given by several equivalent expressions: Emax

 eNa xp eNd xn 2eN Vbi − V =− =− (Vbi − V ) = −2 . = E(0) = − 0  0  0  w

262

11 PN Junction Diode

11.4 SCR Capacitance The insulating SCR is sandwiched between the two conducting QNRs. It can be modeled as a parallel-plane capacitor of thickness w. Its capacitance per unit area is  0  C = = w

e0 N , 2(Vbi − V )

where we used the expression for w obtained in the previous section. Note that the inverse capacitance squared 1 2 (Vbi − V ) = e0 N C 2 depends linearly on the applied voltage, see Fig. 11.3. It becomes zero at V = Vbi . The slope of this straight line is −

Nd + Na 2 = −2 . e0 N 0 eNd Na

Thus, the measurements of C  vs. V allow one to determine the product Nd Na (present in Vbi ) and the sum Nd + Na (present in the slope of 1/C 2 vs. V ). If one knows which side is doped more heavily, one can determine the doping concentrations Na , Nd . A one-sided junction is a highly non-symmetrically doped pn junction, where either Na  Nd or Nd  Na . In the former case, it is denoted as p+ n junction, and in the latter case as pn+ junction. It follows from the neutrality condition xp Na = xn Nd that the depletion layer penetrates primarily into that side that is doped more Na lightly. Indeed, if, e.g., Na > Nd , then xn = xp N > xp . If Na  Nd , we can d + approximate N with Nd to a good accuracy. For a p n junction, the expressions for SCR width and capacitance simplify to Fig. 11.3 The inverse square of the capacitance per unit area of the SCR in a pn junction diode as a function of the applied voltage

11.5 Current–Voltage Relation of a pn Junction Diode

 w = xn =

0 (Vbi − V ) 2 , C = eNd

263

 e0 Nd . 2(Vbi − V )

These expressions are identical to the ones obtained in the discussion of a junction formed by metal and an n-type semiconductor, see Sect. 9.3. In the opposite case of a pn+ junction, the respective expressions are the same, but with Nd replaced by Na .

11.5 Current–Voltage Relation of a pn Junction Diode 11.5.1 Charge Carrier Concentrations Near the Boundaries of the SCR When an external voltage V is applied to a pn junction diode, an electric current will flow through it. Even though the system as a whole is out of equilibrium, its electron and hole subsystems find themselves in local thermodynamic equilibria separately. This is so because equilibration of electrons belonging to the same band proceeds much faster than equilibration between different bands. The former involves intraband scattering processes, where electrons exchange energy in small portions, and the latter requires the much slower generation–recombination processes, in which electrons exchange large amounts of energy of the order of the band gap energy Eg . With this in mind, we can use the language of the electron and hole quasi-Fermi energies (see Sect. 7.7), EF e and EF h , in the p- and n-sides of the pn junctions. Consider the p-side. Far away from the SCR boundary, x  −xp , the minority electrons exchange energy only with the majority holes, and therefore both electrons and holes have a common Fermi energy EFp , which is different from the n-side counterpart, EF n . But near the SCR boundary, the minority electrons on the p-side “communicate” with the majority electrons from the n-side much more efficiently than with the majority holes. This is so because the SCR is so thin that electron transport through it occurs very swiftly. From this, we can conclude that the minority electrons near the SCR boundary at x = −xp must have the same quasi-Fermi energy EF n as the electrons on the n-side of the junction. As we move deeper into the p-QNR, the electron quasi-Fermi energy aligns itself with the hole counterpart, see Fig. 11.4. The same reasoning applies to the minority holes on the n-side. Hence, far away from the SCR boundaries, the minority carrier concentrations are np =

n2i n2 , pn = i . Na Nd

Note that we dropped the subscript 0 because the system is not in equilibrium. Near the SCR edges, the minority concentrations differ from these values. Namely,

264

11 PN Junction Diode

Fig. 11.4 The energy band diagram of a biased pn junction diode, showing the electron and hole quasi-Fermi energies

because the potential difference across the SCR is Vbi − V , and because the carriers of the same type on the two sides of the SCR have the same quasi-Fermi energy, we can relate the electron and hole concentrations on the two sides of the SCR to each other by n(−xp ) = n(xn )e−(Vbi −V )/Vth = Nd e−(Vbi −V )/Vth =

n2i V /Vth e , Na

p(xn ) = p(−xp )e−(Vbi −V )/Vth = Na e−(Vbi −V )/Vth =

n2i V /Vth e . Nd

In the last step of both lines, we used the expression for Vbi obtained in Sect. 11.2. These formulas are called Shockley boundary conditions. We will use them to derive the current–voltage relation of a pn junction diode. It follows from the Shockley boundary conditions that the product n(−xp )p(−xp ) = n(−xp )Na = n2i eV /Vth . On the other hand, it is given by n(−xp )p(−xp ) = n(−xp )Na = n2i e(EF e −EF h )/kT . It then follows that the difference of quasi-Fermi energies is just the applied voltage multiplied by the elementary charge: EF e − EF h = eV .

11.5.2 Current–Voltage Relation of an Ideal pn Junction Diode To figure out the J − V curve of a pn junction diode, we will need a relation between the charge carriers’ concentration and the current density. It is convenient to introduce the excess concentrations of electrons and holes as

11.5 Current–Voltage Relation of a pn Junction Diode

265

Δn = n − n0 , Δp = p − p0 . In terms of the excess concentrations, Shockley boundary conditions read Δn(−xp ) =

n2i V /Vth n2 (e − 1), Δp(xn ) = i (eV /Vth − 1). Na Nd

Let us focus on the QNR on the n-side of the junction, where the excess minority hole concentration is described by the continuity equation (see Sect. 8.8): ∂Δp ∂ 2 Δp Δp = Dhn − at x > xn . ∂t τhn ∂x 2 There is no drift current because the electric field in the QNRs is zero. Dhn is the hole diffusion coefficient, and τhn is the hole recombination time in the quasineutral n-region. The derivative ∂Δp/∂t equals zero because we are interested in the steady-state situation when the excess concentrations and current densities are time-independent. Thus, we have Dhn

∂ 2 Δp Δp − = 0 at x > xn . τhn ∂x 2

Since the steady-state continuity equation is a second-order differential equation, it must be supplemented by two boundary conditions. One is provided by the Shockley boundary condition for Δp(xn ) written above. The other one says that far away from the junction boundary in the quasi-neutral n-region, the hole concentration must approach its equilibrium value, meaning that the excess hole concentration approaches zero: Δp(x → ∞) = 0. The solution of hole continuity equation that respects both boundary conditions is Δp(x) = Δp(xn )e−(x−xn )/Lhn =

n2i V /Vth (e − 1)e−(x−xn )/Lhn at x > xn . Nd

Here, Lhn =

Dhn τhn

is the so-called hole diffusion length in the n-region. We treat excess minority electrons in the p-region in the same manner. The respective diffusion equation in the steady state reads

266

11 PN Junction Diode

Dep

∂ 2 Δn Δn − = 0 at x < −xp , τep ∂x 2

where Dep and τep are the diffusion coefficient and lifetime of electrons in the p-region. In addition to the Shockley boundary condition for Δn(−xp ), we also require that Δn(x → −∞) = 0. With these boundary conditions, the solution of the continuity equation is Δn(x) = Δn(−xp )e(x+xp )/Lep =

n2i V /Vth (e − 1)e(x+xp )/Lep at x < −xp , Na

where the electron diffusion length in the p-region is defined as Lep =

Dep τep .

Once we know the excess concentrations, we can determine the respective diffusive flux densities: jhn (x) = −Dhn

n2 ∂Δp Dhn −(x−xn )/Lhn = i (eV /Vth − 1) e for x > xn , ∂x Nd Lhn

jep (x) = −Dep

n2 Dep (x+xp )/Lep ∂Δn = − i (eV /Vth − 1) e for x < −xp . ∂x Na Lep

Setting x to xn in the first expression gives the number of holes that pass through the SCR per unit area per unit time. Likewise, setting x to −xp in the expression for jep (x), we obtain the number of electrons that pass through the SCR per unit area per unit time. Multiplication of the hole flux density expression by e and the respective electron flux density by −e gives the hole and electron contributions to the current density through the SCR: Jh = ejhn (xn ) = e

n2i Dhn V /Vth (e − 1), Nd Lhn

Je = −ejep (−xp ) = e

n2i Dep V /Vth (e − 1). Na Lep

The total electric current through the pn diode structure must be uniform, i.e., independent of x. Hence, the total electric current density through any part of the structure is the same as through the SCR, J = Jh + Je ,

11.5 Current–Voltage Relation of a pn Junction Diode

267

Fig. 11.5 (a) The J − V curve of an ideal pn junction diode. (b) The electron and hole contributions to the net electric current density as functions of the position x in the diode

giving the ideal pn junction J − V curve: J (V ) = JS (eV /Vth − 1), see Fig. 11.5a. The reverse saturation current is  JS =

en2i

Dep Dhn + Nd Lhn Na Lep



 =

en2i

 1 Nd

Dhn 1 + τhn Na



Dep τep

 .

At large reverse bias, the current density attains the value −JS , and at forward bias 0 < V < Vbi , it increases exponentially with V , see Fig. 11.5a. The current–voltage relation of an ideal pn junction diode is the same as that of an ideal Schottky diode, see Sect. 9.5. However, the saturation current density of the pn diode is several orders of magnitude lower than that of a Schottky diode. The reason is that the current is formed by the minority carriers in the pn diode and by the majority carriers in the Schottky diode.

11.5.3 Current Densities in a pn Diode Coming back to our general expressions for the minority particle current densities and multiplying them by the respective charges, we obtain the x-dependent electric current densities of minority electrons in the p-region and minority holes in the nregion as exponentially decaying functions of distance from the SCR edges: Jhn (x) = e

n2i V /Vth Dhn −(x−xn )/Lhn (e − 1) e for x > xn , Nd Lhn

Jep (x) = e

n2i V /Vth Dep (x+xp )/Lep (e − 1) e for x < −xp . Na Lep

268

11 PN Junction Diode

The total current through the structure, J , must be constant. This is only possible if there are additional contributions to the current density due to the majority charge carriers. For majority electrons in the n-region and majority holes in the p-region, we have \$ % Dep Dhn  2 −(x−xn )/Lhn Jen (x) = J − Jhn (x) = eni 1−e + (eV /Vth − 1) Nd Lhn Na Lep \$ % Dep  Dhn 2 (x+xp )/Lep (eV /Vth − 1). Jhp (x) = J − Jep (x) = eni 1−e + Na Lep Nd Lhn Physically, the onset of the majority currents can be understood as follows. Consider the n-side of the junction, x = xn . At the edge of the SCR, the excess minority holes are injected from the p-region, where they are the majority carriers. Starting from x = xn , the minority holes diffuse into the bulk of the n-region, recombining with the majority electrons on the way. To compensate for this loss of the electrons, electrons have to diffuse from the bulk of the n-region toward the SCR boundary, creating an additional current density Jen . Similar reasoning applies, of course, to the majority hole current density on the p-side, see Fig. 11.5b.

11.5.4 SCR Recombination Current So far, we considered an ideal pn junction diode. Let us consider the deviation from the ideal behavior due to the generation–recombination processes in the SCR. The average electron and hole concentrations in the SCR are related by the mass action law, nSCR pSCR = n2i e(EF e −EF h )/kT = n2i eV /Vth , see the end of Sect. 11.5.1. Because recombination requires both electrons and holes, it is reasonable to assume that the largest recombination rate in the SCR occurs at that position where their concentrations are equal: nSCR = pSCR = ni eV /(2Vth ) . With the charge carrier lifetime in the SCR, τSCR , we can write the total recombination rate as RSCR (V ) =

ni eV /(2Vth ) . τSCR

Generation of carriers is a voltage-independent process that proceeds at a constant rate, GSCR . When V = 0, it must exactly balance the recombination rate. Thus, the generation rate is

11.6 Problems

269

GSCR = RSCR (V = 0) =

ni τSCR

.

The net SCR recombination rate is USCR = GSCR − RSCR =

ni τSCR

(eV /(2Vth ) − 1).

The rate of change of electron and hole concentrations due to the generation– recombination in the SCR is     dn dp ni  V /(2Vth ) Aw e = Aw = AwUSCR = Aw −1 . dt SCR dt SCR τSCR In the steady state, (∂n/∂t)SCR = (∂p/∂t)SCR = 0; this must be compensated by additional electron and hole currents that flow from the n- and p-sides into the SCR. These additional currents produce the recombination current density  ni JSCR (V ) = JS eV /(2Vth ) − 1 , JS = ew . τSCR The total current density is the sum of the two contributions, J (V ) = JS (eV /Vth − 1) + JS (eV /(2Vth ) − 1). At large bias, V , the second term can be neglected, and the J − V curve resembles the one of an ideal pn junction. But at small voltage, the SCR-related second term becomes important. The current–voltage curve of a real diode is often described phenomenologically by introducing the ideality factor, n, as J (V ) = JS (eV /(nVth ) − 1). The value n = 1 corresponds to an ideal diode; the typical value of the ideality factor is somewhere between 1 and 2.

11.6 Problems 11.6.1 Solved Problems Problem 1 The capacitance per unit area of a silicon pn junction at V = 0 is C  = 0.394 nF/cm2 ; at V = −0.5 V, it is C  = 0.283 nF/cm2 . The n-side is doped more heavily than the p-side. Find the doping levels Na and Nd .

270

11 PN Junction Diode

Problem 2 A silicon pn junction has the donor and acceptor concentrations of Nd = 2 · 1015 cm−3 and Na = 8 · 1015 cm−3 on the two opposite sides of the junction. Determine the minority carrier concentrations at the edges of the spacecharge region for V = 0.5 V and −0.5 V. Problem 3 Consider an ideal Si-based pn junction diode at 300 K. The doping levels on the two sides are Nd = 1012 cm−3 , Na = 1017 cm−3 , and the minority carriers mobilities in the respective regions are μep = 760 cm2 /(V · s), μhn = 500 cm2 /(V · s). The current density for a forward bias V = 0.2 V is 2.3·10−4 A/cm2 . Determine the minority hole lifetime in the quasi-neutral n-region.

11.6.2 Practice Problems Problem 1 A pn junction diode is made of an unknown semiconductor. Its capacitance–voltage measurements performed at two different temperatures, T1 = 290 K and T2 = 310 K, revealed the values of the built-in voltages Vbi (T1 ) = 2.38 V and Vbi (T2 ) = 2.44 V, respectively. Find the band gap of this semiconductor material. Problem 2 In the discussion of an ideal pn junction diode, we assumed the resistance of the QNRs to be zero. In reality, it is small, but finite. It can be modeled as a series resistance connected to an ideal diode as shown in Fig. 11.6. Express the voltage V applied to the diode as a function of the current I through it. What is the slope dV /dI of the V (I ) curve at zero current? What is the value of the current when a large voltage V is applied in the reverse direction? What is the slope of the V (I ) curve when the voltage V in the forward direction is large? Problem 3 The doping concentrations in a silicon pn junction diode are Nd = 1016 cm−3 and Na = 1017 cm−3 . At a forward bias V , the minority carrier concentration on one side of the SCR is one-tenth of the majority concentration and exceeds the minority concentration on the opposite side. Find V . Problem 4 Consider a non-ideal Si pn junction diode, as described in Sect. 11.5.4. Assume the following parameter values Nd = Na = 101 5 cm−3 , τep = τhn = 10−5 s, τSCR = 10−7 s, Dep = Dhn = 10 cm2 /s, T = 300 K. The total J − V curve contains the ideal-diode part and the recombination current in the SCR, J (V ) = Jid (V ) + JSCR (V ),

Fig. 11.6 The effect of a finite resistance of the QNRs modeled as a resistance Rs connected in series to the diode

11.6 Problems

271

as explained in Sects. 11.5.2 and 11.5.4, respectively. How are the conductances id (V )/dV due to these two mechanisms related? In other words, find the ratio dJdJSCR (V )/dV at V = 0.

11.6.3 Solutions Problem 1 The inverse capacitance squared as a function of voltage is 1 2 Na + Nd Na Nd = (Vbi − V ), Vbi = Vth ln . 2 e  N N C n2i 0 a d It is convenient to denote S = Na + Nd , P = Na Nd . The graph of 1/C 2 vs. V is a straight line with the slope given by (2/e0 )S/P . Its intercept with the x-axis is Vbi = Vth ln(P /n2i ), from which P can be found as P = n2i eVbi /Vth . Since we have just two data points, the straight line fit is particularly easy. Namely, at V = 0, we have 1/C 2 = 6.442 · 1018 cm4 /F2 , and at V = −0.5 V, we have 1/C 2 = 12.49 · 1018 cm4 /F2 . The straight line fit can be found based on this information: 4 4 1 18 cm 18 cm = −kV + b, k = 12.1 · 10 . , b = 6.442 · 10 C 2 F2 · V F2

From this, we obtain the built-in voltage Vbi =

b = 0.5326 V k

and the product of the doping concentrations: P = n2i eVbi /Vth = (8.59 · 109 )2 e0.5326/0.02585 = 6.546 · 1028 cm−6 . From the slope k of the 1/C 2 vs. V dependence, we find the sum of the doping concentrations as S=

1 e0 P k = 6.572 · 1016 cm−3 . 2

272

11 PN Junction Diode

It remains to solve two equations: Na Nd = P , Na + Nd = S with Nd > Na . We express Na in terms of Nd using the first equation and plug in the result into the second equation: Na =

P , Nd



P S + Nd = S ⇒ Nd2 − SNd + P = 0 ⇒ Nd = − + Nd 2

S2 − P. 4

Numerically, Nd =

6.572 · 1016 + (3.286 · 1016 )2 − 6.546 · 1028 = 6.57 · 1016 cm−3 , 2

Na =

6.546 · 1028 = 9.96 · 1011 cm−3 . 6.572 · 1016

Problem 2 The Shockley boundary conditions (see Sect. 11.5.1) give n0 (−xp ) =

n2i V /Vth n2 e , p0 (xn ) = i eV /Vth . Na Nd

A positive applied voltage exponentially enhances the minority carriers’ concentration relative to their equilibrium values. Plugging in the numbers, we obtain n2i n2i (8.59 · 109 )2 (8.59 · 109 )2 −3 = = 9 223 cm , = = 36 894 cm−3 , Na Nd 8 · 1015 2 · 1015 eV /Vth = e0.5/0.02585 = 2.514 · 108 , e−V /Vth = e−0.5/0.02585 = 3.979 · 10−9 , and thus at V = 0.5 V n0 (−xp ) = 9 223 · 2.514 · 108 = 2.32 · 1012 cm−3 , p0 (xn ) = 36 894 · 2.514 · 108 = 9.28 · 1012 cm−3 . At V = −0.5 V, n0 (−xp ) = p0 (xn ) = 0 for all practical purposes. Problem 3 Assuming the ideal current–voltage relation, J (V ) = JS (eV /Vth − 1), we find the reverse saturation current density (with V = 0.2 V):

11.6 Problems

JS =

273

2.3 · 10−4 J (V ) = = 1.004 · 10−7 A/cm2 . eV /Vth − 1 e0.2/0.02585 − 1

From the theory of the pn junction diodes, the reverse saturation current density is given by the formula 

n2i JS = e Na



n2 Dep + i τep Nd

 Dhn τhn

 ,

and because Nd  Na (by 100 000 times), i.e., 1/Nd  1/Na , we expect that the second term in the brackets produces a much higher contribution to JS than the first term. We thus can approximate n2 JS = e i Nd

 Dhn , τhn

from which the minority hole lifetime is found as 

τhn

n2 = e i Nd

2

 2 n2i Dhn Vth μhn = e , Nd JS2 JS2

where we used Einstein’s relation D = μVth in the second equality. Numerically, 

−19

τhn = 1.602 · 10

(8.59 · 109 )2 · 1012

2

0.02585 · 500 = 3.29 · 10−7 s = 0.179 µs. 1.008 · 10−14

Chapter 12

Optoelectronic Devices

12.1 Solar Cells (SCs) 12.1.1 SC Operation The simplest solar cell (SC) is based on a pn junction diode, see Fig. 12.1. The principle of its operation can be readily understood if we recall a few basic facts about the diode. It consists of two quasi-neutral regions (QNRs) separated by a space-charge region (SCR) with the built-in electric field directed from the n- to the p-part of the diode. The top QNR is referred to as emitter, and the bottom one as base. The incident light generates excess electron–hole pairs in the diode. The excess electrons and holes diffuse toward the SCR, where they get separated by the built-in electric field. The excess electrons produced in the p-QNR are transferred into the n-QNR, and the excess holes generated in the n-QNR are transferred into the p-QNR. As a result, the two parts of the diode become oppositely charged, allowing one to produce electric power. If we connect the two sides of the SC with a wire with zero electric resistance, the so-called short-circuit current, ISC , will flow from the p-side to the n-side as the system will try to restore the thermal equilibrium perturbed by the irradiation. If the emitter and the base are disconnected, the two sides of the diode will be charging up. This process cannot continue indefinitely for two reasons. First, the transfer of the photogenerated holes into the p-side and electrons into the n-side of the SC results in the generation of an additional electric field from the p- to the nside of the diode; this additional electric field counteracts the built-in electric field. Second, the photogenerated electron–hole pairs recombine with each other at a finite rate. As a result, the charging-op of the two sides of the SC eventually stops, and a voltage develops across the SC. This voltage is called the open-circuit voltage, VOC , with the p-side being positive and the n-side negative.

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4_12

275

276

12 Optoelectronic Devices

Fig. 12.1 The structure of a solar cell

12.1.2 Spectral Irradiance (Spectral Intensity) A photon of frequency f and wavelength λ = c/f carries the energy hf =

1.24 eV · µm hc ≈ . λ λ

The short-wavelength photons interact primarily with the valence electrons by promoting them to the conduction band, provided that the photon energy exceeds the band gap energy. The visible light spectrum covers the range of λ from about 450 nm (violet) to about 700 nm (red), which corresponds to the energies from about 1.5 eV to about 3 eV, which is similar to the typical semiconductor band gap energies. The longer-wavelength (and hence smaller-energy) photons interact primarily with the lattice vibration quanta, the phonons. Because this interaction is relatively weak, semiconductors are for the most part transparent to the long-wavelength photons with hf < Eg . Light is quantified by a parameter called spectral irradiance, also called spectral intensity, F (f ). It is related to the power dP (f ) carried by photons of frequency between f and f + df through a unit surface area: F (f ) =

dP (f ) . df

In other words, it is the energy flux density per unit frequency interval. It is measured in [F (f )] = W/(m2 · s−1 ) = J/m2

12.1 Solar Cells (SCs)

277

in the SI units. The total intensity, i.e., the power incident per unit surface area, is obtained by integrating the spectral intensity with respect to frequency:  F =

df F (f ) , [F ] = W/m2 .

0

The photon flux density (f ) is defined though the number dN(f ) of photons of frequency between f and f + df passing per unit time through a unit surface area: (f ) =

F (f ) dN(f ) = . df hf

The light spectral intensity can also be defined as a function of the wavelength: namely, F (λ) is the energy flux (i.e., the energy transferred per unit time through a unit surface area) per unit wavelength interval. That is, if dP (λ) is the energy flux carried by the photons with the wavelength between λ and λ + dλ, then F (λ) =

dP (λ) . dλ

It is measured in [F (λ)] = W/m3 in the SI units. However, since it is more convenient to measure the wavelength in µm or nm, F (λ) is often measured in W/(m · µm) or W/(m · nm). Note that the two quantities, F (f ) and F (λ), are not related to each other by a simple replacement of f with c/λ. Their relation can be obtained by noting that the energy contained in a frequency interval df is dP = F (f )|df | = F (λ)|dλ| . The reason why the magnitude of the frequency and wavelength intervals is used rather than df and dλ themselves is that it follows from the relation f = c/λ that df = − λc2 dλ. The minus sign indicates that an increase of frequency by df means a decrease of the wavelength by dλ. In order to have both F (f ) and F (λ) positive, the minus sign is omitted. Then, the relation between the two kinds of the spectral irradiance is found from F (f )|df | = F (f )

c λ2 . |dλ| = F (λ)|dλ| ⇒ F (f ) = F (λ) c λ2

Likewise, F (λ) = F (f )

f2 . c

278

12 Optoelectronic Devices

Fig. 12.2 The solar spectrum just outside of the Earth’s atmosphere (AM0 spectrum, gray curve) and on the Earth’s surface when the Sun is 48◦ above the horizon (AM1.5G spectrum, black curve)

The power transmitted by the photons of frequencies between fmin and fmax through a unit surface area per unit time is  P =

fmax

fmin

 df F (f ) =

λmax

dλ F (λ) , λmin

where λmin = c/fmax and λmax = c/fmin . The solar spectral intensity in the outer space just above the Earth’s atmosphere is shown as a gray curve in Fig. 12.2. This spectrum is denoted as AM0 spectrum, where AM stands for “air mass.” The solar spectrum on the Earth depends on the time of the day and the geographic location. The current standard spectrum adopted to test the solar cells is the AM1.5G spectrum, which is obtained when the path length traveled by light through the atmosphere is 1.5 times as long as at the normal incidence; the G stands for “global.” Note that the AM1.5G peak intensity is somewhat lower than the AM0 peak intensity, and the AM1.5G spectrum contains a number of minima that are not found in the AM0 counterpart. This is due to the light scattering and absorption by the atmosphere. The total irradiance received by the Earth under the AM1.5G conditions is 1000.4 W/m2 .

12.1.3 Light Absorption When monochromatic light is passing through a semiconductor, it gets absorbed by it. Hence, light intensity should decrease with the distance x from the front surface

12.1 Solar Cells (SCs)

279

of the material. This is quantified by the light absorption coefficient α(λ), defined as the fraction of photons of a given wavelength λ that are absorbed per unit length. It is measured in the units of inverse length, [α] = cm−1 . If the light spectral irradiance at a particular wavelength λ at the distance x from the surface was F (x), then at a slightly larger distance x + dx is smaller by the amount dF (x) = F (x + dx) − F (x) = −α(λ)F (x) dx ⇒

dF (x) = −α(λ)F (x) . dx

The solution of this differential equation is the so-called Bouguer–Lambert–Beer law (Bouguer, early 1700s; Lambert, 1730; Beer, 1852), F (x) = F0 e−α(λ)x , where F0 = F (x = 0) is the intensity of the incident light. After passing through a slab of thickness L, the transmitted light intensity will be F0 e−αL , and the energy absorbed per unit time by a unit surface area of the material will be F0 (1 − e−αL ). Absorption coefficient depends strongly on the wavelength and the material type, see Fig. 12.3 showing the α(λ) curve of silicon. Note that it goes sharply to zero at the photon energy near the band gap energy.

Fig. 12.3 Absorption coefficient of Si at T = 300 K

280

12 Optoelectronic Devices

The dominant absorption mechanism of photons whose energy exceeds the band gap energy is electron–hole pair generation. Assuming that one such photon creates just one electron–hole pair, the respective generation function can be estimated as  G(x) =

df Eg / h

α(f )F (f, x) , hf

where F (f, x) is the spectral intensity of light at the frequency f and distance x from the front surface. Strictly speaking, the integral has to be multiplied by the socalled efficiency factor (less than 1) to take care of the fact that a photon can also be absorbed without the electron–hole pair production. For example, a photon can be absorbed by a free charge carrier. We will neglect the effect of such forms of photon absorption. The light spectral intensity F (f, x) at a distance x from the front surface is related to the spectral intensity F0 (f ) of the incident light. In order to maximize the generation function G(x), both the front and rear surfaces of the SC are often made corrugated. This means that a photon that reaches the rear surface gets reflected at some angle to the normal. If it then reaches the front surface without absorption, it again has a good chance of being reflected at a different angle. Photons whose energy is only slightly higher than the band gap energy are absorbed very weakly by the material, see Fig. 12.3. They perform many back-and-forth trips between the front and rear surfaces before they produce an electron–hole pair. The result is that the light intensity F (f, x) differs from the simple exponential function.

12.1.4 SC Current–Voltage Relation The current–voltage (I − V ) curve of a SC can be obtained from the diode I − V relation in the absence of radiation, the so-called dark I − V curve. Assuming the SC to be a non-ideal diode with the ideality factor n, its dark current is Idark (V ) = −IS (eV /(nVth ) − 1) , where IS is the reverse saturation current. Note that here we adopt a different sign convention than the one used in the discussion of the diodes, see Sect. 11.5.2. Because the photogenerated current flows in the reverse direction, it is convenient to treat the reverse current direction as positive; therefore, we have changed the sign of the dark current. When the SC is illuminated, light generates an additional current, IL . The simplest connection of a SC to an external load is shown in the right part of Fig. 12.4. The current through the resistance R depends on R, and the voltage across the SC is V = IR .

12.1 Solar Cells (SCs)

281

Fig. 12.4 Connection of a SC to a load R (left) and the current–voltage and power–voltage curves (right)

The current–voltage relation in the presence of illumination becomes I (V ) = IL − IS (eV /(nVth ) − 1) , see the right part of Fig. 12.4. As the load R varies from 0 to ∞, the current changes from the short-circuit current ISC = IL at R = 0 to I = 0 at R = ∞ . At the same time, the voltage will change from V = 0 at R = 0 to the open-circuit voltage 

V = VOC

 IL = nVth ln + 1 at R = ∞ . IS

The open-circuit voltage is found from the condition I (VOC ) = 0, as no current is flowing if R = ∞. The power delivered to the load is given by the product P = V I (V ) = V (IL − IS (eV /(nVth ) − 1)) .

282

12 Optoelectronic Devices

It is a non-monotonic function of voltage, see Fig. 12.4. The maximal power delivered to the load can be found by taking derivative: V V /(nVth ) V V /(nVth ) dP e = I (V ) − IS e . = IL − IS (eV /(nVth ) − 1) − IS dV nVth nVth Setting this derivative to zero, we obtain an equation for voltage at maximal power, Vm : IL +1= IS



 Vm + 1 eV /(nVth ) , nVth

which can be solved iteratively. Once Vm is found, the current in the maximal-power regime can be determined by a substitution of Vm into the expression for current, Im = I (Vm ). The fill factor of the I − V curve is defined as the ratio FF =

Im Vm · 100 % . ISC VOC

It measures the deviation of the I − V curve from a rectangular shape. Typically, F F has the value between 70% and 80%. Finally, the photoconversion efficiency is defined as the ratio of the maximal power produced by the SC to the power incident onto the cell in the form of light: η=

Im Vm · 100 % . Pin

Depending on the SC type, photoconversion efficiency ranges from a few percent to about 25% or even 40%. Because solar intensity on the Earth surface is about 1000 W/m2 , a solar panel of 1 m2 area and 10% efficiency can produce the power of 100 W, which is comparable to the power consumption by a TV set. On average, a typical North American household consumes about 900 kWh per month, i.e., the average power consumed is about 1250 W. In order to provide this power, about 12 m2 area must be covered with SCs. This is two or three times smaller than the area of a typical roof of a private household. The price to install solar panels on a roof of a building is about \$15K, but it pays off in saving on the electricity bills after about 5 years. Of course, these estimates may turn out too optimistic in the areas that get little direct sunlight.

12.2 Light-Emitting Diodes (LEDs)

283

12.2 Light-Emitting Diodes (LEDs) 12.2.1 LED Operation The light-emitting diodes (LEDs) have numerous applications in everyday life, such as displays of various sorts (calculators, watches, street signs, etc.), lamps, and light sources in the optical-fiber communication systems. The structure of a LED is shown in Fig. 12.5. It is a forward-biased diode, whose front surface is used for the collection of light, and the rear surface is covered with a highly reflective coating. When a p-n junction is forward-biased, the majority carriers from its two QNRs are injected into the opposite QNRs, where they become excess minority carriers. In the direct-band gap semiconductors, the injected excess carriers recombine with the majority carriers primarily radiatively, i.e., with the emission of light. The region where most of the recombination events occur is called the active region. The rear surface is covered with a reflective coating. The photons that reach the rear surface get reflected from it and have a chance to contribute to the overall light intensity emitted by the device. The effect of light emission by a forward-biased diode bears the name of electroluminescence. The intensity of the emitted light is proportional to the current, which depends on the applied voltage as eV /(nVth ) − 1 ≈ eV /(nVth ) , where n is the ideality factor of the diode. The radiative recombination rates of the minority electrons in the p-QNR and of the minority holes in the n-QNR are, in general, different. It makes sense to collect light from that side of the diode whose radiative recombination rate is the higher; in Fig. 12.5, it is assumed that the radiative recombination rate is the larger in the p-side.

12.2.2 LED Spectrum LEDs employ a radiative recombination of charge carriers, which is most efficient in the direct-band gap semiconductors. Because conduction band energy levels are populated with the probability proportional to e−E/kT , and √ because the density of states in the conduction band depends on the energy as E − EC , the most probable electron energy value can be found by setting the derivative of the product Fig. 12.5 The principle of operation of an LED

284

12 Optoelectronic Devices

√ d[ E − EC e−E/kT ]/dE to zero. The result turns out to be EC + kT /2. Similarly, the most probable energy of a hole in the valence band is EV − kT /2. Then, the most probable energy of a photon emitted as a result of a radiative recombination event is hf = Eg + kT ≈ Eg , and the respective wavelength λ=

hc c ≈ . f Eg

The width of the LED spectrum can be estimated to be f =

kT , h

or, in terms of the wavelength, λ = |(c/f )| =

c kT f = hc 2 . 2 f Eg

kT It is seen that the ratio λ λ = Eg is quite small (about 0.02–0.03), i.e., a single LED emits a rather narrow spectral line. In order to emit in the visible range of λ from about 0.4 to 0.75 µm, the band gap must be between 1.65 and 3.1 eV. GaAs with Eg = 1.42 eV cannot be used for illumination but can be employed in other application, such as telecommunication. The materials that are used in the visible LEDs are ternary and quaternary compounds, such as Alx Ga1−x As (red part of the spectrum), GaAsx P1−x (red), In1−y (Alx Ga1−x )P (yellow/orange light), Inx Ga1−x N (blue/green light), etc. The band gap of those compounds can be adjusted by changing the relative concentrations x, y of the components. To produce white light, one can combine several LEDs of different colors, typically red, green, and blue. A less expensive method that produces the output spectrum comfortable to the eye is to cover a single LED with a photoluminescent material that absorbs the original LED photons and emits light of other, usually lower, frequencies in a broad spectrum similar to the day light.

12.2.3 LED Efficiency The intensity of light emitted by an LED—that is, the power emitted by a unit area of an LED—is directly proportional to the number of recombination events in the active region. This number, in turn, is directly proportional to the number of charge

12.2 Light-Emitting Diodes (LEDs)

285

carriers injected into the active region per unit area per unit time; it is just the electric current density divided by the elementary charge. Since the energy of a photon produced in a radiative recombination event is Eg , the intensity is proportional to J IEL = Eg η , e where the proportionality constant η < 1 is the LED efficiency. The LED efficiency depends on the efficiency of several processes involved in photoemission: Injection Efficiency The net current in the diode consists of three contributions: the minority electron current in the p-QNR, the minority hole current in the n-QNR, and the recombination current in the SCR: J = Je + Jh + JSCR with n2i Dep V /Vth n2 Dhn V /Vth (e − 1) , Je = e i (e − 1) , Na Lep Nd Lhn ni = ew (eV /(2Vth ) − 1) , τSCR

Je = e JSCR

as derived in Sect. 11.5.2. Here, Dep and Dhn are the diffusion coefficients of the minority electrons in the p-region and minority holes in the n-region, Lep and Lhn are the respective diffusion lengths, w is the SCR width, and τSCR is the carrier lifetime in the SCR. Assuming that the light-emitting part of the diode is the p-QNR, it is the current Je that corresponds to electron injection from the n-QNR into the p-QNR and is therefore responsible for the light emission. The SCR recombination, corresponding to the contribution JSCR , usually proceeds not radiatively, but via the trap-assisted Shockley–Read–Hall mechanism. On the other hand, the photons emitted due to hole recombination in the n-region get partly reabsorbed by the material as they travel toward the front surface, and therefore they produce relatively small contribution to the output light intensity. Correspondingly, the emitted light intensity should be proportional to the relative contribution of the electron injection current to the total current. This is parametrized by the so-called injection efficiency ηinj =

Je . Je + Jh + JSCR

In order to make this number close to unity, the n-side of the junction should be doped more heavily than the p-side, so that Je  Jh . Also, the junction must be under a sufficiently large forward bias V in order to ensure that Je  JSCR .

286

12 Optoelectronic Devices

Recombination Efficiency Not all electrons injected into the p-region recombine radiatively. The net recombination rate consists of the radiative and non-radiative contributions, U = Ur + Unr , proportional to the respective inverse radiative and non-radiative recombination times τr and τnr . The recombination efficiency is defined as the relative number of radiative recombination events: ηrec =

Ur τ −1 ≈ −1 r −1 . Ur + Unr τr + τnr

In order to increase ηrec , one needs a high-purity sample with the well-passivated surfaces, so as to reduce the Shockley–Read–Hall and surface recombination rates. At the same time, in order to increase the role of radiative recombination, the p-side of the diode must be heavily doped. Internal Quantum Efficiency Internal quantum efficiency is the product of injection and recombination efficiencies, ηi = ηinj ηrec . Note that ηinj decreases with the p-side doping concentration Na , whereas ηrec increases with Na . Thus, there must be an optimal doping concentration Na that maximizes the internal efficiency. External Quantum Efficiency External quantum efficiency is the fraction of photons produced inside the diode that actually leave the diode. In reality, over 95% of the photons produced in radiative recombination events are lost due to the following reasons: (i) The typical photon energy actually exceeds Eg by about kT , as explained above. The majority of those photons will be reabsorbed by the material. (ii) The photons that reach the front surface of the diode may be reflected back into the semiconductor and be reabsorbed. The probability of reflection depends on the angle of incidence and photon polarization. For normal incidence, reflection probability is polarization-independent and is given by the Fresnel formula

nSC − 1 2

, R =

nSC + 1

where nSC is the semiconductor refractive index. Typically, nSC ≈ 3 − 4, and hence, R ≈25–35%. (iii) Depending on the angle of incidence, θi , the angle of refraction at which a photon exits the material is given by Snell’s law, nSC sin θi = sin θr ⇒ θr = sin−1 (nSC sin θi ) .

12.2 Light-Emitting Diodes (LEDs)

287

Fig. 12.6 Left: Photon refraction as it exits the semiconductor at the incident angle θi below the critical value θc . Right: Photon total internal reflection at the angle of incidence greater than the critical angle

This expression only makes sense when the argument of the inverse sine is below 1. If the argument exceeds 1, light will not exit the material but will undergo total internal reflection back into the semiconductor. This happens when the angle of incidence exceeds the critical angle given by θc = sin−1

1 . nSC

Assuming the typical value nSC = 3.5, the critical angle turns out to be about 17◦ . One can conclude that the light is emitted practically perpendicular to the LED surface (Fig. 12.6). Now, a solid angle corresponding to the angle of incidence θi is given by (θi ) = 2π(1 − cos θi ). The directions of the photons produced in radiative recombination are distributed isotropically, i.e., all directions are equally probable; this corresponds to the solid angle of 4π . Then, the fraction of photons that hit the surface at an angle below the critical angle is (θi ) 1 − cos θc θ2 = ≈ c 4π 2 4 for small θc  1. Assuming θc = 17◦ ≈ π/10, this ratio is about 0.1, i.e., only 10% of the photons have a chance of leaving the material. This has to be multiplied by the transmission coefficient, 1 − R , which is about 0.65 for normal incidence. Thus, we get the external quantum efficiency to be ηe ≈ 6.5 %. This estimate is actually too optimistic because we did not take into account the decrease of (1 − R ) with the angle of incidence and optical losses due to photon re-absorption. The actual external efficiency is about 1% to 2%, i.e., about 98% of the photogenerated photons do not leave the diode. All in all, the number of photons that are emitted by the diode per unit area per unit time is

288

12 Optoelectronic Devices

EL =

J (V ) ηi ηe , e

and the electroluminescence intensity is given by IEL = Eg

J (V ) ηi ηe . e

Assuming Eg = 2 eV, J = 1 A/cm2 , ηinj = 50 %, ηrec = 100 %, and ηe = 1 %, the intensity of the emitted light according to this expression is 0.01 W/cm2 , which is ca. 100 times smaller than the intensity of the light coming from the Sun. This is way too small for practical applications.

12.2.4 Increasing the LED Efficiency The main problem of the homojunction-based LEDs discussed above is the reabsorption of the photons generated in radiative recombination. Because the energy of those photons exceeds the band gap energy by ca. kT , some of them may cause an electron transition from the valence to the conduction band and not contribute to the output light. In a homojunction-based LED, the light-emitting part of the junction must be relatively thin in order to let the photons escape without being reabsorbed by the material. Unfortunately, this implies high probability of the injected minority carriers’ diffusion to the surface and their non-radiative recombination there. Hence, in order to increase the intensity of the emitted light, we need to (i) increase the rate of the radiative recombination in the active region, and (ii) reduce re-absorption of the photons outside of the active region. Both problems are solved with the use of double heterojunction structures. The idea is to produce the diode’s p- and n-sides from broad-band gap semiconductors, and to sandwich the active region in between, see Fig. 12.7a. Usually, the narrowband gap light-emitting region is made of an intrinsic semiconductor. The photons produced in the active region have energy less than the band gap in the adjacent

Fig. 12.7 (a) A heterojunction LED and (b) its energy band diagram

12.3 Semiconductor Lasers

289

p- and n-regions. Therefore, those photons are not absorbed by the structure and eventually contribute to the output light intensity. The second advantage of the double heterojunction arrangement is the fact that the conduction band edge in the active i-region is below the conduction band edge in the n-region, see the energy band diagram in Fig. 12.7b. This implies that the concentration of electrons in the active region is higher than that in the n-region. For the same reason, the valence band edge in the active i-region is higher than that in the p-region, implying higher concentration of holes. In turn, this means high recombination rate and high-output light intensity of the LED.

12.3 Semiconductor Lasers 12.3.1 Stimulated Emission and Einstein’s Coefficients Semiconductor LEDs generate light by spontaneous emission of photons in radiative recombination of electron–hole pairs. Semiconductor laser diodes also generate light by transitions of electrons from the conduction to the valence band. But, in contrast to LEDs, those transitions are stimulated by light quanta (photons) already present in the device. The stimulated emission effect was predicted by Albert Einstein in 1916, more than half a century before the first laser was made. The very name “laser” is an abbreviation for “Light Amplification by Stimulated Emission of Radiation.” Before discussing semiconductor lasers, let us focus on a more intuitive situation of lasing in a gas of atoms that do not form a solid. The atoms find themselves in a cavity of volume V . For simplicity, let us assume that each atom can exist in only two states: the ground state of energy E1 and the excited state of energy E2 . Denoting the concentrations of atoms in the ground and in the excited state as n1 and n2 , the total concentration is given by n = n1 + n2 . Because the concentration of atoms is constant, the rates of change of n1 and n2 are equal in magnitude and opposite in sign: dn1 dn2 dn1 dn2 dn = + =0 ⇒ =− . dt dt dt dt dt Apart from the atoms, the cavity is filled with photons. The photons interact with the atoms via the following elementary processes, see Fig. 12.8: (i) Absorption, in which a photon of frequency f gives its energy hf to promote an atom from the ground to the excited state. In order for this to happen, the photon frequency must exactly match the excitation energy divided by Planck’s constant:

290

12 Optoelectronic Devices

Fig. 12.8 Elementary interactions of a photon with an atom: (i) absorption, (ii) spontaneous emission, and (iii) stimulated emission

f = E/ h = (E2 − E1 )/ h . A photon of frequency below this value cannot excite an atom due to the energy conservation. It is not as obvious why a photon of frequency higher than E/ h cannot give part of its energy to an atom. This has to do with the particle nature of photons. As a particle, a photon cannot be partly absorbed; it can only be either completely absorbed or not absorbed at all. (ii) Spontaneous emission, in which an excited atom returns to the ground state with the emission of a photon of energy hf = E. The emitted photon propagates in a random direction. At a first glance, absorption and spontaneous emission exhaust all possible kinds of matter–light interaction. Let us now describe them mathematically. We denote the concentration of photons of frequency f as nph (f ). The rate of change of the atomic concentrations n1 and n2 due to absorption must be proportional to the concentration of atoms in the ground state and to the total number of photons of frequency f in the volume V : 

dn1 dt

 = −babs n1 V nph (f ) . abs

The parameter babs > 0 is the probability of photon absorption by an atom per unit time. It has the dimension of [babs ] = s−1 . It depends on the atom–photon interaction properties only and does not depend on the concentration of atoms n1 , n2 and on the concentration of photons nph (f ). The minus sign indicates that photon absorption results in a decrease of n1 . The rate at which the concentrations n1 and n2 change due to the spontaneous emission is proportional to the concentration of the excited atoms:

12.3 Semiconductor Lasers

291



dn1 dt

 = bspon n2 . spon

The coefficient bspon is the probability per unit time for an excited atom to return to its ground state with the emission of a photon. In other words, it is the inverse of the average time that an atom spends in the excited state. If only absorption and spontaneous emission were operative, then the total rate of change of the concentration of the atoms in the ground state would be 

dn1 dt



 + abs

dn1 dt

 = −babs n1 V nph (f ) + bspon n2 . spon

Now, let us consider our system in the state of thermal equilibrium. Three statements can be made about the equilibrium state: First, the concentrations of atoms in the ground state and in the excited state are stationary: 

dn1 dt



 = eq

dn2 dt

 =0. eq

Second, they are related to each other by a Boltzmann factor e−E/kT : n2 = n1 e−E/kT ≡ n1 e−hf/kT . Third, the concentration of photons is given by the so-called Planck distribution nph (f ) =

g(f ) , ehf/kT − 1

where g(f ) is the density of photon states; the derivation of this result is performed in Appendix A.5. Hence, in equilibrium, 

dn1 dt



 +

abs,eq

dn1 dt

 = −babs n1 V spon,eq

g(f ) + bspon n1 e−hf/kT . −1

ehf/kT

This should be zero at any temperature. But because the two terms in the right-hand side depend on temperature differently, they cannot cancel each other. This is the problem because it implies that thermal equilibrium state is impossible. To fix this problem, we must, following Einstein, postulate the existence of a third elementary process, namely:

292

12 Optoelectronic Devices

(iii) Stimulated emission This is a process, in which a photon incident on an atom in its excited state induces a de-excitation of this atom into a ground state accompanied by an emission of another photon of the same wave vector as the incident photon, see the lowest diagram in Fig. 12.8. The rate at which the concentration of the atoms in the ground state changes due to this process is proportional to the concentration of atoms in the excited state and the total number of photons in the volume V : 

dn1 dt

 = bstim V nph (f )n2 . stim

The physical meaning of the parameter bstim is the probability for the emission to be stimulated by a single photon per unit time. In thermal equilibrium, 

dn1 dt

 = bstim V stim,eq

g(f ) n1 e−hf/kT . ehf/kT − 1

Combining all three contributions to the time derivative dn1 /dt in equilibrium together, we obtain in the equilibrium state: 

dn1 dt



 =

eq

= −babs n1 V

dn1 dt



 + abs,eq

dn1 dt



 + spon,eq

dn1 dt

 stim,eq

g(f ) g(f ) + bspon n1 e−hf/kT + bstim V hf/kT n1 e−hf/kT . ehf/kT − 1 e −1

This expression can be equal to zero provided that the coefficients babs , bspon , and bstim are related to one another in a special way. Indeed, dividing the second line by n1 e−hf/kT and setting the result to zero, we obtain −babs V

g(f )ehf/kT g(f ) + bspon + bstim V hf/kT =0. ehf/kT − 1 e −1

The sum of the first and third terms is temperature-independent only if the coefficients of absorption and stimulated emission are the same: babs = bstim = b , and that the spontaneous emission coefficient is bspon = bg(f )V . These relations are remarkable. In principle, there is no a priori reason to expect that the coefficients that describe the completely different physical processes can be expressible in terms of each other in such a simple manner. In particular, the last

12.3 Semiconductor Lasers

293

formula tells us that the probability of spontaneous emission per unit time equals the probability of photon absorption b multiplied by the total number of states g(f )V available to an emitted photon of frequency f . The relations between the emission and absorption coefficients follow from purely statistical considerations and are indeed confirmed by the rigorous and rather complicated quantum-mechanical calculations. In the literature, it is customary to work not with the photon concentration nph (f ), but with the photon spectral energy density u(f ) = hf nph (f ) and to express the rates of absorption, spontaneous emission, and stimulated emission as       dn1 dn1 dn1 = −B12 n1 u(f ) , = An2 , = B21 n2 u(f ) . dt abs dt spon dt stim The parameters A and B are called Einstein’s coefficients; they are related to the respective probabilities of the elementary processes to occur per unit time by B12 = babs

V V , A = bspon , B21 = bstim hf hf

and to each other by B12 = B21 = B , A = Bhfg(f ) .

12.3.2 Generation of Light Consider a beam of monochromatic light of frequency f = E/ h propagating in a gas of two-state atoms. As this beam propagates in the x-direction, it interacts with the medium, as described in the previous section. As a result, the concentration of photons in the beam, nph (f, x), depends not only on frequency, but also on the position x. For the sake of brevity, the frequency dependence will be implied, but not written explicitly. We assume the photon concentration to be so high that stimulated emission dominates over spontaneous emission. The photon concentration changes with the coordinate x due to absorption and stimulated emission according to dnph (x) ∂t dnph (x) 1 = = dx dt ∂x c



dnph (x) dt



 −

stim

dnph (x) dt



 abs

294

12 Optoelectronic Devices

=

bV nph (x) (n2 − n1 ) = γ nph (x) . c

Due to the interaction with light, the level populations n1 and n2 will also change. Let us assume that some external agent is operative that maintains them constant; this process is called pumping. In that case, the parameter γ =

bV (n2 − n1 ) , c

called the gain factor, will be constant. Then, the concentration of photons in the beam, nph (x) ∝ eγ x , will either decrease or increase exponentially, depending on the sign of the gain factor, so will the light intensity, i.e., the energy transmitted by the photons per unit time through a unit surface area, F (x) = chf nph (x). The lasing effect means that the intensity of the beam increases. In order for it to be possible, i.e., for the gain factor γ to be positive, population inversion n2 > n1 is a necessary condition. The concentration of atoms in the excited state must exceed the concentration of atoms in the ground state. The physical reason of lasing is quite simple: the more photons are present in the beam, the more stimulated emission events are produced, and the higher the rate of increase of the photon number.

12.3.3 Semiconductor Laser Operation The Structure of a Semiconductor Laser In a semiconductor, one deals not with two discrete energy levels, but with two bands. In order for the diode to lase, it should be in the population inversion state. That is, the electron concentration near the bottom of the conduction band must be higher than the concentration of electrons near the top of the valence band. Clearly, this is impossible in thermal equilibrium, as the following calculation shows. Consider two electron states: state 1 in the valence band and state 2 in the conduction band, with E2 > EC , E1 < EV . The probability for each of these states to be occupied by an electron is given by the Fermi–Dirac formula f1,2 =

1 1 + e(E1,2 −EF )/kT

.

12.3 Semiconductor Lasers

295

Population inversion means higher probability for an electron to be in the state 2 than in the state 1, which is only possible if f2 > f1 . But this implies that e(E2 −EF )/kT < E (E1 −EF )/kT ⇒ E2 − EF < E1 − EF , which contradicts the obvious inequality E2 > EC > EV > E1 . Now consider what happens when the semiconductor consists of two differently doped regions forming a diode. In thermal equilibrium, lasing is not possible also in a diode. Hence, we must bring it out of equilibrium by applying a bias V . In that case, electrons in the n-region and holes in the p-region are characterized by their own quasi-Fermi energies, EF e and EF h , respectively. Inside the space-charge region of the diode, these two quasi-Fermi energies coexist, whereas outside the SCR, the quasi-Fermi energies belonging to the minority carriers quickly align themselves with the majority carriers’ quasi-Fermi energies. Inside the SCR, the probabilities for the states 1 and 2 to be occupied are modified to f2 =

1 1 , f1 = , 1 + e(E2 −EF e )/kT 1 + e(E1 −EF h )/kT

and the population inversion condition, f2 > f1 , implies that we should have E2 − EF e > E1 − EF h or, equivalently, EF e − EF h > E2 − E1 = hf > Eg , where hf is the energy of the emitted photons, and the last inequality follows from the fact that E2 > EC , E1 < EV , and EC − EV = Eg . We conclude that in order for lasing to be possible, one or both sides of the p-n junction must be degenerately doped. A semiconductor laser structure is based on a double heterojunction, where the active region (usually, intrinsic) is sandwiched between the degenerately doped nand p-layers, called the cladding layers, see Fig. 12.9a. Note that a similar structure is used in the LEDs. To increase the optical path length of laser light in the active region, one side of the diode is covered with a highly reflecting coating and the opposite side with a partially reflective coating. This means that lasing effect is possible only for the photons that travel between the reflective sides, and a small fraction of those photons can exit the device through the partially reflective side. As in the LEDs, it is advantageous to make the cladding n- and p-layers of a semiconductor with a slightly larger band gap than in the active region, Egc > Ega ,

296

12 Optoelectronic Devices

Fig. 12.9 (a) Schematic diagram of a semiconductor laser; (b) its energy band diagram; (c) variation of the refractive index along the coordinate z perpendicular to the diode plane

where the subscripts c and a stand for “cladding” and “active,” respectively; see Fig. 12.9b. This band gap difference guarantees strong population inversion. A further improvement is to use the cladding material with the refractive index slightly lower than the refractive index of the active region, nc < na , see Fig. 12.9c. Then, the generated photons will remain trapped inside the active region as a result of the total internal reflection from the boundaries with the cladding layers.

Threshold Current The salient feature of the double heterojunction laser is that its active i-region is very thin. The small size of the central active region implies that the excess carrier concentration there is practically constant. Hence, the physical picture behind the current–voltage curve is quite simple. Namely, the excess electrons are injected into the i-region from the n+ -region, with AJ /e electrons coming in per unit time, where A is the cross-sectional area of the laser. On the other side of the i-region, the excess holes are injected from the p+ -region, with AJ /e holes coming in per unit time. Inside the active region, electrons and holes recombine at a rate U (n)Ad, where d is the width of the active region. Because the number of excess carriers that come in per unit time must be the same as the number of charge carriers that recombine per unit time, the current density is given by J = eU (n)d . To find the current–voltage curve, we note that the excess carrier concentration n depends on the difference between the quasi-Fermi energies of electrons and

12.3 Semiconductor Lasers

297

holes. This difference is nothing else by the applied voltage multiplied by the elementary charge: EF e − EF h = eV , and hence, the excess concentration depends on the applied voltage: n = n(V ) . In a non-degenerate semiconductor, the relationship between n and V would follow immediately from the generalization of the mass–action law, (n0 +n)(p0 + n) = n2i e(EF e −EF h )/kT = n2i eV /Vth . However, since we are considering the case when the quasi-Fermi energies are located inside the bands, we cannot use this relationship and must resort to the qualitative rather than quantitative arguments. When we discussed lasing in a gas of two-level atoms, the gain factor γ turned out to be proportional to the difference between the populations of the two levels. Hence, the light intensity along the beam was increasing according to dF = γ F (x) , γ ∝ n2 − n1 . dx In a semiconductor laser, the difference n2 − n1 must be replaced by the excess carrier concentration, and thus the gain factor is proportional to γ ∝ n. Furthermore, when light propagates in a semiconductor, it gets absorbed with the absorption coefficient α. Hence, the expression for the rate of change of light intensity with distance in a laser becomes dF = (γ − α)F (x) , γ ∝ n . dx After traveling the distance 2L between the two mirrors, light intensity changes by a factor e2L(γ −α) . Light also gets reflected from the two mirrors. Each reflection results in a change of light intensity by a factor equal to the mirror reflection coefficient, 1 and 2 for mirrors 1 and 2, respectively. The net effect of absorption and reflection is a change of light intensity by the product 1 2 e2L(γ −α) . In order for lasing to be possible, this product must be bigger than 1. In turn, it implies that the gain factor must exceed a threshold value, γT , such that 1 2 e2L(γT −α) = 1 ⇒ γT = α +

1 1 ln . 2L 1 2

The gain factor is proportional to the excess carrier concentration. Hence, for lasing to be possible, excess concentration must exceed some threshold value, nT ∝ γT . On the other hand, according to the theory of the current–voltage curve in a p+ -i-n+ structure outlined earlier in this section, the excess concentration

298

12 Optoelectronic Devices

enters into the current–voltage relation as an argument of the net recombination rate. Hence, in order to maintain the excess concentration at the level above threshold, the injection current must exceed the threshold value JT = eU (nT )d . We can make a rough approximation by assuming that the net recombination rate is proportional to the excess carrier concentration, U (n) ∝ n. With this approximation, we conclude that the threshold current must be proportional to JT ∝ nT ∝ γT . Denoting the proportionality constant as β, we can write   1 1 . ln JT = β α + 2L 1 2 At J < JT , very weak light intensity is generated, whereas at J = JT , lasing begins, see Fig. 12.10. The threshold current is thus quite easy to measure. A linear 1 relation between JT and α + 2L ln 112 is indeed experimentally confirmed with β being of the order of 100 A/cm. This implies that the threshold current may be of the order of thousands (or even tens of thousands) A/cm2 , quite a large value. Reduction of the threshold current is one of the main problems in the semiconductor laser technology.

Laser Spectrum The active region of a laser is a resonator, where only photons of certain wavelength can exist. Those photons must satisfy the standing wave condition L = mλm /2 , where L is the distance between the reflecting sides, m is an integer, and λm is the photon wavelength inside the active region. Hence, the laser produces not a single wavelength, but many spectral lines of the wavelength Fig. 12.10 Schematic illustration of the laser intensity vs. current density relation

12.3 Semiconductor Lasers

299

λm = 2L/m . Each such spectral line is called the mode. The frequency of the photons that leave the active laser is the same as the frequency of the photons inside the active region. On the other hand, the velocity of light in the semiconductor is c = c/na , where na is the refractive index of the active region. Therefore, the wavelength of the photons emitted by the laser is λm = c/f = c na /f = na λm = 2Lna /m, and their frequencies are quantized as fm = c/λm = cm/(2Lna ) . The separation between two spectral lines is  λ = λm − λm+1 = 2Lna

1 1 − m m+1

 =

λm 2Lna = . m(m + 1) m+1

For large m  1, the separation between two modes can be approximated as λ =

λ2 λ = . m 2na L

The frequency and energy separations are f = fm+1 − fm =

c hc 1.24 eV · μm , hf = = . 2Lna 2Lna 2Lna

The energies of those photons range from Eg to eV = EF e − EF h > Eg . Hence, eV −E the number of lines in the spectrum of a laser is hf g . Assuming L to be of the order of 100 µm and na of the order of 4, we have the energy separation of the order of 1 meV. For eV − Eg = 1 eV, this means that the number of spectral lines is of the order of a thousand. At a first glance, the higher the bias V , the broader the spectrum of the emitted light should be and the more spectral lines it should contain. In reality, quite the opposite happens: increasing the bias results in a decrease of the number of the spectral lines present in the laser light. In fact, for a large enough bias, the number of spectral lines amounts not to a few thousands, but to just a few. The reason for this paradoxical phenomenon is mode competition. The number of the radiative recombination events that may happen per unit time in the active region is limited by the injection current J ; hence, the growth of the laser intensity

300

12 Optoelectronic Devices

is not infinite but must saturate at some limit intensity value FL . Now, suppose that for some reason, one of the modes contains slightly more photons than others. This means that this mode intensity growth rate due to the stimulated emission exceeds that of other modes. Hence, the more photons a particular mode has, the sooner it should reach the limit intensity. Once a particular mode reaches FL , all other modes cannot be supported because all of the pumping is “consumed” by a particular mode that initially had slightly more energy than the others. As a result, the winner mode gets it all, and a single narrow spectral line is emitted.

12.4 Problems 12.4.1 Solved Problems Problem 1 The irradiance spectrum of the Sun just outside of the Earth’s atmosphere can be modeled as that of a black body with the temperature TSun = 5 778 K. Assume that each photon of energy hf > Eg is absorbed by a SC and produces just one electron–hole pair, which then contributes the energy Eg to the output power. Based on this information, write down an expression for the limit SC efficiency as a function of the band gap, plot the efficiency vs. the ratio Eg /kTSun , and find the Eg value at which it is maximal. Which semiconductor has this band gap value? When solving this problem, you may need to integrate a certain function numerically (use Mable, Mathematica, WolframAlpha, or a similar software). You may also need an ∞ 3 4 identity 0 dx exx−1 = π15 . Problem 2 Consider a p-i-n structure of a heterojunction LED from Fig. 12.7b. It has the following parameter values at T = 300 K: the band gap Eg = 2.5 eV; the width of the i-region d = 0.1 μm; intrinsic concentration ni = 107 cm−3 ; radiative recombination coefficient B = 10−8 cm3 /s; Auger recombination coefficients Ce = Ch = 10−30 cm6 /s; external efficiency ηe = 2 %. The relationship between the excess concentration n in the i-region and the applied voltage V follows immediately from the generalization of the mass–action law, (n0 +n)(p0 +n) = n2i e(EF e −EF h )/kT = n2i eV /Vth . (a) Assuming the i-region to be non-degenerate, find n(V ). (b) Assuming that only radiative and Auger recombination mechanisms are operative in the i-region with the respective coefficients B and Ce,h , find the optimal excess concentration n at which the recombination efficiency in the i-region, ηrec = Ur /(Ur + UA ), is the highest. What voltage is needed to maintain this excess concentration at room temperature? (c) Find the output intensity value obtained at the maximal recombination efficiency. (d) Find the voltage that needs to be applied to the device to have the output light intensity of 0.1 W/cm2 , which matches the typical intensity of the Sun.

12.4 Problems

301

Problem 3 Show that the average time for an atom to remain in the excited state is 1/bspon , where bspon is Einstein’s coefficient of spontaneous emission from Sect. 12.3.1.

12.4.2 Practice Problems Problem 1 Find the intensity of the sunlight just outside of the Earth’s atmosphere. The Sun radiation can be modeled as that of a black body with the temperature 5 778 K, the radius of the Sun is RS = 696 340 km, and the Earth-to-Sun distance is ∞ 3 4 RE−S = 1.5 · 108 km. You may need an identity 0 dx exx−1 = π15 . Problem 2 The total intensity of the monochromatic light incident onto a silicon slab of thickness d = 100 µm is F = 0.01 W/cm2 . Its wavelength is 1 µm. The refractive index of Si at this wavelength is nr = 3.572, and the absorption coefficient α = 62.94 cm−1 . Calculate light intensity F (x) and the electron–hole pair generation rate G(x) for two cases: (a) when the rear surface is untreated and (b) when the rear surface is covered by a perfectly reflecting coating. Here, the distance x is measured from the front surface. Perform these calculations without and with taking into account Fresnel reflection by the silicon–air interface. You may need the sum of a geometric series, 1 + x + x 2 + . . . = 1/(1 − x).

12.4.3 Solutions Problem 1 The spectral irradiance of the Sun is given by (see Appendix A.5) F (f ) = A

f3 ehf/kTSun − 1

,

2 2π h RS , where RS = 696 340 km is the radius of the 2 c2 RE−S 108 km is the Earth-to-Sun distance. The ratio of the two

where the constant A =

Sun and RE−S = 1.5 · radii takes care of the fact that the light intensity decreases with distance r from a point-like source as 1/r 2 . With the simplifying assumptions made in the problem formulation, the incident and the output power per unit surface area of a SC can be written as  Pin = 0

 df F (f ) , Pout = Eg

df Eg / h

F (f ) . hf

302

12 Optoelectronic Devices

In the expression for Pout , we took care of the fact that only photons of energy exceeding Eg are absorbed and contribute the energy Eg to the output power; the spectral photon flux density is related to the spectral irradiance by F (f )/(hf ). The efficiency is ∞ Pout Eg / h df F (f ) η= = ∞ . Pin 0 df F (f ) Using the above expression for F (f ) and changing the integration variables in both integrals to x = hf/kTSun , we have Eg η= kTSun

∞

x2 Eg /kTSun dx ex −1 ∞ x3 0 dx ex −1

=

15 Eg π 4 kTSun



dx Eg /kTSun

x2 . ex − 1

The efficiency vs. the ratio of the band gap to the thermal energy of the surface of the Sun is shown in Fig. 12.11. This curve has a maximum at Eg ≈ 2.17 kTSun . Given that the thermal energy kTSun = (0.02585 eV) · 5778/300 = 0.498 eV, the optimal band gap equals 1.08 eV, which is quite close to the band gap of silicon. This analysis is severely simplified, as it does not account for the radiative and Auger recombination of the photogenerated electron–hole pairs and the optical losses due to the light reflection by the front surface and the escape of some of those photons that got reflected by the rear surface of the SC, as well as a few other, less significant, mechanisms. Nevertheless, the optimal band gap value obtained above is quite close to the truth. Problem 2 (a) With n0 = p0 = ni , we rewrite the modified mass–action law as (ni + n)2 = n2i eV /Vth , from which the excess concentration follows immediately as n(V ) = ni (eV /(2Vth ) − 1) . (b) The concentration of electrons and holes in the i-region is n = p = ni + n. Hence, the radiative and Auger net recombination rate (see Sects. 7.3 and 7.4, respectively) recombination efficiencies are expressed in terms of the excess concentration as ηrec = =

B(2ni n + n2 ) B(2ni n + n2 ) + (Ce + Ch )(3n2i n + ni n2 + n3 ) 1 1+

Ce +Ch B ni f (x)

,

where in the second equality, we divided the numerator and the denominator of the first expression by B(2ni n + n2 ) and denoted

12.4 Problems

303

Fig. 12.11 The limit efficiency of a SC as a function of the semiconductor band gap normalized to the thermal energy on the surface of the Sun

x=

n 3x + x 2 + x 3 , f (x) = . ni 2x + x 2

Clearly, the recombination efficiency is maximal at that x-value at which the function f (x) has a minimum. We find the minimum of f (x) by differentiation at x0 =

5 − 2 ≈ 0.2361 ,

corresponding to n = xni = 0.2361 ni . Based on the result from part (a), we find the voltage needed to be √ V0 = 2Vth ln(1 + x) = 2Vth ln( 5 − 1) = 11 mV . (c) The electroluminescence intensity is IEL = Eg Ur (n)dηe = Eg dηe Bn2i (2x + x 2 ) . With the x = 0.2361, we have IEL = 4.23 · 10−20 W/cm2 , corresponding to the photon flux density

304

12 Optoelectronic Devices

=

IEL = 0.105 1/(cm2 s) . Eg

That is zero for all practical purposes. (d) The desired output intensity corresponds to the x-value found from the quadratic equation x 2 + 2x −

IEL =0. Eg dηe Bn2i

For IEL = 0.1 W/cm2 , the constant IEL = 1.248 · 1018 . Eg dηe Bn2i This corresponds to the value of x  x = −2 +

IEL 4+ = Eg dηe Bn2i



IEL = 1.117 · 109 , Eg dηe Bn2i

as the parameters of the order of 1 can be neglected for all practical purposes. The voltage necessary to obtain this intensity is V = 2Vth ln x = 2 · 0.02585 ln 1.117 · 109 = 1.08 V .

Problem 3 The probability pexc (t) for an atom to remain in the excited state is related to the concentration of atoms as n2 (t) = pexc (t)n. It decays in time as dpexc (t) = −bspon pexc (t) . dt The solution of this equation with the initial condition pexc (0) = 1 is pexc (t) = e−bspon t . The derivative −dpexc (t)/dt has the physical meaning that the atom will return to the ground state at time between t and t + dt. The average time spent in the excited state is, then,    ∞  ∞ dpexc (t) 1 = bspon texc = dt t − dt t e−bspon t = , dt b spon 0 0 as can be obtained by changing the integration variable to x = bspon t.

Appendices

A.1 A Crash Course in Complex Numbers A complex number z is formed by a pair of two real numbers, x and y, as z = x + iy . The number i is called the imaginary unit and is defined as the positive square root of −1: i 2 = −1 , i =

√ −1 .

The two components of a complex number z are called the real part and the imaginary part of z: x = Rez , y = Imz . The operation of complex conjugation is denoted by a star and is defined by changing the sign in front of the imaginary part: z∗ = x − iy . Complex numbers can be added and subtracted. If we have another complex number w = u + iv, then z + w = (x + u) + i(u + v) , z − w = (x − u) + i(y − v) .

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4

305

306

Appendices

Two complex numbers can be multiplied together: zw = (x + iy)(u + iv) = x(u + iv) + iy(u + iv) = xu + ixv + iyu − yv = (xy − yv) + i(xv + yu) . The product of a complex number with its conjugate, zz∗ = (x + iy)(x − iy) = x 2 − (iy)2 = x 2 + y 2 is a positive real number. Its positive square root, √ |z| = zz∗ = x 2 + y 2 is called the modulus of z. A complex number can also be divided by another complex number: zw ∗ z zw ∗ (x + iy)(u − iv) xu + yv yu − xv = = = = 2 +i 2 . ∗ 2 2 2 2 w ww |w| u +v u +v u + v2 Euler’s identity is an extremely useful theorem. Let θ be a real number, and thus iθ is purely imaginary. Then eiθ = cos(θ ) + i sin(θ ) . To prove this identity, we denote two complex-valued functions of θ : f (θ ) = eiθ , g(θ ) = cos(θ ) + i sin(θ ) . Their logarithms have the same derivatives. Indeed, for the function f (θ ), d(iθ ) d ln f (θ ) = =i. dθ dθ As for the function g(θ ), we first observe that dg(θ ) = − sin(θ ) + i cos(θ ) = i (cos(θ ) + i sin(θ )) = ig(θ ) , dθ and hence d ln g(θ ) 1 dg(θ ) = =i. g(θ ) dθ dθ From the identity

d ln f (θ) dθ

=

d ln g(θ) dθ

it follows that

f (θ ) = Cg(θ ) ,

A.1 A Crash Course in Complex Numbers

307

where C is some unknown constant. In order to find this constant, we focus on the specific value of θ = 0, for which f (0) = g(0) = 1. Hence, C = 1, i.e., f (θ ) = g(θ ) for all θ . This completes the proof. As an illustration of usefulness of Euler’s identity, it can be used to derive various trigonometric identities, which one may have a hard time memorizing. Consider the product eiα eiβ = (cos α + i sin α)(cos β + i sin β) = cos α cos β − sin α sin β + i(cos α sin β + sin α cos β) . On the other hand, eiα eiβ = ei(α+β) = cos(α + β) + i sin(α + β) . Two complex numbers are equal if both their real and imaginary parts are equal. We thus conclude that cos(α + β) = cos α cos β − sin α sin β , sin(α + β) = cos α sin β + sin α cos β . These identities can be proven without complex numbers, but the proof will be much longer. Note that the trigonometric functions can be expressed in terms of complex exponentials as follows. Write Euler’s identity for angles θ and −θ : eiθ = cos(θ ) + i sin(θ ) , e−iθ = cos(θ ) − i sin(θ ) . Adding up these two expressions and dividing the result by 2 gives cos(θ ), whereas subtracting these expressions from each other and dividing the result by 2i gives sin(θ ): cos(θ ) =

eiθ − e−iθ eiθ + e−iθ , sin(θ ) = . 2 2i

More importantly, Euler’s identity allows one to represent a complex number z in a convenient manner. Namely, a complex number z can be represented as a point in the complex plane whose coordinates are formed by its real and imaginary parts, see Fig. A.1. The distance from that point to the origin is modulus of the complex number z. The angle formed by the line joining the origin with that point is called the argument of z. On the diagram, this angle must be measured in the counterclockwise direction. Geometrically θ = arg(z) = tan−1

y ; x = |z| cos θ ; y = |z| sin θ . x

308

Appendices

Fig. A.1 Representation of a complex number z = x + iy as a point in the complex plane

Then, a complex number z can be represented as z = x + iy = |z|(cos θ + i sin θ ) . Applying Euler’s identity, we obtain the aforementioned representation of a complex number: z = |z|eiθ .

A.2 Proof of Bloch’s Theorem When a periodic lattice potential is present, then all measurable physical properties of the electron gas, such as its density, should likewise be periodic. The singleelectron wave function (r ), however, does not have to have the lattice periodicity. But the wave function itself is not physically measurable; it is the probability density that can be measured. Hence, we must have for any translation vector d = i a +j b + k c  2. |(r )|2 = |(r + d)| The most general choice for a wave function must with this property is 1 (r ) = √ eiθ(r ) u(r ) , V where the factor periodic,

√1 V

is introduced for later convenience, the function u(r ) is  = u(r ) , u(r + d)

and the unknown function θ (r ) is not periodic.1  = = θper (r )+θnonper (r ) with θper (r + d) θper (r ), then we could define our new periodic function u(r ) as a product of the old u(r ) and eiθper (r ) . Hence, we can explicitly demand that θ(r ) be not periodic in r without loss of generality. 1 If θ( r ) had a periodic and a non-periodic part, i.e., θ(r )

A.2 Proof of Bloch’s Theorem

309

Let us define a new wave function, which differs from the original one (r ) in that its argument r is shifted by the translation vector a : 1 1 shf t (r ) = (r + a ) = √ eiθ(r +a ) u(r + a ) = √ eiθ(r +a ) u(r ) , V V where in the last equality, we used the periodicity property of u(r ) = u(r + a ). Let us define the difference θ (r ) = θ (r + a ) − θ ( a) , in terms of which 1 1 shf t (r ) = √ ei(θ(r )+θ(r )) u(r ) = √ eiθ(r ) eiθ(r ) u(r ) = eiθ(r ) (r ) . V V Because of the translational symmetry of the potential U (r ) = U (r + a ), shifting the coordinate r by a translation vector a does not affect the timeindependent Schrödinger’s equation. This means that shf t (r ) should satisfy the same Schrödinger’s equation as (r ), that is, −

h¯ 2  2 ∇ shf t (r ) + U (r )shf t (r ) = Eshf t (r ) . 2me

Substitution of the relation shf t (r ) = eiθ(r ) (r ), however, produces two new   2 θ (r ). Those terms are not present terms, which are proportional to ∇θ (r ) and ∇ in the original Schrödinger’s equation for (r ). The only way to get rid of those terms is to demand that θ (r ) = θa is a constant independent of r. Hence, shifting the coordinate by one lattice vector a results in an increment of the phase by a constant: θ (r + a ) = θ (r ) + θa . Likewise, we could shift the coordinate by either of the remaining two lattice vectors, b or c, and repeated the above argument. This would lead us to the conclusion that  = θ (r ) + θb , θ (r + c) = θ (r ) + θc θ (r + b) with constant θb and θc .

310

Appendices

The only function θ (r ) that has these properties is a linear function: θ (r ) = k · r , up to an immaterial additive constant. Then, θa = k · a , θb = k · b , θc = k · c .  We do this by imposing the We now need to figure out the wave vector k. periodic boundary conditions. Namely, we view the crystal as a large parallelepiped  and N c. containing N 3 unit cells. It is built on the three translation vectors N a , N b, We demand that the wave function (r ) repeat itself every time its argument gets shifted by one of those vectors:  = (r + N c) = (r ) . (r + N a ) = (r + N b)  and N k · c are all integer multiples of 2π . In This is only possible if N k · a , N k · b, turn, this implies that the wave vector 2π m  , k = N where m  is a vector whose all three components are integers.  We finally substitute the wave function (r ) = √1 ei k·r u(r ) into the V Schrödinger’s equation: −

h¯ 2  2  i k·    ∇ e r u(r ) + U (r ) ei k·r u(r ) = E ei k·r u(r ) . 2me

The first term can be transformed to −

h¯ 2  2  i k· h¯ 2   2  r  r ) − k2 u(r ) ei k· . ∇ e r u(r ) = − ∇ u(r ) − 2i k · ∇u( 2me 2me

Recalling (see Sect. 1.8.1) that electron momentum is identified with the operator  r ), we rewrite this in terms of the momentum as pu( ˆ r ) = −i h¯ ∇u(  2 1 ˆ2 ei k·r  ˆ  p u(r ) − 2h¯ k · pu( p − h¯ k u(r ) . ˆ r ) + h¯ 2 k2 u(r ) ei k·r = 2me 2me 

After canceling the factors ei k·r , we arrive at the equation for u(r ): 2 1 ˆ p − h¯ k u(r ) + U (r )u(r ) = Eu(r ) , 2me

A.3 Properties of Si, Ge, and GaAs

311

 and the square of the operator pˆ − h¯ k where the momentum operator pˆ = −i h¯ ∇, simply means applying it twice to the function u(r ). If not for the term h¯ k in the brackets, the equation obtained would look like a time-independent Schrödinger’s  = U (r ) equation for the wave function u(r ) in the periodic potential U (r + d) produced by the lattice. In the absence of the lattice potential, i.e., with U (r ) = 0, the function u(r ) = 1  u(r ) = −h¯ k,  and E = (h¯ k)  2 /(2me ), as it should for all positions r. Then, (pˆ − h¯ k) be.  = u(d),  this equation Together with the periodicity requirement, u(r + d)  provides full information from which u(r ) and E can be found. We indicate the kdependence of its solution as a subscript in uk (r ) and as an argument of the function  Furthermore, at each given k,  another quantum number n should arise, which E(k).  This quantum number—the labels different solutions of this equation for fixed k.  Hence, band index—is indicated as a subscript both in uk (r ) and E(k).  . u(r ) = unk (r ) , E = En (k)

A.3 Properties of Si, Ge, and GaAs Unless stated otherwise, the numerical data in this section are taken from the online data base of the Ioffe Institute at http://www.ioffe.ru/SVA/NSM/Semicond. Crystal structure and lattice constant: Si (diamond) : a = 5.431 Å ; Ge (diamond) : a = 5.658 Å ; GaAs (zincblende) : a = 5.65325 Å . Bandgap temperature dependence: Eg (T ) = Eg (0) −

αT 2 T +β

with the parameters: Si : Eg (0) = 1.17 eV ; α = 4.73 · 10−4 eV/K ; β = 636 K ; Ge : Eg (0) = 0.742 eV ; α = 4.8 · 10−4 eV/K ; β = 235 K ; GaAs : Eg (0) = 1.519 eV ; α = 5.405 · 10−4 eV/K ; β = 204 K .

312

Appendices

Transverse and longitudinal effective mass components of an electron and the number of valleys in the conduction band: Si : m∗e,t /me = 0.19 , m∗e,l /me = 0.98 ; νC = 6 ; Ge : m∗e,t /me = 0.0815 , m∗e,l /me = 1.59 , νC = 4 ; GaAs : m∗e,t /me = m∗e,l /me = 0.063 , νC = 1 . Heavy and light hole effective masses: Si : m∗hh /me = 0.49 , m∗lh /me = 0.16 ; Ge : m∗hh /me = 0.33 , m∗lh /me = 0.043 ; GaAs : m∗hh /me = 0.51 , m∗lh /me = 0.082 . Effective densities of states at 300 K: Si : NC = 3.2 · 1019 cm−3 , NV = 1.8 · 1019 cm−3 ; Ge : NC = 1.0 · 1019 cm−3 , NV = 5.0 · 1018 cm−3 ; GaAs : NC = 4.7 · 1017 cm−3 , NV = 9.0 · 1018 cm−3 . Bandgap and intrinsic concentration at T = 300 K:2 Si : Eg (300 K) = 1.12 eV ; ni (300 K) = 8.59 · 109 cm−3 ; Ge : Eg (300 K) = 0.661 eV ; ni (300 K) = 1.97 · 1013 cm−3 ; GaAs : Eg (300 K) = 1.424 eV ; ni (300 K) = 2.31 · 106 cm−3 . Relative dielectric permittivities: Si :  = 11.7 ; Ge :  = 16.2 ; GaAs :  = 12.9 .

2 Some discrepancy exists in the literature regarding the intrinsic concentration in Si at 300 K, which is 1010 cm−3 according to the data √base of the Ioffe Institute. For the sake of formal consistency, it is calculated here as ni = NC NV e−Eg /(2kT ) rather than taken from this data base. The most recent experimental result in Si is ni (300 K) = 9.65 · 109 cm−3 , see P.P. Altermatt, A. Schenk, F. Geelhaar, and G. Heiser, Journal of Applied Physics 93, 1598 (2003).

A.3 Properties of Si, Ge, and GaAs

313

Ionization energies of shallow donor impurities: Si : As: 0.054 eV ; P: 0.045 eV ; Sb: 0.043 eV ; Ge : As: 0.014 eV ; P: 0.013 eV ; Sb: 0.010 eV ; GaAs : Si: 0.006 eV ; Ge: 0.006 eV ; Sn: 0.006 eV . Ionization energies of shallow acceptor impurities: Si : Al: 0.072 eV ; B: 0.045 eV ; Ga: 0.074 eV; In: 0.157 eV ; Ge : Al: 0.011 eV ; B: 0.011 eV ; Ga: 0.011 eV; In: 0.012 eV ; GaAs : Si: 0.1 eV ; Ge: 0.03 eV ; Sn: 0.2 eV; Zn: 0.025 eV . Radiative recombination coefficient at T = 300 K:3 Si : B = 4.7 · 10−15 cm3 /s ; Ge : B = 6.41 · 10−14 cm3 /s ; GaAs : B = 7.2 · 10−10 cm3 /s . Auger recombination coefficients at T = 300 K: Si : Ce = 1.1 · 10−30 cm6 /s ; Ch = 3.0 · 10−29 cm6 /s ; Ge : Ce ∼ Ch ∼ 10−30 cm6 /s ; GaAs : Ce ∼ Ch ∼ 10−30 cm6 /s . Electron affinities at T = 300 K: Si : eχ = 4.05 eV ; Ge : eχ = 4.00 eV ; GaAs : eχ = 4.07 eV .

3 The value of B in silicon is taken from T. Trupke, M.A. Green, P. Würfel, P.P. Altermatt, A. Wang, J. Zhao, and R. Corkish, “Temperature dependence of the radiative recombination coefficient of intrinsic crystalline silicon,” Journal of Applied Physics, 94, 4930 (2003).

314

Appendices

A.4 Evaluation of Exponential Integrals Here, we would like to find the value of the integral 

In =

dx x n+1/2 e−x for n = 0, 1, 2, 3, . . .

0

First,√let us focus on the simplest case n = 0. We change the integration variables to y = x, giving  I0 =

dx

x e−x = 2

0



∞ 0

d =− da

dy y 2 e−y = 2



∞ −∞



∞ −∞



−ay 2

dy e

dy y 2 e−y

a=1

2

df (a)

=− . da a=1

In the last line, we introduced a parameter a, later to be set to 1. Differentiation 2 with respect to the parameter a turns the more complicated integral of y 2 e−y into 2 the one with a simpler integrand e−ay . Let us call the function of a that is to be differentiated  ∞ 2 f (a) = dy e−ay −∞

and consider the square of this function:  f (a) = 2



∞ −∞

dy1

∞ −∞

Transforming to the polar coordinates, r =

dy2 e−a(y1 +y2 ) . 2

2

y12 + y22 , θ = cos−1

y1 , y12 +y22

we must

also replace the integration element—the area dy1 dy2 —with r dr dθ . Noting that the integrand does not depend on the polar angle, we can write:  f (a) = 2π 2

dr r e−ar , 2

0

where integration over the polar angle θ = 0 . . . 2π has been performed, giving 2π . In other words, the surface area dy1 dy2 got replaced by the area 2π r dr of a ring of radius r and thickness dr. The last integral is found by changing the integration variables to z = r 2 :  ∞ π f 2 (a) = π dz e−az = . a 0

315

Hence,  f (a) =

dy e−ay =



2

−∞

π . a

Coming back to our original task, 

I0 =

dx 0

x e−x = 2



dy y 2 e−y = − 2

0

√ √ π d π/a

= .

da a=1 2

Now, let us evaluate In for n ≥ 1. For this, let us define a function  F (a) =

dx

x e−ax ,

0

which, upon a change of the integration variable to y = ax, becomes F (a) =

I0 . a 3/2

It allows one to obtain In by differentiating with respect to a and setting a to one: In = (−1)

nd

n F (a)

da n

,

a=1

as can be verified by using the integral formula for F (a) and the fact that (−1)n x n e−ax . In particular, we have I1 =

d n −ax da n e

=

√ √ √ 3 3 π 3·5 15 π 3·5·7 105 π I0 = ; I2 = 2 I0 = ; I3 = ; etc. I = 0 2 4 8 16 2 23

A.5 Planck’s Radiation Law The quantum state of a photon is characterized by two quantum numbers: its wave vector k and its polarization s. The polarization can have two values, s = +1 and −1, which correspond to the counterclockwise and clockwise rotation of the  k|  of photon propagation. We consider electric field vector around the direction k/| the photons in a cube of side length L and impose the periodic boundary conditions. Hence, the three components of the wave vector have quantized values: kα =

2π mα , α = x, y, z and mα = . . . , −2, −1, 0, 1, 2, . . . . L

316

Appendices

The probability to have n photons in the state with particular values of k and s is 

−nhf (k)/kT  s) = e , pn (k, Z

where the frequency of a photon in this state is  = f (k)

ck  , , k = |k| 2π

c being the speed of light. The constant Z has the value that normalizes the total probability to one: Z=

1



e−nhf (k)/kT =

n=0

 1 − e−hf (k)/kT

,

 n where we used the expression for the sum of a geometric series, ∞ n=0 x = 1/(1 − −hf/kT  s) is < 1. The average number of photons in the state (k, x) with x = e  s) =

n(k,

 s) . npn (k,

n=0

It can be obtained by setting a=

 hf (k) kT

and noting that ∞  −na −na d ln ∞ d 1 1 n=0 ne n=0 e  =− ln .

n(k, s) = ∞ −na = − = a −a da da 1 − e e −1 n=0 e We finally replace the parameter a with the ratio of photon energy to the thermal energy to obtain  s) =

n(k,

1  e−hf (k)/kT

−1

.

To find the concentration of photons nph (f ) of frequency f , we need to multiply  s)-state with the density of photon states, the average number of photons in the (k,  s) states in a unit volume per unit frequency interval. The total i.e., the number of (k, number of the photon states with the wave vector smaller than a given value k equals the ratio of the volume of a sphere of radius k to the “volume” (2π/L)3 occupied by

317

one photon state; this ratio needs to be multiplied by 2 in order to account for two possible polarizations. Hence, N(k) = 2 ·

1 4π k 3 k3 3 · = L . 3 (2π/L)3 3π 2

The total number of photon states of frequency smaller than a given value f is obtained by replacing k with 2πf/c: N(f ) =

8πf 3 3 L . 3c3

The photon density of states is obtained as the derivative g(f ) =

8πf 2 1 dN(f ) = . L3 df c3

Hence, in thermal equilibrium, the concentration of photons per unit frequency interval is  s) = nph (f ) = g(f ) n(k,

1 8πf 2 . hf/kT 3 −1 c e

In the literature, it is more common to work with the spectral energy density, i.e., the energy of photons in a unit volume per unit frequency interval. It is given by the Planck’s radiation law: u(f ) = hf nph (f ) =

1 8π hf 3 . c3 ehf/kT − 1

The spectral irradiance is given by F (f ) =

2π hf 3 1 c u(f ) = . hf/kT 2 4 e −1 c

Index

A Absolute zero, 70 Absorption coefficient, 279 Acceptor concentration, 131 dopants, 127 ionization energy, 130 level, 130 AM1.5G spectrum, 278 Atomic order, 43 packing fraction, 47 radius, 47

B Band bending, 160 conduction, 98 diagram, 160 edge, 89 gap, 87, 89 index, 82 valence, 98 Band structure dielectrics, 97 metals, 97 semiconductors, 97 semimetals, 97 Si, Ge, GaAs, 89 Black body, 6 Bloch oscillations, 94 state, 82 theorem, 81, 308

Bohr radius, 10 radius in a semiconductor, 129 theory, 9 Boltzmann approximation, 69 constant, 66 Bonding covalent, 43 ionic, 43 metallic, 43 van der Waals, 42 Bosons, 27 Bouguer-Lambert-Beer law, 279 Brillouin zones, 84

C Charge neutrality equation, 133 Chemical potential, 66 Collision time, 200 Complex numbers, 305 plane, 307 Conductivity, 201 Continuity equation, 206 Crystal basis, 46 lattice, 43 one-dimensional, 85 structure, 46 Crystal momentum, see Quasimomentum, 83 Cubic lattice body-centered, 48 face centered, 49

© The Author(s), under exclusive license to Springer Nature Switzerland AG 2022 M. Evstigneev, Introduction to Semiconductor Physics and Devices, https://doi.org/10.1007/978-3-031-08458-4

319

320 Cubic lattice (cont.) simple, 48 Current density, 198

D de Broglie wavelength, 6 Debye length, 156 screening, 155, 165 Defects of a crystal lattice, 54 Degeneracy, 24 Density of states electrons, 118 holes, 118 photons, 317 Depletion approximation, 156 validity, 158 Depletion region, see Space charge region, 156 Detailed balance, 182 Diamond structure, 50 Dielectric constant, 128 Diffusion, 199 coefficient, 199 length, 265, 266 Diode, 215 Schottky, 215 Donor concentration, 130 dopants, 127 ionization energy, 129 level, 129 Doping, 127 amphoteric, 127 Double slit experiment, 30 Drift, 199 velocity, 200

E Effective density of states electrons, 120 holes, 120 Effective mass conductivity, 123 density of states, 122 of an electron, 102 longitudinal, 102 of a hole, 103 tensor, 101 transverse, 102 Einstein’s relation, 205

Index Electroluminescence, 283 Electron affinity, 216 capture by a trap, 181 charge, 9 concentration, 115, 119 concentration in a non-uniform potential, 152 current density, 198 emission by a trap, 181 energy probability distribution, 121 flux density, 198 mass, 9 Emission spontaneous, 290 stimulated, 292 Energy band, 83 kinetic, 7 of a photon, 8 Energy quantization, 8 Euler’s identity, 306 Excess carrier dynamics, 175 charge carriers, 174 concentration, 174

F Fermi-Dirac distribution, 67 Fermi energy, 67, 69 Fermions, 27 Fluctuations, 62

G Generation of charge carriers, 171 non-thermal, 174 rate, 174 thermal, 174 Gradient, 15 Grand canonical distribution, 64 Ground state, 4, 17 Group velocity, 91

H Hall effect, 202 Heat bath, 64 Hole, 99 capture by a trap, 181 concentration, 120

Index concentration in a non-uniform potential, 152 current density, 198 emission by a trap, 181 energy, 100 energy probability distribution, 122 flux density, 198 heavy, 104 light, 104 occupation probability, 100 Hydrogen quantum numbers, 23, 24 spectrum, 9

I Ideality factor, 228, 269 Image charge, 227 Impurity deep, 173 shallow, 127 Imref, 187 Indistinguishability of particles, 25 Intensity, 277 Intrinsic semiconductors carrier concentrations, 126 Fermi energy, 126 Inversion layer, 160, 165 Ionization regimes complete ionization, 134 freeze-out, 138 intrinsic, 136

L Laplacian, 16 Laser, 289 gain factor, 294 mode competition, 299 population inversion, 294 pumping, 294 spectrum, 298 structure, 294 threshold current, 296 Lattice Bravais, 44 constant, 44 cubic, 44 triclinic, 44 Light-emitting diode, 283 efficiency, 284 heterojunction, 289 spectrum, 283

321 M Macrostate, 62 Magnetic field, 24 Mass action law, 132, 188 Metal-semiconductor contact built-in voltage, 217 energy band diagram, 215 Ohmic, 219 rectifying, 221 Microstate, 61 Miller indices in a cubic lattice, 52 for directions, 51 for planes, 52 Mobility, 200 Momentum operator, 20 MOSFET, 233 accumulation regime, 245 body, 233 conduction parameter, 238 C − V measurements, 245 depletion mode, 234 depletion regime, 246 drain, 233 energy band diagram, 239, 240 enhancement mode, 233 flat-band voltage, 243 gate, 233 inversion layer, 233 inversion regime, 246 I − V curve, 235, 237 oxide capacitance, 242 oxide voltage, 242 pinch-off, 236 source, 233 threshold voltage, 233, 239, 244 trapped charges, 242 O Orbital atomic, 41 hybridization, 50 P Pauli exclusion principle, 27 spin-statistics theorem, 26 Periodic potential, 81 Periodic table, 41 Phase velocity, 90 Photoconductivity, 202

322 Photoelectric effect, 6 Photogeneration, 202 Photon, 6, 172 flux density, 277 Planck constant, 6 radiation law, 291, 315, 317 Plane wave, 5, 14 PN junction, 257 built-in electric field, 261 built-in voltage, 258 C − V measurement, 262 energy band diagram, 258 I − V curve, 264 one-sided, 262 quasineutral region, 257 Shockley boundary conditions, 264 space charge region, 258, 261 space charge region recombination current, 268 Poisson’s equation, 152 exact solution, 161 Primitive cell, 45 Probability a priori, 63 density, 13 of a microstate, 62

Q Quantum numbers, 4, 17 state, 4 Quantum state occupation probability, 67 Quasi-Fermi energy, 187 Quasimomentum, 83 Quasiparticles, 104

R Reabsorption, 287 Recombination Auger, 172, 178 Auger, coefficient, 179 of charge carriers, 171 Energy and momentum conservation, 171 net rate, 175 radiative, 172, 177 radiative, coefficient, 177 rate, 175 Shockley-Read-Hall, 173, 180 surface, 173, 186

Index surface, velocity, 186 time, 176 Resistance, 201 Resistivity, 201 Reverse saturation current of a Schottky diode, 223, 226 Richardson constant, 224 Rydberg’s constant, 10

S Schottky barrier, 217 diode, C − V measurements, 218 diode, J − V curve, 222 Schrödinger’s equation in a periodic potential, 81 time-dependent, 15 time-independent, 17 Semiconductors compensated, 127 direct band gap, 98, 172 indirect band gap, 99, 172 intrinsic, 126 p- and n-types, 128 Silicon, 41 Solar cell, 275 efficiency, 282 fill factor, 282 I − V curve, 280 open-circuit voltage, 281 power, 282 short-circuit current, 275, 281 Solar spectrum, 278 Space-charge region (SCR), 156, 165 electric field, 157 electric potential, 157 recombination, 228 width, 157 Spectral irradiance, 276 Spin, 24 Standing wave, 8 Surface passivation, 173, 187

T Thermal energy, 69 equilibrium, 62, 171 velocity, 125 voltage, 152 Threshold potential, 160 Total internal reflection, 287 Tunneling effect, 219, 228

Index U Unit cell, 45 W Wave angular frequency, 5 equation, 11 number, 12, 85 packet, 92 vector, 5, 82 Wave function, 11 collapse, 19

323 interpretation, 12, 17 modulus, 21 phase, 21 Wavelength, 5 Wave-particle duality, 5 Wigner-Seitz cell, 46 Work function metal, 215 semiconductor, 215 Z Zincblende structure, 50